PrefacePaint has been used for artwork for many thousands of years. The oldest Mediterraneancivilizations including the Greeks, Romans, and Egyptians used encaustics, paintsmade with a mixture of mineral pigments (iron, copper, manganese oxides, etc.),melted beeswax, and resin and then ﬁxed with heat. Tempera, a ﬂuid mixture ofbinder (organic medium), water, and volatile additives (vegetal essential oils) andorganic binders made of materials available from animal sources (whole egg, animalglues, or milk) were used to make paints for hundreds of years. At the end of the Roman Empire and up to the Renaissance period (ﬁfteenthcentury), these ancient formulas were lost and replaced by oil paint and/or tempera.In Italy and Greece, olive oil was used to prepare pigment mixtures, but the dryingtime was excessively long and unpredictable. Gradually, paints were reﬁned withdifferent oils and additives, working in combination with heat, to produce a group ofreliable resin systems and solvent blends for modern industrial coatings that providethe appearance characteristics to satisfy consumers and protective characteristics tomake the product last in different environments and conditions. Modern coatings arenow used on virtually every durable-good product manufactured. In more recent history, the need to clean up the environment has had a profoundimpact on coating formulation. Higher solids content and water content have changedto reduce the solvent included in the blend and reduce waste and emissions generatedby the use of surface coatings. Surface coatings are used on furniture, toys, automobiles, bicycles, computercabinets, televisions, and thousands of other products. Many of these products arecoated with liquid organic paints. Paint provides a decorative or protective coatingon a metal, plastic, or wood product. Paint is also applied for insulation, to reﬂectlight, or conduct electricity. The average person can see the decorative value of paint, and many products arepurchased because of eye appeal. Although it is less obvious at the time of purchase,resistance to the elements is equally important, and consumers appreciate the fact thatthe products they own will stay cleaner, last longer, and resist corrosion because theyare protected by a high-quality industrial coating. xiii
AuthorRodger Talbert is an independent consultant working in surface ﬁnishingtechnology. He designs new systems for liquid spray coating, powder coating,and electrodeposition, and works to improve existing systems through processimprovement, retroﬁt, and training. Talbert began his career in coatings in 1976, working for a company involvedin custom coating and metal fabrication. He also worked 7 years for a companythat designs and builds coating systems. He started his own business, R. TalbertConsulting, Inc., in 1993. Talbert has taught Powder Coating and Finishing System Design and Operation atGrand Rapids Community College, where he designed and implemented a FinishingTechnician Certiﬁcate program and published six training manuals for liquid coating,electrocoating, and powder coating classes. He is the editor of The Powder Coater’sManual, and he is a member of the technical advisory committee for the Iowa WasteReduction Center. He also conducts periodic training workshops in liquid coatingspray technique, powder coating, and systems design. Talbert received his education in business administration at Aquinas College inGrand Rapids, Michigan. He is a member of the Powder Coating Institute (PCI)and a member of the Electrocoat Association. He is the former chairman of theApplication & Recovery Committee of the PCI, chairman of education for ChemicalCoaters Association (CCAI), technical director for CCAI, and former president of theNational Board of Directors for CCAI. He has written and presented numerous technical papers for SME/AFP, PCI, andCCAI. He has contributed to the SME Design for Manufacturing handbook on thesubject of powder coating, is a contributor to the PCI Powder Coating Terms &Deﬁnitions handbook, and is a contributor to the PCI Powder Coating Manual andThe Complete Finishers Handbook. He also wrote the chapter on powder coating inthe Manufacturers Engineering Handbook, published by McGraw-Hill. xv
1 Part Preparation Processes and EquipmentA coating is applied to a part to enhance its appearance and to protect the substratematerial. An organic coating will act as a physical barrier to moisture, but if thecoating surface is damaged, the bare metal is exposed, and corrosion can form andspread. The adhesion of the coating and the corrosion resistance of the productdepend on the preparation of the surface. Part preparation is often referred to aspretreatment. The term pretreatment is used to deﬁne the mechanical or chemical surfacetreatment for a manufactured product, referred to as the substrate, to clean it, andprepare it for the application of a coating. Pretreatment can be accomplished in manydifferent ways. For example, sanding a part to remove dirt is a simple mechanicalmethod of part preparation. Chemical pretreatment may be as simple as a solvent wipe,or it may be a multistage spray washer that cleans the part and applies a conversioncoating. The speciﬁc method and degree of pretreatment used depends on qualityrequirements of the product. Pretreatment typically provides better adhesion of the coating to the part and helpsprevent the spread of corrosion, adding value to a product and extending its useful life.Pretreatment eliminates reactions between metals and between coatings and metals.It also cushions expansion and contraction differences between the substrate and thecoating. Pretreatment is one of the most important steps in ensuring that the coating willperform as intended. A decorative coating will not hide defects, and the performanceof a coating is directly related to the condition of the surface that it is applied to.Application of the coating over a contaminant will prevent it from forming a tightbond to the substrate, and if the contaminant lifts off, so will the coating. Dirt particleswill not dissolve or be hidden by the coating. For good appearance and adhesion,the part must be clean. In addition to cleaning, it may be necessary to develop a conversion coatingon metal surfaces prior to coating application. With the exception of some preciousmetals such as silver, gold, and platinum, metals react with air to form an oxide layeron their surface. Water molecules are tightly held to this oxide layer. This is not agood surface condition for chemical bonding. An example of a surface that has beentreated with a conversion coating is shown in Figure 1.1. Deciding what process can be used to pretreat a particular part depends on theperformance requirements of the ﬁnal part, pretreatment requirements of the paintto be used, the substrate material, and soils on the surface. 1
2 Paint Technology HandbookFIGURE 1.1 Magniﬁed zinc phosphate surface.1.1 CLEANINGManufactured products have a variety of contaminants on their surfaces. Before acoating is applied to the substrate, the surface has to have these contaminants removed.If contamination is left on the surface, the coating may not meet the required qualitystandards for appearance, adhesion, or corrosion resistance. The kind of pretreatment to use will depend on the types of soil found on thesurface and the quality goals for the product. A good deﬁnition of the level of per-formance that is required will lead to a cleaning process that is effective and reasonablein cost.1.1.1 TYPES OF SOILRaw materials that are stored, handled, or used for manufacturing products willalways have some surface contamination. On metals, the probable contaminantsare oily soils, including petroleum products, animal fat, or vegetable oils depos-ited during manufacturing operations for rust protection, drawing, machining, andforming. There may also be heavy-duty drawing compounds and lubrication greases orwaxes and some solid soils such as carbon, graphite smuts, metal shavings, polishingproducts, metal oxides, welding scale, and rust or corrosion. Plastics may have mold release, skin oils from handling, plastic particles fromsanding, and dust and dirt from the atmosphere. There are a variety of mechanical and chemical methods that can be used toclean metals and plastics. Accurate identiﬁcation of soils leads to the proper cleanerselection and helps verify cleanliness. The ﬁrst step is to do a soil audit to determinewhat types of soils will need to be removed.
Part Preparation Processes and Equipment 18.104.22.168 Rust InhibitorsLubricants, parafﬁn waxes, oils, drawing compounds, and similar rust inhibitorsare made from petroleum oils. Oils will usually break down pretty well in alkalinechemical cleaners.22.214.171.124 Shop DirtDust, shop dirt, and other forms of particulate can be removed with most alkaline oracidic cleaners and can also be removed by mechanical blasting or grinding, followedby a blow off.126.96.36.199 CarbonCarbon is present in all organic compounds and in a few inorganic compounds. It isabundant in various steel alloys in the form of metal smut. Carbon smut is extremelyinert and nonreactive due to electrostatic attraction to metal surfaces. Chelants do avery good job of breaking down smut whereas alkalis, solvents, and most acids arenot very effective. Mechanical cleaning can also be very effective at removing smutfrom a steel surface.188.8.131.52 OxidationAn oxide of any metal can develop on the metal surface right after the metal isformed or cast. Aluminum oxide and zinc oxides are white, while iron oxide is redrust. Copper oxide is recognized as a green tarnish. Acids are extremely good forthe removal of oxides since all oxides are acid soluble. Some alkaline products thatare not inhibited will remove zinc and aluminum oxides. Solvents are typically noteffective. Mechanical cleaning is very effective for the removal of oxide layers. Laser cutting is a commonly used process for many different gauges of steel.The laser cutting process creates an oxide layer on the edge that has been cut. Paintwill adhere to the laser oxide but the laser oxide is not tightly adhered to the steel.If the coating is cracked along the edge it may completely delaminate, especiallyif the product is used out-of-doors. Sanding, grinding, chipping, and blasting can be very effective for the removalof laser scale. Hand methods are somewhat limited due to the high labor content andthe inherent inconsistencies associated with manual operations. Some shapes may bedifﬁcult to clean by hand. Automated blasting can be very effective if the steel is heavy enough to withstandthe pressure and all surfaces are accessible to the blast media. Blasting may be agood way to treat laser edge when hot-rolled steel (HRS) is used because the scaleand other inorganic soils can also be removed. Acidic chemical solutions have also been effectively used for the removal oflaser oxide. Many of these solutions are phosphoric acid-based solutions applied byspray or in immersion systems. Phosphoric acid is aggressive enough for the taskwithout over-reaction that may occur with some other acids.
4 Paint Technology Handbook The disadvantage of phosphoric acid is the signiﬁcant volume of iron phosphatesludge, which, over time, without proper circulation and ﬁltration, builds up in thetank, fouling heat exchangers, clogging plumbing systems, and eventually resultingin expensive system cleaning and downtime. In addition, in some cases, the strongacid solution will leave ﬁne metal particles on the surface that show up in the coating. In some instances, blends of acids are the most effective chemical approach. Thereare commercially available blends of acids that work synergistically to remove laserscale without many of the negative aspects of a single acid. In addition to selectingthe proper chemistry, you must also apply the product properly. Adjusting cleanerconcentration and bath temperature can optimize cleaning time. It is very important to involve the chemical supplier for a wash system to makesure that the design for chemical removal of laser scale considers the compatibility ofall the system chemistry with the process equipment’s material of construction. Laserscale can be effectively removed when necessary using acid-resistant equipment andblended engineered chemicals.184.108.40.206 WaxWaxes are similar in composition to fats and oils. Some are hydrocarbons, whileothers are esters of fatty acids. They are water repellent, nontoxic, smooth textured,and resistant to many chemical cleaning products. Waxes are often used on tubingas a rust inhibitor. They are solids at ambient temperatures so the cleaner used mustreach the melting point of the wax to break it down. They are soluble in most organicsolvents and alkaline cleaners, providing that the contact time is long enough and thetemperature is high enough.220.127.116.11 SoapsSoaps are sometimes formed by the water-soluble reaction of a fatty acid andan alkali. Soaps lower the surface tension of water and permit emulsiﬁcation of fatbearing soils. Soft soaps, heavy metal soaps, and vegetable oil soaps can be foundin products such as metalworking ﬂuids. Alkaline cleaners are generally the best atsaponifying soaps. Acids will turn the soap to a semisolid mass and make rinsing moredifﬁcult. Solvents are usually not effective, too expensive, and not environmentallydesirable.18.104.22.168 PolymersPolymers are sometimes used in compounds to provide good lubricity and releasingproperties during certain manufacturing processes. Organic polymers can be natural,synthetic, and semisynthetic molecules such as phenolic materials and celluloses.Inorganic materials include siloxanes, silicones, and sulfurized polymers. Acids,alkaline cleaners, solvents, and detergents can be used to remove polymers.22.214.171.124 SiliconeSilicones are sometimes used as lubricants or release agents in manufacturing pro-cesses. Silicones can be liquid, solid, or semisolid. These are long, straight-chain
Part Preparation Processes and Equipment 5polymers, very low in surface tension, and they are not easily broken down usingalkaline or acidic products. They can be removed with organic solvents, but thesolvent will become contaminated very quickly.1.1.2 MECHANICAL CLEANINGAs brieﬂy discussed earlier, there are many types of soil on manufactured products,including organic substances such as oil or inorganic materials such as mineral-typerust inhibitors, scale, or rust. Many of these soils can be effectively removed bymechanically abrading the surface. Mechanical methods, including wire brushing,abrasive blasting, grinding, and sanding, are used to smooth as well as clean surfaces.Mechanical cleaning with a hand-held grinder or a manual blast system can be veryeffective, but it is very labor intensive. In-line blasting can be used to automate theprocess. Mechanical cleaning is sometimes the only way to remove excessive dirt,rust, or scale.126.96.36.199 BlastingBlasting with sand or grit will remove mill scale, rust, or previous coatings from asubstrate and create a surface proﬁle that provides good coating adhesion. The dry ﬁlmthickness of coatings used over a shot-blasted substrate is determined by the proﬁleproduced. A general rule of thumb would be 1 mil over the peaks of the proﬁle.Thicker ﬁlms are recommended, if the part will be used in an outdoor application. Blasting operations can be manual batch systems or automated in-line systems.Blasting systems can use high-pressure nozzles or a centrifugal wheel to deliver theblast media. Nozzle blast systems require compressed air for delivery of the media,while a wheel system uses centrifugal force. Even though the compressed air is anadded cost, it may be necessary to direct nozzles into hard to reach areas of a part.The blast area must be enclosed to contain the blast media and dust. A blasted surface will create a very good anchor pattern for a coating. A blastsystem does not require as much space as a spray washer. Chemical use, mainten-ance, and the associated efﬂuent are avoided. Mechanical treatments may be theonly treatment required for ﬁnishes, where initial coating adhesion is the only crit-ical requirement. However, mechanical cleaning alone will not provide undercoatcorrosion resistance or extend the life of the ﬁnished product. Adequate coveragewith the coating material is critical, if extended life is expected over a blast-onlysurface. The ﬁlm thickness of the coating on a blasted surface must be thick enoughto cover the peaks and valleys of the anchor pattern created by the abrasion. Handheld air-blast systems are very dependent on the concentration of the oper-ator, and the quality may vary. Blast cabinets are often suction-feed systems thatdraw particles into the spray gun by induced vacuum and accelerate the media with ametered stream of compressed air. Pressure-blast systems use a pressurized vessel todeliver the media, providing higher nozzle velocity that can clean the surface muchfaster than a suction system. Blast cabinets function similar to any booth designed for containment of over-sprayed material. Negative pressure within the cabinet is maintained with a fan that
6 Paint Technology Handbookdraws air into the enclosure through a suitable ﬁlter. Typically, this exhaust systemwill use a cyclone separator to remove the dust and ﬁne particles from the airstreamand recover the media for reuse. The scrap material that is separated out of theairstream is collected for disposal in a container attached to a dust collector. Thisscrap material should contain a small percentage of the heavier, reusable media toindicate that the fan pull is sufﬁcient to prevent the buildup of ﬁnes in the recoveredblast media. A vibratory screener can be added to the process to further reﬁne therecovered material and maintain consistent particle size. Turbine-blast systems use high-speed turbine wheel with blades. The media ismetered to the center of the wheel where it is fed onto the blades, which sling theparticles at the surface being blasted. These systems are more energy efﬁcient thanair-blast systems, because they do not use compressed air for delivery. Abrasive blasting is most often used for the preparation of heavy structural parts,particularly HRS welded components. It does an excellent job of removing rust,smut, carbonized oils, and inorganic surface contaminants that are characteristicof this type of product. It can also effectively remove organic soils as long asthe blast media is maintained to avoid a buildup of oil that can cause contamina-tion. The blasting dust needs to be washed away or blown off before the coating isapplied. Different blast media can be used to vary the proﬁle created on the metal surface.Less aggressive media will remove most soils without cutting too deeply into themetal and leaving a visible texture on the metal surface. More aggressive mediacan be used to cut stubborn encrustations, such as red oxides, but it will leave moretexture on the surface. A blast system requires less space than a spray washer that uses chemical clean-ing and it does not generate any wastewater. Mechanical cleaning may be the onlytreatment required for ﬁnishes where initial paint adhesion is required. However,mechanical cleaning alone will not provide undercoat corrosion resistance or extendthe life of the ﬁnished product. The degree of cleaning with the blast operation depends on the qualityrequirements of the surface. Published documents clearly deﬁne quality grades ofblast-cleaned steel surfaces. Pictorial standards were originally developed by theSwedish Corrosion Committee and later adopted by the Steel Structures PaintingCouncil (SSPC) (Table 1.1) and other organizations. The principal four grades ofblasting endorsed by the SSPC are as follows: White metal blast: Removal of all visible rust, mill scale, paint, and foreign matter. Used for conditions where corrosion resistance is very important and the environment is highly corrosive. Near white metal blast: Blast cleaning until at least 95% of all surface area is free of all visible residues. Used for harsh environments where product is exposed to heavy usage. Commercial blast: Blast cleaning until at least two-thirds of the surface is free of all visible residues. For applications where tightly adhering contaminants are allowable on the surface; used for products with lower quality standards and noncorrosive environments.
Part Preparation Processes and Equipment 7 TABLE 1.1 Metal Blast Standards Degree of Cleanliness SSPC Standard NACE Standard White metal blast SSPC-SP 5 NACE No. 1 Near white metal blast SSPC-SP 10 NACE No. 2 Commercial blast SSPC-SP 6 NACE No. 3 Brush of blast SSPC-SP 7 NACE No. 4 For additional information on blast cleaning standards: Plaster, H.J., Blast Cleaning & Allied Processes, Vols. I and II, Industrial Newspapers Ltd., London, 1973 and Fuchs, F.J., “Abrasive Blasting Systems,” in Metal Finishing Guidebook & Directory, Vol. 95, No. 5A, Metal Finishing, Hackensack, NJ, 1997, p. 49. Brush-off cleaning: Blast cleaning of all except tightly adhering residues of mill scale, rust, and old coatings, exposing numerous evenly distributed ﬂecks of underlying metal. Acceptable in noncorrosive environments where long-term coating life is not expected. The Swedish Standards Association (SIS) includes good equivalents of thesestandards. The British Standards Institute (BSI) also includes very close equivalentsof the ﬁrst three of these standards. The National Association of Corrosion Engineers(NACE) has also developed a set of encapsulated steel coupons that simulate the fourdegrees of cleanliness (Table 1.1).188.8.131.52 Blast MediaThe blast media affects the depth of the blast proﬁle and surface roughness afterblasting. Blast media can be made of natural material such as silica, sand, mineralsand, ﬂint, garnet, zircon, and other mineral products. Some natural by-products arealso used for blasting, such as walnut shell or corncob. Other blast materials aremanufactured using a variety of metal and nonmetal compositions such as steel, iron,aluminum oxide, silicon carbide, plastic, wheat starch, and glass bead. The size of the media particles will affect the blast pattern. Other media selectioncriteria include how well it will cut, how well it will recycle, and how much it cost.It is also important to know if there are any health and safety issues, such as lungproblems associated with silica, and if the media will leave by-products on the surface,such as oils from walnut shells. Table 1.2 shows some common blast media and theircomparative characteristics. In addition to the comparative issues listed in Table 1.2, it is a good idea to testdifferent media to have a visual idea of the effect that they will have on the part. Hard grit media such as aluminum oxide will cut faster and deeper than soft,angular media such as plastic or agricultural grit. Mineral, ceramic, or metallic gritmedia are used in air-blast systems. Iron and steel media are more often used inturbine-blast equipment.
8TABLE 1.2Comparison of Blast Media Mesh Density Mohs FriabilityMaterial Size (US) Shape (lb/ft3 ) (Hardness) (Breakdown Factor) Initial Cost No. of Cycles Cost per UseSilica sand 6–270 A, S 100 5.0–6.0 High Low 1 Med.Mineral slag 8–80 A 85–112 7.0–7.5 High Med. 1–2 Med.Steel grit 10–325 A 230 8.0 Low High 200+ Med.Steel shot 8–200 S 280 8.0 Low High 200+ LowAluminum oxide 12–325 A 125 8.0–9.0 Med. High 6–8 Med.Glass bead 10–400 S 85–90 5.5 Med. Med. 8–10 LowPlastic 12–80 A 45–60 3.0–4.0 Low/med. High 8–10 Med.Wheat starch 12–50 A 90 2.8–3.0 High High 10–12 HighCorn cob 8–40 A 35–40 2.0–4.5 Med. Low 4–5 LowA = angular product that cuts more sharply; S = spherical product that peens and does not cut as sharply; Med. = medium. Paint Technology Handbook
Part Preparation Processes and Equipment 9 Materials that are more prone to fracture, reﬂected in the chart by friability, arenot good materials for recycling, because the particle size is reduced during the blastprocess and the media may not be of sufﬁcient size and sharpness to cut soils fromthe surface. The recirculated material will not be as effective, and the surface willvary widely after blasting.184.108.40.206 Vibratory Cleaning or TumblingVibratory systems use an abrasive media in a cleaning solution to remove burrs, roughedges, and surface contamination. They can be useful for preparation of small castingsor parts that have trim die ﬂash or rough edges. They will remove the roughness anddried-on compounds that are often present on a cast surface or the burrs left behindon a sawed edge. Vibratory cleaning will leave some residue on the surface, and it isa good idea to spray clean parts after the vibratory polishing so that and residualcleaning compound is removed before coating.1.1.3 CHEMICAL CLEANINGThe ﬁrst step in the chemical pretreatment process is the removal of dirt, oils, andother soils that could cause surface defects, interfere with the development of agood quality conversion coating, or interfere with paint adhesion. Chemical cleaningmethods include wiping the part with a rag, dipping the part into a solution, or usinga spray cleaning system. The cleaner may be alkaline, acidic, neutral, solvent, oran emulsion. The particular cleaner and process used will depend on the soils to beremoved, the size and substrate material of the part, the type of coating to be applied,and the quality goals for the product.1.1.4 CHEMICAL CLEANING PROCESSESThe different methods of chemical cleaning have certain applications where they ﬁtand limitations that make them unsuitable for other applications. A review of thevarious methods of applying a chemical cleaner helps to understand these strengthsand limitations.220.127.116.11 Hand WipeThe most inexpensive method of cleaning from an equipment perspective is manualcleaning of parts. This would normally involve hand-wiping parts with a solvent oraqueous (water based) cleaning solution. Manual cleaning can be somewhat effectivein terms of soil removal but is very costly in terms of labor and very slow in termsof production time. Because of this, hand-wiping of parts is rarely done except on aspot basis. Hand wiping with a clean cloth does not require any capital investment, but it isnot very effective at soil removal; it has a high labor content, is inconsistent, and maycreate health and safety problems.
10 Paint Technology Handbook18.104.22.168 Immersion CleaningCleaning by immersion in solution is often used for small parts in a batch system.Immersion systems can be either static (still) or agitated. Immersion cycle times aretypically longer than spray cleaning methods, because spray systems have the addedcleaning power of mechanical energy from spray pressure. Systems with no agitationrequire longer cycle times, and they are not as effective. Agitated immersion systems have the added beneﬁt of physical movementbetween the solution and the parts being cleaned. This aids in the overall speed ofreaction taking place between the cleaning compound and the soil. Agitation may beachieved in the tank through air addition or blade mixing. Some dip systems mayalso use a hoist to lift a basket of parts up and down in the tank to provide agitation.Dip systems normally require higher chemical concentration than spray systems andlonger operation times, even with agitation. When the parts are lifted up from the chemical solution, they may retain someresidual chemicals or oil that may ﬂoat to the surface of the solution. Cleaners usedin dip systems should be products designed to emulsify oils rather than products thatdisperse the oils and allow them to ﬂoat to the surface. Many systems use some immersion cleaning along with spray stations.Automotive systems often include some immersion stages to make sure that all ofthe surfaces of the product are fully wetted and dirt is loosened inside and outside ofthe part. The use of immersion with spray stages can enhance overall performance.22.214.171.124 Hand-Held Spray WandHandheld spray wands or steam spray systems are often used to clean parts in abatch powder coating operation. A manual operator has the time to focus attentionon stubborn soils and hard-to-reach areas, providing very thorough removal of soils.Spray wands are often used for larger parts that cannot be easily transported throughautomated systems. The spray wand is used inside a booth. The booth encloses the process so thatthe water vapors is captured and exhausted to atmosphere. Over-sprayed solutioncan be run straight to drain or captured, ﬁltered, and reused. As in manual wiping,this process is time consuming and is not efﬁcient for large numbers of small parts. High-pressure spray wands can use hydraulic pressure as the force to do thecleaning. This type of cleaning is done at pressures ranging from 400 to 1000 psi. Thetemperature ranges from cold water to hot water (200◦ F) for high-pressure washing.This type of washing is done with or without cleaning compounds. The water volumeused ranges from 2 to 35 gal/min. Steam generators are sometimes used to produce dry saturated steam for spraycleaning. In a coil-type, forced-circulation steam generator, water is forced into thecoil toward the discharge point. As the water passes through the coil, it becomesprogressively hotter as steam is formed. Most of the water is evaporated before it dis-charges into the steam generator. This type of steam generator is designed to circulatemore water than is evaporated. This excess water carries loose scale particles andother foreign matter through the coil and into the separator. Here, the water and scaleparticles are separated from the steam, providing high-quality, dry, saturated steam.
Part Preparation Processes and Equipment 11 Steam systems are not as effective as hot-water systems. They do not provideas much energy at the parts surface and do not wet out the surface as well. The energyrequired to generate steam is higher than the hot-water systems. Spray wand systems provide ﬂexibility for contact time and angle and the highpressure can remove heavy greases. Higher foaming surfactants may be used, becausefoam is generally not a concern and higher temperatures are possible, so it may beeasier to melt waxes and grease. The labor content and the chemical cost are high. Cycle times are long, and spraywands are not suitable for higher volumes of small parts. Spray wands do not offerthe wide variety of chemicals and process steps that are possible with multistage spraywashers.126.96.36.199 Ultrasonic CleaningUltrasonic cleaning utilizes high-frequency sound waves to increase the effective-ness of the cleaning chemicals and the agitation at the soil–substrate interface onthe material. Transducers are located either inside or outside the cleaning vessel toproduce the sound waves. When the sound waves reach the surface of the materialto be cleaned, they cause cavitation. Cavitation is the formation and collapse ofvapor bubbles and voids in liquid by acoustic energy at high frequencies. These tinyexploding bubbles act as a brush to carry particles and used chemical away from thesurface of the substrate. This increases the capabilities of the chemicals by continu-ously replacing inactive, reacted product, with fresh chemical. In addition, it gives thechemicals new sites to work on by breaking away loose dirt and other contaminants. Metals are the best candidates for ultrasonic cleaning, since their crystallinemolecular structure allows vibration to occur relatively freely. Rubbers and plasticsdo not work nearly as well, because the molecular structure of these materials is morelikely to absorb the shock waves rather than vibrate with them. Ultrasonic cleaning works very well for cleaning metal surfaces and they aremultimetal safe. Complex geometries and blind holes do not diminish the effective-ness of the sound waves since they clean the part throughout; these are not line-of-sitedevices. The consistency of ultrasonic cleaning is much higher than conventionalcleaning methods as well. Cleaning occurs on all surfaces of the object for the entireduration of the process. Ultrasonic is particularly effective for some porous metalssuch as bronze. Larger loads do not clean, as well as smaller loads, given the same time frame,due to energy absorption. Large, heavy parts can block each other out and cause poorcleaning.188.8.131.52 Recirculating Spray WashersSpray washers are the most common way to chemically clean and treat a part forapplication of a coating. A spray washer uses a series of spray stages that featuredifferent solutions for different tasks. Each stage of a spray washer consists of thesolution tank, the recirculating pump, plumbing for delivery of the solution, a tankheating system, and the gauges and controls that operate the system. A tunnel ismounted over the tanks to contain the spray process. Parts are usually transported
12 Paint Technology Handbook Spray Tunnel risers Gauges Spray Pump nozzles Overflow Tank Drain Elevation view End view Profile plate Tank Pressure valve access lid Plan viewFIGURE 1.2 Spray washer components.through the washer tunnel on an overhead conveyor, although smaller parts washersmay use a belt-type conveyor. The cleaning solution is recirculated through the sprayheader up to the risers and out through nozzles onto the parts. The parts of the spraywasher are shown in Figure 1.2. The nozzles on the risers aid in the cleaning process by providing a directedpressure spray in a predetermined pattern to completely cover the part. The most com-mon nozzle used in this application is the vee-jet, which produces a ﬂat, fan-shapedspray of uniform density. The angle of spray (20◦ –90◦ ) is determined by the nozzleand riser spacing in the washer stage and the desired level of overlap in the spraypattern. As seen in Figure 1.2, the nozzles are placed so that all surfaces of the partare reached as it proceeds through each of the various stages. The recirculating spray washer is the most efﬁcient process for continuousproduction ﬂows. It can handle large volumes of products and provide excellentcleaning and treatment of most parts. Spray washers are signiﬁcantly more expensive than manual cleaning methodsand they also cost more to operate. They require more maintenance and control toperform properly. The number of stages of a spray washer depends on the substrates to be processed,the type of cleaning and other processes that will be used, space availability, and cost.The end use of the part and the performance requirements of the coating will alsoimpact the number of stages. Generally speaking, more stages will improve cleaningand ﬁnish performance. Three-stage washers are common for products that do not need exceptional cor-rosion resistance. The ﬁrst stage is normally a cleaner or cleaner/conversion coatingfollowed by two rinse stages. The rinse stages are usually recirculated water rinses
Part Preparation Processes and Equipment 13with a volume of water (typically 3–5 gal) overﬂowed to drain and made-up withfresh water to maintain relatively clean rinse water. The cleaner stage is usuallyheated to enhance the performance of the cleaning solution. Rinses are not typicallyheated, although the ﬁnal rinse is sometimes heated to leave the part surface warmand accelerate drying after wash. Stepping up from three stages of pretreatment to ﬁve stages allows the separationof the cleaning and the conversion coating steps, with a rinse in between each pro-cess to reduce cross-contamination of the cleaner and conversion coating solutions.As washers increase in complexity from ﬁve- to seven-stage systems, the added stagesare generally additional cleaners or rinse tanks. Good cleaning is an essential part ofthe pretreatment process. Excellent rinsing ensures that the residual chemicals andsoils are removed before the coating is applied. Proper cleaning of some parts may require a combination of spray and immersionstages. The spray stage combines the chemical properties of the cleaner with theimpingement action of the solution applied under pressure. Immersion penetratesareas of the part that may be inaccessible to the spray and improves wetting of hardto reach surfaces.1.1.5 COMMON INDUSTRIAL CHEMICAL CLEANERSThe selection of the correct chemical product for an application is critical to theproper operation of the cleaning system. Products typically used in pretreatmentinclude alkaline cleaners, neutral cleaners (which also act as detergent additives),acid cleaners, and solvent emulsion cleaners. In each group, there are speciﬁc attrib-utes to be considered. The cleaner selected must have the ability to remove a widevariety of soils, prevent redeposition, provide cleaning even when contaminated,provide foam control, be easily rinsed, and be cost effective. Cleaners are often classiﬁed according to their pH. The pH of the solution isa measurement of the relative alkalinity or acidity. On the pH scale, pure water isneutral and has a pH of 7. A pH below 7 is considered acidic and above 7 is alkaline.Caustic soda has a pH of 13 or 14, while hydrochloric acid has a pH of less than 1.A typical range of pH is shown below. • Alkaline cleaners—mild, pH 9–10.5 — medium, pH 10.5–11.5 — high, pH > 11.5 • Neutral cleaners—pH 6.5–9 • Acid cleaners—pH 1.0–5.5The various components that are used to build an industrial cleaner have their ownunique mechanisms that affect certain soils.184.108.40.206 Alkaline CleaningAlkaline cleaners are popular for metal cleaning operations, primarily because ofthe versatility of their components and their ability to break down organic soils.
14 Paint Technology HandbookMost of the soils that commonly occur in metal processing can be effectively removedby the correct selection of these individual components. The most important elementsare the alkalinity source and level, the addition of chelants or chelating agents, andthe surfactants. The key to an alkaline cleaner is the source of alkalinity selected for theformulation. Alkalinity source selection considers both free and total alkalinity. Free alkalinity refers to the material in the solution that is easily reactive.It can be either sodium or potassium hydroxide-based. Sodium hydroxide (NaOH)is very reactive with organic soils such as animal and vegetable fats and issaponiﬁable (able to be reacted with free alkali to form water-soluble materials).As sodium hydroxide tends to cause some rinsing difﬁculties because of its afﬁn-ity for metal, the slightly less reactive potassium hydroxide (KOH) is sometimesused to create a product that is easier to rinse. Products having high levels of freealkali (NaOH or KOH) are good cleaners for products with heavy deposits of organicmaterials. In some cases, high levels of free alkalinity are not desirable. Hydroxide-basedproducts can attack some metals, such as aluminum, resulting in etching or dis-solving of the metal. Alkaline builders, actually alkaline salts such as carbonates,phosphates, and silicates, are often used to clean these metals. These builders con-tribute to total alkalinity and they often have other properties that contribute to morethan just alkalinity. For example, silicated products that are normally considered tobe aluminum safe can be used to form a protective barrier on the metal to preventfurther oxidation/attack by the alkalinity of the product. Silicates are also effectivedispersants for particle soils. Phosphates also help to disperse particulates and aid intying up water hardness. Caustic is a generic term for hydroxides. Sodium hydroxide, which provides thehighest level of free alkalinity, is very effective at saponiﬁcation but tends to resistfree rinsing. Potassium hydroxide provides better rinsing, but is slightly less effectivethan sodium hydroxide. Caustic gives the most alkalinity punch for the pound of anyof the alkalinity sources. Caustic also creates a water-soluble soap from the previouslynonsoluble oil or fat. Sodium hydroxide (NaOH) is cheap and plentiful. Caustic soda, or sodiumhydroxide, is often used for pH adjustment (to raise pH). Sodium hydroxide is usedin many cleaning compounds, electro-cleaning products, and alkaline-based paintstrippers. Potassium hydroxide (KOH) is more expensive, more soluble, and freer rinsingthan sodium hydroxide. It is still high in free alkalinity and offers excellent soilsaponiﬁcation. Carbonates are a less potent source of alkalinity than hydroxides but one that willstill provide some degree of saponiﬁcation of oils and fats. They are often used asa base for mild alkaline cleaners. Sodium carbonate, also called soda ash, is also usedfor pH adjustment, especially when a lower level of alkaline pH is desired. One ofthe major disadvantages of carbonates is their tendency to form calcium carbonatescale in high temperature and hard water conditions. Sodium meta-silicate is used for several purposes in cleaning formulations.It contributes alkalinity, and it can provide limited saponiﬁcation. It has excellent
Part Preparation Processes and Equipment 15particle soil dispersion capabilities and prevents particulate matter from redepositingon an already clean surface in an aqueous environment. Silicate inhibits attack onaluminum and zinc surfaces by plating out on the metal surface as soon as the cleansurface is available to protect the clean surface from high alkaline attack. Phosphates serve several roles in a cleaner formulation, including alkalinitybuilding, pH elevation, saponiﬁcation, and particulate soil dispersion. Phosphatesare especially effective where smut and other particulate soils are encountered.Phosphates come in many forms from the polyphosphates to orthophosphates. Tri-sodium phosphate (TSP) is used in development of orthophosphates. TSPis moderately alkaline, moderate on particulate soil removal, moderate for oils andgreases, and has some limited dispersant capabilities. Two sources are typically used for complex phosphates; they are sodiumtri-polyphosphate (STPP) and sodium hexametaphosphate. Complex phosphates areexcellent sequestrants, complexing calcium to act as a chemical water softener. It hasexcellent particle soil removal capabilities (pigments, for example) and very goodparticulate soil dispersion capabilities. It is a good corrosion inhibitor for ferrous surfaces and functions as a thresholdscale inhibitor. Polyphosphates are, however, environmentally objectionable in someareas. Chelants are often added to alkaline cleaners to aid in the removal of particulatesoils such as carbon smut or metal ﬁnes. Chelants are compounds, which tie upmetal ions, allowing them to be dispersible in water. Chelating chemicals can beinorganic materials, such as ethylenediamine tetraacetic acid (EDTA), or organicmaterials, such as citric acid. Chelated products are often required when cleaningmetals with high carbon content, such as steel that has been hot-rolled or metals thathave undergone processes, which may have contributed particulates, such as drawingor lapping compounds. Chelants are not often used on aluminum because of attackon the metal, so most aluminum-safe products will be chelant-free. Chelants can alsocause some problems in plants, where waste recovery of heavy metals (such as lead)is carried out in-house. Common chelating agents include EDTA, sodium gluconate,and organic acids. EDTA is extremely free rinsing and exceptionally effective as a chemical softenerwhen high levels of calcium and magnesium are present in the water. In alkalineproducts, EDTA is also very effective on taking off light surface rust. Sodiumgluconate is used in formulating most hot tank paint strippers, because it is parti-cularly stable and effective on paints. Paint pigments are often metallic-based, andsodium gluconate helps to pull them off and keep them dispersed in solution. Organicacids are used in acidic formulations. Common organic acids used include citric acid,ascorbic acid, acidic acid, hydroxy-acidic, and formic acid. Typically, a mild alkaline cleaner (pH of 9–10) will provide better soil removaland longer bath life than a high caustic solution. Residues of alkali salts will killthe free acid, drop out metal salts, and kill the phosphate bath. High caustic canalso be too aggressive in attacking zinc and aluminum surfaces, possibly creatingsmut and adding zinc to the solution. A mild alkaline cleaner prior to the phosphatestage will aid in the formation of a more uniform, dense phosphate coating, leadingto better paint adhesion and corrosion protection. If the cleaning is not adequate,
16 Paint Technology Handbookit is usually better to increase the time in the cleaner rather than the concentration.Two mild alkaline cleaner stages are better than one high caustic stage. Mild alkalinecleaners are good for multiple metals and they can be run at a wide variety of tem-peratures. In some cases, a higher pH cleaner may be necessary on occasion for verydifﬁcult soils. A list of the functions of different alkaline cleaner components is shownbelow. • Silicates—(sodium metalicate, sodium orthosilicate) High alkalinity, good saponiﬁer and dispersant, softens water by precipitation, inhibits dissolu- tion of zinc and aluminum. May leave a whitish residue on parts, if not properly rinsed • Phosphates—(TSP, STPP, tetrasodium pyrophosphate, disodium phos- phate) Softens water alkalinity, improves rinsing, saponiﬁer • Carbonates—(sodium carbonate, sodium bicarbonate) Alkalinity, good buffering • Hydroxides—(sodium hydroxide, potassium hydroxide) High alkalinity, saponiﬁer • Nitrites—(sodium nitrite) Minimizes oxidation of metal due to cleaner drying • Chelants—(versene) Softens water, changes form of precipitation • Surfactants—Provide water/oil solubility. Enable cleaners to work more efﬁciently by reducing surface tension at the metal surface. Also, prevent part from drying between stages or the spray washer • Defoamers—Control foam • Inhibitors—Minimize attack on metalThe alkaline cleaner is added to water (typically 2–10%) and applied hot. Solutions ofthis type have low surface tension, which means they can easily penetrate beneath andbetween dirt particles. In addition, the soap or detergent present can often combinewith dirt, oil, or grease and emulsify them in water to remove them from the sur-face of the part. When used with pressure spray or mechanical scrubbing, hot alkalinecleaning for 1–2 min is a very effective cleaning method.220.127.116.11 Neutral CleanersCleaners with a neutral pH are basically surfactant-based formulas without the addi-tion of alkaline materials. These can be used alone in cases where only light soils ornonsaponiﬁable soils are present. Often, they are used as cleaning boosters in com-bination with an alkaline or acid cleaner or a phosphatizer where additional cleaningis required.18.104.22.168 Acid CleanersAcid-based cleaners are typically used for special applications in metal cleaning,such as weld-smut or rust removal. In these applications, the base acidity, combined
Part Preparation Processes and Equipment 17with additives such as organic chelants, is doing most of the cleaning throughremoval of deposits from the metal. Surfactants can be built into acid cleaner formu-lations, but the choice of surfactants active at an acidic pH is somewhat more limitedthan alkaline cleaners. Acids include a number of chemicals that are acidic when dissolved in water(lower than 7.0 on the pH scale). Acids are typically especially good on removingmetal oxides and are also typically better cleaners where high levels of smut areencountered, such as on hot-rolled metal. Some common acids used in industrial cleaners are phosphoric, hydrochloric,sulfuric, hydroﬂuoric, and sulfamic. Phosphoric acid is a primary building block of many acid-based products. It doesa good job of contributing to smut removal with a relatively mild attack of the metal.It is also the primary source of phosphate in phosphating solutions. Hydrochloric acid, also commonly referred to as muriatic acid, is a very aggress-ive and corrosive mineral acid. It is used extensively in descaling and rust removaloperations where a very strong, aggressive acid is needed to remove heavy rust.Hydrochloric acid is also frequently used for pickling operations and mill scaleremoval. Sulfuric acid is another aggressive acid that is used primarily for pickling ferrousmetals and mill scale removal. It is often used to neutralize alkalinity prior to dis-charging alkaline solutions to sewer and is a very effective calcium carbonate scaleremover. Nitric acid is an extremely aggressive acid with limited use in industry. Its primaryuse is in the passivation of stainless steel, where it preferentially dissolves the ironaway from the chromium on the surface. The remaining top metal layer, being excep-tionally rich in chromium, is then polished to achieve a very dense, high chromiumstain resisting surface on the metal. Hydroﬂuoric is an extremely aggressive acid used primarily in industry for thebrightening of aluminum. Hydroﬂuoric acid has the ability to remove the very denseand tenacious oxide coating, which forms on aluminum surfaces. It is also used inthe etching of glass. Hydroﬂuoric acid is sometimes used as an additive to phos-phate solutions to activate them for prepaint preparation of aluminum surfaces.Hydroﬂuoric acid is extremely dangerous. It is extremely corrosive to skin and mucousmembranes. Sulfamic acid is primarily used in descaling. It is much safer to handle thana liquid hydrochloric acid. It is also particularly good at dissolving old corrosionproducts. It is highly soluble in water and its end-use temperature should be keptbelow 140◦ F.1.1.6 SURFACTANTSSurfactants (surface active agents) are short-chain organic polymers that are lipo-philic (fat/oil-loving) at one end of the molecule and hydrophilic (water-loving)at the other. This unique construction gives them the ability to penetrate and stabil-ize oils and greases in a water environment. The lipophilic end of the molecule isattracted to oils and greases and, in turn, allows the dispersion of these captured oils
18 Paint Technology Handbookdue to the attraction of water to the other end. Oil is broken into droplets, which canthen form an emulsion in the water solution or split out from the water, ﬂoating to thesurface, depending on the surfactant type chosen. Cleaning compounds often have 1–5% surfactant(s). Surfactants act as penetratingagents, wetting agents, emulsiﬁers, suspension agents, and coupling agents. Soaps, natural anionic surfactants, are made through a process called saponiﬁca-tion, reacting fatty acids with caustic soda. Soaps are typically high-foaming materialsand good oil emulsiﬁers, but are unstable in acidic conditions. Anionic synthetic detergents provide excellent penetrating and wetting properties,but they are high foamers and are relatively poor at suspending soils. Cationic synthetic detergents are low foamers, but are relatively poor cleaners,with little detergency. Cationic materials are sometimes used as emulsiﬁers. Amphoteric synthetic detergents are low foaming at most temperatures but arenot particularly good soil dispersants or stabilizers. The key feature of amphotericsis their ability to penetrate soils. Nonionic synthetic detergents do not have a plus or minus charge and are themost broadly used. They are not as good at penetrating and wetting as the anionicsare, but they are excellent soil stabilizers and emulsiﬁers. They can be low to highfoamers depending on their cloud point and pH. Cloud point is the temperature atwhich a nonionic surfactant loses solubility, partially comes out of solution, andfunctions at the water surface as an active defoamer. Cloud point is the temperatureabove which a nonionic-based detergent can be used in a recirculating spray washer.Nonionic surfactants are most active within a 10–20◦ F range on either side of thecloud point. For this reason, most nonionic-based detergents are formulated usingseveral carefully chosen nonionics to provide good detergency and low foam overa wide range of temperature. A typical spray cleaner stage in a washer is 60–90 s. A dip stage may be anywherefrom 3 to 5 min with temperatures ranging from 120 to 180◦ F. Times, temperatures,and cleaner concentration vary depending on the cleaner used and the condition ofthe substrate. The rinse stage following the cleaner is ambient tap water to remove any residualalkaline cleaner or loosened soil. Rinse stages are overﬂowed with fresh water asparts are processed to continuously reduce the soil buildup in the water. Cleaning and rinsing alone prior to coating is sufﬁcient as a stand-alone pretreat-ment in a limited number of situations. Like mechanical cleaning, initial adhesioncan be good, but without a conversion coating the product does not have any long-termcorrosion protection. When cleaning prior to conversion coating, it is important to consider how thecleaner and its effect on the substrate may interfere with the formation and depositionof the conversion coating. Chemical solutions must be isolated by proper drain timeand rinsing to prevent transfer of residual chemistry from one stage into another. If asigniﬁcant amount of chemical is carried from one solution to another, it may interferewith the performance of the washer and add cost to the operation. In a pretreatmentprocess, the cleaner should not be viewed as a separate process but as an integralpart of the total pretreatment process that can affect the quality of the conversioncoating.
Part Preparation Processes and Equipment 191.1.7 FACTORS THAT AFFECT THE PERFORMANCE OF THE CLEANERThe key factors that affect cleaner selection include soil, substrate, quality goals, andmethod of application. Three other important issues that must be addressed prior toselecting a cleaning product are the quality of the incoming water, the cost of thecleaning products, and compliance with local regulatory rules.22.214.171.124 Quality of Water SupplyWhether drawing from a well or tapping into a municipal water supply, the kind ofwater you use can impact chemical performance and ﬁnished goods quality. Some ofthe most common constituents of water you should manage are as follows. Water hardness and the inverse solubility of calcium and magnesium ions, particu-larly in the presence of carbonates, can lead to problems such as scale buildup. Layersof scale in the piping can restrict ﬂow and contribute to the plugging of nozzles. Scalebuildup also reduces the efﬁciency of heat exchange surfaces and increases energyconsumption dramatically. Hard water can also cause spotting on part surfaces and it can reduce the effect-iveness of some detergents, because they will react with the minerals in the waterinstead of the soils on the part. Water hardness can be controlled with mechanical methods such as water soften-ing (ion exchange) or deionizing (dissolved solids removal). The cost of the equipmentfor softening the water can be recovered by the savings in improved production quality,reduced energy use, and reduced chemical use. Chemically, water hardness can be “tied-up” by complexing these ions witha more soluble agent like certain phosphates. In addition, holding these metalsin a soluble state with chelating agents will eliminate most of the problems theycreate. Some water supplies will have a higher concentration of iron, especially if thewater is supplied from a well. Excess iron can cause streaking and staining on thesubstrate. In addition, deposits of iron can create corrosion cells on the part surface andpossibly lead to premature corrosion on ferrous metal surfaces. Iron can be removedwith ultra-ﬁltration, chelants, precipitation, or deionizing systems. Silica in the water can be a problem for pretreatment systems. High levels ofsilica, from incoming water or the manufacturing process, can create a glass-like ﬁlmthat is very hard to remove and substantially reduces heat transfer efﬁciency. Filmingon parts, especially glass and plastic, may interfere with subsequent processing ofparts or their ﬁnished quality. High levels of bacteria in the water supply can cause rapid slime growth in tanksand raise the level of dissolved solids in solution. This can result in contaminated partsthat can show up as corrosion under a coating and it can also cause increased levelsof foaming in a solution. Iron reducing bacteria can cause deterioration of processequipment. The incoming water should be monitored to develop a standard for supplywater. Variations from the standard may show that the local supply has not beenadequately treated. If a well is used and bacteria levels are beyond the acceptablerange, cleaning of incoming water is necessary. If a cleaning solution or rinse has
20 Paint Technology Handbookgone bad due to bacteria growth, the process should be thoroughly cleaned, sanitized,and rinsed. The selection of a cleaner is based on the soils to be removed, the substrate, andother variables. The performance of a cleaning solution depends on proper adjustmentand maintenance.126.96.36.199 Soils in SolutionSoils that are removed from the parts will build up in the cleaner solution over time.Solid particles will settle to the bottom of the tank as sludge and oils, grease, and someﬂoating debris will ﬂoat on the top of the solution. There is a limit to the amount ofcontamination that a cleaner bath can tolerate before it will cease to clean and needto be dumped and recharged. Overﬂowing the solution can help to reduce the accu-mulation of ﬂoating debris, but solids can still cause a problem and overﬂowing thesolution will create a need for more chemical. Oil skimming and sludge removal canextend the life of the cleaner and techniques for this are explained in the section ofthis book on washer design. Certain operating parameters need to be controlled for good performance. Thecontrol parameters that affect the performance of the cleaner include contact time,chemical concentration, temperature, spray pressure, drain time, and the volume ofcontaminants in the solution. These are the items that must be monitored, recor-ded, and maintained within proper ranges in order to achieve predictable cleaningperformance.188.8.131.52 TimeIt is important to have enough contact time to provide complete wetting breakdownof soils. The longer the contact time, the more the reaction will be. The control ofcontact time is usually equipment related. If the cleaning method is manually operated,the time can be adjusted for different soil loads. If the cleaning system is automatedthe time will depend on the conveyor line speed.184.108.40.206 TemperatureAs a rule of thumb, cleaning chemical processes can be accomplished more quicklywith higher temperatures. The chemical supplier will recommend a temperature rangeneeded to provide satisfactory performance with their product. With some clean-ers, elevated temperatures can adversely affect substrates and chemical compounds.Improper temperature may also cause excess foaming with some cleaner products.Managing the temperature requires a properly maintained thermostat and heatingsource (boiler, heating elements, burners, etc.).220.127.116.11 Spray PressureThe physical force of solution under pressure, agitation in a chemical solution,or scrubbing will enhance the performance of a cleaning solution. This factor is
Part Preparation Processes and Equipment 21extremely important in removing tough soils such as particulate matter and heavybuildup of grease and oil. Controlling the scrubbing force in a system depends on the method of applicationused. In the case of spray systems, it is important to keep the nozzle oriﬁces clear ofscale and shop debris to help maintain the proper pressure. Immersion systems or diptanks can use air agitation, solution circulation systems, or a mixer blade.18.104.22.168 ConcentrationChemical concentration is related to the particular product being used. Concentrationsshould be consistent with the suppliers’ recommendations. Too much cleaner maycause poor rinsing or excess carryover. If the concentration is too low, the parts maynot get adequately cleaned. The substrate, types of soils, and the equipment used all inﬂuence chemical selec-tion and solution strengths. Certain blends of chemicals work well for immersionsystems but not in other applications. Problems may occur in the degree of reaction,ﬂash rusting, or foaming. Concentration control is very important. Cleaning solutionsshould be monitored regularly and controlled. Simple titration is typical, using eitherdropper or burette techniques. The effectiveness of a cleaner solution gradually decreases as the soil loadbuilds up. The effective life varies depending on hours of operation, the volumeof metal processed per hour, the type of metals processed, the amount of carry out,the use of ﬁltration, and the types of soils removed.1.1.8 METHODS USED TO MEASURE CLEANING RESULTSThe cleanliness of the substrate will have a big impact on subsequent treatmentsand the ultimate performance of the coating. It is very important to keep track ofcleaner performance. Visual inspection is useful as a routine part of supervising theoperation, but it is subjective and does not provide any data to conﬁrm the results.Still, if a product does not look clean, it probably is not. Wiping the surface with a clean white cloth is good for determining the presenceof inorganic and particulate matter, such as carbon smut, that oftentimes does not showup until substrates are cleaned. It is not a perfect test as some phosphate coatings mayleave some minor smut without interfering with performance, but it does help tomonitor daily operation. Parts should be routinely observed as they exit the washer to see if the waterbeads up or sheets off in a “water-break-free” condition. A water-break-free condi-tion indicates an absence of organic materials that could interfere with adhesion andultimate performance. Another qualitative test aimed at determining if soils remain on a part after cleaningis the scotch tape test. Clear adhesive tape is laid on a part and rubbed ﬁrmly over thesurface; when pulled back, the “sticky” side will have particulate matter attached to itthat can be viewed and referenced. Besides providing a relative degree of cleanliness,
22 Paint Technology Handbookthis test will measure the degree of adherence of soil such as carbon smut and weldsmoke. Residue testing is a quantitative method of testing the cleanliness of a surface.Soils are removed by solvent extraction with an organic solvent followed by evapor-ation of the solvent. Once the solvent has been ﬂashed, the remaining residue fromthe part is carefully and accurately weighed and expressed in terms of milligrams persquare meter of surface area. Another helpful test of cleanliness is the use of a black light. An oil solubleﬂuorescent dye can be mixed with an oily soiling material and applied to the testpanels. After the panels are cleaned, the remaining soil is visible under ultraviolet orblack light. Many common metal working ﬂuids ﬂuoresce under a black light. Blacklights are relatively inexpensive. In order for this test to work, it is important to knowthat the soils being tested will ﬂuoresce under a black light. Yet another method to test cleanliness is a contact angle water drop test. A dropof water is placed on the test surface; the contact angle is then measured photo-graphically or by a contact angle goniometer. The contact angle varies with the levelof cleanliness of the substrate. Although this is an accurate method of determiningsurface cleanliness, it can only be used under laboratory conditions. Infra red (IR) spectroscopy can also be used to test cleanliness. A cleaned surfacecan be stripped with a solvent cleaner. The solvent used for cleaning is then analyzedfor any soils remaining that would indicate the part is not clean. Another way ofusing spectroscopy is to rub a salt onto the surface to pick up any impurities. The saltis then pressed into a pellet. The pellet is analyzed with the spectrophotometer forimpurities.1.1.9 SUMMARYCleaning is a very critical step in the coating process. Adhesion, appearance, andcorrosion resistance are directly related to good cleaning. Proper cleaning requirescareful and accurate management of the washer and the cleaning chemical solutions. Planning and managing a cleaning process begins by recognizing the relationshipbetween the substrate, soil, method of application, and the appropriate chemicalsolutions and how each impacts the cleaning process. The four factors of time, temperature, mechanical force, and chemical concen-tration combine to provide the necessary quality level. These four factors must bemeasured and maintained routinely for consistent results. Good system manage-ment and regular testing of the cleaning results is the ﬁrst building block of coatingsuccess.1.2 CONVERSION COATINGSA conversion coating is a chemically applied treatment that is used over a clean metalsurface to enhance adhesion and corrosion resistance. Iron and zinc phosphate coat-ings are the most commonly applied conversion coatings. Other conversion coatingsinclude manganese, chromate, zirconium-based products, and vanadium/zirconium-based products. A conversion coating converts the surface of a metal substrate to
Part Preparation Processes and Equipment 23a uniform, inert surface, which increases paint bonding, minimizes the spread ofcorrosion under the ﬁlm if the coating is cut, and improves the overall corrosionresistance of the ﬁnal product. Conversion coatings are developed on both ferrous (iron based) and nonferroussurfaces (zinc, aluminum, terne, and manganese). Parts are subjected to an acidic bathin which a chemical conversion forms a complete ﬁlm on the part surface, changingthe chemical and physical nature of the metal surface.1.2.1 IRON PHOSPHATEIron phosphate is the most commonly used conversion coating in the generalindustrial market. An iron phosphate solution produces a thin, bumpy, or amorphousmetal phosphate top coating over an iron oxide base. The surface of the material willtypically have a gray to blue iridescent or blue-gold iridescent color after applicationdepending on the coating weight and the base metal. A typical iron phosphate consistsof phosphate salts, accelerators/oxidizers, and an optional surfactant package. The acid salt content, type and amount of accelerator, and the type and amountof acid etchants are adjusted to produce different formulas. Iron phosphate coatingformulations commonly contain oxidizers and/or accelerators to generate reactivityon the metal surface. Oxidizers, such as nitrite or chlorate, act to initiate attackon ferrous parts, providing the iron for the iron phosphate coating. Accelerators,such as molybdate or vanadate, provide active sites for iron phosphate deposition.The particular oxidizer or accelerator used in a particular product may affect theperformance or appearance of the ﬁnal coating. In a three-stage iron phosphate washer, the cleaning and coating are combinedby incorporation of a surfactant package in the iron phosphate solution. A source ofﬂuoride ions may be added if aluminum is also being processed to increase the etchingeffect on the oxide surface of the aluminum. Iron phosphate coatings can be applied by hand wipe, handheld wand, immersion,or spray washer. The most effective and commonly used method is a multistage spraywasher. The number and type of process stages is directly dependent on ﬁnished partrequirements. Spray washers for iron phosphating are built with as few as two stagesand as many as eight. The following list shows the typical sequence of stages fromtwo to eight. • Stage two—clean/coat, rinse • Stage three—clean/coat, rinse, rinse/seal • Stage four—clean/coat, rinse, rinse/seal, deionized (DI) water rinse • Stage ﬁve—clean, rinse, phosphate, rinse, rinse/seal • Stage six—clean, rinse, phosphate, rinse, rinse/seal, DI rinse • Stage seven—clean, clean, rinse, phosphate, rinse, rinse/seal, DI rinse • Stage eight—clean, rinse, clean, rinse, phosphate, rinse, rinse/seal, DI rinseThe iron phosphate coating weight, measured in milligrams per square foot(mg/ft2 ) or grams per square meter (g/m2 ), varies with phosphate formulas and
24 Paint Technology HandbookTABLE 1.3Performance Results with Different Spray SystemsNumber of Metals Degree of Coating Coating CorrosionStages Treated Cleaning Weights (mg/ft2 ) Adhesion ResistanceTwo Steel Light 25 Fair PoorThree Steel, zinc, aluminum Moderate 25 Good FairFour Steel, zinc, aluminum Moderate 25–45 Good FairFive Steel, zinc, aluminum Moderate 25–70 Good GoodSix Steel, zinc, aluminum, Good 25–90 Very good Good stainless steel, copper, bronze, magnesiumwasher arrangements. The quality of paint adhesion and corrosion resistance isaffected by the coating weight. Table 1.3 shows typical results of additional stepsin the iron phosphate spray washer.1.2.2 COATING WEIGHTPhosphate coating weight is measured with test panels that have been run through thewasher with all of the process variables under control. After a clean, fresh panel is runthrough the washer, it is removed, dried, and tested by weighing the panel, removingthe coating, and weighing the panel a second time as described next. Clean cotton orsurgical gloves are worn to avoid contamination of the sample with skin oils. • Determine the area of the panel in square feet (width × length) • Weigh the panel, correct to three decimal places (0.000) and record the ﬁrst weight • Immerse the panel in 10% CrO3 in water by weight at 160◦ F for 10 min • Rinse with tap water or DI water, if it is available and dry • Weigh the part again, correct to three decimal places, and record the second weightThen, complete the formula: 1st wt. in grams − 2nd wt. in grams × 1000 = mg/ft 2 Area in square foot1.2.3 IRON PHOSPHATE CONTROLSIn addition to the number of process stages, the factors that will affect the weight ofan iron phosphate coating are time, temperature, concentration, acid consumed (pH),the condition of the substrate, and the spray pressure.
Part Preparation Processes and Equipment 25 The contact time must be long enough to allow the chemistry to form a uniformcoating on the surface. Longer times will generally allow the solution to build adenser and heavier coating. Too much time can cause a more powdery and lessdurable coating.22.214.171.124 TemperatureManufacturers recommend a proper operating temperature for a given phosphatesolution. Solution temperature affects coating weight and density. Soils become morereactive in a heated solution and the chemicals become more aggressive. The temper-ature should be within the manufacturers recommended range (typically 120–140◦ F).Tests should be run to determine the optimum temperature for good coating weightwith a given system.126.96.36.199 Chemical ConcentrationThe chemical concentration can be adjusted to achieve the correct coating weight ata particular time and temperature. A higher concentration of chemical will providemore total acid, more accelerators, and typically more coating weight.188.8.131.52 Acid ConsumedThe last factor that affects iron phosphate performance is acid consumed (pH).A higher pH will provide less acid and less coating, while a lower pH will providebetter cleaning and more acid. More acid will provide more pickling and heaviercoatings. Excessive acid can cause too much pickling and the dissolve the phosphatecoating. The following graphs show the relationship of each of these control factors to thephosphate coating weight.1.2.4 ZINC PHOSPHATEZinc phosphate is a nonmetallic crystalline coating that chemically adheres to thesteel. A zinc phosphate coating will provide improved paint adhesion properties,better coating in recessed areas, and better corrosion resistance than can typically beobtained with iron phosphate. A typical zinc phosphate consists of • Phosphoric salts • Accelerators • Zinc salts • No surfactant packageUnlike the iron phosphate, a zinc phosphate solution cannot clean and coat simultan-eously in a three-stage process. A separate cleaning stage is required and a prezincconditioning stage is usually required.
26 Paint Technology Handbook1.2.5 ACTIVATING (PRIOR TO ZINC PHOSPHATE)An activator is used prior to the application of a zinc phosphate. Activators/conditioners are mild alkaline suspensions of specialized active titanium salts thatadhere to steel, zinc, and aluminum surfaces. The conditioner will set up a networkof uniform acceptor sites for zinc crystals to deposit to increase the number of zincphosphate crystals and decrease the size of the crystals. The small densely formedcoating provides the best possible adhesion and corrosion resistance. A large crystalstructure is more porous, has poorer corrosion resistance, and requires more paint toachieve a complete ﬁlm. The control measures for zinc phosphate coatings are the same as iron phosphate(concentration, contact time, temperature, and pH). The bath life is also a factor insolution performance. Accelerators such as nitrate, chlorate, or nitrite are added to control the rate ofcoating formation. The proportion of these various ingredients affects the coatingweight and phosphate crystal size. Fluorides are added if aluminum must beprocessed. The reactions at the surface of the part during zinc phosphating are 1. Pickling attack on the metal and oxidation of hydrogen to water 2. Increase of the pH at the interface of the metal and the phosphate solution 3. Oversaturation of the ﬁlm with coat forming substances 4. Nucleation on the metal 5. Growth of phosphate coating 6. Oxidation and precipitation of iron as sludgeThe composition of the bath, the temperature, exposure time, and the pre-vious cleaning process will affect the phosphate composition and crystallinephase. Zinc and polycrystalline phosphate solutions do require more careful attentionthan iron phosphate processes to produce consistent high-quality results. Automaticfeed pumps can be used for additions of zinc phosphate and nitrite accelerator tothe bath to maintain the proper concentration and ensure consistent good qualityand minimum chemical consumption. An improper concentration of these materialsmay result from bulk additions and produce coatings that are soft or too heavy,and it may also create excessive sludge. If the materials are allowed to run toolow, the coating will be coarse and spotty, resulting in poor adhesion and corrosionresistance. Zinc phosphate is the preferred conversion coating used by the automobileindustry because of the need for superior corrosion resistance. The coating is ﬁrmlyattached to the metal by ionic bonding, the porous crystalline structure provides anextended surface for paint bonding, and if the paint surface is scratched, the inorganiccoating helps stop the spread of corrosion. A zinc phosphate solution will continually produce sludge through oxidation ofsoluble iron to an insoluble state that precipitates. A sludge removal system must be
Part Preparation Processes and Equipment 27 Zinc settling tank Zinc solution tankFIGURE 1.3 Zinc phosphate tank.used to provide constant removal of this sludge. A simple sludge removal system isshown in Figure 1.3. The rinse stage following the phosphate should be ambient tap water. Phosphatesalts are more soluble in cold water. The overﬂow volume should be sufﬁcient to keepthe rinse clean and reasonably cool.1.2.6 COMPARISON OF IRON PHOSPHATE TO ZINC PHOSPHATEFrom an environmental standpoint, iron phosphate is the clear winner. In some muni-cipalities, an iron phosphate solution can be neutralized and released to drain. Somecoaters have waste treatment for iron phosphate or they have it hauled away fortreatment by a licensed waste hauler. Zinc is listed by the Environmental ProtectionAgency (EPA) in the Resource Recovery and Reclamation Act (RCRA) as a hazard-ous substance that is subject to waste regulations. It must be treated prior to dischargeand the sludge must be waste hauled. In terms of performance, zinc phosphate with a chrome sealer will typicallyprovide far superior corrosion resistance. Table 1.4 compares the two phosphate processes in more detail. When deciding between zinc and iron phosphate, the end use of the product is themost important factor. For indoor use in noncorrosive environments, iron will workwell, and it has several economic and environmental advantages. Zinc will providethe undercoat protection needed for the more demanding product used outdoors or inhighly corrosive environments. The quality of the cleaner and the ﬁnish coat is also an important part of corrosionresistance. The ultimate life of a coating is related to the conversion coating combinedwith the paint applied over the surface. A very good job of cleaning and high-qualitytopcoat may allow the use of a less resistant conversion coating.
28 Paint Technology HandbookTABLE 1.4Comparison of Zinc and Iron Phosphate Iron Phosphate Zinc PhosphateAverage coating weights 15–90 (mg/ft2 ) 50–100 (mg/ft2 )Surface structure Amorphous (less paint needed Crystalline (more paint needed to cover) to cover)Paint adhesion Very good ExcellentSalt spray resistance 200–500 h 600–100 hCost One product typically 3–4 components Average $4.00–8.00 per gallon 1. Zinc phosphate—$8.00/gal 2. Accelerator—$8.00/gal 3. Activator—$7.00/lb 4. pH adjust—$3–5.00/galSludge formation Moderate HeavyBath life Very good Very goodControl of bath Very easy Difﬁcult 1–2 tests 3–4 test, control of zinc bath and conditionerEquipment Mild steel or stainless steel Stainless steel or similar noncorrosive construction; sludge removal equipment needed; more washer stagesMaintenance Minimal Higher (sludge removal)1.3 RINSINGRinsing is a critical part of successful pretreatment. Proper rinsing between processstages is essential to successful pretreatment. Poor rinsing will leave residues on thepart surface that will interfere with subsequent steps in the process. Final rinsing isalso critical. Soils or unreacted salts left on the surface can cause adhesion failure orpremature corrosion. If the alkaline cleaner is not thoroughly rinsed off, it will carry over into the acidicphosphate solution, where it will increase chemical usage and decrease performance.If the ﬁnal rinse overﬂow or dump cycle are inadequately maintained, then, saltswill accumulate in the rinse. These salts will dry on the substrate and interfere withcoating adhesion and corrosion resistance. Water impurities or salts can ruin all ofthe hard work of the coating process and shorten the useful life of the product. Watersalts can consume pretreatment chemicals such as ﬂuoride, phosphate, and silicateto produce scale. Organic materials such as rust preventatives, metal working ﬂuids,and surfactants can produce scale, sludge, and create foam. The insoluble inorganicand organic matter can produce surface defects and plug risers and nozzles in thechemical as well as the rinse stage. Maintaining clean rinse water will help avoidthese problems and will reduce maintenance requirements to the washer nozzles andplumbing. The rinse following the cleaner should have an aggressive spray pressure to assureremoval of all residual alkaline cleaner and soils. The overﬂow rate is adjusted to keepa slight amount of alkalinity in the water, reducing precipitation, helping to avoid ﬂash
Part Preparation Processes and Equipment 29rust, and ensuring more complete rinsing of soaps, fats, oils, grease, and surfactants.Some carry-over heat will warm the rinse water and improve solubility. The rinse following the phosphate stage is operated at a lower spray pressure toavoid disturbance of the freshly deposited conversion coating. A degree of acidityaids in the removal of nonreacted metal phosphate salts. The postphosphate rinse isoperated cooler than the cleaner rinse to stop the reaction between the solution andthe metal. Lower temperature and spray pressure rinsing will reduce streaking orstriping. If the postphosphate rinse is operated too hot and is too contaminated, then,the pretreatment quality will be compromised. Phosphate removal and ﬂash rustingcan occur under these conditions. Both rinses should be overﬂowed at a rate that will keep them clean enough toensure the integrity of the steps in the pretreatment process. Overﬂow rates are typic-ally maintained between 3 and 10 gal/min. Rinse tanks should be dumped frequentlyto reduce the accumulation of contaminants and to avoid bioactivity. Overﬂow ratesvary due to the amount of drag out or carry over from the previous stage. Dragout varies based on part conﬁguration, rack design, and drainage time. Excessivechemical carry over can be minimized by proper rack design, part orientation, anddrainage time. Rinse water hardness in the ﬁnal rinse should be maintained below 300 parts permillion (ppm). Hardness or water solids can be measured with a total dissolved solids(TDS) meter. A conductivity meter can also be used to indicate the amount of solidsin a rinse solution. Conductivity and TDS values are used as a reference point forsolution control purposes. Fresh water can be added directly into the rinse tank orthrough a riser located after the recirculating rinse stage. The added dilution ratio ofthe residual recirculating rinse water combined with the ﬂushing action of the sprayreduces the chemical residues to a point near zero. The fresh water riser increases theefﬁciency of the rinse by a factor of 400+, using the same quantity of fresh water.1.3.1 RINSE AND RINSE SEALWater rinsing only removes the active chemicals (acid) left on the metal surface.Nonreacted chemicals left on the surface can cause corrosive conditions under theapplied coating. The rinse seal neutralizes any residual water-soluble salts to preventhumidity blistering and further removes phosphate solution residue. The ﬁnal sealrinse stabilizes the surface pH to prevent alkaline undercutting, typically leaves thesurface slightly acidic, and sometimes can seal voids in the phosphate coating. A ﬁnalrinse pH of 4.0–5.5 eliminates carbonates in the water and prevents the precipitationof metal hydroxides. Historically, ﬁnal rinses were dilute chromic acid solutions in water. Environ-mental legislation has driven a demand for nonchrome rinses that can provide thesame corrosion protection provided by rinses that contain chromic acid. Some nonchrome rinses perform quite well. For example, some dry-in-placenonchrome rinses can dramatically improve corrosion resistance on aluminum.Chromium containing rinses still provide the best results over a broad variety ofparts and operating conditions. In some cases, a nonchrome rinse is not needed and provides marginal beneﬁt.DI or reverse osmosis (RO) water may provide a great ﬁnal rinse treatment.
30 Paint Technology Handbook1.3.2 REVERSE OSMOSIS (RO) OR DEIONIZED (DI) WATER RINSEFinal rinsing may or may not include a proprietary chrome or nonchrome product.Some ﬁnal rinse compounds require a DI rinse to remove any accumulation of theseal rinse or phosphate that might impair the quality of the applied coating. Somenonchrome seal rinses should not be followed by a pure water rinse. Phosphate residue left on the metal surface can cause nonuniform paint depositionand adhesion problems. DI rinsing will eliminate mineral spotting and corrosive saltsthat can cause humidity blisters and organic particulate that can cause surface defects. A DI rinse often includes a recirculated spray zone followed by a fresh DI halo inthe exit vestibule of a spray application. The DI water in the recirculation tank shouldnot exceed 50 µmho conductivity. The fresh DI make-up water supplied by the ﬁnalhalo should not exceed 10 µmho. RO puriﬁes water by using pressure to force it through a membrane that will notpass dissolved salts. Because an RO system is a pressure-driven ﬁltration method, itmay not take out certain ions and it may be slightly less effective than deionization.However, RO water can be used for ﬁnal rinsing in the same manner as DI water. DI water systems may cost less than RO systems in some cases for a particular ﬂowrate. Some of the cost consideration is related to the features of the particular system,like holding tanks, types of regeneration (manual, semiautomatic, or automatic), mon-itoring equipment, and gauges. It is difﬁcult to compare the equipment cost withoutan expert to relate the features and beneﬁts. In general, the DI system will not be muchless expensive than the RO system unless it is lacking certain important features. One thing that is consistent is the cost per gallon. RO water is less expensiveby the gallon. The list of features in Table 1.5 gives some idea of how the two sys-tems compare. A comprehensive comparison of the features is recommended beforeTABLE 1.5Features of Reverse Osmosis Versus Deionized WaterDeionized water system—ion-exchange Reverse osmosis system—membranetechnology for the removal of dissolved separation technology for the removal ofminerals, salts, and gases all categories of impurities except gasesCan be fouled by precipitated material or Membranes may be fouled by excesses of organics submicron particulate or some organicsMay have trouble with excessive bacteria May be scaled by mineral depositsEfﬂuent must be neutralized Hardness needs to be inhibited by softening or chemical additionCO2 gas increases cost of operation Feed water temperature will affect ﬂow rateRequires storage and handling of strong acids May need to add ﬂocculent periodically and bases for regeneration chemicalsTime required for regeneration Sometimes higher equipment costHigher operating costSystem may cost less than RO Do not require acids or caustics No regeneration required Lower cost of operation
Part Preparation Processes and Equipment 31making a decision to buy a DI system. They are harder to own and operate and thewater is more expensive per gallon. Cost Assumptions TDS 340 ppm Hardness 18 grains /gal Hours of operation 20/d Flow rate 30 GPM Electricity $0.05/kWh Water $1.60/1000 gal Municipal sewer $1.43/1000 gal Labor 50.00/h Operating days per year 365 d 30% HCl (55-gal drum cost) $1.00/gal 50% NaCH (55-gal drum cost) $1.31/gal Commercial antiscalant $13.27/gal Commercial ﬂocculent $26.00/gal NaCl (softener salt) $0.07/lb Activated carbon media $69.00/ft3 Cation resin $95.00/ft3 Anion resin $232.00/ft3 8′′ Spiral TFC RO membranes $1000.00 each 10′′ poly wound RO cartridges $7.00 eachTABLE 1.6Cost Comparison of DI and RO Water Auto DI System Reverse Osmosis System Cost/1000 gal Cost/year Cost/1000 gal Cost/yearAcid (HCl) 2.93 30,761.43 Heat 1.43 15, 065.40Caustic (NaOH) 1.73 18,119.37 Electric booster 0.10 10, 052.92 pumpActivated 0.02 200.00 Activated 0.02 200.00 carbon carbonCation resin 0.05 500.00 Preﬁlter 0.06 672.00 replacement replacementAnion resin 0.22 2,350.00 Softener salt 1.19 12, 584.37 replacementElectric 0.10 1,074.56 Membrane 0.12 1, 200.00 recirculation replacement pumpRegen. water 0.55 5,811.48 Electric RO 0.28 2, 909.37 and sewer pumpLabor 3.62 38,084.21 Electric dist. 0.10 10, 052.92 pump Water and sewer 1.30 13, 688.50 Labor 0.40 4, 2451.67Total operating $9.21 96,846.05 Total operating $5.00 52, 667.14 cost cost
32 Paint Technology Handbook1.4 TYPICAL SPRAY WASHER SYSTEMSThe three-stage iron phosphate washer is commonly used for applications that do notprocess heavily soiled parts or parts with lower quality speciﬁcations. The three-stageiron phosphate process combines the cleaning and phosphating steps in a single stage,reducing pretreatment costs and space requirements. Cleaner solutions in more complex washer arrangements are usually alkalinewhile the phosphate solutions are acidic. The three-stage washer uses an acidicsolution with a detergent package. In a three-stage system, the cleaning and phosphating processes are comprom-ised and the result is adequate but not good enough for higher quality standards.Much better cleaning and phosphating is accomplished when these processes areseparate with rinses in between. Separating the cleaning and phosphating allows theprocesses to be adjusted for maximum beneﬁt of each process function. The res-ult is much more complete cleaning and a more uniform and complete phosphatecoating. Rinsing between chemical stages prevents excess contamination and the result-ant higher cost of added chemical is an addition to maintain high quality. Someprocesses incorporate two rinses between chemical stages to reduce cross contam-ination. Adding the extra rinse tank will turn a three-stage washer into a four-stagewasher and a ﬁve-stage into a six-stage washer, and so forth. Some typical processsequences for spray washers are shown below.1.4.1 STAGES OF PRETREATMENTThree-Stage Iron Phosphate Stage 1—Clean/phosphate: 90 s at 160◦ F (71◦ C) Stage 2—Rinse: 30 s at ambient Stage 3—Rinse/seal: 30 s at 120◦ F (49◦ C)Five-Stage Iron Phosphate Stage 1—Alkaline cleaner: 90 s at 160◦ F (71◦ C) Stage 2—Rinse: 60 s at ambient Stage 3—Iron phosphate: 60 s at 140◦ F (60◦ C) Stage 4—Rinse: 30 s at ambient Stage 5—Rinse/seal: 30 s at 120◦ F (49◦ C)Seven-Stage Zinc Phosphate Stage 1—Alkaline cleaner: 90 s at 160◦ F (71◦ C) Stage 2—Rinse: 30 s at 110–120◦ F (43–49◦ C) Stage 3—Activating rinse: 30 s at ambient Stage 4—Zinc phosphate: 60 s at 140◦ F (60◦ C) Stage 5—Rinse: 30 s at ambient
Part Preparation Processes and Equipment 33 Stage 6—Chromic seal: 30 s at 120◦ F (49◦ C) Stage 7—DI rinse: 30 s at ambient (Recirculated) Fresh DI halo in the exit vestibule.Eight Stage Iron Phosphating—Dip Spray Stage 1—Immersion clean: 2 min at 150◦ F (66◦ C) Stage 2—Spray clean: 1 min at 100–150◦ F (38–66◦ C) Stage 3—Spray rinse: 1.5 min at 100–150◦ F (38–66◦ C) Stage 4—Immersion rinse: 0.5 min at 140◦ F (60◦ C) Stage 5—Immersion phosphate: 2 min at 140◦ F (60◦ C) Stage 6—Immersion rinse: 0.5 min at 140◦ F (60◦ C) Stage 7—Spray chromic rinse: 1.5 min at 100–150◦ F (38–66◦ C) Stage 8—DI-water rinse: 0.5 min at ambientFive Stage for Plastics Stage 1—Preclean: 20 s at ambient Stage 2—Cleaner: 60 s at 130–140◦ F (54–60◦ C) Stage 3—Cold water rinse: 30 s at 70–110◦ F (21–43◦ C) Stage 4—Rinse with rinse aids: 30 s at ambient Stage 5—DI water rinse: 20 s at ambientMany variations may be used depending on the mixture of substrates, types of soils,and quality goals of a particular coater. Cleaning and surface conversion applications utilize immersion or spray tech-niques. Each method has advantages and limitations and some pretreatment systemsuse a combination of immersion and spray stages to provide complete cleaning ofthe part. Car bodies usually require immersion stages for complete wetting and spraystages for good rinsing and effective scrubbing action on the exterior. Immersion systems have the advantage of reaching recesses and other areas ofthe parts that might not be accessible by spray. Pockets of trapped air, however,can cause problems for immersion systems. Entrapped air can prevent the entry ofcleaning solution into recesses and in extreme cases, make it impossible to submergea part. Consistent temperature control and heat transfer is generally better and faster inimmersion applications. Heat is lost more quickly when a solution is sprayed throughcooler air. Heat transfer is better due to consistent solution contact temperature. The disadvantages of an immersion system include soil redeposition and solutionimpact. If contaminants are allowed to ﬂoat on the top of the immersion tank, thensoil redeposition may occur. Agitation of immersion solution will help prevent soilredeposition. Spray halos have also been employed to ﬂush away any redepositedsoil. If the solution is not agitated, it will not be as effective at removal of softenedsoils. Eductor systems can help keep the solution in motion and improve cleaning,as well as reduce soil redeposition.
34 Paint Technology Handbook Spray systems use pressure to provide impingement energy to dislodge dirt andremove loosened soils. Sprays can often be directed into recesses. Spray systems mayhold less water in cupped areas of the part. Spray nozzles must be properly maintained to perform correctly. A routine main-tenance procedure should be put in place to examine the nozzle oriﬁces for obstructingdebris, nozzle alignment for spray angle, and the nozzle body for proper seating.Routine nozzle maintenance will avoid clogging or other problems that lead to a poorspray pattern and reduced process effectiveness.1.5 SUBSTRATESSubstrate is a reference to the material that the product is made of. The type ofsubstrate, along with the desired performance characteristics of the ﬁnished part tobe coated, will inﬂuence the selection of pretreatment chemicals and the systemused to clean and treat the product. Different materials will have different soilsand surface conditions that require different chemistry and process sequences toproperly prepare them for paint application. It is very important to understand dif-ferent substrate surfaces and the types of treatment that work best with differentmaterials.1.5.1 METAL SUBSTRATESMetal surfaces are highly reactive and the oxide layer that forms on the surface caninterfere with adhesion, appearance, and performance. Rust inhibitors, such as milloil and metal working products containing rust inhibitors, are used to temporarilyprevent rust, but the metal will eventually begin to oxidize. The rust inhibitors andmetal working ﬂuids age and they may react with the substrate to form compoundsthat interfere with the appearance and quality of the ﬁnished substrate. Therefore, therust inhibitors must be removed and the surface must be free of oxides before thepaint can be applied. The base metal itself is also a factor that must be considered in selection andapplication of a particular treatment method. The components that make up the metalcan cause contamination on the surface that will interfere with good coating adhesionand corrosion resistance. For example, higher carbon steel alloys will create moresmut than lower carbon alloys. Mill scale and other substances that are difﬁcult toremove chemically may interfere with paint adhesion. Other examples of surface con-ditions that create metal treatment issues are silicon in aluminum alloys and chromatepassivation on aluminum or galvanized steel. The substrate and the surface of the partmust be thoroughly understood to make a reliable system for pretreatment. The most common metal substrate materials that gets painted are cold-rolledsteel (CRS), HRS, aluminum (cast and extruded), galvanized steel, galvaneal, andcast zinc. Copper, brass, bronze, and stainless steel are sometimes painted but notas often as other metals. Metals have certain natural properties as well as modiﬁed physical properties thatoccur through alloying and heat-treating. Alloying occurs by mixing two or moremetals or nonmetals to achieve a certain desired property in the ﬁnished product.
Part Preparation Processes and Equipment 35Different alloys are available in various forms such as castings, wire, or sheet products.Aluminum is alloyed with silicon, copper, magnesium, and other materials to provideproducts with slightly different properties such as hardness.184.108.40.206 SteelSteel is the most common substrate material used in manufacturing. Steel, availablein a variety of alloys and forms, is made from iron and a small controlling amountof carbon (∼2%) with small amounts of various alloying additives. Initial reﬁning ofsteel produces thicker and rougher grades of structural steel and plate. Further reﬁningof iron reduces the carbon and other impurity levels. Steel is sometimes classiﬁed bycarbon content.Low Carbon, 0.25% • Machining steel, mild steel (MS) • Easy to cut and form: typical uses—nails, bolts, automobile bodies, and metal furnitureMedium Carbon, 0.25–0.55% • Greater hardness and strength • More difﬁcult to form: typical uses—axles and drive shaftsHigh Carbon, 0.55–2.00% • Greatest hardness and strength • Most difﬁcult to form: typical uses—cutting tools, ﬁles, and hammers A four-digit system is used to classify different types of steel. Primary four-digit numbers • First digit, basic kind of steel • Second digit, general class of steel • Third and fourth digits, allowable range of carbon (in hundredths of %) Example: 1010 carbon steel has 0.10% carbon content • Fifth digit used where carbon is greater than 1% Steel stock is available in plate (0.23′′ minimum thickness), sheet, or coil(0.23′′ maximum thickness), bar stock, rod stock, tubing, and structural forms. Steel is available in different forms that can affect the pretreatment selection. • HRS—rolled (ﬂattened) while red hot. A blue/black coating consisting of iron oxide forms on the surface as the steel cools. Used in applications requiring substantial structural strength.
36 Paint Technology Handbook • CRS—rolled to ﬁnished size while at ambient temperature. No oxides form during processing. Much better aesthetics, superior surface, and mechanical properties. Many common products are produced from CRS. • Hot rolled, pickled, and oiled (HRPO)—HRS that has had the oxides removed through acid pickling. The steel is rinsed and then oiled to inhibit corrosion. Used in applications that require heavier gauges of steel and a better surface condition than HRS. • Cast iron—usually refers to gray cast iron, but can mean any of a group of iron-based alloys containing more than 2% carbon (alloys with less carbon are carbon steel by deﬁnition). Used to cast heavy parts in machinery and other applications. • Stainless steel—contains at least 11% chromium by weight—some alloys also contain nickel. Used for appearance and corrosion resistance. • Hot-dipped galvanized steel—steel that is coated with a thin layer of zinc by passing the steel through a molten bath of zinc at a temperature of around 460◦ C to form zinc oxide to protect the steel below from the corrosion. Galvanized steel is widely used in applications where rust resistance is needed. • Electro-galvanized steel—zinc coatings applied to steel electrolytically in zinc ion solutions can provide the same corrosion protection as hot-dipped zinc coatings, but they are smoother and lack some of the impurities that occur in the hot-dip process. Differences in steel composition can affect the quality of the ﬁnished product byaffecting the performance of the organic coating. Iron phosphate provides modestperformance characteristics and corrosion resistance over steel. Zinc phosphate isused for applications that require more severe performance properties.220.127.116.11.1 Hot-Rolled SteelHRS represents the ﬁrst reduction in the processing of the steel slab in heavier gauges,0.1–0.2 in. in thickness or higher. The surface proﬁle is generally rough and porouswith a blue/black oxide mill scale covering. Most HRS is used for structural steelcomponents, building trusses, heavy bar stock, and other interior applications. HRS will have mill scale, carbon smut, and possibly rust, in addition to the soilsthat have collected during manufacturing. To ensure good quality of the coating,the mill scale and rust must be removed by abrasion, such as a blasting opera-tion. A chemical process may be used after blasting to provide better corrosionresistance. The inorganic contaminants can also be removed by acid pickling solutions, butthere is some risk of ﬂash rusting. Strong acid solutions may also be a health andsafety issue and they are sometimes hard to maintain. Pickling solutions will alsoaccumulate iron sludge that must be ﬁltered or removed.18.104.22.168.2 Cold-Rolled SteelCRS is characteristically thinner and has a more uniform surface proﬁle than HRS.This is achieved by further processing of the HRS through a cold roll mill and
Part Preparation Processes and Equipment 37a tempering process. The difference in surface proﬁle and reduction in porosity isone of the reasons why CRS is used for exterior products. Typically, a series ofchemical processing tanks will be sufﬁcient pretreatment for CRS. Oils and otherorganic soils can be removed with a cleaner, and conversion coatings can be addedfor enhanced performance. Surface rust or weld burn may need mechanical cleaningto ensure good coating adhesion and corrosion resistance.22.214.171.124.3 Hot-Rolled Pickled and Oiled (HRPO)HRPO steel is hot-rolled coil or sheet steel that has been descaled of oxide ﬁlmby either a chemical method, mechanical method, or a combination of both andoiled to help retard corrosion during storage. HRPO is available in various gauges,widths, and cut lengths or coil. HRPO is often used for products that need a bettersurface for appearance. Most chemical cleaning processes are effective for preparationprior to painting. HRPO will develop less scale on the edges during laser cuttingthan HRS.126.96.36.199.4 Cast IronThere are many variations in the composition of cast iron products to impart differentproperties for strength, hardness, softness, and abrasion resistance. The high carboncontent of cast iron should be considered when cleaning prior to phosphating andpainting. Cast iron can be cleaned with an alkaline cleaner for the removal of dust, oil, andother organics. The high carbon content may cause smut if the alkaline cleaner istoo strong. Acid cleaners or pickling solutions can be used to remove rust and otherinorganic substances. Iron phosphate is the most common conversion coating usedon cast iron.188.8.131.52.5 Galvanized SteelHot dipped galvanizing is an extension of the HRS/CRS process. The CRS isimmersed in a molten zinc bath and withdrawn to provide a smooth coating thatfrequently has a crystalline spangled appearance. Some coatings may not adhere toa galvanized surface. A wash primer is one of the few products that can be used ongalvanized steel as a tie coat or adhesion promoter between the substrate and thesubsequent application of a primer and topcoat. Alkaline cleaners work well on hot dipped galvanized surfaces, and mostmultimetal cleaner/coater products will provide sufﬁcient etching for good adhesion.184.108.40.206.6 Electro-GalvanizedIn an electro-galvanizing process, the zinc coating is applied using an electrical chargeto attract the zinc to the steel surface. It produces a more uniform surface without someof the variations in appearance that are common with hot-dipped galvanized steel.The surface resembles sharkskin with many very small pores. It is highly reactive,so oil is applied to prevent white rust. The oil needs to be removed, but the reactivity limits the possible chemicals thatcan be used. A hot neutral cleaner followed by a mild etch with ﬂuoride will providea good surface for paint bonding.
38 Paint Technology Handbook Galvanized material may also have trapped air or gasses that will expand andrelease in the cure oven, causing small pinholes in the surface. Some testing of cureoven cycles is recommended before production is started. Galvanized steel sometimes goes through a “passivation” process, which makesthe surface of the steel almost inert to chemical attack. This type of galvanized steel isoften used with no coating applied over it in applications such as highway guardrails,barn roofs, or fencing. This surface is almost impossible to coat without specialpreparation or coatings.220.127.116.11.7 GalvannealGalvanneal is prepared by heat-treating hot dipped galvanized steel so that the alloylayer grows to the surface. It provides superior corrosion resistance compared to hotdipped galvanized, and it can be treated with similar processes to electro-galvanized.18.104.22.168 AluminumAluminum is produced from a mineral called bauxite. It is used for its low density,corrosion resistance, and electric and thermal conductive properties. It conducts heatﬁve times better than steel. Aluminum forms a natural aluminum oxide layer thatprotects from air and elements. Aluminum products are available in a variety of alloys possessing differentphysical and chemical properties. Aluminum may be cast, extruded, forged, or rolledstructural forms. Aluminum alloys need to be cleaned and etched so that the organiccoating has a porous surface to adhere to. Coating lines that process both steel andaluminum typically use an etching additive, such as ammonium ﬂuoride, to producea surface conversion on aluminum. Wrought aluminum is available in several grades, which are identiﬁed bya four-digit numbering system. • First digit represents the main alloying agent • Second digit represents modiﬁcation of alloy’s impurity limits • Last two digits identify particular alloy or indicate purity of the aluminum • In addition to the four-digit alloy number, a letter or letter/number indicate the temper Treating aluminum for outdoor products requires a more robust chemical processthan simple etching with ﬂuoride in a multimetal treatment chemistry. Traditionaltreatments usually include chrome to prevent oxidation. Dry-in-place nonchromeseal rinses can also provide the necessary treatment to prevent rapid oxidation andloss of adhesion. Without a suitable chemical treatment the coating is vulnerable tomoisture penetration that can lead to rapid coating failure.1.5.2 PLASTIC SUBSTRATESAdhesion may be a problem on some plastics, due to nonpolar materials such aspolyethylene and polypropylene or release agents used in the molding process.
Part Preparation Processes and Equipment 39Some plastics, such as polyamide, polycarbonate, and polyester, are easier to coat;however, they are also more expensive. Types of soils that may be present on plastics include internal mold releases suchas fatty acid salts, oils, and polymers; external mold releases such as waxes, fattyacid salts, and polyvinyl alcohols; shop dirt, such as handling oils, skin oils, lubricantfrom equipment, dust, and smoke tar; and fabricating soils such as plastic grind andsanding dust. In some cases, plastic substrates can be painted without cleaning. However, stepsmust be taken to ensure that no surface contamination develops between fabricationand ﬁnishing. Because plastic builds a static charge that will attract dirt, parts areusually destaticized prior to painting. Some plastics must be primed, treated witha mixture containing chromic and sulfuric acid, plasma treated, or ﬂame treated topromote adhesion between the substrate and the coating. In some cases, plastics are hand wiped with solvent prior to the coating applicationprocess. Solvent wiping is not consistent and it may not be effective. The use of solventis not desirable from an environmental compliance standpoint. The process is alsoless desirable as it is labor intensive. Aqueous cleaning with a cleaner and a DI rinse or series of rinses, followed byDI air is usually the best way to clean most plastics.1.5.3 WOOD SUBSTRATESStrictly speaking, the application of coatings on wood does not require pretreatment.Like all other substrates, wood must be free of surface defects and contamination. The wood substrate may have surface blemishes that are part of the material orcontaminants that got onto the surface during machining operations. These defectsshould be removed before the ﬁrst primer coat is put on. Sanding between coats will improve the appearance. Sanding between coatsshould be done with a ﬁne grain and a light touch. Over-sanding can remove toomuch pigment and cause a visual defect after the topcoat is applied. The goal is toremove the raised grain from the wood so the surface is smoother before applying thenext coat. It is also important to remember that wood is an organic substance that has itsown color variance and grain. Not every piece of wood will look identical, even ifthe same paint is used to coat its surface.1.6 WASHER DESIGNIn higher volume production lines, a spray washer is often used to clean and treatparts prior to coating. An industrial washer uses a series of stages that clean andtreat the surface to be coated. The number of stages and types of chemistry usedin a washer depends on the quality requirements of the coated product and the sub-strate material. The desired level of quality for the end product should be used todevelop a written standard for performance with values for the speciﬁc needs ofweathering, corrosion resistance, and other properties needed to meet the establishedstandard.
40 Paint Technology Handbook1.6.1 WASHER COMPONENTSEach stage is an independent spray or immersion process that cleans, rinses, orprovides some other treatment to improve the surface for paint adhesion, appearance,or performance. The solution used for treatment is held in a tank. In an immersionstage, the parts are dipped directly into the solution. A circulating pump is used toprovide agitation in the tank. In a typical spray stage, the part passes through a tunneland the solution is sprayed onto the surface through a series of nozzles mounted onvertical risers. Heaters, valves, gauges, and so forth are added for control. An understanding of the pretreatment system, materials, design, and controls isvery important to the ﬁnishing system operator.22.214.171.124 Solution TanksThe size of the tank that holds the chemical solution for a spray stage is based on thepump volume. The amount of solution held should be three times the GPM of thepump plus enough space for internal heat exchangers. The length of the spray process zone is determined by multiplying the requiredprocess time by the design conveyor line speed. In width, the tank will extend beyondthe tunnel from 30′′ to 40′′ as required for the tank access lids and pump mountingplate. The tanks should be around 42′′ in depth to allow for the depth of the pumpand enough space to keep the pump impeller well above the tank ﬂoor. Double pump screens should be installed to isolate the pump inlet from grossparticulate that could be passed to the pump impeller and cause plugging. A singlepocket for two screens should be provided so that a cleaned screen can always beslipped in back of the screen still in place. The pump screens should be removedand cleaned regularly with a high-pressure hose to ﬂush off built up dirt andgrease.126.96.36.199 Drainage SpacesSufﬁcient space must be allowed between spray zones to guard against mixing ofsolutions by over spray or drainage from the work being processed. The drain zone isthe distance from the center of the last spray pipe in one group of sprays to the centerof the ﬁrst spray pipe of the next stage. The length of the drain zone is inﬂuenced by time, the part shape and size andconveyor speed. Usually, the drain time will be 30–60 s. Long, horizontally hung,parts can have a big impact on the size of the drain zone. It must be long enough sothat a part or rack of parts is never entering a process stage while the tail of the partis still in the previous stage. For example, if the parts to be run are 10′ -0′′ long andthe line speed is 8 ft/min, a 60-s drain zone will not work. A 60-s drain zone wouldbe 8′ -0′′ , allowing the part to extend into two stages at the same time, channelingsolution directly from one stage into another and producing an unacceptable amountof “cross contamination.” However, when the drain zone is extended beyond 60 s,misting nozzles should be installed in the drain zone to prevent the part from drying,because ﬂash rust may occur. A set of misting nozzles is one riser set (opposing pair)with low volume nozzles that apply a gentle mist of fresh water.
Part Preparation Processes and Equipment 41 The drain deck between stages is sloped to run solution back into one of the twostages. The drain deck is usually sloped with 70% of its length angled back to the sprayzone being exited and 30% of its length angled to the next spray zone (Figure 6.4)However, the apex of the drain zone may have to be in a different position if the partscup substantial amounts of solution, or if, it will channel solution backward into thepreceding stage. The length of inlet and exit vestibules for the conveyor should be long enoughto prevent vapor roll out or excessive dripping from exiting parts. As parts exitthe washer, they will still be dripping, so, it is a very good idea to install a draintrench directly under the conveyor for a few feet to prevent water accumulation onthe ﬂoor.188.8.131.52 Tank and Housing MaterialsAlthough it is well known that MS will rust, many spray washers have been builtover the years with MS tanks and tunnels. With MS construction, the cleaner tankand rinse tanks are generally made of 1/4′′ thick plate, while zinc phosphate solutiontanks are made of at least 3/8′′ plate. In washers constructed of MS, the housing shrouds, conveyor splash guards,drip shields, and vestibule ends, including ﬂoors, should be constructed of notless than #10 gauge sheet steel, and ﬂoor plates in drain spaces or over opentanks should be of 3/16′′ steel plate. The zinc phosphate stage housing is madeof heavier plate, because it will rust faster from contact with the corrosive zincsolution. Stainless steel, either type 316 or type 304, is necessary in some stages, suchas a DI water rinse or a zinc phosphate stage. Stainless steel is preferred through-out the machine, because it offers a signiﬁcant increase in useful life. The stainlesssteel washer is less likely to contaminate work in progress, it is corrosion resist-ant, and another important advantage is easier maintenance. The surface remainssmooth and does not ﬂake or chip like MS, so screens stay cleaner, solutions staycleaner and longer and nozzles do not plug as easily. Long-term repairs or replacementof shrouds, proﬁles, and screens is eliminated. In addition, with some companies thereis increasing emphasis on the clean, high-quality appearance provided by stainlesssteel. Another alternative material to MS is a composite ﬁberglass. It offers excel-lent corrosion resistance and a very cleanable surface and has a good appearance.A composite washer will insulate heated stages and it has the same low-maintenancecharacteristics as stainless steel. Another material that can be used for washer construction is polypropylene. Itcan be welded to provide a leak proof washer and the tunnel will allow some lightto penetrate to the interior. The tanks will typically be 3/4′′ thick material, providingsome insulating capacity. Care must be taken to strengthen the tunnel and tanks withsteel to avoid sagging or stress fractures. Polypropylene does not expand and contractvery well so leaks are possible over time. An expanded metal or ﬁberglass walkway should be provided throughout thelength of the washer with suitable structural support. It should be as wide as possible
42 Paint Technology Handbookto protect workers from stepping off the edge and to keep parts from falling intothe tanks. The tank drain connections should be large enough for rapid draining. In normalinstallations, a 2′′ overﬂow gutter drain and a 3′′ tank drain from the sump in the tankbottom are provided. The tank drain should be ﬂush mounted or split nipple and ﬁttedwith a valve close to the tank. The overﬂow gutter drain line should be connected tothe tank drain line outside the drain valve (Figure 6.5).184.108.40.206 Zinc Phosphate TankZinc phosphate solutions are corrosive and generate a lot more sludge than an ironphosphate solution. Because of this, it is necessary to use thicker material or stainlesssteel in the zinc tank, and provisions must be made for sludge removal. The zinc tank should be designed with a sloped bottom to facilitate the removalof sludge through a permanent suction line to the transfer pump, or through a suctionhose and sweeper type hand tool. Heating coils and pumps should be kept well abovethe tank bottom.220.127.116.11 Sludge Removal TankA sludge settling tank should be located on a structural steel frame conveni-ent to the zinc phosphate solution tank, equipped with piping between the tanksand transfer pump, to be used for periodic transfer of sludged solution from theprocess tank. The sludge-settling tank may be square or round and should have a sloped bottomof approximately 30◦ from the vertical. Tank capacity should be at least one-third ofthe working volume of the zinc phosphate solution tank. The settling tank should have a safety overﬂow line back to the phosphatingsolution tank and a valved draw-off line located in each cone section and connectedinto the overﬂow line for returning the clear solution to the solution tank. The draw-off should be located so that approximately 40 gal of solution can be held in the conebottom below the draw off line. The bottom of the cone should be ﬁtted with a 4′′ dump valve for sludge removal.The tank should be elevated high enough above the ﬂoor level to allow a barrel orsuitable container to be placed under the dump valve for sludge removal and also toprovide for gravity return of the clear solution to the phosphate solution tank.18.104.22.168 Access Doors, Ladders, and LightingDoors should be built into the housing walls between the spray zones to provide accessfor maintenance workers or operators to view the spray zones while in operation. Thearea around the tunnel access door is one of the ﬁrst places to rust, so the door shouldbe constructed with a vapor tight ﬁt and rugged hinges and latches. Steel ladders at each access door and at the ends of the housing can be installedfor easy access to the inside of the washer. The best design includes a platform and adock light to illuminate the washer interior (Figure 6.7).
Part Preparation Processes and Equipment 422.214.171.124 PumpsSolution pumps are usually standard side suction, centrifugal type, with open impellerand double bearing shaft supports for direct connection to the drive motor. Pumps withenclosed type impeller are sometimes used, but experience, especially in handlingphosphate solutions, indicates that this type of pump requires more maintenance anddoes not maintain volume delivery and head pressure as well as the open impellertype pump. Barrel mounting pumps are used for dependable performance and easeof maintenance. Solution pumps for cleaner and all rinses, except a chromic acid rinse, can beall iron construction. Zinc phosphate solution pumps should always be stainless steelconstruction. Stainless steel pumps add cost to the construction of a washer, but theyreduce maintenance and provide substantially longer useful life.126.96.36.199 NozzlesGlass reinforced polypropylene, clamp-on type nozzles are commonly installed inspray washers. They are relatively easy to clean, change, and adjust when comparedto threaded steel nozzles. In most cleaner and rinse stages a 50–50 ﬂat spray nozzle is best. Nozzle sizes,such as 50–50, refer to the gallons per minute (GPM) of output and fan spray angle at40 psi. A 50–50 nozzle will spray 5.0 GPM at a 50◦ spray angle at 40 psi. The outputand spray angle will change at lower pressures. Nozzles are mounted in a staggered pattern to provide good impingement on theentire work surface. Fan spray patterns should be adjusted on a 10◦ angle from verticalas shown in Figure 1.4. Nozzles near the end of the process stage should be adjusted in slightly to helpprevent carry over into another stage as shown in Figure 1.5. Riser 6” 12” Nozzle Nozzle Risers Nozzle @ 10° angleFIGURE 1.4 Vertical spacing of spray washer nozzles. Spray pattern Risers Top view of washer tunnel and risersFIGURE 1.5 Plan view of spray pattern for spray washer nozzles.
44 Paint Technology Handbook In the phosphate section, a hollow-cone-type nozzle should be used. A ﬂoodingtype nozzle should be used in a ﬁnal DI halo rinse and most chromic ﬁnal rinses,where high impact pressure can remove coating. Typical nozzle volume and pressures • Cleaner and rinses, 4–5.0 GPM at 15–20 psi • Iron phosphate, 2.8 GPM at 10–15 psi • Zinc phosphate, 5.0 GPM at 10 psi • Misting nozzles (for wetting in drain zones), ﬂooding type, 0.5 GPM at 10 psiNote: It is good practice to connect the last riser in a rinse stage to a fresh water supply anduse it as make up water. This gives excellent rinsing and a ﬂow meter and valve attached to theinlet gives very accurate control of the overﬂow rate.1.6.2 WATER CONSERVATIONWater conservation can save money by reducing water usage and preserving thelife of the chemical solutions. Proper use of water can also improve quality andreduce maintenance. Counterﬂow and ﬁltration methods can be used that will improveperformance and reduce costs. Counterﬂow of the rinse stages from the last rinse back toward the preced-ing stages is one popular way of saving water. The proper way to do this isto attach a pipe from the discharge of the ﬁnal rinse, plumb it to the precedingstage and connect it to a pair of risers with nozzles that have a very low ﬂowrate, 0.3–0.5 GPM. This set of risers will spray the parts as they exit the processstage, providing extra rinsing, and the overﬂow will drain to the process tank asmake up. Fresh water will be introduced to the ﬁnal rinse to make up for this over-ﬂow to the preceding stage. The make-up pipe and the counterﬂow pipe shouldbe equipped with a ﬂowmeter and manual ball valve to regulate the volume. Thiscounterﬂow method makes the ﬁnal rinse the cleanest water and reuses overﬂowedwater. The chemical supplier can suggest the proper stages to overﬂow and whatvolume. Oil skimmers used on the cleaner stages can signiﬁcantly increase the life ofthe cleaner bath and improve the performance of the cleaner solution. Belt type oilskimmers are inexpensive, but they do not remove a signiﬁcant volume of oil per hour.A circulating system that separates the oil and returns the solution back to the tankcan remove much higher volumes of oil. Membrane type systems can also be veryeffective, but they do require more maintenance. Bag ﬁlters can be used on chemical stages to ﬁlter solution and keep the volumeof solids to a minimum. A ﬂoor sweeping pipe and independent circulation pumpwill make the ﬁlter work better by providing a push to the heavier solids along thetank ﬂoor. Solids are ﬂushed along the ﬂoor of the tank toward an outlet by rows ofnozzles or eductors. A circulating pump pulls the solution out, passes it through theﬁlter to remove the solids, and returns it to the tank. This arrangement is more costly
Part Preparation Processes and Equipment 45than a system that uses the process pump, so, it is more practical for line speeds over15 ft/min with larger tank volumes.1.7 WASHER MAINTENANCE AND CONTROLThe washer is one of the most critical components in the ﬁnishing process. Goodchemical and mechanical maintenance is essential for reliable coating performance.A regular maintenance schedule with daily, weekly, monthly, and annual tasks shouldbe used to keep the system working properly.1.7.1 MECHANICAL MAINTENANCERegular inspection of the washer is needed to make sure that it is able to performup to standard. The inspection should be used to determine that the washer plumbingis clean and in good working order. Nozzles can become worn, plugged, or misaligned so that the chemical perform-ance is reduced. Nozzles should be inspected daily to conﬁrm proper spray patterns.Worn nozzles will not produce a ﬁnely atomized spray pattern and should be replaced.Plugged nozzles will not spray at all and should be removed and cleaned by removalof obvious debris and soaking in a descaling solution. Pump screens should be removed daily and rinsed with high pressure. Water replenishment systems should be checked daily to make sure that valvesare functioning properly. It is important to keep the level sensors clean to make surethat they function correctly. Thermocouples, temperature gauges, and pressure gauges should be calibratedat least once a year. Pumps should be greased as recommended by the manufacturer and inspectedmonthly for vibration, leaks, or overheating. The inside of the spray risers will develop scale over a period of time and restrictﬂow of solutions. The inside diameter should be inspected regularly and end capsremoved to drain debris. The frequency for inspection and cleaning can be determ-ined by observing the condition of the bottom nozzles; if the bottom nozzles plugfrequently, the risers probably have excess scale buildup. Scale buildup will restrictthe ﬂow of the process solutions, reducing the volume that will affect the pressureand performance of the sprayed solution. Internal heat exchangers will build scale on their surfaces that will reduceefﬁciency. A scale buildup of 1/32′′ can reduce heating efﬁciency by 2%. Limescale deposits conduct only 3% of the amount of heat as an equivalent thicknessand area of steel. The heat exchangers should be inspected monthly and descaledperiodically. Gas ﬁred burners should be serviced twice a year as part of a preventive mainten-ance contract with a suitable service contractor. The burner inlet ﬁlters will provide aminimum of 1 month service in harsh conditions. They should be washed or replacedon a regular basis.
46 Paint Technology Handbook Plate and frame heat exchangers are external to the tank, but they still requirecleaning. The cleaner stage should be ﬂushed with a chelated acid during off hours,and the phosphate should be ﬂushed with a chelated caustic. If the plates are notcleaned regularly, they will restrict the ﬂow of solution and the heating efﬁciencywill drop substantially. Chemical removal of scale buildup will prevent loss of effective performance andefﬁciency. Actual time to descale will vary dependent on the size of the system butusually can be completed in 4–8 h. Acid descaling solutions are effective for removing lime scale and rust, but theyare not very effective at removing oily soils or product residues. Usually, it will benecessary to thoroughly ﬂush out the system with a hot (140–160◦ F) alkaline type ofmaterial to remove the oils and grease that build up in the washer. Once the system is degreased, rinsed, and drained, the plumbing should be inspec-ted to see if any parts are in need of repair or adjustment. Heavy deposits should bechipped away and the sludge should be removed from the bottom of the tank byﬂushing with a hose or shoveling. Pretesting the descaling material on a small sample will help to determine the cor-rect material and concentration. Usually, lime scale and rust will form carbon dioxidein an acid solution. Some types of scale, such as those formed by iron phosphatesor combination cleaner/phosphates, may produce little or no reaction by exposure toacid based descaling solutions. In cases where pretesting an acid solution does notproduce satisfactory results, an alkaline solution should be tested. In general, the descaling product will be opposite in pH to the process solutionthat is being removed. Descaling should typically be done once every 6 months to1 year. Regular service reports should be kept that document the condition of thewasher, including the nozzles, operating temperature, pressures, general appearance,conveyor, and washer interior condition, and so forth. Monitoring the washer condi-tion with this report will give the operator the information necessary to schedule themaintenance in advance. Any existing leaks in the washer will be enlarged when the descaling solution isrun through the system.Descaling Procedure 1. While the solution is hot, remove as much free oil as possible by overﬂowing or use of an automatic skimmer. 2. Drain the solution from the tank. 3. Flush sludge and solids to drain. 4. Reﬁll the tank with water. 5. Add a high caustic, high chelate alkaline descaler to reach 4–6 oz/gal. 6. Heat and circulate the solution for 1–2 h at the highest possible heat. A low foam detergent may be added at 0.5–1.0 % by volume to help displace oils. 7. Allow the solution to remain static for 20–30 min. 8. Overﬂow to displace surface oils or use an automatic skimmer to remove oils.
Part Preparation Processes and Equipment 47 9. Drain the solution from the tank (treat the solution if necessary or drain to a holding tank). 10. Flush sludge to drain. 11. Remove the nozzles. 12. Fill the tank two-thirds full with fresh cold water. 13. Add 10% by volume, inhibited descaling acid (muriatic). To minimize fuming in the plant, use a low volume chemical hand pump with the discharge line immersed below the solution level in the tank. 14. Circulate and heat the solution to 120◦ F for 1–2 h. 15. Drain the solution from the tank (neutralize the solution prior to discharge). 16. Flush sludge from the tank bottom. 17. Inspect the nozzles, clean by soaking in a descaling solution, repair or replace as necessary, and reinstall them in the washer. 18. Reﬁll the tank with fresh water and heat. 19. Add 0.1–1.0% by volume of proprietary type phosphate. Circulate washer for 5–10 min. 20. Drain the tank and rinse sludge from bottom. 21. Fill the tank to operating level. 22. Charge the tank with the appropriate processing chemical product.1.7.2 CHEMICAL MAINTENANCEChemical performance is very dependent on the process control and maintenance ofthe solutions. The factors that affect the performance of the chemistries are the amountof exposure time, the pressure at which the solution is sprayed, the concentration ofthe chemical in the solution, the temperature of the solution, and the control of oiland solids in the tank. To achieve the intended quality that the pretreatment system was designed for,the chemistry of the washer must be carefully monitored, recorded, and maintained.Speciﬁc ranges of operation must be established and controlled. The speciﬁc variablesto be controlled are process time (line speed), temperature, chemical concentration,pH, and TDS. Titration is the test process used to check the chemical concentration of a solution.Acid base titration is based on the fact that it will take a certain amount of an acidwith a known concentration to neutralize a sample of an alkaline cleaner and a certainamount of an alkaline solution to neutralize a sample of an acid solution. A solution called an indicator is added to the solution sample prior to titrating.The indicator is usually an organic liquid such as phenolphthalein that will cause thesample to change color when it is neutralized. Frequency of chemical readings depends somewhat on the volume of productbeing processed. In most cases, the cleaner stages should be checked for temperatureand pressure at the start of a shift, middle, and end. The results are recorded andadjustments are made if necessary. In the rinse stages, the TDS and conductivity should be tested three times ashift. The TDS and pH should not be allowed to rise very much over the initial rawwater readings. Adjustment of the overﬂow volume will help to control the rinse
48 Paint Technology Handbookwater quality. In addition, tanks should be drained and cleaned on a regular basis asnecessary. The tank dump schedule and overﬂow rate are related. If a comparativelylow volume of water is overﬂowed, say 1.5 GPM, the rinses may need to be dumpedas frequently as once a day. If the overﬂow rate is 5–7 GPM, the rinses can be typicallybe dumped once a week. In cases where maintenance of the water quality is critical,softened water can be helpful. Automated rinse control based on conductivity is alsopossible. The key is to maintain good quality rinse water with low TDS and nearneutral pH.188.8.131.52 TDSTDS can be measured with a Myron L Model 532 MI dissolved solids meter, or aMarkson Conductivity/TDS pocket tester, measuring how conductive a water sampleis in units of micromhos (µMho), or similar device. Pure water, such as distilled water,conducts electricity very poorly and so it will give a dissolved solids or conductivityreading close to 0 µmho. Ionic matter, such as acids, alkalis, water hardness, or salts,will make the water much more conductive and the dissolved solids reading will rise.The more dissolved water in the solution, the more conductive it becomes. A low level of conductivity is desirable, because the water will perform better forrinsing. To measure the conductivity of a sample solution, make sure that the meteris calibrated.184.108.40.206 TemperatureThe temperature of the solution can be determined with a thermometer such asthe Tel Tru Model GT 100B thermometer in degrees Fahrenheit. The thermometermust be immersed past the groove on the lower portion of the stem in order to getaccurate readings. To convert degrees Fahrenheit to degrees Celsius, use the followingformula: (◦ F − 32) × 5 ◦ = C 220.127.116.11 pH MeasurementThe chemical symbol pH represents a measurement of the relative acidity or alkalinityof a solution. A pH of 7 is considered neutral, acidic solutions are below 7, and alkalinesolutions are above 7. The pH can be measured with a Markson Model 88 pH meter,a pocket-type pH meter, or pH paper. Measurement of the pH provides a numericalvalue to relative acidity or alkalinity, an important feature in the controlling theperformance of a solution. For a solution to perform as designed, the desired pH must be known and thesolution must be controlled. To illustrate the point, consider the manufacturing ofjelly. In order to jell the fruit, the mixture must be slightly acidic. At a pH below 2.6,the mixture will not jell; at 2.6, a white precipitate forms and the resultant jelly isunmarketable; at 2.8, there is a separation of water droplets from the mixture; at 3.1,the mixture will produce a jelly with maximum stiffness; a pH of 3.2 will produce
Part Preparation Processes and Equipment 49medium stiffness, and at a pH of 3.3 the jelly will be thin. Above a pH of 3.5, themixture will not jell at all. Within a few tenths of pH unit, the mixture will go from “no jell” to maximumstiffness and back again to no jell. This clearly illustrates the importance of tightcontrol of the pH of a solution. Acids, from sulfuric acid that can dissolve metal to boric acid that can be usedas eyewash, all produce hydrogen ions (H+ ) in solution. The measure of acidity isthe numerical value of the hydrogen ion concentration. Expressed in chemical terms,the numerical values for hydrogen ion concentrations are usually extremely smallfractions such as 1/10,000,000. The pH scale was developed to avoid the use ofsuch inconvenient numbers. The pH scale is deﬁned mathematically as the negativelogarithm of the hydrogen ion concentration or the power to which 10 must be raisedto equal the hydrogen ion concentration. The name pH comes from the power ofhydrogen. This mathematical transaction provides us with a convenient scale from 0,for an acid solution of unit strength, to 7 for a neutral solution of pure water. Alkalis owe their alkalinity to the hydroxyl ions (OH− ) that they produce insolution. Alkalinity, measured on the same pH scale as acidity, is expressed as a value from7 to 14. Any number below 7.0 is an acid and for each whole number of decline there isan increase in the intensity of (H+ ion concentration) the acid by a factor of 10×.Any number above 7.0 is considered alkaline and for each whole number of increasethere is an increase in the intensity of (OH− ion concentration) the alkaline by a factorof 10×. In a solution with the same number of H+ ions and OH− ions the pH is 7.0. Water from the tap may be a little on the alkaline side due to the addition of causticsoda lye to make the water potable. Proper measurement and adjustment of the wateris essential to the pretreatment process. The pH of the water is measured by insertinga probe into the water that is attached to a meter. To ensure that the measurement isaccurate, the meter must be properly calibrated. The pH electrode used with the meter must not be allowed to dry off. When not inuse the electrode should be soaked in pH buffer solution. The electrode should not beused in solutions above 140◦ F, and it should be protected from freezing. The electrodeshould be rinsed with distilled water before being transferred from the test solutionto the buffer solution and it should be shaken off to reduce solution contaminationwhenever it is transferred from one solution to another. If a coating has formed on the electrode tip, it should be removed by stirringbriskly in a detergent solution or by spraying with a squirt bottle. If this does notwork and the meter responds slowly or improperly, the glass bulb can be gentlycleaned with a soft brush. If it still does not work properly the bulb or meter shouldbe replaced. The pH buffer solutions should be checked periodically by comparing their pH tothe pH of fresh buffer solution. The solution should be replaced when a pH differenceof 0.1 or greater is measured. For proper pH control of a phosphate solution, it is important to establish adesired coating weight and adjust the pH to the level that will provide that establishedstandard. The proper chemical concentration, pH, and temperature should be
50 Paint Technology Handbookmeasured (and adjusted if necessary) at the start of the shift, middle, and end, to main-tain the balance necessary to provide the desired coating weight. Because all phos-phate products and vendors have there own unique blends, the guidelines providedby the chemical supplier should be followed for proper solution maintenance. In a seal rinse solution, the variables to be controlled are pH and conductivity. Thestandard recommended pH level for a seal rinse is based on the chemicals used andthe standard for conductivity level is the raw water plus any additional conductivityadded by the seal rinse solution. These variables should be monitored along with theother rinses, three times a day. The conductivity of a DI/RO water rinse should be around 50 µmho for recircu-lated DI water and 10 µmho for fresh DI water. Manufacturers’ guidelines should befollowed for maintenance of the DI generation system.18.104.22.168 Washer Control MethodsControl of the washer solutions can be done by manual titration or with automatedsystems. Effective control depends on the speciﬁc method chosen and the dedicationof the people responsible for the washer.22.214.171.124 Manual Bath ControlA manually controlled line depends on regular titration and the correct additionsas needed. Depending on the philosophy of the operators, this could consume more,less, or the same volume of product as an automated controlled system. If the operatorchecks the washer frequently and adds small volumes of chemistries, the consumptionshould equal the automated system and performance should be excellent. Larger, lessfrequent additions should be avoided so that the solution remains fairly consistent. In amanual controlled system, the operator will normally add product using 5-gal buckets.This involves ﬁlling the bucket, lifting it to the eye level, and pouring the product intothe sump of the stage. Proper personal protection equipment (safety glasses, rubberapron, rubber gloves, etc.) is essential for worker safety.126.96.36.199 Automated Control TechniquesRegardless of the quality of the chemistries used in the washer, they must be prop-erly adjusted and maintained to perform effectively. Maintenance of the chemistriesthrough titration and measurement of operating conditions such as pH and TDS willprovide optimum performance. Any probe used in a chemical solution must be cleanedfrequently to provide accurate readings.188.8.131.52 Metering PumpsA metering pump will provide a continuous ﬂow of a small volume of productto the bath. The pump can be tied into the conveyor or washer electrical cir-cuits and only operated when the production line is running. The metering pumpeliminates slug additions and reduces the handling of the product. Over time, theoperator, based on the chemical tests, will adjust the pump output volume to maintain
Part Preparation Processes and Equipment 51the bath within speciﬁcation. Metering pumps are a great improvement over manualcontrol techniques and when combined with a chemical controller they provide thebest method of process control.184.108.40.206 Theory of Automated ControlAs mentioned previously, the best way to maintain a consistent, controlled solution isto make small, frequent product additions as required. A continuous, online chemicalcontroller will activate the metering pump and hold the concentration of chemicalin the bath to an extremely tight level for consistent performance. The cost of thesecontrollers is quite low and the quality is excellent. An automatic controller will not eliminate the need to titrate and perform chemicalanalysis of the bath, but it may be possible to perform the checks less frequently. Themanual checks are still the best method to determine bath chemistry and make surethat the controller is operating properly. Like any instrument that provides a value,that value must be veriﬁed for accuracy. Bad information from a controller or anyother instrument is worse than no information at all.220.127.116.11 Conductivity ControlAs certain molecules dissolve in water, the ability of the resulting solution to conductelectricity is increased. This holds true for most chemistries used in ﬁnishing lines.Thus, the concentration of products, such as alkaline cleaners, will be directly relatedto the conductivity of the bath. A conductivity controller will measure the conductivity of the bath and when itfalls below the target or set point, the controller will activate the metering pump toreplenish the bath. The ﬂow rate on the metering pump should be set to maximum sothat when the controller calls for product the set point is reached as soon as possible.Some controllers will feed until the set point is reached and others will feed to a presetvalue above the set point and then turn off the pump. Many controllers include an alarm function. The alarm mode would activate ifthe controller calls for product to be added, but the set point was not reached in apredetermined length of time. This could occur if the chemical drum was empty, thefeed pump was not functioning, the sensor has failed, or if a ﬂoat valve was stuckopen, feeding fresh water. Alarms can be wired to a lamp or buzzer to alert the operatorof the problem. In more sophisticated controllers, the units have diagnostic features,which will internally check the system and display an error message if a problem isnoted. The controller needs periodic adjustment for nonproduct-related conductivitysources such as soil being removed from the substrates or reaction products fromconversion coating baths.18.104.22.168 Contacting ConductivityContacting conductivity probes have carbon tipped sensors that measure the con-ductivity of the solution. While acceptable for certain processes such as rinse waters,
52 Paint Technology Handbookcontacting conductivity sensors in most processing tanks can be easily fouled by soilor scale and quickly yield unreliable information. These sensors are more sensitive in reading low levels of conductivity than non-contacting probes, but noncontacting or electrodeless conductivity systems providemore effective process control.22.214.171.124 Noncontacting ConductivityElectrodeless conductivity sensors have been available for considerable time now andhave proven their ability to accurately and reliably control most ﬁnishing processes.The fact that the sensing elements in this type of probe do not contact the pro-cess solution means that these sensors avoid fouling and require signiﬁcantly lessmaintenance. These probes use two “toroidally” wound wires that are encapsulated in thering- or doughnut-shaped sensor body. The controller supplies current to one of thewires. The second wire has a speciﬁc current induced upon it based on the conductivityof the solution in which it is submersed. The controller measures this and calculatesthe conductivity of the solution. These systems must be temperature compensated.Some systems allow for the input of custom calibration curves for the speciﬁc productbeing measured. These systems allow the option of displaying the units in a percentagevalue. Electrodeless conductivity systems are the ideal choice for cleaner baths andconversion coatings. For very dilute processing baths, chemistries with very low con-ductivity values and rinse waters, contacting conductivity should be used, becausethey are better at monitoring low levels of conductivity than the noncontactingsystems. For rinse water tanks the controller should be programmed to open a fresh-waterfeed valve when the conductivity rises above the set point. For DI/RO water systems,a resistivity controller system with the appropriate sensor should be used to handlethe extremely low conductivity.126.96.36.199 Zinc Phosphate ControlA standard electrodeless controller is usually effective for monitoring iron phos-phate baths. Zinc phosphate solutions have more complex chemistry and requiremore thorough control techniques. This is especially true of spray zinc phosphatesystems. Zinc phosphate solutions often have multiple products being added to the bathsimultaneously, such as accelerators and replenishing packages. In addition, it is oftenthe titration ratio value and not the total or free acid that is used to control the bath.Controlling the process based on the overall conductivity is not reliable. These baths should be run either manually or with an auto-titrating system capableof running a series of different tests. In a limited number of cases, a conductivitycontroller can effectively be used to hold the total acid value constant and acceptablycontrol the bath.
Part Preparation Processes and Equipment 5188.8.131.52 pH ControllerspH controllers can be used on certain processes to add product when a set pointis reached in either a rising or falling direction. The sensors on pH electrodes arecontacting the process solutions. Most of these sensors are semipermeable glasssurfaces that are very sensitive. They require calibration on a regular basis. The best method is a two-pointcalibration with buffer solutions. In some cases, a single point calibration with a“grab sample” tested on a second, calibrated meter is acceptable. pH control shouldbe veriﬁed frequently for reliable results.184.108.40.206 Interfacing Controllers with a ComputerChemical controllers are powerful tools and sufﬁcient on their own in most applica-tions. Combining controllers with computers provides a number of additional featuresthat can add beneﬁt to the system. The computer can be used as a data acquisitiontool or it can be used to actually control the process.220.127.116.11 Data Acquisition ToolsMost useful controller systems have an output signal that directly relates to the value ofthe display. In most cases, this is an analog signal in units of milliamps (usually 4–20).This signal can be directed to a computer where the information can be displayed andstored. The signal is usually digitized using input/output (I/O) hardware and software.Once in the computer, the information can be displayed in several ways. The computercan be networked or accessed remotely to view the data from different locations. These systems allow for powerful alarming features with varying levels of alarmsand can call or page personnel if required and they are ideal for real-time statisticalprocess control (SPC) systems and manipulation of data. They also allow the systemto store information that can be reviewed and used to deal with product problems.18.104.22.168 Computer Control SystemsComputers can be used to actually control the process using programmable logiccontrollers or a PC with appropriate software from a remote location. Computer-controlled systems can alter the process at any networked or accessed computerstation with all of the display and data manipulation features of a computerized dataacquisition system. Recipe functions can be used to allow the operator to activate a program at theterminal that activates a series of events. This can be used to adjust the contact timesor temperatures by recipe for different substrates or other variables. In general, thesesystems use lower cost “transmitters” at the baths in place of controllers and allowthe computer to “analyze” the data. These systems can provide complex functionswith links to the entire plant operation, from order entry, to inventory, production,and shipping.
54 Paint Technology Handbook Regardless of the type of control system used, strict process control techniquesmust be practiced to consistently obtain a quality ﬁnish. This can be accomplishedby simply titrating the baths every 2–3 h or by implementing an automated controlprocess. Learning and understanding each step in the operation and having the abilityto measure that the operating parameters of each step is the key to a successful processcontrol system. While automated addition of chemicals is better from the standpointof process control, the automatic controls must be checked to be sure that they areperforming properly. There is no substitute for regular titration.
2 Paint ComponentsA liquid paint is an engineered product made of several different ingredients thatmix to create a speciﬁc product with its own unique properties. The selection ofcomponents used to manufacture paint will affect its stability (shelf life), applicationcharacteristics, handling, cleanup, disposal, and most importantly, the performanceof the product on which it is applied. Paint formulas usually include 1. Resin (binder) 2. Pigments 3. Solvents 4. Additives2.1 RESIN (BINDER)The resin is the ﬁlm-forming component that identiﬁes the paint. A variety of resinsand polymers (materials that will undergo reaction to form a resin) are used inpaints. The formulation of a paint material and the particular chemicals used areinﬂuenced by the particular resin or resin combination used. The blend of resin(sometimes referred to as the binder) and solvent is sometimes referred to as the paintvehicle. Paint binders may be referred to as convertible and nonconvertible types. Convert-ible paints are materials that are used in an unpolymerized or partially polymerizedstate and undergo reaction (polymerization) to form a solid ﬁlm after application tothe substrate. Nonconvertible paints are based on polymerized binders dispersed ordissolved in a medium that evaporates after the coating has been applied to leave acoherent ﬁlm on the substrate surface. Convertible binders include oils, oleoresinous varnishes, alkyds, amino resins,epoxy resins, phenolic resins, polyurethane resins, and thermosetting acrylics. Nonconvertible resins such as cellulose, nitrocellulose, chlorinated rubber, andvinyl resins will not be covered in this text, because they are usually used in low-solid, high-solvent content coatings that are not compliant for the majority of modernindustrial applications.2.1.1 OILS AND OLEORESINOUS VARNISHESOils were commonly used in paint formulation but have declined as improvedpolymers were developed that could be used for a broader variety of coatings.With the exception of limited use of reﬁned linseed oil and linseed stand oil incertain types of primers for steel and timber, oils are rarely used as the binder 55
56 Paint Technology Handbookin an industrial paint. However, oils are often used as modifying components inthe preparation of oleoresinous varnishes and especially in the oil-modiﬁed alkydresins, one of the most widely used binders in modern paint technology. Vegetable oils are generally classiﬁed as either drying or nondrying oilson the basis of whether they will react with air temperatures to form a rubbery,poor solvent-soluble ﬁlm. For example, linseed and tung oil are referred to as drying oils, because they willreadily dry when exposed to oxygen. Another group of oils that includes soybean oilis called semidrying oils, because they do not dry as quickly. Some oils, such as castor oil or olive oil, are classiﬁed as nondrying oils.Nondrying oils like castor may be converted to drying oil by heating to 530◦ F (280◦ C)for several hours to break down some of the constituent acids of the oil. The drying process is a complex oxidation reaction involving the centers ofunsaturation in the carbon chains of the fatty acid triglycerides of the drying oil.The reaction is referred to as oxidative polymerization or auto-oxidation. Oxidationof a drying oil and ﬁlm formation will occur naturally, but the rate of reaction isslow and so it is usually accelerated by the addition of driers such as cobalt or leadnaphthenates. Linseed oil as extracted from the ﬂax plant is dull and cloudy and needs to bereﬁned to remove the natural impurities. The method of reﬁning depends on thepurpose for which the oil is to be used. The oil can be treated with alkalis, acids, orbleaching processes to lighten the color of the ﬁlm. Alkali reﬁning is more commonly used than acid reﬁning. In this process, the oilis treated with sodium hydroxide solution in a calculated quantity to neutralize theacid value of the oil. The acid value is the number of free acid groups in a polymer.The number is actually the milligrams of potassium hydroxide required to neutralizeone gram of the polymer. The resultant soap is then removed by centrifuging. Thereﬁned oil is then washed with water to remove all traces of the alkaline material.Although certain treatments are needed to clean up linseed oil, it is still used in anunmodiﬁed state. The reﬁned linseed oils are usually low in viscosity and need to be heat treatedto produce thicker linseed stand oil. The oil that is processed by heat-treating(520–575◦ F, 270–300◦ C) will thicken from polymerization. This makes a moreﬂexible and durable coating, but one that takes longer to dry.2.1.2 ALKYD RESINSAlkyd resins are modiﬁed with a number of oils including soya, linseed, dehydratedcastor, and coconut. They in turn can be combined with such resins as acrylics, vinyltoluene, silicones, and amino-resins. The latitude of compatibility of the oil-modiﬁedresins makes them popular for use in industrial coatings. They are fairly inexpensiveand they have a variety of properties. Alkyds can be prepared directly from oil (triglyceride), a polyol, or an acid.The percentage of oil contained in an alkyd classiﬁes the end use of the alkyd andaffects such properties as speed of drying, ﬂexibility, durability, and so forth. Twomanufacturing methods are used in the preparation of alkyd resins: the alcoholysis
Paint Components 57TABLE 2.1Oil Modiﬁed AlkydsAlkyd Oil Length % Characteristics UsesShort 20–25 Nonoxidative. Soluble in aromatic As modifying resins in baking hydrocarbon solvents systems for interior use Hard brittle ﬁlmsMedium 45–60 Air-drying or baking cure. Soluble in As above for interior and exterior aliphatic–aromatic solvent blends Also used in fast drying systems More ﬂexible ﬁlmsLong 60–80 Air-drying (oxidative). Soluble in Exterior air-dry systems aliphatic solvents. Very ﬂexible ﬁlmsprocess, by which oil-modiﬁed alkyds are produced, and the fatty acid process, whichis used to prepare fatty acid-modiﬁed alkyd resins. The fatty acid resins tend to have a paler color than the oil-modiﬁed resins becauseof the greater purity of the fatty acids. In the fatty acid process, all three components,the fatty acid, the polyhydric alcohol, and the polycarboxylic acid, are heated togetherat temperatures in the range of 240◦ C until esteriﬁcation of polymerization is com-plete. In the alcoholysis process, the polyhydric alcohol and the modifying oil areﬁrst reacted together and then the polycarboxylic acid is added. Both processes yieldoil-modiﬁed alkyds, classiﬁed on the basis of the amount and type of oil used asshown in Table 2.1. Drying and semidrying alkyds cure by auto-oxidation, so they are good resins touse in formulation of air-dry coatings. Nondrying oil alkyds, particularly the short-oilresins, require exposure to heat for curing. They can also be used as plasticizers forother synthetic resin systems. The composition and simpliﬁed structures of a short,medium, and long oil alkyd are shown in Table 22.214.171.124.3 POLYESTER RESINSPolyester resins are typically used in heat-cured coatings that need to be high in paintsolids and low in solvent content. They have extremely good color retention thatprovides good over-bake protection and very good UV resistance, and they can beapplied using a wide range of spray equipment. Polyesters are very similar in chemicalstructure to the earlier-discussed Type I oil-free alkyd resins. Polyesters are oftenformulated in two-component products that are used for plastics. The catalyst systemin the 2K products allows them to be cured at low temperature, and the ﬁnished ﬁlmhas excellent appearance and UV resistance.2.1.4 ACRYLIC RESINSIn the coatings and plastic ﬁelds, the term “acrylic” resin applies to the polymers andcopolymers of the esters of methacrylic and acrylic acids. Copolymers of these esters
58 Paint Technology Handbookwith nonacrylic monomers such as styrene, butadiene, or vinyl acetate are also referredto as acrylic resins. Acrylic resins are very versatile and popular for industrial liquid coatings. Theyprovide toughness, good weathering ability, and resistance to abrasion and chemicalattack. They are also considered to be better than alkyd resins for gloss retention.Acrylic thermosetting resins that are cross-linked with epoxy or amino resins areused in the appliance industry because of their excellent physical and chemicalproperties. Solid and solution polymers are used in lacquer ﬁnishes for metal, wood, leather,ceramic, and plastic surfaces. Acrylic emulsions, which are manufactured directly inthe latex form, are used in both indoor and outdoor paints. Along with the stabilityof the acrylic resins and their toughness and chemical resistance, they also providean appealing, high-quality coating. The hardness and slip properties can be varied overa wide range to suit the demands of the application. Adhesion and solvent resistancecan be built into acrylic coatings by adding other functional monomers into the resinsystem by copolymerization. Acrylic polymers are used for decorative and protective functions. For decor-ative applications, they provide high gloss, good pigment binding characteristics,and clarity. For protective applications, they provide good adhesion, hardness, anddurability. Acrylic lacquers are used for both ferrous and nonferrous substrates. Lacquersare solutions of resins in organic solvents that harden as the result of the evaporationof the solvent. This can be forced or accelerated with heat. The acrylic can be eitherthe major or minor portion of the lacquer. There are thermoplastic lacquers that allow thermal reﬂow and better dispersab-ility of metallic colors than thermoset enamels. Applied over a primer and baked, theacrylic lacquers resist many years of outdoor exposure. Harder acrylics made of almost straight polymethyl methacrylate resin systems areused to make hard, durable ﬁnishes for toys. Automotive touch-up lacquers in aerosolcans are another large market. Plastic substrates are a growing market for acryliccoatings, especially since there are now more grades of acrylic polymers that aresoluble in solvents that do not attack the plastic. These solvents include ethanol,isopropanol, naphtha, and straight-chain hydrocarbons. The resin systems are usuallylow to medium molecular weight homopolymers and copolymers of ethyl and n-butylmethacrylate. Thermosetting acrylics are generally harder, tougher, and more resistant to heatand solvents than the thermoplastics. They are less resistant to UV light and of course,they must be heat cured to obtain cross-linking. Thermosetting acrylics are easierto apply. The relatively low molecular weight copolymers of methacrylate withother acrylic or nonacrylic monomers constitute the uncured resin. These functionalmonomers provide sites for subsequent cross-linking, usually by reaction with non-acrylic additives. These low molecular weight copolymers make it possible to applyhigh solids, low volatile organic compound (VOC) coatings, which will level muchbetter before cross-linking and result in a smoother coating. Most thermosetting acrylic resins available for commercial coating applicationscontain relatively high amounts of styrene, vinyl-toluene, epoxies, or amine resins to
Paint Components 59enhance their in-use properties, to lower their cost, or to effect cross-linking. The term“acrylic thermoset” is even applied to coatings that have only the acrylic monomerpresent to establish the curing or cross-linking sites for the coating. Because of thenonacrylic nature of these coatings, they may not exhibit the characteristic propertiesnormally sought in an acrylic coating.2.1.5 AMINO RESINSAmino resins are generally used in baked coatings as cross-linking agents. They areused in proportions up to 50% of the total vehicle binder. They can be used withalkyds, polyesters, epoxies, thermosetting acrylics, phenolics, and other heat reactiveresins. Melamine and urea–formaldehyde are the most common examples of thisresin.2.1.6 EPOXY RESINSEpoxy resins are known for their excellent corrosion and chemical resistance. Becauseof their tendency to fade and chalk when exposed to sunlight, they are used for interiortopcoat applications or as primer for exterior applications. Excellent corrosion resistance can be obtained with ﬁlm thickness as low as0.5 mil. The epoxy resin is usually cross-linked with melamine or urea resin at curingtemperatures of 350–425◦ F. Epoxy coatings are characterized by excellent adhesion,a high degree of impact and abrasion resistance, and resistance to chemicals andsolvents. This combination of properties makes the epoxy formulas a good ﬁt forchemical laboratory furniture and similar applications. They also have good insulat-ing properties, making them a good ﬁt for the electrical industry, and they can provideexcellent wear on tools. Epoxy resins are rarely used as-is in paint formulations because of their lowmolecular weight. The low molecular weight does not allow adequate ﬁlm builds, sothey are usually cured into higher molecular weight complex polymers called epoxyglycides. The terminal or reactive groups are epoxy and secondary hydroxyl in nature.These complex molecules are then cross-linked with commonly used curing agents. The most commonly used epoxy paint system is the two-component amine-curedcoating where the resin and hardener are mixed just prior to application. The hardenercreates a reaction that will create a hardened ﬁlm after the components are mixed. Thepot life (time that it takes for the coating to harden) can range from a few minutes toseveral days depending on the formulation. Heat is often used in industrial applicationsto accelerate the cure process. Epoxy formulas are used as maintenance coatings, can coatings, pipeline coatings,tank linings, and so forth. They have also been formulated using special extendersand thixotroping agents to allow one coat ﬁlm builds of 6–40 mil. Epoxy formulasare also often used as a primer. Epoxy resins can also be used in epoxy-acrylic thermosetting systems to providea combination of ﬁlm hardness, mar resistance, gloss and color retention, and chemicalresistance. These formulas make good coatings for major household appliances andautomobiles.
60 Paint Technology Handbook2.1.7 URETHANE RESINSUrethane is the accepted description for a group of polymers that are sometimescalled polyurethanes. Urethane resins are very popular with formulators, providinga combination of chemical resistance, toughness and abrasion resistance, and exteriordurability. Effective application on plastics has led to substantial growth in urethanetechnology. Urethanes are the reaction products of isocyanates with materials that havehydroxyl groups. They contain a signiﬁcant number of urethane groups regardlessof what the rest of the molecule may be. The basic chemistry of isocyanates andurethanes has been known for over a hundred years. In 1848, Wurtz prepared methyland ethyl isocyanates by reacting potassium cyanate and alkyd iodides. He also foundthat ethyl isocyanate reacted with ethyl alcohol to form ethyl carbamate, which waslater named urethane. The modern industrial development of urethane polymers stems largely fromthe pioneering work of Professor Otto Bayer in Germany in 1937. The basic rawmaterials, the isocyanates, are produced in a number of different forms, but themost widely used is toluene diisocyanate (TDI). The TDI has a noticeable vaporpressure and has an irritant effect on the mucous membranes and so requires specialhandling. Table 2.2 compares some of the properties of the various resins discussed. Many different vehicle systems are used for various applications and environ-mental conditions with a wide range of properties as shown above.TABLE 2.2Resin Properties Modiﬁed Alkyd Baking (Styrenated) Cellulose Catalyzed Alkyd Amino Polyester Alkyd Acrylic (Lacquer) Epoxy UrethaneExterior E E E G E E G E durabilitySalt spray E G G G E E E EAlkali P F G G G P E F resistanceSolvent G E E F F F E E aliphaticSolvent ketone P P G P P P G EFlexibility E G E G E E F EImpact G E E G E E G EHeat resistance G G E G G P G GColor retention G G E G E E F EGloss retention E G E F E G P EE = excellent; G = good; F = fair; P = poor.
Paint Components 612.2 PIGMENTSPigments are particulate solids that are dispersed in paints to provide certain char-acteristics to them, including color, opacity, durability, mechanical strength, andcorrosion protection for metallic substrates. In order to achieve the desired res-ults, pigments have to possess certain properties. Pigments may be inorganic andorganic materials. Organic pigments are used primarily for decorative purposes,while inorganic materials have traditionally been added for protective proper-ties. Extenders are used in conjunction with pigments to modify the properties ofthe paint. The size and shape of the pigment particles are important considerations, sincethey affect the agglomeration or packing within the paint binder or matrix. Mostpigments are crystalline and the crystal form often affects the characteristics of thepigment. Particle size also affects the ﬁnished gloss, settling of the pigment duringstorage, and wetting by the binder. Other factors such as color, tint strength, color-fastness, and opacity are inherent characteristics of the pigment. Density is anotherimportant factor affecting not only settling, but also the volume of pigment for a givenweight addition. Pigments have to be uniformly dispersed in the binder to provide a consistentappearance. They have to remain in suspension or be easy to disperse if settlingoccurs. When the paint is mixed, the pigments are incorporated mechanically in amill. The pigment has to be able to withstand the milling process. A wide variety of coloring agents can be used to provide a considerable range ofcolors and shades. The number of pigments used and the amount of each is related tocolor, hiding, and many other ﬁlm properties. Some common pigments are discussedin the following section.2.2.1 WHITE PIGMENTSAlmost all paint formulas include some white pigments to adjust the lightness–darkness of the ﬁnal color. Some of common white pigments are listed as follows.126.96.36.199 Titanium DioxideTitanium dioxide is a widely used, nontoxic, stable synthetic pigment used for bothprotective and decorative paints. It comes in two different crystalline forms, rutileand anatase. The rutile crystalline form is more compact and has a higher speciﬁcgravity, greater refractive index, enhanced stability, and enhanced durability. The high refractive index of titanium dioxide (2.7 for rutile and 2.5 for anatase)enables it to provide a higher degree of opacity in paint ﬁlms than any other whitepigment. Rutile titanium dioxide is photochemically inert and the pigment protectspaint ﬁlms from degradation by scattering absorbed light. In contrast, the anataseform is photochemically active and paints formulated with this pigment are subjectto heavy chalking. The anatase grade is used mainly for interior applications due toits cleaner white color.
62 Paint Technology Handbook188.8.131.52 Zinc OxideA synthetic based pigment that will inhibit mold growth, if present in high levels(about 30% by weight). The basic nature of zinc oxide leads to interaction withpaints of high acid value with the formulation of zinc soaps. These can mechanicallyreinforce the ﬁlm but can cause embrittlement on exterior exposure.184.108.40.206 Antimony OxideA synthetic inert pigment often used with chlorine-containing binders in the formu-lation of ﬁre-retardant paints. When exposed to ﬂames, the antimony chloride vaporthat is released is heavier than air and acts as a blanket to the ﬁre. This pigment alsohas good opacifying characteristics.220.127.116.11 White LeadA synthetic basic pigment used for centuries, now limited in use because of its toxicity.Being basic, white lead will react with acidic paints to form lead soaps, which willenhance ﬁlm elasticity, useful for timber primers. However, the pigment has a highchalking rate and a tendency to darken in polluted atmospheres due to the formationof lead sulﬁde.2.2.2 YELLOW PIGMENTSYellow pigments are used to adjust the yellow–blue axis of the color spectrum.18.104.22.168 Yellow DyesAzo dyes, ranging in color from orange to green-shade yellows. They have good lightstability in full shade unless the dye is reduced with white pigments. They providegood opacity and are nontoxic, so they are often used instead of lead chromates.Yellow dyes are soluble in ketones, esters, and aromatic solvents, but they have poorsolubility in aliphatic solvents. This makes them suitable for use in air-dry coatingsthat contain aliphatic hydrocarbons or in emulsion systems.22.214.171.124 Benzidine YellowsInsoluble azo dyes prepared in a range of shades from yellow to red. They havegood opacity and are insoluble in most solvents used in paint formulations. Theyare nontoxic and have good resistance to acids and alkalis, and they can withstandtemperatures up to 300◦ F. The benzidine yellows are not lightfast, even when used atfull shade, so their use is generally restricted to interior applications.126.96.36.199 Lead ChromatesChromate pigments are rarely used today because of the environmental problemsassociated with chrome. A wide range of synthetic pigments, ranging from pale yellowto deep orange in color, have been used in paint formulation. Lead chromes have
Paint Components 63high tint strengths, good lightfastness, and opacity, but they also darken in pollutedair and they will bleach in the presence of sulfur dioxide. Lead chromates interactwith alkaline substrates resulting in color loss. Nevertheless, the lead chromates areuseful coloring pigments and are used in undercoats and ﬁnishing systems. The colorof the pigment is determined by the process conditions during manufacture.188.8.131.52 Zinc ChromateThree forms of zinc chromate are used for pigmentation of paints. The pigment gradeshave good lightfastness and are stable in polluted air, but they are of low opacity. Thezinc chromates are slightly basic and will react with acid paints, leading to a thickeningof the paint during storage. The form of zinc chromate used for corrosion-protectionmust be free from residual chloride, which is usually present in pigment grades.A third form of zinc chromate, the tetroxichromate, is used in metal pretreatmentprimers.184.108.40.206 Yellow Iron OxidesNaturally occurring iron oxides, ranging in color from dull yellow to dark yellow-brown, but more restricted in the range of color shades than synthetically preparedoxides. Natural oxides have cleaner and brighter colors combined with greater colorstrength because of their greater purity. Both natural and synthetic oxides are resistantto alkalis and organic acids, but they can be discolored by mineral acids. Shadevariations can occur at elevated temperatures. Iron oxides will absorb UV radiationand have a protective effect in exterior paints.220.127.116.11 Cadmium YellowSynthetic pigments varying in color from primrose to orange, the shade being determ-ined by manufacturing process conditions. They are stable at high temperatures. Theyare unaffected by alkalies, but they can be decomposed by acids. They may be usedon a variety of substrates, especially where alkali resistance or temperature resistanceis required. Cadmium, like chrome and lead, was a staple in the formulation of paint, espe-cially performance coatings, for many years. These heavy metals have long beenrecognized as undesirable components in paint due to their negative impact on theenvironment and have been all but phased out of paint formulation in the United Statesand many other industrialized nations.2.2.3 GREEN PIGMENTSGreen pigments are used to adjust the blue–yellow axis of the color.18.104.22.168 Phthalo GreenA toner, which, unlike the azo dyes, is not purely organic in nature but is asalt-like compound. Toners are formed by the reaction of a basic dyestuff with a
64 Paint Technology Handbookcomplex acid or by the reaction of an acidic dyestuff with a metal or metal salt; theyare more resistant to solvents than the organic dyes. Phthalocyanine green pigment has a blue–green color with good opacity in paints.It has good resistance to solvents, heat, and alkalis, but it can be decomposed by acids.It is widely used in decorative ﬁnishes.22.214.171.124 Chromium OxideChromium oxide is a dull green, synthetic pigment with good stability to light, heat,acids, and alkalinity, but it provides poor opacity. It is useful as a pigment for paintsthat requires high chemical and photochemical resistance. Chrome oxide is also usedas a pigment for concrete and cement. Once again, chrome is no longer a commonpigment used in paint formulation in North America.126.96.36.199 Lead Chrome GreensSynthetic pigments ranging from grass green to deep green in color, the shade beingcontrolled by the Prussian blue admixed with the lead chrome yellow. They havegood opacity, but they tend to discolor in polluted air. They also tend to ﬂoat in paintformulations. Owing to toxicity, these products are not often used today.2.2.4 BLUE PIGMENTSBlue pigments are used to adjust the blue–yellow axis of the color.188.8.131.52 Phthalocyanine BluesThese vary in color from reddish-blue to yellowish-green; they tend to have hightint strength and high opacity along with very good lightfastness. They are nontoxic,temperature stable, and resistant to most solvents and chemicals except strong acids.These pigments are used in a great many paints and ﬁnishes.184.108.40.206 Prussian BlueThis is a bright blue synthetic pigment having high staining power but low opacity.It is lightfast and acid resistant, but it can decompose to iron oxide by exposure toalkalinity and elevated temperature.220.127.116.11 Ultramarine BlueA complex synthetic aluminosilicate pigment, it occurs naturally as the semipreciousstone lapislazuli. The color of the pigment is related to the presence of sodium sulﬁde.The shade can be altered by the amount of silica used in its manufacture. The pigmenthas a coarse texture and is subject to hard settling, but it has good lightfastness, heatresistance, and alkali resistance. It will decompose in an acid.
Paint Components 652.2.5 RED PIGMENTSRed pigments are used to adjust the red–green axis of the color.18.104.22.168 Toluidine RedsNontoxic azo dyes characterized by bright, clean colors, good lightfastness, and highopacities although the color stability is reduced when they are mixed with whitepigments. Toluidine reds have good color stability, are resistant to acids and alkalis,and heat up to 350◦ F for short periods. They are soluble in aromatic solvents andslightly soluble in aliphatic solvents and alcohols, so they are susceptible to bleedingin many systems.22.214.171.124 Arylamide RedsNontoxic azo dyes ranging in color from orange to red or deep crimson. Theyhave good lightfastness even if reduced with white pigments and they are tem-perature stable up to 300◦ F. Arylamide reds are slightly soluble in solvents.They are resistant to acids and alkalis and are used in many decorative exteriorapplications.126.96.36.199 Red Iron OxideNatural red oxides, mined as hematite ore, and synthetic red iron oxides are used aspigments. The presence of impurities together with the variation in the iron oxidecontent provides pigments with colors ranging from orange-red to deep brown. Thenatural oxides are used in timber stains and low-cost metal primers. Synthetic oxides have softer texture and greater purity, giving brighter, cleanercolors, and greater tinting strength. Colors are determined by manufacturing condi-tion. Natural and synthetic oxides are resistant to alkalis and organic acids but mayreact to mineral acids and high temperatures. They absorb UV radiation and increasethe resistance of paint ﬁlms to fading. Two other inorganic red pigments, red lead and basic lead silicochromate, wereused in the past, primarily for their corrosion-protecting properties. They are seldomused today due to the environmental risks associated with such materials.2.2.6 BLACK PIGMENTSBlack pigments are present in many paint formulas to adjust the lightness–darknessof the coating.188.8.131.52 Black Iron OxideA synthetic pigment of low tinting strength, mainly used as a colorant for ﬁllers,primers, and undercoats. The pigment is reddened by heat, but otherwise the oxidehas good chemical resistance.
66 Paint Technology Handbook184.108.40.206 Carbon BlacksPigments that are produced by the carbonization of hydrocarbon minerals, plants,and animals. Properties vary according to the source of the carbon and the impuritiespresent. Purer carbons are of a ﬁner texture, have better color and opacity than carbonof lower purity. Carbon blacks are lightfast, insoluble in acids and alkalis, and are resistant tosolvents. They provide good opacity, even at low addition levels. Carbon blacks arevery common pigments used in paint formulations.2.2.7 METALLIC PIGMENTSMetallic pigments are very popular for paints that will be used on products such asautomobiles, motorcycles, metal ofﬁce furniture, and other products that requireexceptional appearance characteristics. While aluminum is the most commonlyused metallic pigment, stainless steel, lead, and zinc have also been used in paintformulation.220.127.116.11 Aluminum PigmentA pure metal that is rendered resistant to many aggressive agents by the presence of asurface ﬁlm of alumina. It is available in two powdered forms, leaﬁng and nonleaﬁnggrades. Particles of the leaﬁng grades, which are coated with stearic acid or a similarsurface-active agent, tend to ﬂoat toward the surface of a paint ﬁlm and becomeoriented parallel to the plane of the ﬁlm. The close packed layer of aluminum plateletsprovides the ﬁlm with a reasonably efﬁcient moisture barrier and functions as aprotective pigment. Normally, low levels of aluminum are used, often with no otherpigments. The aluminum may also prevent corrosion by being a sacriﬁcial anodewhen the surface of the coating has been damaged. The nonleaﬁng grade does not migrate to the surface of the coating but is morerandomly distributed throughout the ﬁlm. Again, low levels of the nonleaﬁng alu-minum are used and the pigment’s main function is to provide a sparkle effect tothe ﬁlm.18.104.22.168 MicaA naturally occurring potassium alumino-silicate used in the form of ﬁne platelets.The lamellar structure of mica results in a leaﬁng effect like that in leaﬁng-gradealuminum that reduces water permeability in the paint ﬁlm. The incorporation of micaimproves weathering resistance in paint by reducing the tendency to fail by crackingand checking. These properties permit mica to be used in exterior decorative coatings.2.3 EXTENDERSExtenders are paint additives that are insoluble in the binder and solvents of theformula and have little or no opacity or color effect on the ﬁlm. They are added to
Paint Components 67modify the ﬂow and mechanical properties of the paint as well as the, permeability,gloss, and leveling characteristics of the paint ﬁlm.2.3.1 BARITESA hard, dense, naturally occurring inorganic mineral that is very resistant to the actionof acids and alkalis. It is transparent in oil and resinous media so that it can be usedin solvent based paints without affecting the color or opacity of the ﬁlm. The highspeciﬁc gravity of barites can result in settling problems in stored paint. It is usedas chemically inert ﬁller that reinforces the mechanical properties of the ﬁlm. It willreduce the durability of the ﬁlm, if used at high levels in a coating. A synthetic form ofbarium sulfate is also used as an extender and has properties similar to those of barites.2.3.2 KAOLIN CLAYA naturally occurring hydrated aluminum silicate used in a ﬁne particulate form. It isused as ﬁller in solvent-based paints but in small amounts, because the small particlesize can adversely affect the ﬂow characteristics of the paint. The ﬁne particle sizedoes help to prevent settling in storage. Kaolin clay is used as a ﬂattening agent (glossreducing) in undercoats and eggshell ﬁnish paints and widely used in emulsion paints.2.3.3 TALCA naturally, occurring hydrated magnesium silicate mineral. It occurs as a mixture oflamellar and ﬁbrous particles, the latter providing a reinforcing effect while improv-ing ﬁlm ﬂexibility. The platelets have an effect similar to mica in reducing waterpermeability. As a result, talc is often used in protective paints where high durabilityis required. The exact nature of how talc and mica improve corrosion resistance isnot fully understood.2.3.4 CALCIUM CARBONATE (LIMESTONE)Naturally occurring limestone that is (also produced synthetically) widely used ininterior and exterior emulsion paints and undercoats. Acids will attack limestone, soit cannot be used in aggressive environments. Nevertheless, it has wide usage in bothaqueous and solvent-based ﬁnishes. There are many other pigments that will provide corrosion resistance and otherproperties such as improved adhesion, mechanical properties, and viscosity control.The precise blend selected for a coating is related to the needs of the end user.Color, performance, cost, and environmental concerns affect the particular blendof pigments used. Figure 2.1 is a pictorial representation of the optimum pigment loading that canbe calculated. The common term for this is the pigment to binder ratio. Althougheveryone talks about pigment to binder ratios, experience has shown that very fewpaint formulators can actually determine the pigment-to-binder ratio. The optimumpigment loading is generally based on empirical observations, trial and error, andhistory.
68 Paint Technology Handbook A B C Binder Pigment VoidsFIGURE 2.1 Three different pigment to binder ratios. TABLE 2.3 Usual Variation of Film Properties with Increasing Pigment Levels Usual Effect of More Property Pigment Levels Viscosity Increases Adhesion Maximum at CPVC Tensile strength Maximum at CPVC Moisture permeability Minimum at CPVC Cost Increases Gloss Decreases Impact resistance Maximum at CPVC Figure 2.1 shows three different pigment-to-binder ratios. The pigment volumeconcentration (PVC) at which the pigment particles just touch each other with binderﬁlling the space between them is called the critical pigment volume concentration(CPVC). The picture A in the ﬁgure has too little pigment, B is the correct CPVC,and C has too much pigment. The percentage of pigment required to achieve the CPVC depends on the size andshape of the particles. Smaller particles can be packed together with greater efﬁciency,resulting in higher CPVC. The signiﬁcance of PVC is illustrated in Table 2.3. It shows how a number ofimportant ﬁlm properties vary with pigment level. The amount of pigment in paint isoften a compromise between several of the properties listed in Table 22.214.171.124 SOLVENTSA solvent is a pure or mixed liquid that is used to make the paint ﬂowable prior toits application. In practice, the term solvent, solvent blend, and thinner are oftenused interchangeably. Solvents are chemical substances that can dissolve, suspend,or extract other materials, usually without chemically changing either the solvents orthe other materials. Solvents make it possible to process, apply, clean, or separatematerials. Solvents work on the principle of “like dissolves like.” Therefore, for asolvent to work, it needs to have similar chemical characteristics to the substance thatit is trying to dissolve. Water is also a solvent, which is described as “inorganic” (notcontaining carbon).
Paint Components 69 Some important terms relating to solvents are as follows: • True solvent—A liquid that can dissolve the binder. • Diluent—A liquid that cannot dissolve the binder by itself but can be added to a solution to increase its capacity for the binder. • Latent solvent—A liquid that cannot dissolve the binder by itself but increases the binder’s tolerance for a diluent. • Thinner—Any pure or mixed liquid added to a paint to reduce its viscosity (make it more ﬂowable). • Front-end solvent—A fast evaporating solvent that leaves the paint very soon after application, usually before the part reaches the oven. • Exempt solvent—Solvents that do not react with sunlight to form smog and whose use is not controlled by regulation. A few chlorinated compounds are now considered exempt as well as acetone and methyl acetate. Review of the status of solvents in ongoing. • Middle solvent—A medium evaporation rate solvent that leaves the paint primarily during ﬂash-off and oven warm-up. • Tail-end solvent—A slow evaporating solvent that leaves the paint primar- ily during the baking cycle. • Retarder—A slow evaporating solvent added to a paint to prolong the drying time. Typically used to reduce orange peel or blushing. • Solvent blend—The particular mixture of liquids that gives a paint the desired ﬂow or evaporation properties. Skillful solvent blending allows a paint shop to adjust purchased paint for local variation in temperature, humidity, line speed, application equipment, and so forth. The selec- tion of a solvent system is often a complex task, best handled by the paint vendor. Important considerations in blending solvents are solvency, viscosity, evaporation rate, safety, and cost. • Solvency—The ability of the solvent to dissolve the binder. The solvent must be able to keep the binder in solution. • Evaporation rate—The solvent must evaporate within the time allowed by the curing schedule. Available oven length and temperature, as well as production volume is important. If the solvent is a mixture of two or more liquids, their individual evaporation rates become very import- ant. For example, if the solvent remaining on the workpiece should become excessively rich in diluent, the binder might come out of the solution as small sticky lumps, rather than the smooth even ﬁlm that is desired. • Viscosity—The ﬂuidity or ﬂow-ability of the paint. Paint viscosity is adjusted to provide good atomization and ﬂow-out.The proper solvent for a given task will depend on the required properties of theformula and other considerations such as safety and cost. Safety issues affect the solvents chosen for formulation. For example, naphtha-like hydrocarbons are very ﬂammable and chlorinated hydrocarbons are very toxic,so they must be used with extreme care.
70 Paint Technology Handbook Many times, the choice of a solvent system is dictated by simple economics. Thepurchase price of the solvent is not the only factor here. The cost of handling anddisposal must also be considered. These factors help account for the current interestin waterborne and powder coating systems. Solvents are volatile liquids added to paints to dissolve the binder (the resin com-ponent) and/or to modify the paint viscosity. The paint viscosity must be compatiblewith the storage and application methods. The solvent must have an evaporation rate that works well in the applicationenvironment. Ideally, the solvent should also be nontoxic, of low cost, and have anacceptable odor. The particular solvents that may work in a given formula will depend on theirsolubility characteristics. There are three classes of solubility: strongly hydrogenbonded, moderately hydrogen bonded, and weakly hydrogen bonded. Alcohols ﬁtinto the ﬁrst category; ketones, ethers, and esters into the second; and hydrocarbonsin the third class. The approximate ranges of these parameters for the various classesof solvent are given in Table 2.4. The above selection criteria are valid for solvents used for convertible binders.In nonconvertible coatings, solvents have more complex functions, contributing tothe coating application characteristics, the drying time, and the properties of the ﬁnalﬁlm. In this case, a blend of solvents is used to dissolve the binder and provide adiluent. The diluent may not be a true solvent for the binder, but it can increase thecapacity of the primary (or true) solvent to dissolve the binder. It also costs less thanthe true solvent so that its inclusion reduces the overall cost of the formulation. Resins used as paint binders have a range of parameter values that affect solventselection. The solvent and the binder must be compatible. Epoxy resins, which havea range of 8–13, are soluble in ketones, ethers, and esters but insoluble in hydrocarbonsand alcohols because the values are zero. If a coating needs to be solvent resistant, it will be formulated with a resin thathas a solubility parameter signiﬁcantly different from the solvent(s) that need to beresisted. TABLE 2.4 Solubility Parameters for Classes of Solvent (Hydrogen Bonding) Solvent Class Strong Moderate Poor Alcohols 11–13 — — Ketones — 8–10 — Ethers — 9–10 — Esters — 8–9 — Aliphatic — — 7–8 hydrocarbons Aromatic — — 8–9 hydrocarbons
Paint Components 71 Typically, compatibility of two or more resins in a coating requires that there isno more than one unit difference in the midpoints of their ranges. Usually, when selecting solvents for a particular resin, the solubility parametersof the solvents have to lie within the range of the resin. Other selection criteria includecost, paint viscosity, and drying time. A blend of diluent with the primary solvent willusually create a mixture with a mean that is within the mid-80% of the resin solubilityrange. The evaporation rate of a solvent is particularly important for nonconvertiblecoatings. Slow-evaporating solvents may cause long drying times and create problemsin batch coating operations or excessive ﬂow and sag of the wet ﬁlm. High evaporationrates may cause problems with ﬂow and ﬁlm integrity. Selection is affected by themethod of application. Typically, slower evaporation rates are required for brush-applied coatings while faster rates are used for spray methods. Some properties ofsome common solvents are given in Table 126.96.36.199.1 HYDROCARBON SOLVENTSAliphatic and aromatic hydrocarbons are commonly used to formulate and reducea paint material. They are complex mixtures of different compounds with differentﬂash points, density, and other properties.188.8.131.52 TolueneToluene is an aromatic hydrocarbon used in solvent blends for air-drying vinyl andchlorinated rubber coatings as well as a diluent in nitrocellulose paints. TABLE 2.5 Properties of Some Solvents Speciﬁc Boiling Evaporation Flash Solvent Gravity Point (◦ C) Ratea Point (◦ C) Acetone 0.79 56 944 −18 Butyl acetate 0.88 125 100 23 Butyl alcohol 0.881 118 36 35 Ethyl acetate 0.90 77 480 −4.4 Ethyl alcohol 0.79 79 253 12 Ethylene glycol monoethyl 0.93 135 24 49 ether (2 ethoxyethanol) Methyl ethyl ketone 0.81 80 572 −7 Methyl isobutyl ketone 0.83 116 164 13 Toluene 0.87 111 214 4.4 Mineral spirits 0.80 150–200 −18 38 (min) Xylene 0.87 138–144 73 17–25 a Evaporation rate values based on butyl acetate = 100; these values relate to pure solvents and will be lower where dissolved solids or diluents are present.
72 Paint Technology Handbook184.108.40.206 Mineral SpiritsMineral spirits are largely aliphatic (but containing 15–18% aromatics) blend of par-afﬁns of variable composition. They are slow-evaporating and dissolves most naturalresins, oleoresinous varnishes, and medium- and long-oil alkyd resins. Mineral spiritis commonly used as the main (often sole) solvent for brush-applied decorative andprotective paints based on these binders. It is also used as a cleaning and degreasingsolvent.220.127.116.11 XyleneXylene is an aromatic hydrocarbon widely used as a solvent for short-oil alkyd,chlorinated rubber, and polyurethane resins. The good solvating power and moderateevaporation rate permit xylene to be used for sag-resistant spray-applied coatings(even of relatively thick ﬁlms) as well as for baking-cured coatings.2.4.2 OXYGENATED SOLVENTSOxygenated solvents include alcohols, glycol ethers, ketones, esters, and glycol etheresters that are synthesized from other chemicals to form a desired solvent that istypically 99% pure.18.104.22.168 Butyl AlcoholButyl alcohol is a slow-evaporating solvent for a wide variety of oils and resins, par-ticularly amino and acrylic resins and also, in solvent combinations for nitrocelluloseresins.22.214.171.124 Ethyl AlcoholEthyl alcohol is usually used admixed with methyl alcohol, dyes, and toxins inthe form of industrial alcohol (methylated spirits). Ethyl alcohol, a fast-evaporatingsolvent, is used for poly(vinyl butyryl) as well as with other solvents for nitrocellulose.126.96.36.199 Ethylene Glycol Monoethyl EtherGlycol ether is a slow-evaporating solvent for many resins, which is often added tobrush-applied formulations that cannot incorporate aliphatic hydrocarbons such aswhite spirit. The high-boiling ethers are widely used as coalescing aids (solvents) inemulsion paints.188.8.131.52 AcetoneAcetone is a fast-evaporating powerful solvent used for vinyl copolymers andnitrocellulose. It is also blended (at low addition levels) with many othersolvents, when its high solvating power and evaporation rate modify the prop-erties of the liquid paint and the ﬁlm. They are treated just like water on theHEARS (Health, Environmental and Regulatory Services) program and will bereported as VOC-less exempt solvents.
Paint Components 7184.108.40.206 Methyl Ethyl Ketone (MEK)MEK is a powerful solvent with a fast evaporation rate, widely used for vinyl copoly-mers, epoxy, and polyurethane systems. It is often blended with less powerful solventsto modify the ﬁlm-forming properties and application characteristics of coatings.220.127.116.11 Methyl Isobutyl KetoneMethyl isobutyl ketone is a fast-evaporating powerful solvent used in similar applica-tions as MEK but where a somewhat slower evaporation rate is required. It is also usedat low addition levels in solvent blends where its fast evaporation rate and high solventpower will beneﬁt the properties of the liquid paint and ﬁlm-forming characteristics.18.104.22.168 Butyl AcetateButyl acetate is an ester solvent, with moderately fast evaporation rate, of generalapplicability. Formerly butyl acetate was the major solvent for nitrocellulose coatings;it is now used for a wide variety of synthetic resins but is less powerful than the ketonesolvents.22.214.171.124 Ethyl AcetateEthyl acetate is another ester solvent with rapid evaporation rate. The major applica-tion of ethyl acetate was formerly in nitrocellulose coatings, but it now has a somewhatwider application. It has a lower solvating power than the ketone solvents.2.5 ADDITIVESAdditives are chemicals added to paint, usually in small quantities, to achieve specialeffects. Although additives have been used in paints for centuries, it is not alwaysunderstood how they operate. Typical paint additives may be classiﬁed by their effecton the properties of liquid or dry paint. Additives can affect the paint material characteristics and the ﬁnished ﬁlm proper-ties. Examples of properties that can be adjusted with paint additives include viscosity,foaming, skinning, pigment dispersion, stability, ﬂexibility/hardness, gloss, UVresistance, ﬁre resistance, bacteria resistance, and many more.2.6 SUMMARYIndustrial paints are engineered products that include a variety of ingredients toproduce the desired results. The coating that works best for a given application isa balance between the needs of the ﬁnish and the cost of the coating. The speciﬁcrequirements for coating appearance and performance are very important to theselection process.
3 Liquid Organic CoatingsThe resins and other paint components that have been discussed in the previouschapter are used to provide properties to coatings for speciﬁc applications. Theseproperties are determined by the substrate to be covered, the end use for the product,and the environment in which the coating will be applied. There are a tremendous number of industrial and trade sales paints available.Paints are manufactured for industrial applications, building maintenance, housepainting, architectural steel, tanks, and bridges. This text is focused on industrialcoatings applied to manufactured durable goods.3.1 COATINGS SELECTIONVirtually any desired property can be built into the coating if the need exists.Ultraviolet light resistance, chemical resistance, impact resistance, glossy appear-ance, smoothness, and many more characteristics can be part of the formula. It isimportant to carefully deﬁne the needs of the end product to be sure that the coatingwill perform properly. Keep in mind that any special characteristics will probablyraise the cost of the paint. The primary factors to consider in choosing a coating are the task to be performed,(appearance or performance) and the environment the product will be used in.3.1.1 APPEARANCE • Gloss level—high, medium, low • Finish appearance—smooth, slight texture or orange peel, heavily textured or spatter coated3.1.2 PERFORMANCE • UV resistance • Corrosion resistance • Abrasion • Solvent/chemical attack • Hardness • Impact resistance3.1.3 OTHER FACTORS • Manufacturing abuses (forming, machining, or welding after coating) • Substrate to be coated: plastic, wood, steel, aluminum and castings 75
76 Paint Technology Handbook • Value of the product and cost per square foot applied • Exterior or interior use • Product life expectancy3.2 PAINT CLASSIFICATIONSThere are different ways to classify paint materials based on their formulations anduse. The speciﬁc task they perform, the physical type of paint they are known as, andother factors may be used to identify a particular product.3.2.1 PAINTS CLASSIFIED BY TASKPaints are often identiﬁed by the task they perform, such as primers, sealers, surfacers,and topcoats. Each type of paint has a different function.126.96.36.199 PrimersA primer is the ﬁrst coat applied to a surface. Its usual job is to ﬁght corrosion andenhance the adhesion of subsequent coatings applied over the primed surface. Mostindustrial primers are cross-linking or thermosetting type. The binder used in the primer must be compatible with the substrate and thesecond coat. Thus, different primers are required for wood, stone, metal, andplastic surfaces. Primers must be able to tolerate the differences in thermal expansionbetween substrate and paint. When primers are used for protection against corrosion, they are usually highlypigmented. They usually have relatively low gloss, because the primer particles extendup to the surface of the ﬁlm and give it a rough, pebbled texture. The best corrosionresistance is usually achieved at a pigment level near the critical pigment volumeconcentration (CPVC). Primer ﬁlm thickness is typically 1.0–3.0 mil. Primers for metal are frequently alkyd systems that cure by a solvent reac-tion mechanism. A typical industrial primer might have the following approximatecomposition, as sprayed: • Alkyd resin: 20%—binder • Pigment: 15%—for corrosion protection • Solvent: 60%—to liquefy • Additives: 5%—viscosity control, antifoam, and so forth In recent years, there has been a trend toward using epoxy-modiﬁed alkydbinders for primers. These resins have better adhesion and corrosion resistance thanconventional alkyds.188.8.131.52 Sealers and SurfacersSealers are paint ﬁlms applied between a primer and a topcoat to improveadhesion. This is often necessary if the primer and topcoat have different adhesive,
Liquid Organic Coatings 77thermal expansion, or impact resistance properties. When the interface between theseﬁlms is stressed, the layers sometimes separate, and the topcoat can then chip, crack,or break off. Sealers are also sometimes used to provide a barrier coat between a paint ﬁlm andthe solvent in a subsequent coat. This may be necessary if the pigment in the lowercoat has a tendency to bleed into the solvent of the upper coat. Sealers have special binders that stick well to both the primer and the topcoat.In addition, they are slightly elastic, acting as ﬂexible glue to hold the primer and thetopcoat together during periods of mechanical or thermal stress. Sealers are usuallylow in pigment. Typically, sealers are applied as thin ﬁlms less than 0.5 mil thickwhen dry. A surfacer is a coating used to ﬁll irregularities in the primer. Since primers areoften heavily loaded with pigment, they sometimes bake out with rough surfaces thatare difﬁcult to sand. A surfacer is designed to be sanded and provide a smooth surfacebefore topcoat application. The typical ﬁlm thickness for a surfacer is 1.0–3.5 mil.184.108.40.206 TopcoatThe ﬁnal layer of paint, the topcoat, is the one that provides the necessary appearanceand possibly improves performance. Topcoat may be applied as a single coat, or itmay be applied as more than one thin coat to achieve the ﬁnal ﬁlm build. Whenseveral coats are applied, it is not always necessary to completely dry each coat. Theﬁrst coat is allowed to ﬂash off before receiving the next coat. This is referred to aswet-on-wet application. The topcoat provides the surface with the desired color, gloss, abrasion resistance,and weatherability. Usually, the corrosion resistance of the topcoat is minimal.The highly pigmented primer is expected to provide most of the paint’s corrosionresistance. Many binders are used for topcoats. The ﬁnal choice of a topcoat usually requiresa trade-off among several properties (Table 3.1). In the automotive industry, forexample, it may be necessary to sacriﬁce some impact resistance to achieve thedesired gloss. TABLE 3.1 Comparative Properties of Common Paint Resins Moisture Chip Temperature Light Resin Resistance Resistance Resistance Stability Cost Acrylic Medium Low Medium High Medium Alkyd Medium Medium Medium Medium Medium Asphaltic High High Low Low Low Epoxies High High High Low High Urethanes Medium High Variable Medium High Polyester Medium Medium Medium Medium Medium
78 Paint Technology HandbookTABLE 3.2Characteristics of Waterborne FormulationsProperty True Solutions Colloidal Dispersions EmulsionsMolecular weight 15–50,000 20–200,000 Up to 1 millionViscosity Depends on molecular Depends on molecular Independent of weight weight molecular weightParticle size Molecules Less than 0.1 µm Greater than 0.1 µm% Solids Low Medium HighPhysical appearance Clear Hazy MilkyPigment stability Good Variable Variable3.2.2 PAINTS CLASSIFIED BY PHYSICAL TYPEPaints are also grouped by physical type such as high-solids, waterborne, or powdercoating. The following is a description and comparison of the most common types ofindustrial liquid coatings, high-solids, and waterborne coatings.220.127.116.11 Waterborne CoatingsWaterborne coatings are materials in which water is the major solvent or dispersant.The coating may be a true solution, a colloidal dispersion, or an emulsion. Thecharacteristics of these formulations are shown in Table 3.2. Waterborne paints contain 5–40% organic cosolvent to aid in wetting, viscositycontrol, and pigment dispersion. Some systems, especially emulsions, may alsocontain a polymeric thickener. Numerous resins are used for waterborne systems. Modiﬁed epoxies, polyesters,acrylics, alkyds, vinyl acetate-acrylics, and styrene-acrylics are available. Boththermoplastic and thermosetting (cross-linking) formulations are used. Some resinsystems cure when heated while others require the addition of a cross-linking agent.Advantages of Waterborne Coatings • Reduced ﬁre hazard (some are ﬂammable because of the organic cosolvent) • Reduced solvent emission • Lower toxicity • Use equipment similar to solvent sprayLimitations of Waterborne Coatings • Stainless steel or plastic pipe and ﬁttings are necessary • Some formulations must be protected from freezing • Better control of booth temperature and humidity is required • Longer ﬂash-off times are necessary • Requires better pretreatment
Liquid Organic Coatings 79 Waterborne systems are available for most substrates although some plasticsmay be difﬁcult to wet and have poor adhesion. Color, impact resistance, gloss,weatherability, corrosion resistance, and repairability characteristics of waterbornesare similar to conventional coatings. There are certain differences from conventional coatings that will affect theplumbing, tanks, booths, and pumps used with waterborne products. These differ-ences are important enough to inﬂuence the installation cost and ease of applicationof waterborne coatings. Pumps, tanks, and piping must be of noncorrosive material. Black iron systemswill corrode, so plastic or stainless steel is recommended due to the composition ofthe paint. Screens and ﬁlters are an important part of the paint distribution system,especially when emulsions are used, and they should be generously sized and regularlyserviced. Centrifugal pumps can be used, but positive displacement pumps give bettercontrol of pressure and ﬂow rate. Provisions should be made to keep waterborne coatings from freezing and toavoid storage above 90◦ F (32◦ C). The viscosity of many waterborne coatings istemperature sensitive, so paint heaters are often used to ensure good control of thisimportant variable. Spray booth air velocities for waterborne coatings can be lower than those used forsolvent paints, because they contain little toxic, ﬂammable, or bad-smelling solvent.This can provide savings in capital and operating cost. In some cases, booths mayneed to be longer than usual because of the slow evaporation rate of water. Linespeeds may have to be reduced for the same reason. Keeping the part surface and the spray equipment clean is particularly importantwith waterborne coatings, because they are less tolerant to oil and dirt. This is becausewater does not “wet” or “pick-up” these materials as readily as solvents. Even smallamounts of oil or grease, which might ﬁnd its way into tanks, pumps, or lines willnot mix with the paint and can cause surface defects on the parts. Dip systems and air spray systems are commonly used for the application ofwaterborne coatings. Electrostatic systems are less common. Since waterborne for-mulations are somewhat electrically conductive, it is necessary to isolate electrostaticsystems from ground to avoid loss of current through the supply line. Temperature and humidity control are more critical for waterborne coatingsthan for solvent paints, because water evaporates more slowly than many organicsolvents. The slow evaporation rate of water affects several areas of the system: 1. Longer ﬂash-off times are needed 2. Sagging and popping are more likely 3. Wet-on-wet coating may not be possible In areas where the humidity is very high for an extended period, it may benecessary to air-condition the spray booth to avoid excessive sagging or popping.Air pressure, wet-ﬁlm build, and gun-to-part distance may also require extra-closeattention.
80 Paint Technology Handbook The cure of waterborne coatings is similar to that of solvent paints. The liquidsin the ﬁlm must be driven off in a reasonable time and, in the case of thermosettingenamels, cross-linking is accomplished in an oven. Waterborne paints must have somewhat longer ﬂash time than solvent-basedpaints. Sometimes, it is also necessary to use a slower heat-up rate in the oven.If temperature is applied to the wet ﬁlm too quickly, it may cause popping. Since water from the paint may be corrosive, it is necessary to use rust resistantpanels in the oven and exhaust system. Once cured, waterborne ﬁlms are much like other coatings. Overbaking leads tocold-cracking and poor adhesion of subsequent coats. Underbaking means reduceddurability and lowered corrosion resistance. The repairability of the ﬁnished ﬁlm isrelated to the resin and additives in the paint rather than the fact that it is a waterborneformula.18.104.22.168 High-Solids CoatingsHigh-solids coatings are solvent-based paints that contain greater amounts of pigmentand binder than traditional solvent-based paints contain. At least 65% and as high as85% of the formula is solids content. Ultra-high solids paints may have an evenhigher percentage of solids. The much lower solvent content of high-solids paintsoffers some advantages over traditional materials.Advantages of High-Solids Coatings • Less paint must be shipped, stored, pumped, and sprayed compared to traditional solvent-based paint. • Lower oven-air volumes are required. • Less paint must be sprayed to provide a given ﬁlm build. • Booths may sometimes be shorter. • Less oven exhaust volume is necessary. • Less solvent is emitted to the atmosphere. This means less difﬁculty in meeting regulatory requirements.Limitations of High-Solids Coatings • High viscosity. Paints must often be heated to around 100–120◦ F to achieve sprayability. • High viscosity does not perform well in dip tanks or ﬂow-coaters. • Difﬁculty in pumping and atomizing, especially when cold. • Cleaning and phosphating quality may be more important than for con- ventional paints, because there is less solvent present to “clean as it coats”. • Sticky over-spray which is messy to clean up, because it remains in the uncured state.
Liquid Organic Coatings 81 High-solids paints are baking enamels. Alkyds are the most common resins usedfor high solids, but there are also polyester and acrylic products. Once the painthas been applied and cured, ﬁlm properties are essentially the same as for othersolvent formulations based on the same resin. Because of the high viscosities involved, high-solids paint lines are usuallyequipped with paint heaters. Heaters are usually located near the guns and are set tokeep the paint in the range of 110–150◦ F (43–95◦ C) with tolerance of a few degrees.The elevated temperature drops the paint viscosity enough so that good atomizationis possible. Most spray guns can handle the additional air pressure required for breaking uphigh-solids paints. However, the capacity of lines, pumps, and ﬁlters may have tobe increased to ensure trouble-free performance. Pressure-feed pumps are usuallyrequired. Paint agitators should be of low-speed, high-torque design rather than theother way around. Since high-solids paints are heavy (up to 360 kg or 800 lb per barrel), it may benecessary to increase hoist and forklift capacities. Cure oven exhaust volumes can be lower than conventional solvent-basedcoatings, because there are less volatile gases in the oven. Filters and ﬂoor papers may need to be changed more often and they are difﬁcultto handle due to the fact that the material may not air-dry. High-solids coatings are applied with air, airless, conventional, or electrostaticspray. Electrostatic disks and bells are also commonly used. Atomization with thesedevices is usually excellent at speeds of at least 25,000 rpm. Film buildup of less than 12.5 µm (1/2 mil or 0.0005′′ ) are possible with 15–30 cm(6–12′′ ) discs. Film builds up about twice as rapidly with high-solids paints as it doeswith conventional products, so there may be an initial tendency to apply too muchpaint. Overspray can be a real nuisance, since it contains about twice as much solids asconventional paint. Like all liquid coatings, it is important to control the application process and usethe right equipment to reduce overspray. Fluid and atomizing pressures, ﬂuid tips,and air caps should be carefully chosen to maximize application efﬁciency. Some equipment modiﬁcations and operator retraining will be required whenconverting to higher solids coatings. Larger diameter lines and more powerful pumpsare the most common changes required. The cure of high-solids coatings is similar to conventional enamels. Thirty minutesat 300◦ F (150◦ C) is typical although cure schedules can vary considerably. No specialovens are required for high-solids coatings. Before the paint can be applied, it must be prepared and set up for delivery to thespray system. Good paint preparation and system set up can help to avoid applicationproblems. When the paint container is ﬁrst opened, the paint should be checked visually forkick-out. Kick-out refers to the binder coming out of solution as small lumps of softor hard material. Sometimes, the process can be reversed by agitation, but in manycases the paint is no good. Kick-out results when the binder and solvent are no longercompatible.
82 Paint Technology Handbook The paint should be thoroughly mixed so that there is no separation of theingredients. Normally, over the course of time, the paint solids will tend to settleto the bottom while the solvents will rise to the top. If applied unmixed, an unevenﬁlm will result with differences in ﬁlm properties. In small batches, the paint can bestirred and in larger operations it is mixed with a powered agitator. To avoid applicationproblems and surface defects, it must be blended to consistent, uniform viscosity. Proper paint viscosity is critical for obtaining a quality ﬁnish. Viscosity is theresistance to ﬂow exhibited by ﬂuids, a result of the internal friction of moleculesagainst each other during movement. In conjunction with air and ﬂuid pressure,viscosity controls the size of the paint droplets when the paint is spray-applied. Excessive viscosity can cause orange peel while a low viscosity can create a ﬁlmthat is too “wet” and creates runs. A general rule of thumb for application viscosity is20–25 s on a #2 Zahn cup for conventional air spray and 25–40 s for airless application.However, the product data sheet should always be referred to before application. Forhigh-solids paints, the spray viscosity is usually between 13–20 s on a #3 Zahn cup.Materials and applications vary widely, so viscosity adjustments should be madeaccording to the manufacturers’ recommendations. The viscosity of the paint should always be checked before and during application.An important factor in checking viscosity is the temperature of the paint. Signiﬁcantchanges in viscosity will occur with relatively small changes in temperature. Forexample, a coating that has a viscosity of 40 s on #2 Zahn at 70◦ F could drop to 25 sat 90◦ F. Viscosities should always be tested at 77◦ F (25◦ C). Viscosity is measured with a viscosity cup and a stopwatch. Viscosity is expressedin terms of seconds of time it takes to ﬂow through the cup that has been ﬁlled toa speciﬁed level. To take this measurement, the cup is immersed in the paint, ﬁlled,and then withdrawn. When the cup is withdrawn from the liquid level of the paint,the stopwatch is started. Paint will ﬂow out of the oriﬁce in the bottom of the cup.The watch is stopped when a deﬁnite break in paint ﬂow is seen. Viscosity is sometimes lowered by reduction with solvent. In some cases, a com-pliant coating may be delivered ready to spray. Reduction of compliant coatings willreduce the solids content as sprayed and may constitute a violation of an air qual-ity permit. In some cases, it is best to have the coating supplier adjust the materialviscosity to make sure that it is not out of compliance. The relationship of viscosity to temperature can be problem if the spray areadoes not have climate controls. The plant temperature and humidity will change withthe seasons and time of day. This can affect paint viscosity and paint cure charac-teristics. Different solvent blends may be needed to provide the proper cure duringdifferent seasons. Temperature control of the paint can provide the paint consistencyneeded to maintain proper application viscosity throughout the day. This temperaturerelationship is illustrated in Figure 22.214.171.124 FILM FORMATIONThe resin is the primary ingredient of an organic coating, the part of the coatingthat forms a ﬁlm when it dries. The resin is mixed with other ingredients to create an
Liquid Organic Coatings 83 70 Viscosity seconds #2 Zahn 60 50 40 30 20 10 50 60 70 80 90 100 110 120 Paint temperature (°F)FIGURE 3.1 Paint viscosity at different temperatures.engineered product for application. As the coating is applied, it will ﬂow and stabilizeinto a relatively uniform ﬁlm. This stage is referred to as ﬁxation. After the coatinghas stabilized, it will be cured by time, temperature, or some other means.3.3.1 APPLICATIONApplication is the spreading of the composition into a thin layer over the surface of aproduct. Many methods of application can be used including a brush, a roller, a spraygun, curtain coating processor, or electrodeposition system. The method of application and effective process control will determine the thick-ness of the coating, uniformity, and efﬁciency. The application equipment and set-upmust be compatible with the particular viscosity and ﬂow characteristics of the coatingto provide uniform and consistent results.3.3.2 FIXATIONDuring ﬁxation, the coating is stabilized so that it will not run off or form an unevenlayer on the painted surface. Fixation usually occurs by evaporation of volatile solventfrom an organic solvent system or of water from a latex system. Rheological resistanceto ﬂow grows within the ﬁlm as the nonvolatiles concentrate. Fixation may also resultfrom thixotropy built into the paint by the formulator. An ideal liquid paint would be free ﬂowing during application, ﬂow evenly overthe work surface, stabilize quickly, and remain in place. In reality, there is a timeinterval between the ﬂowing and the nonﬂowing states. A paint material may neveractually be completely free ﬂowing. In many cases, some resistance to ﬂow has to bebuilt into the paint to avoid sagging on the work surface. Several conditions affect the formulation for ﬂow. • The solvents used must have sufﬁcient dissolving power for the resin in the paint.
84 Paint Technology Handbook • The desired ﬁnal dry-ﬁlm thickness and the number of coats. • The amount of surface texture that can be tolerated. The behavior of the ﬁlm is affected by the rate of evaporation of the solvent mixand the rheology built into the paint.126.96.36.199 The Evaporation FactorSome house paints that are formulated with raw and modiﬁed vegetable-type oils arelow enough in viscosity to be free ﬂowing without solvent addition. However, mostother coating compositions need solvent to ﬂuidize the solid resins in the binder. Thesolvents used to blend the coating evaporate at different rates during application anddrying. In the simplest model, evaporation takes place through at least two mechanisms.One is solvent evaporation from the surface of the ﬁlm that is similar to the samefactors as evaporation from the surface of the pure solvent by itself. The other is solventdiffusion from within the body of the ﬁlm from the lower depths to the surface. Therate of solvent evaporation can affect ﬁxation. Some problems can occur during solvent evaporation. The rapid cooling effectthat occurs as solvent evaporates from the applied ﬁlm will also cool water vaporin the atmosphere around the paint ﬁlm. If its vapor pressure is higher than thesaturated vapor pressure of water at the surrounding ambient temperature, it willcause condensation on the paint ﬁlm. The condensed moisture is trapped in the coatingwhere it can cause a white discoloration called solvent-blush. Another problem sometimes experienced during spray application is dry spray.If a particular solvent evaporates in the atomized paint stream before it reaches thesurface of the part, it may affect the ﬂow-out of the coating and create a grainyappearance. Dry spray is often caused by problems with spray technique (gun too farfrom target), but it can also be a result of using the wrong solvent or the incorrectvolume of a particular solvent.188.8.131.52 RheologyEven a material with high viscosity will tend to ﬂow downward on a vertical surface.A paint material needs some physical structure to prevent sagging. Finely dividedpowders that make up the pigments and extenders in the paint can provide physicalstructure through thixotropy. When stirring causes a temporary decrease in viscosity, the paint is said to bethixotropic. The more vigorously a thixotropic paint is stirred, the less viscous itbecomes. The viscosity will go up again if the stirring is stopped. Thixotropy is often due to reversible ﬂocculation of pigment. If the pigmentﬂocculates without settling, the network of loosely associated particles resiststhe movement of a brush or stirring paddle. As the brush or paddle is forced throughthe liquid, the ﬂocculated structure breaks down and allows the liquid to ﬂow moreeasily. Once the stirring has ceased, the particles again form a network in the container.The network restores “body” to the paint and the viscosity increases.
Liquid Organic Coatings 85 When mechanically disturbed, such as agitation during application, a thixotropiccomposition thins out to become comparatively free ﬂowing. Left in an undisturbedstate, it will build up structure over time. The time, depending on the actual com-position, may be a fraction of a second, minutes, or even hours, and the ultimatelevel of structure may be low or high. Thixotropy may therefore be harnessed toprovide a nearly ideal coating, free ﬂowing during application but rigid immediatelythereafter. A coating needs to be uniformly mixed to perform properly. There are otherconditions commonly encountered in a coating where ingredients separate due toﬂocculation, settling, or kick-out.184.108.40.206 Flocculation and SettlingFlocculation is the formation of loose clusters of pigment particles in a liquid paint.A certain amount of ﬂocculation is desirable in a paint, because it gives the liquidmore “body” than what it has with isolated pigment particles and helps resist sagging.Flocculated pigments that have settled to the bottom of the paint container may some-times be successfully blended back into the material unless they form hard, compactlayers.220.127.116.11 Kick-OutThe term “kick-out” refers to the binder coming out of solution as small lumps ofsoft or hard material. Sometimes the process is reversible, but more often the paint isruined. Kick-out results when the binder and the solvent are no longer compatible. Thebinder may kick-out if the wrong thinner is used. Kick-out usually occurs becausea paint is too old and the binder has chemically changed to the point where it isincompatible with the original solvent blend. This is one reason why the oldest paintin stock should be used ﬁrst.3.3.3 CUREFixation is followed by cure. Fixation and curing may be combined or overlapped.Common lacquers combine ﬁxation and cure in the evaporation of solvents during andafter application. A catalyzed paint material begins to combine ﬁxation with curing. Some coatings are in or near their ﬁnal state of cure when they complete the ﬁxationperiod. Lacquers are a broad group of coatings that cure by solvent evaporation alone. Many coatings need thermal energy or light energy to cure. Thermosettingproducts are very common for industrial applications.18.104.22.168 Air DryIn an air-dry coating, the formulator sets the period of cure with the proper blend ofdrier catalysts. As a rule, the oxidation process does not start as soon as the paintis spread and exposed to the air. An introduction period is involved, after which theunsaturated vegetable-type acid esters in the paint start to absorb oxygen to create
86 Paint Technology Handbookchemically reactive sites in the constituent molecules. These molecules combine toform larger molecules, which result in a paint ﬁlm. Actually, the drying process never stops. It slows down greatly and must becontrolled to avoid the ultimate formation of an excessively brittle ﬁlm. An increase in temperature will increase the rate of the chemical reaction. Curingprocesses that take place at normal temperatures do so much faster under the inﬂuenceof heat.22.214.171.124 Catalyzed MaterialsCatalyzed materials have two major or more constituents that will begin a curingreaction when they are mixed together. The cure time varies and temperature may vary,but is possible to reach full ﬁlm properties, even at room temperature. Application ofheat will accelerate the cure cycle. Obviously, the coating components are separately packaged until they are blendedfor application. A catalyst may be added, if it cannot be included in one of thecomponents. Catalyzed materials are typically very durable coatings. One example of a two-component coating is the epoxy-polyamide system. Epoxyresins are chemically reactive oxygen atoms that are bound in the molecule to twoadjacent carbon atoms to form a three-part ring. Such rings are sensitive to a numberof other reactive groups. The polyamide resins are low-molecular-weight relatives ofthe nylons. Their amide groups can tie up rapidly at room temperature with epoxygroups to form large, bulky molecules that are excellent binders in coatings.126.96.36.199 Baking EnamelsSome coatings do not cure at room temperature and fortunately remain stable in thepaint container for extended periods. They convert rapidly (in a fraction of an hour)when exposed to heat. Typical temperatures for baking enamels range from 280 to350◦ F (135–175◦ C) for 10–30 min. Amine resins are one of the many convertible coatings of this type. Broadly speak-ing, they divide into urea–formaldehyde derivatives and melamine–formaldehydederivatives. When heated, these products can become brittle, so many common bakingenamels are formulated with plasticizers, such as alkyd resins. High molecular weight variations of certain resins are tougher and more dur-able but unfortunately much less soluble than their chemical counterparts of lowermolecular weight. Therefore, even though they would provide excellent ﬁnishedﬁlms, these high molecular weight materials cannot be dissolved in solvents. These high-molecular-weight resins in ﬁne powder form can be mixed with pig-ment and with a nonvolatile liquid to yield a tough, durable coating. The nonvolatileliquid serves as a plasticizer for the resin. When it is heated, the resin will softenand create a matrix that includes the plasticizer and the pigment. These materialsare called plastisols and are commonly based on high-molecular-weight polyvinylchloride and related polymers. This is cure by fusion. If the plastisol mixture is too high in viscosity to be properly applied by theselected method, it may be thinned with a minor amount of solvent for the plasticizer.
Liquid Organic Coatings 87These variations are called organosols. After the solvent evaporates from the ﬁlm, thecure is also by fusion. A coat of latex paint dries in two stages. First, the water evaporates and all theingredients, other than the latex globules, are concentrated in the space between theglobules. These become more closely packed in a geometric array and ultimatelytouch each other. The ﬁlm at this juncture has no particular strength and may beeasily wiped away. Second, if a latex ﬁlm is warmed sufﬁciently, the globules will sinter at theirpoints of contact and form a hardened coating. Of course, it is not practical to applyheat to paint on a wall. Fortunately, it is possible to design latex compositions thatcoalesce at ordinary ambient temperatures. It is possible to create latex-based systemsin which coalescence does not take place in the bulk package in storage but proceedssmoothly once the coating has been applied as ﬁlm. Cure is a relative term. What may be an adequately cured ﬁlm for gentle hand-ling may still be raw in respect to solvent attack. Many methods are available fortesting the degree of cure. The individual end use will dictate the most appropriatemethod.3.3.4 DRY FILM PROPERTIESOnce the paint is cured, the concern switches to dry ﬁlm properties. In somerespects, the properties of a dry paint ﬁlm are the most important of all since itis the dry ﬁlm, which is exposed to the service environment and to the customer’sinspection.188.8.131.52 GlossA high-gloss surface reﬂects nearly all of the light that falls upon it. Reﬂection of morethan 90% of the incident light is possible with modern industrial ﬁnishes. High glossrequires a smooth surface. Surface roughness results in scattering of incident light andlow gloss. Smoothness can be obtained by polishing or by using processes that allowthe paint to dry smoothly without cracks, wrinkles, pinholes, or protrusions. Highlypigmented paints often have low gloss, because pigment particles extend through thesurface and reduce smoothness. Gloss can be manipulated by addition of ingredients that provide hazing to reducereﬂection or smoothness to increase reﬂection.184.108.40.206 Hiding Power (Opacity)The ability of a paint to cover a surface and mask it from view is referred to as hidingpower. Since most paint binders are transparent, the job of hiding the surface fallsprimarily to the pigment. Pigments contribute to hiding power in three ways. Theymay reﬂect, refract, or absorb the light that enters the paint ﬁlm. With reﬂection and refraction, the light is turned back out of the ﬁlm before itreaches the painted surface. Figure 3.2 illustrates reﬂection, refraction, and absorptionby a paint ﬁlm.
88 Paint Technology Handbook A B C D E A: Reflected at the surface; B: Reflected by the pigment; C: Absorbed by the pigment; D: Refracted by the pigment; E: Reflected by the substrateFIGURE 3.2 Light behavior on a painted surface.220.127.116.11 ColorThe color of a paint material is primarily due to the pigment interaction with light.Ordinarily, white light is composed of all the colors visible to the human eye. Pigmentshave the ability to absorb some of these colors and reﬂect or transmit others. The paintﬁlm will be the color of the reﬂected or transmitted light. Therefore, the pigment ina red paint absorbs all colors except red. Pigments can be mixed to give colors different from the pigments themselves.Awhite pigment is often added to a paint to give a lighter color. The difference betweena light and a dark blue is often the presence of white titanium dioxide particles in theﬁlm with dark blue pigment.18.104.22.168 Strength, Hardness, and BrittlenessThese terms describe important properties of a dry paint ﬁlm. They depend on howeffectively the binder molecules, pigment particles, and additive materials attract oneanother. When there is high attraction between components of a paint material, theﬁlm will be strong, hard, and able to resist bending and stretching. This is not alwaysdesirable. Such strong, hard ﬁlms may not be able to bend or stretch and recoverunder ordinary use conditions. The paint must have some resiliency or stretchiness,because the solid surface under the ﬁlm may shrink and expand due to temperaturechanges in the surrounding atmosphere. Brittleness is the tendency to crack under impact. Paint is brittle when it cannotdeform in response to a mechanical stress. This inability to deform, results fromexcessively high attractions between the paint components. The degree of attraction between the binder and the pigment can be controlled bythe nature of the materials themselves and by the use of additives. Paint binders may be linear or cross-linked. Linear binder molecules are like ran-domly intertwined strands of spaghetti. They are generally softer, more ﬂexible, lessbrittle, more soluble, more water permeable, and less heat resistant than cross-linkedbinders. Cross-linking means that the linear, threadlike binder molecules have becomelaterally bonded together at various positions along their length. The resulting 3-Dnetworks are usually stiffer, harder, more brittle, less soluble, less water permeable,and more heat resistant than linear binders are. Binders are often classiﬁed on the basis of their heat behavior. Linear bindersthat can be melted are called thermoplastic. Cross-linked binders that do not melt are
Liquid Organic Coatings 89called thermosetting. Most primers and many industrial topcoats have thermosettingbinders while sealers and some topcoats are linear binders. A high degree of pigmentation gives strength and stiffness to a paint ﬁlm. Thisis because the pigment particles can act as a load-bearing part of the ﬁlm and alsobecause the particles resist movement within the ﬁlm. Another means of controlling strength, hardness, and brittleness is by the use ofadditives. Plasticizers weaken, soften, and decrease the brittleness of a paint ﬁlm.They are small molecules that are thoroughly mixed throughout the ﬁlm and separatethe binder molecules and pigment particles from themselves and from each other. Thisseparation reduces the attractive forces between the paint components and providesa more ﬂexible, softer, less brittle ﬁlm. Because plasticizers are small molecules,they have a tendency to slowly evaporate from the ﬁlm over a period of monthsor years. The result is that many paints tend to become harder and more brittlewith age.22.214.171.124 Depth of Color (Metal-Flake Paints)Some industrial paints are formulated to give an appearance of depth. Automobilesare usually ﬁnished with metallic coatings designed for depth of ﬁnish. The depth-of-color look comes from small metal ﬂakes scattered throughout the paint. Theseﬂakes, which are usually aluminum, reﬂect light back to the surface and out of theﬁlm. Although the ﬂakes are too small to see individually, they give the effect oflight coming from various depths within the ﬁlm. The paint will have a dazzling orsparkling appearance.3.3.5 HOW PAINT WEARS OUTAll paint ﬁlms are semipermeable layers that are susceptive to wear. Exposure tothe atmosphere, physical abuse, sunlight, water, corrosives, and general wear willcause discoloration, loss of gloss, cracking, chipping, or peeling from their sub-strate. The three greatest natural enemies of a paint ﬁlm are sunlight, moisture, andtemperature changes. 1. Ultraviolet radiation degrades the binder molecules by breaking bonds between atoms. 2. As binder molecules shrink, ﬁlm strength declines and moisture penetration increases. 3. With temperature cycling, the moist paint ﬁlm is ﬁrst heated and then cooled. The accompanying expansions and contractions put a strain on the ﬁlm that is poorly resisted, because the binder molecules are now smaller and mechanically weakened. 4. The weakened ﬁlm surface is now subject to mechanical rub-off and water wash-off. 5. As the unpigmented surface ﬁlm wears away, the pigment particles become exposed to the elements. Continued degradation of the binder may actually set the pigment mechanically free, at which point the paint begins to chalk.
90 Paint Technology Handbook 6. Once exposed to sunlight and moisture, many pigments begin to fade and lose gloss. 7. These changes occur because of a gradual loss of plasticizer from the ﬁlm that makes it more brittle. The stiffening ﬁlm is less able to resist the strain of thermal expansion and contraction. Microcracks form and allow moisture to penetrate. This exerts a lifting pressure when warmed by an increase in the surrounding air temperature.Water can more easily penetrate a weakened ﬁlm. The overall result is that the paintﬁlm gradually erodes away.
4 Paint Manufacturing ProcessWhen paint was ﬁrst discovered in ancient days, it was produced by mixinga natural resin from a plant or tree with natural colorants from the earth or plants.The ingredients were mashed together in some type of container. It was not verydurable, but it allowed people to create art and illustration. Modern paint manufac-turing is much more sophisticated, but it still involves a blending process to dispersepigment into a vehicle system. The vehicle system, typically a resin or a varnish type material, is ﬁrst chargedinto a mill with thinner and grinding aids. Pigments and extenders are added. The millis then operated until the pigment particles are broken down and uniformly dispersedto create a grind paste. The grind paste is extended with additional resins and thinnerand dropped into a thin-down tank. There, other materials are added to the tank tomake the ﬁnished product. At this point, a sample of the material is brought into thequality control laboratory and a number of tests are conducted to compare the batchversus the standard parameters it is designed to meet. Trained technicians evaluatethe results and then make adjustments for color matching and other characteristicssuch as viscosity and gloss. In addition to the normal adjustments made to batches,quality checks are performed throughout the manufacturing cycle. When the paint in the tank meets all the prescribed speciﬁcations, quality controlapproves it for ﬁlling. The paint is then ﬁltered to strain out any large or unwantedparticles and ﬁlled into containers. The most critical operation in the manufacturing process is the paste grindingprocess. This is where the solid pigments are broken down into their ﬁnest particlesize in the resins, solvents, and additives (the vehicle system).4.1 EQUIPMENT USED FOR PIGMENT PASTE MANUFACTURINGThe equipment used to grind the pigment is an important part of the process. Differentmills work well with different pigment materials.4.1.1 HIGH-SPEED MIXERS (HSD, HLM)Among the different types of mills used for grinding, the most widely used is thehigh-speed disperser (HSD). This mill consists of a tank that is jacketed for coolingwater, a motor, and a shaft with an impeller that resembles a saw blade with teeth thatare bent 90◦ . 91
92 Paint Technology Handbook The dispersion is achieved at or near the surface of the impeller by the violentchanging of direction of the mill paste. This shearing action is used to handle easilydispersed pigments such as those found in whites and light pastel colors. An HSD is used in conjunction with the continuous mill (COM) to premix themill paste. Both the sand mill and COM are used for the more difﬁcult dispersingpigments such as those found in blue, green, and red colors. These mills use a variable speed saw-tooth blade rotating at high speed. Peripheralspeeds range from 3000 to 6300 ft/min. HLM mixers also have a slow speed sweepagitator at the tank wall to aid in movement from the tank walls. • Critical parameters: paste viscosity, RPM of shaft, and level of paste in the tank (optimum range 2.0–2.5 times blade diameter) • Advantages: requires least amount of labor, easy cleanup, and low maintenance • Disadvantages: high power consumption, easy dispersing pigments needed, and generates heat • Typical products: latex, some primers, plastisols, high solids polyesters, polyurethanes, and acrylics4.1.2 VERTICAL OR HORIZONTAL CONTINUOUS MILLAnother device is a COM. It is also charged with glass or ceramic media and dispersesby shear and attrition. In this case, the degree of dispersion is determined by the ﬂowrate of the premixed paste through the COM. These mills have a high-speed shaftwith multiple discs of various conﬁgurations rotating in a long chamber ﬁlled withbeads. • Critical parameters: high-throughput rates, easy to clean, low yield losses, and large batch size • Disadvantages: requires premix tank, expensive to maintain, and cannot grind tougher pigments in one pass • Typical products: primers, polyurethane, water reducible (W/R) primers, clean colors, alkyds, and lacquers4.1.3 SAND MILLAnother type of grinding device is a sand mill. It uses a different type of impeller,and it is charged with glass or ceramic as a grinding media. Pigments are ground byshear and attrition and the ﬁnesse of the dispersion is determined by the length oftime the paste is in the mill, or residency time. This mill consists of a high-speed shaftwith one or two solid disc impellers rotating off center in a cylindrical tank with acone-shaped bottom, ﬁlled with small grinding beads. • Critical parameters: ratio of paste volume to media volume and paste viscosity; impeller speed = 3500 ft/min • Advantages: can grind most pigments, low maintenance
Paint Manufacturing Process 93 • Disadvantages: batch operation—requires many mixes, slow discharge, yield loss high, and cleanup is difﬁcult • Typical products: high-solids polyesters, plastisols, water-based baking enamels, alkyds (light colors), and lacquers (light colors)4.1.4 ROLL MILLA roll mill, another milling device, can use two or more rollers to blend the paintingredients. The material to be milled is placed between the feed and center rolls.Each adjacent roll rotates at progressively higher speeds. For example, the feed rollmay rotate at 30 rpm, the center roll at 90 rpm, and the apron roll at 270 rpm. Materialis transferred from the center roll to the apron roll by adhesion. The dispersion isachieved by the shear forces generated between the adjacent rolls. The milled materialis removed from the apron roll by a knife that runs against the roll. • Critical parameters: roll pressure, roll clearance, paste viscosity, and tack • Advantages: can grind concentrated pastes with high polyvinyl chloride (PVC) loadings, no wash needed, very ﬁne dispersions obtained, and no metal contamination • Disadvantages: requires premix operation, slow process, and expensive to maintain • Typical products: electrodeposition paste, high-solids polyesters, alkyds, and acrylics4.1.5 BALL MILLOne of the older types of milling equipment that is still used is the ball mill. Thismill consists of a cylindrical tank mounted horizontally. It is loaded to one-third ofits apparent volume with 5/8′′ steel balls as a grinding media. There are lifter barslocated on the inside wall of the mill and as the mill rotates the balls are lifted andthen cascaded downward, dispersing the pigment by attrition and shear. These millsare used for the most difﬁcult pigments to disperse such as blacks and organics. • Critical parameters: ball charge = 33% of mill volume; normal paste charge = 25–40% of mill volume • Advantages: no premixing required, no solvent loss, low maintenance, and can handle hard grinding pigments • Disadvantages: long grind times, limited batch size, discoloration from metal, yield losses, and difﬁcult to clean • Typical products: primers, high solids polyesters, alkyds (dark colors), acrylics (colors), acrylics (colors), and lacquers (dark colors)After the paint is milled, it is ﬁltered and put into containers. Filtration methods vary,depending on the paint material and the needs of the customer.
5 Color Matching and Color ControlThe appearance of a ﬁnished product is often one of the most critical aspects of quality.The way it looks has a signiﬁcant psychological impact on the perception of qualityby the potential customers and on their willingness to buy the product. Color is themost important appearance attribute of an object. There are other attributes such assize, shape, gloss, and texture, but color is by far the most important. Color, gloss, and texture are imparted to a product by a coating. The coatingmanufacturer has the responsibility for formulating an accurate color match basedon the customer’s sample. The applicator also plays a role in accurate color match,since mixing, storage, application, and curing can impact color. It is necessary for themanufacturer to have a quality control program for the desired color and appearanceof their product. But it is equally important to be able to detect all sources of errorthat affect color and appearance. Color match is usually judged by visual evaluation in standard lighting. Somewill use color difference measurement devices as well. An inspector will compare thecolor of the product to a color standard sample. If there is some color difference, it will be necessary to judge if it is within accept-able tolerance levels. When there are guideline panels that represent the maximumallowable color difference limit, the task is a little less difﬁcult. Any difference ingloss or texture will further complicate the visual process, because the color matchwill vary as the angles of view and illumination vary. Usually, the coating is checked for color by the quality control lab before thecustomer uses it. A number of sources of error can cause a poor match.Examples of sources of error: 1. Different color standard 2. Metameric color standard 3. Metameric batch 4. Gloss difference 5. Texture difference 6. Observed metamerism 7. Panel preparation differences 8. Substrate differences 9. Film thickness variance 10. Disagreement between color measuring instruments In addition to these items, it is possible that the paint needs to be adjusted foraccurate shading. 95
96 Paint Technology Handbook A color difference measurement can provide accurate numerical color match ordeﬁne a difference from the speciﬁcation. When measurement equipment is not used,it is hard to describe the visual difference and make an adjustment.5.1 COLOR VARIABLESColor has three visual variables: hue, saturation, and lightness. Hue is a color variabledenoted by red, orange, yellow, green, blue, violet, and purple. Saturation is thevariable of color that denotes its purity or its degree of departure from grayness.Lightness is the variable of color that distinguishes black from white, without regardto hue, as represented by a neutral gray scale ranging from black to white. Hue, saturation, and lightness are often called the three dimensions of color,because it takes a three-dimensional space to represent them. Lightness is distancealong the vertical axis, saturation is radial distance away from the vertical axis, andvariation in hue is angular distance around the vertical axis. Color matching is the process of selecting colorants to match a given color andadjusting their concentrations until the hue, saturation, and lightness of the trial (batch)match the hue, saturation, and lightness of the given color sample. Knowing that color has three variables, leads to the four-colorant principles ofcolor matching. To match a color, hue, saturation, and lightness must be adjustable orcontrollable and can only be done with a minimum of four colorants. For example, ifonly one colorant—white—is used, there is no way to change it. It can only be white.By adding black as a second colorant and varying the concentration of the white andblack, any number of colors, varying essentially only in lightness can be made. Byadding a third colorant, for example red, any number of colors can be made, varying inlightness and saturation but all having essentially the same red hue. By adding a fourthcolorant, yellow, then all three color variables—hue, saturation, and lightness—canbe varied, and a color can be matched exactly. If a color is formulated with less than three, then the match can only be obtainedwhen all of the colorants are exactly as they were originally. There is no latitudefor production variation. If more than four colorants are used, then it becomes moredifﬁcult to determine which colorant will correct a hue difference, a saturation differ-ence, or a lightness difference, because two colorants in a ﬁve-colorant formula willcontrol the same variable. For example, a green made with white, black, blue, and twodifferent yellow pigments, needs to be more yellow. Which yellow is added? Someyellow pigments will make it more yellow but also less saturated. Other unsaturatedpigments may be more effective in correcting the hue without affecting the saturation.To correct the hue, the effect on saturation must be considered.5.2 METAMERISMAnother reason why a ﬁve- or more-colorant formula should not be used is metamer-ism. Metamerism is when the colors match under one set of illuminants, observer,and viewing conditions, but do match under another. To prevent this, the matchmust not only contain the same colorants but also the concentration must be
Color Matching and Color Control 97the same. In a ﬁve or more colorant formula, it is almost impossible to producebatches repeatedly, with the colorants at the same concentrations. Color may notalways be controlled. A four-colorant formula is unique, because only one set ofconcentration of the colorants will produce a match and therefore no batch-to-batchmetamerism is possible. When matching colors by the visual approach, the color matcher selects thecolorants by trial and error, experience, and knowledge of subtractive color mix-ture. It does not take long to learn that mixing blue and yellow together can makea green color. Colorant adjustments are made until the appearance is correct. Blue,black, or some other color is added until a match is made. A quantity of a colorant isadded and the change in color is evaluated. If more is needed, the amount is estimatedby that change. This process is repeated until a satisfactory match is obtained. Withgood technique and accurate weighing of colorants, an experienced color matchercan make a match fairly quickly. The problem with the visual approach is that the matches may be metameric,which may or may not be acceptable. The metamerism occurs because the colorantsused are different from those that were used to produce the color sample. There are three types of metamerism: illuminant, geometric, and observer.Illuminant metamerism is what is normally thought of when the word metamerism ismentioned, a change of light that causes a change of color. Geometric metamerism is when the colors will match only at a certain angle ofviewing and illumination. This is caused by difference in gloss and/or texture. A ﬂatcolor will only match a gloss color at one viewing angle. Observer metamerism is when colors are a match for one observer and not foranother. It is caused by differences in the color vision of the observers and is quiteevident when illuminant metamerism also exists. When there is difﬁculty in gettinga match accepted by a customer, it may very well be observer metamerism. Dr. Henry Hemmendinger is a leader in understanding the breakdown of a colormatch by change of either illuminant or observer. Hemmendinger and Davidsondeveloped the D&H Color Rule, a device to quantify the extent of observer meta-merism, which is still viewed as an indispensable aide in teaching the principles ofobserver metamerism. Dr. Hemmendinger, also developed methods to use metamericpairs as tools to assess instrument performance. An observer can readily get a matchwith highly metameric samples. The pairs chosen are noted and compared to the pairschosen by another observer. If the pairs are the same under the same light source,the observers have the same color vision. If the pairs appear different under the samelight source, it indicates a difference in color vision between the observers. Visual color measurement is done in a light booth such as a Macbeth Spectralite.This light booth provides three light sources that are commonly used to visuallyevaluate color and color differences. They are North Daylight, Incandescent, andCool White Fluorescent (CWF). The International Commission on Illumination (ICI)has standardized on North Daylight and Incandescent and given them the designationsilluminant D65 and illuminant A, respectively. CWF has no standard as yet. The important feature about the booths is that they supply a light source thatis constant. Natural daylight varies with the time of day. In addition, metamerismcan be evaluated very readily, because two different light sources are provided.
98 Paint Technology HandbookTwo ASTM (American Society for Testing Materials) standard practices—D1729,Visual Evaluation of Color Difference of Opaque Materials and D4080, VisualEvaluation of Metamerism—are methods that recommend the use of light booths. When matching a color where metamerism is obvious, the match under daylightmay look like it requires red to correct it, but under incandescent it needs green.When there is no concern about metamerism, color match is done under one lightsource, preferably the one under which it will be viewed. When metamerism cannotbe tolerated, other colorants are selected and tried until the combination does notproduce a metameric match. This trial and error method can be very time consumingand is outmoded by methods using color measuring instruments and computer colormatching (CCM) systems.5.3 COLOR MEASUREMENT EQUIPMENTIntelligent use of color-measurement instruments will increase the efﬁciency ofmatching colors. They measure color difference in terms that allow description ofhue, saturation, and lightness, and also quantify these differences. This makes itpossible to estimate the amount of colorant to add to correct the color. Colorimeters measure color in terms of three numbers called tristimulus values—X, Y , and Z. These values are the amounts of three primary colors—red (X), green (Y ),and blue (Z)—needed to match or specify a color under illuminating and viewingconditions as standardized by the ICI. Each color has its own tristimulus values, andidentical values are identical colors. Differences in tristimulus values between colorscan be analyzed to determine the direction and magnitude of the color difference. To facilitate the translation of the color difference from numbers to the moremeaningful visual descriptive terms and quantify color difference, the XYZ values areconverted into the Hunter L, a, b Scale. This transformation is simple, and all moderninstruments offer it as an option. L is lightness–darkness, a is redness–greenness, andb is yellowish–bluish. If the difference between the trial values and given color inL, a, b values was −0.5, −0.5, and +0.5 respectively, the trial values indicate thatthe color is darker, greener, and yellower than the given color. If the color differenceis unacceptable, then the trial must be corrected by adding white to make it lighter,adding the bluest colorant to make it bluer or less yellow, and adding the reddestcolorant to make it redder or less green. By keeping records of the readings and the addition of the colorants, it is possibleto estimate the amounts of the colorants for a correction. For example, one poundof blue lowered b from +0.5 to +0.25. The goal is to minimize b. Therefore, ifone pound of blue changed b by 0.25 units, then another pound of blue would lower bto 0. The other colorants are estimated similarly. Some instruments indicate color difference in the tristimulus values. The colordifference is in terms of XYZ ratios, expressed as percent between the values of thebatch and the standard. XYZ ratios of 100, 100, 100 indicate that the values of thestandard and the batch are the same and the colors match. Any values other than 100indicate that a color difference exists. It is much more difﬁcult to translate these valuesinto visual descriptive terms as opposed to L, a, b values.
Color Matching and Color Control 99 As an example, green reads 101.5, 100.5, 100.5. The Y ratio, which is a measureof lightness, is greater than 100 indicating the batch is lighter. In order to determinethe hue and saturation difference, it is necessary to compare the relative values ofXYZ ratios. The hue of a green can only be yellower or bluer so the Z ratio is the hueindicator. However, it must be compared to the X ratio that is the saturation indicatorfor a green. In the example, Z is lower than X meaning that the batch is yellower.For saturation, the X ratio must be compared to the Y ratio and since the X ratio isgreater than the Y ratio, the batch is less saturated or grayer. Another way of lookingat this is that there is more red than needed. Red is the complementary color of green.Complimentary colors when mixed produce gray. The logic is similar for analyzingthe remaining category of colors blue, yellow, and red. XYZ values are the basic measurement of color, and for this reason estimating acorrection to a batch is easier and more reliable than other color scales but still requiresexperience. A green reads 110, 110, 110 and is made with white, blue, yellow, andblack. An addition based on experience of one pound of blue, one pound of yellow,and 0.1 pound of black is made. The result of the addition was 105, 104, 105 andanother addition is necessary to correct the match. To estimate the amount of blue,the ratio affected the most is used to compute the addition. Although this can be determined experimentally by adding some blue by itselfand seeing which ratio has changed the most, it is more expedient to use the followingrule. The bluest colorant will lower the X the fastest, the reddest colorant the Y , andthe yellowest the Z. Therefore, X will be used to estimate the amount of blue, Y theblack, and Z the yellow. One pound of blue lowered the X ratio by 5 and to get 100,another pound is added. A pound of yellow will lower the Z by 5 so another poundof yellow is needed. The black lowered Y by 6, so 0.06 pounds more is needed. This method works very well, but experience is needed for the ﬁrst addition andall colorants must be added simultaneously or too much of the colorants will beestimated. Once a batch is shaded using this method, and the readings and colorantadditions are recorded, the information can be used for succeeding batches. This hasbeen called the “historical” method and has proven to be very successful. This method would not have been possible without color measurement. The mostdifﬁcult decision to make when matching a color is deciding when to stop. Viewing colors that differ and judging whether or not it is a close enough matchis very subjective. No two people see color alike. It is a rare occasion when totalagreement will occur, and this is especially true when colors are metameric. Everyindividual has his or her own idea as to what is an acceptable match, and this maychange from day to day because of deadlines imposed to get the job done. This iswhere instruments perform well. Measurements are objective and consistent and notinﬂuenced by external pressures.5.3.1 COLOR DIFFERENCE EQUATIONSQuantiﬁcation or color difference makes it possible to establish a meaningful meas-urement of the closeness of a color match. The basic unit is a just noticeabledifference (JND). One JND is a very close match whereas three would be easilyperceptible.
100 Paint Technology Handbook Color difference equations calculate the color difference in units of E, the errorof the color match.5.3.2 TRISTIMULUS FILTER COLORIMETERSThe Hunterlab D25 and the Gardner XL 805 are useful for color correction (shading)and quality control, where the colorants are known and there is no metamerism ofany sort. The tristimulus data they provide is for only one illuminant (usually C), andtherefore, metamerism cannot be identiﬁed or checked.5.3.3 SPECTROCOLORIMETERSSherwin Williams Macbeth MS2020/TRS-80 system, Spectroard, MacbethMC 1500, and Applied Color System (ACS), Spectro Sensor compute XYZ valuesfrom the spectrophotometric curve of the color, making it possible to get tristimu-lus values for any and all of the Commission Internationale de L’Eclairage (CIE)standard illuminants, including CWF. Metamerism is detected by measuring E of thesamples under the various illuminants. If the FMC2 E is 1.0 for D65 and 2.0 for A,there is metamerism, because the color difference is not the same. Visual evaluationshould conﬁrm it. When a nonmetameric match is needed, the trial and error method of selection ofthe proper colorants is very inefﬁcient compared to spectrophotometric curve analysis.The spectrophotometric curve of a color is a plot of reﬂectance of light at eachwavelength of the visible spectrum. It is the primary physical measurement of a colorand is often referred to as the ﬁngerprint of a color, because identical curves areidentical colors and nonmetameric. The instrument that gives spectrophotometric curves is called a spectrophoto-meter. Spectrocolorimeters are spectrophotometers and when equipped with a plotter,will provide spectral reﬂectance curves that are used to identify colorants. Each colorant has its own characteristic spectral curve that remains identiﬁablein a mixture, making it possible to ascertain the colorants in an unknown. The colorantsare identiﬁed by comparing the absorption maximum (reﬂectance minimum) of thecurves of the known to that of the unknown, a method that is only as good as thelibrary of known. If the unknown contains a colorant for which there is no curve, thenit cannot be determined. This method easily outperforms experienced visual trial anderror. It can readily discern the difference between a red and a green shade phthaloblue pigment, which is difﬁcult by visual means. There are times when a colorant cannot be determined, because the concentrationis very low, or the difference between the curves is insufﬁcient to identify the colorantwith any degree of certainty. In these cases, a trial match is made and the spectralcurve compared to the unknown. It will be obvious if the wrong colorant was selected.This trial and error method is continued until the curve indicates the proper colorantshave been chosen.
Color Matching and Color Control 1015.3.4 COMPUTERIZED COLOR MATCHINGCCM is the best tool for matching colors. In the hands of a skilled color matcher, thequality of matches and gain in efﬁciency can be quite dramatic. It is a big improvementover visual trial and error and the instrumental methods mentioned previously. CCM systems are available from Diano, Macbeth, ACS, Universal Color Sys-tems, X-Rite, and Instrumental Color Systems. All are good and all have advantagesand disadvantages as far as user friendliness is concerned. None of them will doexactly what you would like them to do, but this is true of any software that isnot custom designed. Several companies, DuPont, Sherwin-Williams, PPG, andBenjamin Moore, to name a few, have developed proprietary software to satisfytheir own needs. Color matching is a science that is best left to formulators and quality controlexperts. For the applicator, it can be expressed in more general terms. There are manypigments that can be used to obtain a color. All these pigments vary from one anotherwithin the same color group. For example, there are red pigments with yellow cast,orange cast, blue cast, and so forth. The pigments can be clean, meaning that theyreﬂect light in a very limited wavelength range, or they can be dirty and reﬂect lightin a much wider wavelength range. Pigments are not pure compounds and many are naturally occurring compounds.This means they can vary from one production lot to another. What this all meansis that the color will vary slightly from one batch of paint to another, but fortunatelythe human eye cannot detect very slight differences. For most applications, a E of0.5–1.0 is an acceptable color match. It is important to have a color standard program for consistent color match fromone batch of paint to another within established limits. The company that will usethe material and the manufacturer of the paint must agree on a color standard that ispractical and reproducible in a paint production facility. This is necessary to maintaincolor consistency and reduce manufacturing errors. Consider, for example, that a paintcolor cannot be exactly duplicated with a printed catalog color. Similarly, some lead-bearing pigmented material cannot be nonmetamerically duplicated with lead-freepigmented material. For a new color, the paint supplier should be consulted to see if the color is feasible.They can usually determine how easy it will formulate a color match. If a colorstandard is already available, the paint supplier can match the established standardand submit a sample. When the sample is approved a master standard is prepared.The painted panels can be used as the master standard and working standard. Colortolerance charts can be prepared to monitor differences. Since color standards change with time and use, the Macbeth color programensures a consistent standard. They can also generate color tolerance charts thatestablish a range of color variation that is acceptable for production color matchingand establish the visible limits of an acceptable color match. If colorimetric instrumentation is used for color matching, the applicator andthe manufacturer must use the same programs for color measurement (e.g., Fri-ele, MacAdam, Chickering [FMC] II or LAB) and both machines must agree with
102 Paint Technology Handbookone another. An accepted color variation should be established from one batch toanother, since there is usually batch-to-batch variation. In general, using an FMC IIprogram, a E of less than 1.0 is acceptable for a production batch. For visible color match system, the following parameters should be included incolor control: 1. Light source to be used for viewing, that is, daylight or CWF. By using only one light source one can eliminate metamerism from one light source to another. The light should be the one that the product will normally be seen in. 2. Angle at which panels will be viewed. 3. Viewing distance from panel. At 50 ft, all colors look good. At 6 in, color matches are very difﬁcult. Remember, when comparing colors, that the appearance of the panels must be thesame, that is, both smooth or both textured. In addition, the gloss should be the samewithin limits, generally ±5 gloss units.5.4 COLOR GLOSSARY • Appearance—the way an object looks. It involves not only color but also other visual attributes such as gloss and texture. • Color—a visual response to light consisting of three variables; hue, sat- uration, and lightness. The most important appearance attribute of an object. • Color difference—magnitude and character of the difference between two colors. • Color tolerance—limit of color difference from a standard that is accept- able. It is generally expressed in terms of a particular color difference equation. • CIE LAB of L ∗ a ∗ b ∗ E—the color difference based upon the 1976 CIE color difference equation. One CIE LAB E is approximately 2 JND units of color difference. • L—designates lightness differences. • a—designates redness–greenness. • b—designates yellowness–blueness. • E—a unit of color difference. It constitutes the total differences in hue, the differences in saturation, and the differences in lightness. • FMC2 E—the color difference based upon the Friele, MacAdam, Chick- ering color difference equation. One FMC2 E is approximately 1 JND unit of color difference. • Gloss—subjective term used to describe the relative amount and nature of mirror-like (speculate) reﬂection. Different types of gloss are frequently arbitrarily differentiated, such as sheen, distinction-of-image gloss, and so forth. Trade practice recognizes the following stages, in increasing
Color Matching and Color Control 103 Glossy panel Low gloss panel Textured panel surface surface surfaceFIGURE 5.1 Geometric metamerism. order on gloss; ﬂat (or matte)—practically free from sheen, even when viewed from oblique angles (usually less than 15 on 85 degree meter); egg-shell—usually 20–35 on 60 degree meter; semi-gloss—usually 35–70 on 60 degree meter; full-gloss—smooth and almost mirror-like surface when viewed from all angles, usually above 70 on 60 degree meter. • Geometric metamerism—phenomenon exhibited by a pair of colors that appear to be a color match at one angle of illumination and viewing but which are no longer a match when the angle of illumination or viewing is changed, caused by gloss and/or texture differences (see Figure 5.1). • Hunter Lab E—the color difference based upon Hunter’s color differ- ence equation. One Hunter Lab E is approximately 3 JND units of color difference. • Metamerism—when two or more samples match under one set of viewing conditions (kind of light source and angle of view) for an observer, but do not match under a different set of viewing conditions for the same observer. Those samples may not match for a different observer under either viewing condition. • Master color standard—the absolute reference color standard; a color standard panel to which all standards of a given color are compared. • Primary working color standard—a color standard that is compared to painted items (usually) such as paint test panels and ﬁnished goods. It is used to color check everything, where the Master Standard is used only to check color standards and settle color disputes. • Secondary working color standard—a back-up to the primary working color standard. It becomes the primary working standard when the original primary working color standard is determined to be unusable. • Texture—nonuniform surface. Like gloss, texture affects the appearance of color. The visual evaluation of a color match is a very subjective human judgment. If thenature of the process is not fully understood and appreciated, poor color control willresult, or much more time than that is necessary will be spent in getting acceptablematches.5.5 COLOR STANDARDS AND METAMERISMThe color standard is the most important part of a color control program. Whetherthe color is controlled by visual observation, color measurement, or a combination of
104 Paint Technology Handbookboth, it is important that the color standard and the product are not metameric to oneanother. Metamerism is when colors match under certain viewing conditions and mismatchwhen the conditions are changed. The various viewing conditions that can causemetamerism are • The type of light source • The angle of illumination and angle of view • The human observer Metamerism can occur with all three conditions. Classiﬁcation of the metamerismdepends on the source. 1. Light source metamerism—colors will match under one light source (daylight) but do not match under another (incandescent). Cause: colorants different than those in the color being matched were used. Solution: use the same colorants. 2. Geometric metamerism—colors will match at only one angle of illumin- ation and viewing. For example, samples will match when they are oriented so that they are illuminated at a 0◦ angle to the surface and viewed at the 45◦ angle, but will be mismatched when the viewing angle is changed to 75◦ . Cause: the gloss and/or texture is different. Solution: control gloss and/or texture. 3. Observer metamerism—colors will be a match by one observer but not by another. Cause: individuals have different color visions, and it becomes evident when light source metamerism exists. Solution: eliminate light source metamerism.
6 Liquid Paint Application SystemsLiquid paint can be applied in many different ways. The three major components ofa paint line are pretreatment, application, and cure. The type of industrial applicationprocess will be determined by the product, the volume, the quality requirements,and other factors. It may be as simple as a dip tank and a method of hanging parts,or it may be a fully enclosed automated system that allows continuous pretreat-ment, application, and curing. A basic conveyorized paint line layout is illustrated inFigure 6.1. The actual layout and speciﬁc equipment vary widely, but all paint lines have thesame general stages: a loading area, pretreatment or cleaning stage, application stage,curing stage, and unloading area. The loading/unloading stages are where parts are put on and taken off the paintline. The pretreatment stage is where the parts are prepared for the coating applicationstage. Cleaning can be done mechanically, such as blasting, or chemically by solventwashing, solvent wiping, power washing, or dipping. After cleaning, the parts aredried by heat or forced air or a combination of the two so that they are ready to bepainted. Paint can be applied by spray method using conventional handheld spray guns,high-volume-low-pressure (HVLP) guns, automatic guns, automatic rotary bells,or disks. The spray equipment can be either nonelectrostatic or electrostatic. Dipsystems, ﬂow coaters, curtain coating, or roll coating are other application methods. The curing stage is where the paint ﬁlm is formed. Paints can be cured by airdrying or heating. Ovens for heating are conventional gas-ﬁred, high air velocity gas-ﬁred, electric, infra red, UV energy, electron beam, or induction. The ovens can be Pretreatment system Dry off oven Load Paint application area area Unload area Cure ovenFIGURE 6.1 Basic paint system layout. 105
106 Paint Technology Handbookeither batch type or continuous. Parts are moved from one stage to another by manualor automated conveyor systems.6.1 PART PREPARATIONAs discussed in Chapter 1 on pretreatment, a properly prepared surface is critical tothe success of the coating. Paint does not hide defects or clean a substrate. If thesubstrate is dirty or has a ﬁlm on it, the paint will adhere to the dirt ﬁlm, since it isthe ﬁrst surface it comes in contact with. If that ﬁlm adheres poorly to the substrate,then the paint will lift off. In many cases, the dirt or ﬁlm may not be compatible with the paint. This willcause the paint to pull away from that area and cause ﬁsh eyes or crawling on thesurface of the substrate. With the need to use high-solids, solvent-based paints,or water-based paints, the cleaning step becomes more critical. Prior to the reg-ulation of organic solvent emissions, paints were commonly 20–30% solids—theremainder being solvent. In many cases, this excess of solvent could attack thesurface ﬁlm and allow the paint to adhere through it to the substrate. Today this is notthe case. With regard to surface defects such as scratches, welding marks, porosity, andso forth paint will only ﬂow over a surface in a uniform manner and will not hide adefect as shown in Figure 6.2. The only way to hide the defect at this point is to sandthe paint until smooth and then recoat. Surfaces to be painted must be clean and dry to ensure paint adhesion. They mustalso be nearly as smooth as the desired ﬁnal ﬁnish. Generally, paint cannot be used tohide surface defects. Paint will often highlight surface defects by reﬂection and makethem more noticeable. In addition to cleaning and smoothing, surfaces are often converted to a mater-ial different from the original before painting. Phosphated steel and ﬂamed plasticsurfaces are examples. Surface conversion is generally used to improve paintadhesion, reduce corrosion, or both. A Defect B 2 mil Substrate With one coat of paint C D With two coats of paint With three coats of paint E F Sanded Repainted after sandingFIGURE 6.2 Repair of a paint defect caused by particulate on the surface.
Liquid Paint Application Systems 1076.1.1 SMOOTHINGSome surfaces require grinding, ﬁling, or sanding to make them smoother before thepaint is applied. Grit blasting or heavy grinding can be used to remove burrs or scale.In some cases, the substrate will require a combination of these processes. Large pits,holes, seams, or scratches in a surface can be ﬁlled with a liquid or paste material andthen sanded after they harden. Typical grinding papers use aluminum oxide or silicon carbide (carborundum)abrasives. Blasting abrasives may be sand, glass, metal grit, or walnut hulls. Thesemedia are available in a variety of grit sizes. Abrasives must be replaced or cleanedregularly so that they do not become oily and contaminate the surface.6.2 SPRAY APPLICATION OF PAINTPaint can be applied to a substrate in many different ways. Each method has advant-ages and limitations. The needs of the product and the manufacturing process willhelp determine the correct application method. An understanding of the differentapplication processes is necessary in order to evaluate them for a speciﬁc task. Most industrial paint systems apply liquid coatings with spray equipment. Theliquid coating is delivered from a container to a spray device that uses pressure tobreak the liquid stream into ﬁne droplets. The even distribution of the liquid paintinto a ﬁnely divided mist of droplets is called atomization. There are several differenttypes of spray guns and different methods of atomization and pattern control that canbe used to control quality and efﬁciency.6.2.1 METHODS OF ATOMIZATION • Air-spray is one of the earliest methods of atomization. An air-spray device mixes a high-velocity air stream with a low-velocity ﬂuid stream and the resulting friction creates the paint droplets. • Hydraulic atomization occurs when a high-velocity ﬂuid sheet that is formed by a small oriﬁce at the spray gun tip exits into a stationary atmosphere. The resulting friction causes atomization into droplets. • Centrifugal atomization occurs when a ﬂuid stream is introduced at the back of a disk that is rotating at high speed. The centrifugal force of the rotating disk delivers the paint to the edge of the disk and breaks it into a ﬁne mist. There are certain features that all spray applicators have in common, but eachdifferent spray device has particular differences that make it ﬁt with a certain applic-ation. An understanding of the different applicators and their strengths is useful in theselection of the correct device for a particular application.6.2.2 MANUAL SPRAY GUNSThere are a number of different spray gun technologies used for manual spray applic-ation of industrial coatings. Most coating systems use manual spray guns, alone
108 Paint Technology Handbookor as reinforcement for automated application. Manual spray equipment provides thefreedom to spray in hard to reach areas at different angles that would be difﬁcult toreach with a stationary automatic gun. Manual spray technology is available with or without electrostatic capability forbetter transfer efﬁciency. Handheld spray guns are typically identiﬁed by the followingnames: • Conventional air-spray • HVLP • Airless • Air-assisted airless (AAA) • Electrostatic HVLP • Electrostatic air-spray • Electrostatic AAA Each of these devices has features that make it work well in a given situation.Selection often depends on the cost of the device, the coating(s) to be used, and thedifference in application efﬁciency. Other factors may also inﬂuence the speciﬁc gunused in a certain application.6.2.3 AUTOMATIC SPRAY EQUIPMENTAutomatic spray equipment is used when the volume of work exceeds the capabilitiesof manual operators, the product is too large for men to reach, there is an interest inreduced labor, or there is an interest in automation for more precision. It is availablein all standard forms of air atomization and also uses centrifugal or rotary devices foratomization. Most automatic spray systems use a device that moves the spray guns and controlsapplication. Programmable logic controllers (PLCs) use part recognition systemsto trigger guns on, initiate color change, and adjust the equipment for optimumefﬁciency. In addition to control of paint application, PLCs are used for paint mixing,color changes, and other control tasks.6.2.4 SPRAY SYSTEMSConventional air-spray guns are common spray tools that can be used with and withoutelectrostatics. A conventional air-spray gun is a precision tool that uses energy in theform of compressed air to atomize the material. Air and paint enter the gun at differentpoints and meet at the head of the gun. The high-velocity air stream from the annularhole around the nozzle passes the low-velocity ﬂuid stream and the resulting frictioncreates a pattern of ﬁne droplets. The pattern of ﬁne paint particles provides a uniformthin ﬁlm of coating on the part surface. When the gun trigger is pulled back slightly, an air valve, usually located in theupper portion of the handle, will open and allow air only to reach the gun tip. Whenthe trigger is pulled back further, the ﬂuid needle is retracted and paint begins to ﬂowfrom the ﬂuid nozzle. Immediately upon leaving the nozzle, it is mixed with air from
Liquid Paint Application Systems 109 Needle Fluid Pattern packing needle adjustment knob Air cap Fluid adjustment Fluid knob nozzle Trigger Fluid inlet Air inletFIGURE 6.3 Spray gun components.the air nozzle, and the spray pattern is formed. Figure 6.3 shows the inside of a typicalair-spray gun.126.96.36.199 Suction or Siphon SystemsA suction or siphon feed gun uses a stream of compressed air to create a vacuum,allowing atmospheric pressure to force the ﬂuid material from an attached containerto the spray head. A siphon cup is a simple system for testing, for very short runs,for shading operations, or similar situations that require a small amount of paint anda short run. These systems typically use a one-quart container, and they are not veryeffective for high-viscosity materials. A siphon cup system is shown in Figure 6.4. Another system that works well for small volume applications uses gravity to feedthe paint to the gun tip. It is lightweight and uses virtually every drop of paint in thecup so that almost no paint is wasted in the cup. A gravity cup is shown in Figure 188.8.131.52.4.2 Pressure Feed SystemsA pressure feed system applies paint that has been forced to the gun by pressure,either from compressed air or a pump. Pressure-feed systems are used in situationsrequiring more volume, delivered from a larger vessel, rather than the small cupsused in gravity and siphon systems. It is also suitable for paints with higher viscosity.
110 Paint Technology Handbook Regulator Siphon cup Air line Oil and water extractorFIGURE 6.4 Siphon feed system.FIGURE 6.5 Gravity feed system. Pressure pots use compressed air to create ﬂuid pressure and force the paintthrough the ﬂuid hose to the spray gun. There are many sizes of pressure vesselsthat can be used depending on the size of the operation. Five-gallon pots are fairlycommon. A system with a 5-gal pot is shown in Figure 6.6. A pump is often used tosupply coating material from a larger container such as a 55-gal drum.184.108.40.206 Circulating SystemsSome systems deliver paint to the booth but do not circulate it back to the container.Circulation systems are more effective for maintaining a stable paint material andlimiting waste materials.
Liquid Paint Application Systems 111 Oil and water extraction Regulator Air line Main line outlet Fluid line Pressure tankFIGURE 6.6 Air-spray pressure feed system. Fluid regulator Fluid supply line 70 lbs. Air regulator Piston Bypass valve pump 20 lbs. Spray gun Backpressure regulator Fluid filter Shut-off valve Fluid return line Fluid siphon line Material supply containerFIGURE 6.7 Paint circulation system. Many paint lines are installed with paint supply systems that bring ﬂuid to thebooth and circulate it back to a supply container in a “paint kitchen.” A typicalcirculating system is shown in Figure 6.7. Circulation systems have several advantages over pressure tanks. The materialvolume is not limited to the pressure pot size. Material is supplied directly from thecontainer it was shipped in or a large tote. If a container is running low, a new onecan be attached without any lose of production time. There is very little waste with a circulating line. The material in the hose fromthe color manifold to the applicator is usually a very small volume, often as low as6–8 oz of material. A circulation line is only useful when the paint can be consumed
112 Paint Technology Handbookin a reasonable period. If it is circulated through the system for more than a weekwithout any consumption, the material may become unstable and create appearanceand performance problems. Circulating systems often use a manifold of independent valves for differentcolors and supply of solvent and compressed air. Automatic color changers are oftenused to speed up color change and minimize wasted paint. These systems usuallyhave different valve arrangements that facilitate efﬁcient color change options. Thevalves are normally closed and interlocked to prevent any ﬂow of material intothe manifold or other color valves. The color valves open in sequence to shut offthe color in use, purge the system using solvent and air, and introduce the freshcolor. The supply containers are often located in an isolated room and material is pumpedto the booth or series of booths through a hard pipe system. These rooms are oftencalled paint kitchens, red label rooms, or paint lockers. They contain any number ofcontainers depending on the number of colors required. Each system has an inde-pendent pump, material agitator, pump surge chamber, paint ﬁlters, backpressureregulator, and other components of a circulation line. They can provide material toone or more spray stations at the same time in addition to providing good materialcirculation while the speciﬁc color is not being sprayed. Circulation systems route the paint to the booth and circulate it back to thecontainer. Regulators are used to control the ﬂow and make sure that the materialmaintains pressure and does not settle or separate in the line. Systems that use a paint kitchen with multiple colors could have a two pipecirculating system similar to the one shown below. A regulated ﬂow of material issupplied to each station from a central location. The supply line passes through thespray station and returns to the drum to close the loop. Circulation of paint in this wayprovides a consistent ﬂow and homogenous blend of paint. It reduces the labor ofmixing and transporting pots and improves control of the process. However, this typeof system has many components to maintain and has greater potential for materialdegradation. Some circulation systems use graduated pipe designs. The graduated pipe systemis typically used in automotive ﬁnal assembly and tier-one ﬁnishing plants wherematerial ﬂow; pressure and velocity consistency are most important. The gradu-ated pipe system uses the material viscosity and pipe and hose diameters to createthe system back-pressure and material ﬂow. The system typically incorporates apump, high-ﬂow surge chamber, ﬁlter housing, and back-pressure regulator. Theonly adjustments are the pump output pressures and material return pressures to thepaint kitchen. Pig-able systems are fast becoming the choice of design for frequent color changeswhere material recovery and reduced solvent usage are imperative. The pig-able system incorporates special color valves that allow for cleaning(pigging) as part of the circulation system. While traditional circulation lines aredifﬁcult and costly to color-change, a pig-able line can be color-changed fairly quicklyand inexpensively. When a line is color-changed a small diameter plug, referred to asa “pig,” is passed through the ﬂuid delivery line to clean out any paint solids that arestill present after a solvent/air purge.
Liquid Paint Application Systems 113 The typical pig-able paint system allows faster color-changes, recovery of morematerial, and reduced solvent usage during ﬂushing. A pig-able type system canprovide large cost savings for users responsible for numerous colors. The traditional approach to paint circulation line design did not provide simple orfast color change. In order to color-change them, the user had to ﬂush main circulatinglines or provide booth mounted mini systems. The waste material to ﬂush this type ofsystem could include 2+ gallons of paint and 30+ gallons of solvent per ﬂush. Thereturn on investment by utilizing pig-able technology is generally 6 months or lessand provides a more ﬂexible material-friendly circulating system.220.127.116.11 Plural Component Mixing EquipmentTwo component materials must be mixed prior to spray application. Mixing canbe as simple as mixing the two materials at the desired ratio into a siphon cup orpressure feed tank in an appropriate batch size. For high-volume mixing requirementsa mechanical proportioner, gear driven mixer, or an electronic mixer may be thebetter choice. In all cases, the objective is to consistently mix two or sometimes threematerials at the recommended mix ratio while always generating little or no waste.Mix ratios may range from 1:1 to 50:1 or greater. It all depends on the coating andthe application requirements. Mechanical proportioners are typically one or two pumps that are mechanicallyconnected together in either a ﬁxed ratio or variable ratio conﬁguration. A ﬁxed ratiopump system with a 1:1 ratio has one pump air motor with two identical pump-lowers that deliver the same volume of material when the pump is actuated. Fixedratio systems are available in many sizes and the pumps are sized to produce theparticular ratio needed. A variable ratio system has one pump to deliver the resinmaterial with an adjustable arm that actuates a smaller catalyst pump at the desiredcycle rate to deliver the correct material mix ratio. Mechanical systems, like the dual piston pump system shown in Figure 6.8, costless money than the cost of more sophisticated systems, but they are maintenanceprone and ﬂushing is difﬁcult and expensive. Ratio is adjusted by move the fulcrumposition by trial and error. A gear-driven system uses a PLC or PC to control the speed of each pump toestablish a mix ratio. The gear driven system requires a low-pressure material deliverysource to supply the two different gear pumps, then the gear pumps supply the desiredoutput and ratios to the spray gun. There is typically one system for each spray booth and spray application. Thesesystems can be more complex with the amount of components required, but they areaccurate, ﬂexible, and can consistently deliver very low material ﬂow rates with lessconcern for mix ratio variances. Some gear-driven systems use two gear pumps on a common drive. Some gearsystems use independent motors for the two gear pumps. Mix accuracy depends onthe speed of the drive motor. These systems are sensitive to the coating viscosity, andthey do not provide veriﬁcation of mix accuracy. The electronic mixer requires a separate material delivery source that could be assimple as two pressure tanks to a large circulation system. The electronic mixer has a
114 Paint Technology Handbook Component A Component B PistonFIGURE 6.8 Dual piston pump mixing system. A C B Supply Control signal A C B D A. Material supply Supply B. Flow control valves C. FlowmetersFIGURE 6.9 Two component proportioning system.back plate that may be mounted outside the booth, inside the booth if hazardous rated,or mounted directly on the gun mover or robot. It typically includes anAand B materialﬂow meter, ﬂuid ﬂow regulators, and a mix manifold and static mixer. These systemscan be used on one spray booth with one spray gun or can be networked togetherwith other systems in multiple spray booths. It is recommended that one back platebe used with only one applicator. Electronic systems provide precision mixing and information such as notiﬁcationif the material supply is low. A well-designed system can supply reliable mix ratiosand provide alarm conditions so that problems are quickly identiﬁed and corrected.A typical system is shown in Figure 6.9. The right proportioner is dependent on the application, material, and productionspeed. Electronic mixers use a small PLC to control the mix ratios and often the materialdelivery rates. These systems are very ﬂexible, have a wide range of mix ratio options,
Liquid Paint Application Systems 115provide documentation for environmental reporting, and are very consistent. Manyelectronic mixers use a PC, which is more ﬂexible and allows a windows format forease of control.18.104.22.168 Air NozzlesThe air nozzle directs the ﬂow of compressed air through a series of holes into thepaint stream at the gun tip. The air atomizes the paint and directs the ﬂow of atomizedpaint into the pattern. A proﬁle is shown in Figure 6.10 with ﬂuid ﬂowing around theﬂuid needle and air introduced by the air horns at the gun tip. Figure 6.11 shows theair nozzle. Some air nozzles are referred to as internal-mix. With an internal-mix nozzle, theair and paint are mixed inside the nozzle and the pattern is formed as the mixture exitsthrough a hole in the nozzle tip. An air nozzle introduces the compressed air to theﬂuid stream at the gun tip. Air FluidFIGURE 6.10 Spray gun air nozzle. 1 3 1. Annular ring 2. Containment holes 3. Horns 2 4. Fan pattern holes 5. Angular converging holes 5 4FIGURE 6.11 Air-spray air nozzle.
116 Paint Technology Handbook22.214.171.124 Fluid NozzlesThe ﬂuid nozzle and needle combination is used to control the volume of coatingmaterial delivered at the spray tip. The ﬂuid needle is pulled back when the gun istriggered and ﬂuid ﬂows through the nozzle. When the trigger is released, the needleslides back into place and shuts off the ﬂow. Atomization occurs at the gun tip whencompressed air is directed into the paint stream as it exits the ﬂuid nozzle. The ﬂuidoriﬁce in the nozzle assembly provides the lowest possible velocity ﬂuid stream.A properly sized air cap will provide a high-velocity air stream from the annularholes to provide atomization at the gun tip. Atomization is measured by micron size and distribution in a given area by aMalvern or similar in-ﬂight particle analyzer. The size of the paint droplets willdepend on the particular material being sprayed and may vary widely from a low ofaround 5 µm to above 100 µm. The particle size distribution needed to achieve aparticular ﬁnish with a particular paint will depend on the product being painted andthe ﬁlm build requirements. Typically, a ﬁner droplet size will provide a smootherﬁnish. Selection of a particular ﬂuid nozzle depends on the viscosity of the coatingmaterial and the required level of atomization. Different sized ﬂuid nozzles areavailable for materials including paint, adhesives, mastics, ﬂocking materials, andso forth. Hardened steel ﬂuid nozzles are commonly used for solvent-based paints. Forpaint materials that are abrasive, the ﬂuid nozzle may be an alloy. Stainless steelis required for water-borne coatings or other corrosive ﬂuids. For materials that areunusually abrasive, the tip can be ﬁtted with a carbide insert. Some plastic ﬂuidnozzles work well due to their low surface friction and their ability to conform toworn ﬂuid needles. Usually, a nozzle with a smaller oriﬁce will work ﬁne with a lower viscositymaterial while a higher viscosity material may require a larger nozzle. If the nozzle istoo small to deliver the volume of paint needed, the ﬂuid pressure must be increasedin order to compensate. Excessive pressure can create application problems so it isimportant to select the correct nozzle for the material being sprayed. Nozzle size, ﬂuid ﬂow, and pressures are related. Selection of a ﬂuid nozzle shouldconsider the viscosity of the material, the amount of material required to achieve thedesired ﬁlm thickness, and the maximum desired ﬂuid ﬂow rate. Table 6.1 shows some examples of different ﬂuid tip oriﬁce sizes and the typesof products that they are likely to be used with them. Materials with high viscosity will ﬂow slower than thinner ﬂuids, usuallyrequiring a larger oriﬁce and higher ﬂuid pressure to achieve the desired ﬂuidﬂow. Low-viscosity materials ﬂow more readily at lower pressure through smalleroriﬁces. To determine a ﬂuid ﬂow rate for a speciﬁc oriﬁce size, turn off the atomizingair, trigger the gun, and ﬁll a graduated beaker for 30 s. Measure the amount inthe container and multiply it with 2 to determine the volume in ounces or cubiccentimeters per minute. Record the ﬂuid pressure, material viscosity, and oriﬁce sizefor reference.
Liquid Paint Application Systems 117 TABLE 6.1 Fluid Tip Oriﬁce Sizes Oriﬁce Viscosity Range Range Example 0.022–0.028 Very thin Solvents, stains 0.040–0.052 Thin Lacquers, primers 0.059–0.070 Medium Varnish, urethanes 0.086–0.110 Heavy Epoxies, vinyls 0.125–0.500 Very heavy Block ﬁllers TABLE 6.2 Delivery in Ounces per Minute at Different Pressures Oriﬁce Size At 8 psi At 12 psi At 18 psi 0.040 14 18 24 0.046 18 22 30 0.052 22 28 36 0.059 31 36 48 0.070 40 48 60 Table 6.2 shows the difference in ﬂuid ﬂow at different pressures for a materialwith a viscosity of 21 s in a #2 Zahn viscosity cup. Control of ﬂuid ﬂow can be adjusted by changing the ﬂuid nozzle, by turning theﬂuid adjustment knob located on the rear of the gun handle, or by changing the airpressure through the ﬂuid regulator. The ﬂuid control knob on the gun is provided so that the gun can be adjusted whenused with a siphon feed system. A pressure feed system should typically be adjustedby air pressure regulation with the ﬂuid control knob left in the full-open position.Fluid control by adjustment of the needle position is not recommended. Triggering a spray gun with no atomizing air can be useful for setting the properﬂuid pressure. The resulting paint stream should ﬂow in a solid stream for approxim-ately 1′ 0′′ to 2′ 0′′ before falling off. Anything in excess of 2 ft indicates that the ﬂuidpressure is too high.126.96.36.199 Proper Fluid PressureThe ﬂuid needle ﬁts into the oriﬁce of the ﬂuid nozzle. When the gun trigger is pulled,the ﬂuid needle is pulled back from the oriﬁce and paint material is allowed to ﬂowfrom the gun. When the trigger is released, the ﬂuid needle moves forward and stopsﬂuid ﬂow.
118 Paint Technology Handbook Fluid needles are machined from hardened steel or stainless steel with a taperedend. Fluid needles are also made of engineered plastics. The tapered end is designedto match the oriﬁce of a family of ﬂuid nozzles. The ﬂuid nozzle and needle is a pair. If a needle does not match a particular ﬂuidnozzle, the taper will not match and ﬂuid will leak from the nozzle tip, the gun willspit and drip. The nozzle and needle should be replaced. The manufacturers catalogwill list the correct needle and nozzle families. Sometimes it is necessary to make a needle adjustment to compensate for wear.Every time the gun is triggered, the needle slides back across the inner surface of theﬂuid nozzle and causes a small amount of wear. Eventually, there is enough wear tocreate a gap between the needle and the seat of the oriﬁce and the gun will leak.6.3 AIRLESS SPRAY GUNSAirless spray systems use hydraulic pressure to force the ﬂuid through a spray tip ororiﬁce at high pressure. The combination of pressure and oriﬁce size creates a pattern.Oriﬁce sizes are catalogued by ﬂow capacity and degree of spray angle. An airless spray gun does not use compressed air for atomization, so there is noair nozzle with atomizing ports like those found on an air-spray gun. There is onlyone trigger position, full open. An airless system works with a high-pressure pump that delivers ﬂuid to the guntip at 500–6000 psi and forces the ﬂuid through the oriﬁce. Airless systems can be used with heaters to reduce the spray viscosity and improveﬁnish quality. The heater helps to control spray viscosity for consistency and may beparticularly helpful with thicker materials. Figure 6.12 shows an airless spray system.6.3.1 FLUID NEEDLES AND TIPS FOR AIRLESS SYSTEMSUsually an airless needle will be a permanent assembly having a ball, approximately1/8′′ diameter, silver soldered to the end. This ball will “seat” or act as a seal toprevent ﬂuid from leaking through the ﬂuid tip when the gun is not in use. Pump Air supply line Air compressor Siphon line FilterFIGURE 6.12 Airless spray system.
Liquid Paint Application Systems 119 TABLE 6.3 Oriﬁce Sizes for Airless Systems Oriﬁce Size Viscosity Range Material 0.009–0.010 Very thin Acetone 0.011–0.013 Thin Water 0.015–0.021 Medium SAE #10 oil 0.026–0.036 Heavy SAE #50 oil 0.043–0.072 Very heavy Vaseline 0.072–0.081 Extra heavy Mastics The reason an airless needle is not smooth and tapered like an air-atomized needleis that the high ﬂuid pressures would unseat a tapered needle and cause a leak. The ball at the ﬂuid needle tip provides a surface for the ﬂuid to push ball into aseated position at the ﬂuid tip and prevent the needle from lifting or retracting. It isrounded so that when the trigger is pulled, the ﬂuid is deﬂected and it can retract. If itwere ﬂat, you would have to exert considerable force on the trigger to overcome theresistance generated by the high ﬂuid pressure. Typically, there is only one size ﬂuidneedle for all tip sizes for an airless gun. The oriﬁce size in the ﬂuid tip will start around 0.009′′ and range upward in excess0.081′′ . The larger oriﬁces can handle heavier materials that require higher pressures.Table 6.3 will give a general idea of oriﬁce size for typical materials. The oriﬁce size and the spray angle will deﬁne the pattern size. The pattern sizecan only be adjusted by changing ﬂuid tips. A ﬂuid tip with the widest possible angleand the smallest oriﬁce size that will work well with a given ﬂuid viscosity willprovide a wide area of coverage and controlled ﬁlm build. With an air-atomized gun, the operator can adjust the pattern size, alter the atomiz-ation, and increase or decrease ﬂuid ﬂow. There is no way to make similar adjustmentson an airless gun. An airless spray gun works like a typical spray nozzle. Atomization is achievedwhen the ﬂuid is forced through the oriﬁce at high pressure. The oriﬁce will providea speciﬁc pattern size and a speciﬁc ﬂuid delivery at a designated pressure. Airless systems can operate at pressures up to 6000 psi. The systems are manu-factured with safety features to protect the operator from the high-pressure discharge.Operators of airless systems need to be careful not to trigger the gun toward any partof their body. Airless units and all connected components must be grounded to prevent staticdischarge. Electric units have three-wire grounded plugs, air driven pumps haveground straps, and a proper airless hose has a ground wire built into the jacket ofthe hose. Solvent should not be sprayed under pressure through the airless tip and/ordiffuser. An explosion or ﬁre could result from static buildup in the presence ofﬂammable vapors. Never attempt to remove a hose, gun, or any piece of the system without ﬁrstreleasing the pressure and disabling the pump.
120 Paint Technology Handbook An airless spray gun does not produce the ﬁne atomization required for class Asurfaces. It is used primarily in wood ﬁnishing, leather tanning, fabricated metalmanufacturing, and painting contractor applications. Transfer efﬁciency can be verygood and a lot of ﬂuid can be delivered per minute making the airless system a gooddevice for ﬁeld applications. An airless spray gun delivers more ﬂuid with less fogthan a conventional air-spray gun. If ﬁner atomization is required, a ﬁne ﬁnish tip and the use of a diffuser may help.The diffuser will shear the material by disrupting the ﬂuid ﬂow before it gets to theﬂuid tip where it is atomized.6.4 AIR-ASSISTED AIRLESS SPRAY GUNSTheAAAgun uses a lower ﬂuid pressure (typically 400–800 psi) with an airless tip andan air nozzle for atomization. This combination of elements provides faster applic-ation of material than air atomized spray provides, reduces overspray and rebound,and provides enough forward velocity to penetrate some recesses and cavities. Thepressure range used with AAA spray guns is much higher today for high solids andultra high solids materials. A picture of an AAA gun is shown in Figure 6.13. Notethe “duck bills” at the gun tip that provide protection against accidental exposure tothe high-pressure spray. AAA does not provide the ﬁne atomization necessary for extremely high-qualityﬁnishes. It is very popular in the wood ﬁnishing industry where stains, sealers, ﬁllers,glazes, lacquers, and polyurethane materials are common. It is also very effectivefor applications that require high-TE, low overspray, fast application, and modestappearance standards.FIGURE 6.13 Air-assisted airless spray gun.
Liquid Paint Application Systems 121 AAA spray guns are often used in systems with very high line speeds, but theyare particularly well suited to systems with slow to medium line speeds and coatingmaterials that are thin to medium in viscosity, a typical maximum of 28–32 s on a#2 Zahn cup. Material is typically delivered with a conventional air driven pump ina range of 10:1 to 30:1 power ratio. Unlike airless, this type of gun relies heavily on the correct air pressure in relationto ﬂuid pressure. AAA uses an air cap that is similar to the one that would be used witha conventional air-spray gun, but the air is used primarily to distribute the dropletsmore evenly and to assist the air in remaining stationary in relation to the ﬂuid streamor sheet. The ﬂuid is at a higher pressure in an AAA gun. Primary atomization isstill achieved by ﬂuid ﬂow through an oriﬁce. The compressed air helps to create amore uniform pattern, better paint particle distribution, and ﬁner atomization than anairless spray gun. Airless and AAA systems are often used with heaters to reduce the spray viscosityof materials that are higher in solids. Airless systems are often used for ﬁeld painting or shop painting that does notrequire ﬁne atomization. AAA systems are suitable for a wider variety of applications. Like an airless system, atomization is achieved by the choice of ﬂuid tips andthe pressure used to propel the coating through it. The added feature of compressedair has very little effect on atomization. Its main function is to ﬁll the pattern so thatthe coating is uniformly deposited on the surface. Figure 6.14 shows a typical AAAsystem with a heater. A comparison of the three gun types that have been discussed is outlined inTable 6.4. Air supply Heater Siphon Recirculation Back pressure regulator lineFIGURE 6.14 Air-assisted airless system with heater.
122 Paint Technology HandbookTABLE 6.4Comparison of Different Spray Guns Air Atomized Spray Airless Spray Air Assisted AirlessFinish appearance Excellent Coarse Very goodTransfer efﬁciency Low Good GoodFluid ﬂow rates Very low to medium, High or very high Wide range, usually less than ﬂow rates, over 7 ﬂuid oz/min to 30 ﬂuid oz/min 80 ﬂuid oz/min 78 ﬂuid oz/minBooth maintenance Lot of rebound and Less rebound and Least rebound and overspray, booth overspray, less overspray, maintenance is high maintenance maintenance is lowPattern adjustment Yes Tip selection Yes (limited)Tip plugging Virtually none Yes YesEquipment life Very long due to very Very high ﬂuid Less tip wear, lower low ﬂuid pressure pressure, high tip wear ﬂuid pressure and shorter pump lifeaNoise Noisy Quiet QuietEmission level High Lower Lowa If the pump is sized properly to reduce cycles, the wear is not different than the AAA. Regulator Oil and moisture extractor Pressure potFIGURE 6.15 High-volume, low-pressure spray system.6.5 HIGH-VOLUME LOW-PRESSURE (HVLP)HVLP gun technology is a form of air-spray that uses a restrictor to reduce the velocityof the coating material for increased transfer efﬁciency. It has become a favoredtechnology by environmental agencies, because it uses about the same volume of airas a conventional air atomized gun, but it operates at much lower air cap pressures.An HVLP system is shown in Figure 6.15. HVLP can provide higher transfer efﬁciency compared to other conventionalspray guns without electrostatic charging. This makes it particularly useful fornonconductive surfaces such as plastic and wood.
Liquid Paint Application Systems 123FIGURE 6.16 HVLP versus conventional air-spray gun. It takes a speciﬁc velocity of air to effectively overcome the cohesiveness of apaint material and atomize a coating. With air-atomized systems, more compressedair volume will increase the breakup of the material and produce ﬁner atomization.The illustration in Figure 6.16 shows the difference in the spray pattern between anHVLP and a conventional air-spray gun. HVLP technology delivers the same air volume at a lower pressure. This isintended to reduce the forward velocity of the sprayed material for reduced reboundand increased transfer efﬁciency. The lower tip velocity creates a softer ﬂuid deliverywith less overspray. Electrostatic capability can be added to an HVLP spray gun tofurther enhance transfer efﬁciency. The amount of ﬂuid ﬂow and the method of applying the compressed air foratomization are what differentiate HVLP from other forms of air-atomized equipment. Many of the early versions of HVLP equipment used electric motor driven tur-bines as a source for air. Unlike a compressor, a turbine works against very littlebackpressure so the horsepower to cubic feet per minute (CFM) ratio is reduced. Tur-bine systems are expensive and noisy. They can generate discharge temperatures ashigh as 225◦ F from a seven-stage turbine. This can be useful if a fast ﬂash or accel-erated cure is desired for materials such as waterborne adhesive or contact cement.However, high air temperature can also cause dry spray and other undesirable surfaceeffects. Turbine systems usually have a large and bulky air hose for heat resistance. Thelarge hose makes the gun bulky to handle and inﬂexible. The gun handle may requireinsulation, making it bulky and tiresome to hold over long periods. The turbine system can be useful for very small installations as an alternative to anair compressor or in ﬁeld painting operations. Where an air compressor is present withsufﬁcient air volume and the proper air quality (ﬁltration and moisture elimination),it is better to work with an HVLP gun that does not require a turbine. Most HVLP guns are run on standard compressed air. The air supply is passedthrough a high-volume, low-pressure, air regulator with reasonable accuracy at lowpressure. Compressed air HVLP guns use a restrictor or vortex, built into the air passageof the gun. The restrictor reduces the air output at the nozzle. A regulated inboundair pressure of 50 psi will typically produce 10 psi at the air cap. Typically, the gun
124 Paint Technology Handbookis intended for operation in the range of 2–10 psi at 15–18 ft3 /min. If the rated inputpressure is exceeded, the air volume and pressure will increase and the beneﬁt of theHVLP is limited. The regulator must be capable of controlling a large volume of airﬂow in apressure range of 0–100 psi. Typically, the air hose for the HVLP system is lar-ger in diameter than that of an air-spray gun. A minimum of 5/16′′ diameter hose isrecommended. These guns resemble an air-atomized gun in shape and size and they can be usedwith the same equipment setup as the air-spray gun. They use a common 1/4′′ or 5/16′′airline running to the handle directly from a compressed air line. The compressed airpowered HVLP gun is more easily accepted by a hand spray operator, because itclosely resembles an air-atomized gun in control, size, and appearance. An HVLPcan provide good atomization for most coatings, but it may be difﬁcult to atomizesome materials with high viscosity. In some cases, air heaters are used to help controlspray viscosity and improve atomization with thicker materials. HVLP guns can be used with pressure pots or with gravity feed systems, but theydo not work as well with a siphon cup. The HVLP spray gun does produce a very soft paint pattern, and it can improvetransfer efﬁciency when compared to an air-atomized gun. An HVLP gun may notatomize high-solids coatings well enough for class “A” surfaces, and some experi-enced painters complain that it is slower than a conventional air-spray gun due tolower ﬂuid outputs. These issues are related to the restrictor. The amount of ﬂuidoutput is limited by the ability to atomize. If the ﬂuid output is too high, there isnot enough velocity to break it up, and the paint droplets are coarse, so ﬂuid volumeis somewhat limited. The same issue affects the ability to atomize a material withheavy viscosity. The heavy paint material will require more energy to break it upinto ﬁne droplets. A high-solids coating applied with an HVLP may have too muchorange peel. In some situations, it is possible that the HVLP may not have sufﬁcient output tokeep up with a high-volume production operation. In other cases, the perception thatan HVLP gun is too slow may be caused by the use of the wrong gun, the wrong ﬂuidtip, or the wrong technique. Following these rules will make sure that the HVLP gunwill work as designed: • Several guns should be tested before a purchase is made to make sure that the chosen spray gun handles the coatings to be sprayed. • Different ﬂuid tips and air cap combinations need to be tested to ﬁnd the one that works best with a particular coating material. • Heaters can be used to help maintain a spray viscosity that will atomize with an HVLP spray gun. Spray technique with an HVLP has subtle differences from using an air-spraygun. The gun should be held closer to the part due to the slower forward velocity ofthe droplets; 6–8′′ is the typical gun-to-target distance. Material will build quicklywith fewer and slower strokes than an air-spray gun.
Liquid Paint Application Systems 125 Used correctly, the HVLP spray gun reduces overspray and fog in the booth,improves transfer efﬁciency, reduces volatile organic compound (VOC) emissions,extends the life of the ﬁlters, and reduces clean-up time.6.6 ELECTROSTATIC APPLICATIONElectrostatic application is designed to enhance the attraction of the paint materialto an earth-grounded surface. The basic features of the spray gun are the same, buta power supply is used to provide voltage and charge the sprayed coating material.Electrostatic attraction uses the elementary science where two surfaces that havethe same charge will repel each other and unlike charges attract. Figure 6.17 shows ahand-held electrostatic spray system with an air-spray gun and Figure 6.18 is a systemwith an airless gun. High-voltage electric charge is added to the atomized paint particles as they leavethe gun. A voltage generator is connected to an electrode at the gun tip. The voltagesource can be external or internal. When the gun is triggered, the electrode dischargesa concentrated ﬁeld of negative ions. Paint particles travel through this ionized areaand become charged with negative ions. The charged particles of atomized paint are directed toward the earth groundedpart from the spray gun. As they approach the target surface, the electrostatic chargecreates a strong attraction to the part surface. The charged particles are stronglyattracted to all bare surfaces of the grounded part as shown in Figure 6.19. Some of the particles that are carried wide of the part by compressed air are drawnto the back and edges, a phenomenon referred to as “electrostatic wrap.” Coating thatwraps around edges may be beneﬁcial on some parts, but it may have a limited beneﬁtif no coverage is required on the back of the part. The atomized paint droplets will be attracted to the best available ground. It isimportant to maintain a clean conveyor and clean hooks, and the ground should bechecked regularly. Air supply Air Spray gun Fluid High voltage cable Pressure tank Power supplyFIGURE 6.17 Electrostatic handheld air-spray system.
126 Paint Technology Handbook Pump Spray gun Fluid Heater Air supply (optional) High voltage cable Power supplyFIGURE 6.18 Airless electrostatic system. Paint Voltage droplets lines Spray gun electrode Grounded part Negative ions AirflowFIGURE 6.19 Electrostatic attraction. Effective use of electrostatic systems requires certain conditions to be met. 1. The coating must be in the proper conductivity range. The majority of solvent-borne coatings will work with electrostatic systems. 2. The atomized droplets should be round and remain as wet as possible. Sometimes a slow evaporating solvent is added to maintain this wetness.
Liquid Paint Application Systems 127 3. An electrical ﬁeld must be established and maintained in the proper position to direct the charged particles toward the part. 4. Forces such as excessive spray booth velocity and abnormally dry air will interfere with the electrostatic attraction process. 5. The parts to be coated must be electrically conductive to earth ground. Earth grounding of the part is very important to provide the maximum beneﬁt fromthe electrostatic spray applicator. The National Fire Protection Association (NFPA)states that all conductive objects in an electrostatic coating area must be groundedand have a resistance of no more than 1 meg-ohm. In a well-grounded application, the charge of the paint at the surface induces anopposite charge in the part that is equal to the ﬁeld strength of the arriving ions andpaint droplets. When a part is not conductive to ground, it will initially attract coating,but as more and more coating is applied, the ﬁeld strength at the part surface increasesrapidly and may begin to repel paint droplets. With no path to ground, the charge maybuild to a point where the voltage discharges and a spark occurs. Volatile solventvapors in the immediate area can get ignited. The process can be compared to that of a bolt of lightning that strikes the tallestobject in its vicinity. As clouds move through the atmosphere, they sometimes developa charge. The charge builds up in the cloud and then moves downward, building achannel with charge deposited along its length. Eventually, it encounters somethingon the ground that is a good connection. When a good connection is made, the circuitis complete and the charge is lowered from cloud to ground. The return stroke is aﬂow of charge (current) back to the cloud. It is essential to have a good path to ground and maintain it religiously to avoid adischarge. Earth-ground is measured with an electrical megohm meter. A good groundhas a resistance of less than 1.0 meg-ohm as recommended by NFPA. The meteruses two probes to measure resistance between the conveyor and the parts hangerand between the hanger and the part. All paint systems must have good ground toavoid static electric discharge. It is particularly important in electrostatic systemsdue to the high voltage of the system. The use of a megohm meter that can generate500–1000 VDC is essential. Devices powered by small batteries are not an acceptableway of determining earth ground. If parts are sprayed on a cart or a support other than a conveyor, they shouldhave a cable attached to provide a path to ground. Lack of ground reduces transferefﬁciency and creates an unsafe environment. All electrostatic operations should workefﬁciently to be sure that the parts are grounded.6.6.1 MANUAL ELECTROSTATIC SPRAY EQUIPMENTThere are several types of handheld, manually triggered electrostatic spray guns usedfor industrial application. • Air-spray electrostatic guns • Airless electrostatic spray guns • AAA electrostatic spray guns
128 Paint Technology Handbook • HVLP electrostatic spray guns • Electrostatic rotary atomizers Electrostatic spray guns have an electrode inside the barrel of the gun that extendsto the tip. The electrode may be in the material stream or near it on the cap. Electrostatic systems have a safety monitoring circuit that reduces the voltageoutput in direct relation to the approaching ground. At a closer distance to ground,the voltage drops and the current draw increases. The equipment can monitor the“closing speed” and will shut the entire system down if the rate of approach is toogreat. This is helpful on an automatic system where a part may be swinging free in thebooth or if the high-voltage cable to the gun breaks. All resistive systems do this withno monitoring circuit. Most systems today are fully resistive and require no monitor.Bells or discs are an exception. Automatic systems typically operate at a maximum of 90,000 V, while handheldunits can operate between 20,000 and 90,000 V. Although the voltage is high, theamperage is very low. Current draw increases as the electrode nears a ground path.Safety monitoring circuitry will shut down the generator if the current draw reachesapproximately 150 µA. It would take much more current draw to create a potentialgreat enough to present a risk of injury. The high voltage at the electrode will vary depending on the amount of current orresistance encountered between the generator and the electrode. With a resistance-freesystem, the voltage measured at the tip and at the generator are the same. In actualpractice, the cable, the electrode, and the coating itself provide some resistance. Not all coatings have the correct resistivity needed for electrostatic application.When a company changes from conventional air-atomized spray to electrostatic spray,they should inform their paint supplier(s) of the change so that they can conﬁrm thatthe paint material is compatible with electrostatic application. If the resistance is toolow, it will draw more current from the power supply, reducing the electrode voltage.If the resistance is too great, the electrostatic attraction is diminished and coatingtransfer efﬁciency and wrap will be poor. With some equipment, the generator is located in a control panel and the signalto the gun is a high-voltage signal. Some systems use a cascade multiplier in the gunbarrel. A low-voltage signal, typically 20–25 VDC, from an external power sourceis carried to the gun barrel where it is multiplied to the required gun tip kV. Thelow-voltage cable is much more lightweight and more ﬂexible than a high-voltagecable used in external systems. Some spray guns have an alternator in the spray gunthat puts out low AC voltage that is converted to the same low-voltage DC that otherunits send from the power supply. These systems typically have an on/off switch onthe back of the spray gun, so voltage can be shut off for ﬂushing and maintenance. The use of electrostatic systems with waterborne coatings presents a challenge.The coating material is so conductive that it will carry current through the ﬂuidsupply lines to the coating container, creating a potential hazard and reducing transferefﬁciency. Isolation systems are used for safety reasons and for optimum system per-formance. Isolation stands were ﬁrst used to protect workers from the “hot”container. An isolation stand is constructed of a nonconductive material that keeps
Liquid Paint Application Systems 129 Spray booth Isolation cage Paint Power supply supplyFIGURE 6.20 Isolation cage for waterborne electrostatic spray application.the container and the ﬂuid supply hose away from ground and typically, they areenclosed in a cage where operators cannot access the container without automaticallygrounding the system. An isolation cage used with a waterborne coating is shown inFigure 6.20. An alternative to isolation of the ﬂuid supply is a voltage-block system. One typeof voltage-block system features two single-stage, pneumatically operated reservoir-type pumps, one as a transfer pump and the other as a spray pump. Shuttle valveswith quick-connect couplings connect the pumps during operation. The electrostaticgenerator supplies voltage to the spray pump and the pump transmits a charge to thecoating material. During operations, the shuttle valves alternately connect the transferpump to either the grounded paint-supply source or to the electrostatically chargedspray pump. Another type of voltage block system has a pneumatically actuated rotary valvethat works in conjunction with a material supply chamber to ﬁll the valve and rotateit to an isolated area in the valve to supply coating to the electrostatic applicator.An isolation material is used to constantly wash the rotary valve and create isolationbetween the coating supply containers. In both cases, the shuttle valves provide an air gap to maintain electrical isolationbetween the charged coating material and any grounded material or equipment. Thesearrangements provide a continuous ﬂow of charged material while keeping the chargeisolated from the ﬂuid supply. Another alternative to an isolation system is an externally charging electrostaticgun or bell. This type of applicator has charging probes located on the exteriorof the applicator. The external probes allow the application of waterborne paintselectrostatically without isolating the paint supply. In many cases, the voltage is adjusted to its maximum output level. However,many coatings, particularly, light metallic coatings, operate better at lower voltage.Coverage problems, such as edge build-up, can usually be resolved by adjustmentsto triggering points, shaping air, gun-to-target distance, and so forth.
130 Paint Technology Handbook TABLE 6.5 Solvent Polarity Non or Low Polarity Medium Polarity High Polarity Mineral spirits Ethyl acetate MEK, MIK, acetone VM and P naphtha Butyl carbitol Isopropyl alcohol SC-100, SC-150 Ethyl alcohol Xylol, toluol Methyl alcohol Butyl acetate Methyl acetate6.6.2 COATING FORMULATION FOR ELECTROSTATIC APPLICATIONIn handheld systems, the polarity of the solvent should provide a coating that isstable under voltage at above 10 meg-ohm cm3 (typical). For efﬁcient application, itis usually recommended not go beyond 200 meg-ohm cm3 (see Table 6.5). Addition of polar solvents may be necessary when the coating is so dead, or sononconductive that without the solvent it will not accept a charge. Electrostatic systems require special care and maintenance practices. All parts ofthe system must be kept clean, including the outside surfaces of the ﬂuid hose andspray gun. Any possibility of a direct path to ground, resulting in a system shut down,must be eliminated. The exterior of the gun must be kept clean of overspray thatwill allow the voltage to “track back” to the operator who provides a great groundpath. Automatic systems are even more demanding with regard to system cleanliness,because they operate at even higher voltages. Advantages and disadvantages of electrostatic spray.6.6.3 ADVANTAGES • Material savings due to electrostatic attraction and wrap; more material on the parts, less on the ﬁlters • Reduced VOC emissions • Reduced booth cleaning and frequent ﬁlter changes • Increases in production rates • Reduced equipment wear because of lower ﬂuid and atomizing air pressures6.6.4 DISADVANTAGES • Minor coating adjustment may be necessary. • The part must be conductive to ground or must be prepped with a solution that will provide a ground path. • Conveyors and parts carriers must be well grounded and kept clean. • The relatively high cost of an electrostatic gun compared to that of a conven- tional air atomized gun or and HVLP gun. Efﬁciency should still provide the necessary return on investment (ROI).
Liquid Paint Application Systems 131 An electrostatic spray system can be a great advantage in increased transfer efﬁ-ciency, reduced VOC emission, reduction of labor, and reduced coating usage. Onthe other hand, if it is not fully understood, not properly used, or not maintained, itcan become an expensive air-spray gun. There are a few simple rules to remember in order to use an electrostatic systemeffectively and safely. • The parts being coated must be electrically conductive to ground. • Part carriers, racks, ﬁxtures, carts, and so forth must be designed to provide a consistent ground path, and must be kept clean in order to maintain a good ground path. • All items in the vicinity of the spray booth must be grounded. They can develop a static charge and discharge it to ground. A spark may ignite volatile vapors. • The spray operator should never wear gloves that isolate them from the grounded gun handle. If gloves are worn, they should be designed with a conductive palm or a hole should be cut that allows skin to contact the gun handle. In addition, metallic objects, coins, watches, keys, and so forth that are normally kept in pockets should be removed as they, also, can build up a static charge. Rubber boots or insulated shoes should not be worn; leather soles will dissipate any static charge. • Flooring in and near the spray booth should be conductive. In older build- ings where wooden ﬂoors are still found, sheet metal should be used as a covering, making sure all pieces are mechanically connected to one another and the booth walls. • It is very important that only items designed for electrostatic spray be used. Air hoses should contain a ground wire built into the jacket. Air or ﬂuid moving through the hose can create a static charge. Be sure to use the proper high or low-voltage cable for your gun. Do not mix brand “A” with brand “B”. • The voltage should be turned off before servicing or cleaning the electrostatic device. If the gun has a built in cascade type generator or multiplier, the atomizing air must also be turned off. Be sure the gun is wiped clean and that no solvent remains in the ﬂuid line before turning on the voltage.6.6.5 AUTOMATIC SPRAY EQUIPMENTAutomatic spray equipment can add substantial capability to a system by increasingthe amount of coating that can be delivered in a given time and controlling the volumeof output. Automatic application reduces the labor required for application and itcontributes to the consistency and quality of the product. Many factors enter into thedesign of a paint application system and contribute to the decision to apply paint withmanual equipment only or add automation to the process. The beneﬁt of using automatic equipment is the ability to use any number ofapplicators in one spray zone and the consistency and repeatability of an established
132 Paint Technology Handbookautomatic application program. An individual sprayer can apply a limited amount ofmaterial to a surface in a given amount of time. An automatic spray station is limitedonly by how many applicators are in use for that spray station. The chief reasonswhy a company will invest in automation are to produce more volume, achieve moreconsistency, and save money through reduced material usage and reduced labor cost. Operation and maintenance of an automatic system requires a higher skill levelthan a manual spray operator. Instead of a quick adjustment of the ﬂuid and air pressurefrom a pressure tank or the fan spray pattern at the back of the gun, the operator willbe responsible for several important controls. Depending on the level of automationand electronically controlled functions, the operator will need to at least monitor andmaintain • Applicator operation • Fluid ﬂow controls and components • Equipment programming • Applicator movers • Material supply system • Safety interlocks Once they have been properly set, automatic gun settings should not be continuallyadjusted, but they should be routinely monitored. In spite of the added responsibilityand skills required for their operation, automatic application equipment can provideneeded volume and superior control. An automatic application system can coversubstantially more area than a single manual operator. In order to take advantage of the additional capacity, the application equipmentmust be installed with complimenting control equipment and it must be well main-tained, workers must be well trained, and good scheduling practices must be in placeto ensure that the system capacity is used. Racking arrangements must be more pre-cise and consistent to get the best transfer efﬁciency. Part recognition systems mustbe well designed and maintained to make sure that the guns are triggered accurately. There are many different models and types of automatic application equipmentfrom many different manufacturers, but they break down into three main categories;air-spray guns, bells, and disks.188.8.131.52 Automatic Air-Spray GunsAn automatic air-spray gun closely resembles a manual spray gun without a handleand manual trigger. It may be mounted in a stationary position or designed for use witha reciprocator or robot. They have one or dual spray heads and different spray anglesto best ﬁt the application. Automatic spray guns are triggered by a part identiﬁcationsystem that “reads” the position and size of the part as it approaches and turns theguns on and off at the appropriate times. A more detailed triggering system usesa manually entered part number or style code at a manual input station (MIS) thatutilizes a detailed application program that is speciﬁc to that part style and color. Fluid tips and pattern shapes can be changed for different applications, makingthese guns ﬂexible for a variety of products and paint materials. Air-spray guns will
Liquid Paint Application Systems 133typically provide better penetration into recesses than a bell or disk. Typical transferefﬁciency can be very good, if parts are properly racked and the triggering programsare well deﬁned. However, the air pressure required for atomization can result inmore overspray than a bell. The bell atomizes the paint in a ﬁner droplet and morenarrow range, so the grounded part is able to attract a higher percentage of the paintsprayed. The bell also has a lower forward velocity, so the paint is less likely to becarried past the target by the force of the spray.184.108.40.206 Rotary AtomizersA system that uses a “bell” (rotary atomizer) or a disk is sometimes referred to as atrue electrostatic system. The rotating bell or disk provides the atomization, and thehigh voltage causes the coating to go to the part. The rotation of the bell or disk causesthe paint to move parallel to the target with the voltage off and the high-voltage ﬁeldredirects the atomized droplets toward the target. Shaping air is also used with bells tocontrol paint pattern size and aid penetration into recessed areas. Shaping air is usedto direct the droplets toward the part where electrostatic attraction helps to draw thepaint droplets onto the target. Figure 6.21 shows atomized paint at the edge of a bell. Bells range in size from about 15–70 mm in diameter. Rotational speeds areanywhere from 10,000 to 60,000 rpm. Usually, a smaller bell diameter will have afaster rotational speed. The bell can be fed from a pressure pot as shown in Figure 6.22or from a larger container. Typically, a faster rotational speed will provide more ﬁnely atomized paint. Highsolids and waterborne coatings may be difﬁcult to atomize at rotational speeds below15,000 rpm. The charged paint droplets will take the shortest path directly to the part. Althoughthis provides high transfer efﬁciency, it can cause some difﬁculty in coverageFIGURE 6.21 Paint ﬁlaments from the serrated edge of a rotating bell.
134 Paint Technology Handbook Air Air High voltage cable 110 V Bell Electro- Fluid static high voltage supply High voltage cableFIGURE 6.22 Electrostatic bell system.inside recesses. When the paint takes the shortest, most direct route to ground, it willbe more likely to build on the ﬂatter surfaces and the edges. Any crevices, interiorcorners, or complex shapes will be difﬁcult to coat due to electrical resistance. With a bell, the charged droplets in the air do not travel to the part with muchvelocity. Without the force of compressed air to drive them into the crevices andcorners, manual touch up may be the only way to achieve the necessary coverage. If the product is ﬂat sheet steel, the transfer efﬁciency will be extremely high andthe ﬁlm buildup will be very even without touch up. Voltage or triggering adjustmentscan be made to overcome excess buildup on the edges. Most bells use air as the bearing surface for the shaft that turns the bell. Air ispressurized between 60 and 100 psi and delivered between the high precision bearingsand the shaft, creating a thin but very stiff cushion of air. The shaft can rotate on theair cushion, free of metal-to-metal contact. On a bell, the ﬂuid is normally fed through a tube down the center of the turbineshaft where it ﬂows evenly over a cone at the back of the cup. The centrifugal forceof the rotating bell evenly disperses the ﬂuid to the edge of the rotating cup. The ﬂuidpasses through small holes on the outside of the bell, it is centrifugally atomized andattracted to the grounded work surface by electrostatic attraction. The shaping air isdirected from an opening behind the bell to provide pattern control from 15′′ to 48′′in diameter. The inside of the bell is shown in Figure 6.23. A bell is often used on applications where the best appearance on the part isrequired. A bell atomizer virtually eliminates “mottling” and produces less “orangepeel” than other automatic applicators. The bell can be mounted on a single or mul-tiaxis gun mover or it can be used on a robotic arm to obtain more than three axis ofmotion. Disks are much larger in diameter and they spray perpendicular to the target.Increasing or decreasing the rpm of the rotary atomizer controls the droplet size ofatomized paint. The disk sizes can range from 6′′ to 12′′ in diameter. Like the bell,the larger diameter disk usually has a slower rotational speed. As mentioned previously, an automatic spray gun employs compressed air todeliver the paint to the part. It will provide somewhat better penetration of the Faradayareas and deep recesses but has the potential to generate more overspray. It is important
Liquid Paint Application Systems 135 Voltage cable Bell cup Shaping air supply Center feed fluid delivery tubeFIGURE 6.23 Inside of a rotary bell.to consider this and compare the efﬁciency of a bell or disk and the related touch-uprequired to that of an automatic electrostatic spray gun when planning a system.Testing is important to see just what device works best. Typically, a bell works well for simpler geometries requiring high transfer efﬁ-ciency and even ﬁlm or for the ﬁrst application in a multiple application process. Anair-spray gun may be the best application device for more complex geometries or forcut-in and touch-up. The combination of automatic electrostatic and hand spray will always be morecost effective than a hand-spray-only operation. The return on investment for theautomatic equipment will vary with the application. Jobs that have very low pro-duction rates may not be candidates for automation. However, process consistencyimprovements can provide greater ﬁrst time quality and often justify the cost.220.127.116.11 Automatic Spray Supporting EquipmentAutomation requires much more than just the correct selection of applicationequipment. There are many small but important application equipment and ﬂuidﬂow control components. Multiple gun stations must be designed for accurate andcontrollable ﬂow of air, ﬂuid, voltage, and movement. Hoses must be kept as smalland as short as possible for quick color change and low material waste. Color changemanifolds should be located near the spray station so that the purge of material fromthe supply line is quick and there is very little material in the line. Color change pro-grams should be written to fully utilize the material from the color change manifoldsto the applicators to further reduce waste and color change time.18.104.22.168 Gun MoversAutomatic guns are sometimes mounted in a stationary position. More often, theyare mounted on a reciprocator or robot. There are long-stroke (Figure 6.24) andshort-stroke reciprocators with vertical or horizontal movement. There are multiaxisgun movers that can move the guns in three dimensions: in/out, up/down, and inthe direction of the conveyor. Moreover, there are robots (Figure 6.25) that can
136 Paint Technology HandbookFIGURE 6.24 Long stroke reciprocator with bells. Grid scale: 1 block = 100 mm (3.9″) 3 5 95° 4 LH wrist configuration 6 660 mm 2 134.0 mm (26.0″) (5.3″) 1200 mm 150 mm (47.2″) (5.9″) 1 390 mm 320 mm 2040 mm (15.4″) (12.6″) (80.3″) 2229 mm 860 mm (87.8″) (33.8″) 873 mmPedestal mounted robot with (34.4″) six axis of motion 363 mm (14.3″)FIGURE 6.25 Movement of robotic arm.move the gun in multiaxis patterns similar to a manual operator but with much moreprecision. The use of a gun mover is product dependent. They can help the guns to covermore surface of product and get into deep recesses, such as cars, ofﬁce furniture, orappliance shells.
Liquid Paint Application Systems 137 One important thing to consider is that the machine selected is a durable pieceof industrial equipment. Examine the construction and motion design to make surethat it is solid and will last. These machines will be expensive, so the testing must bethorough. The stroke of the machine must be electronically integrated with the productand the line speed and controlled accordingly to avoid irregular patterns on the partsurface. Establishing the correct stroke distance and stoke speed based on the linespeed, surface to be covered, and desired ﬁlm thickness will provide uniform coatingapplication. Reciprocator mounting bars can be conﬁgured with a variety of patterns for dif-ferent products. They can be mounted over the top of product on a ﬂoor-mountedconveyor or in vertical positions to coat from the side. One short stroke reciprocatorcan hold a double bar of three or four spray guns or bells each. This kind of versatilityis one of the advantages of automation. Several guns can be brought to bear on theparts in a very short time span. The number and position of the guns can be designedto provide excellent coverage with low overspray.22.214.171.124 Robotic PaintingA spray gun or bell mounted on a robotic arm provides the advantages of manualapplication (focused application and multiaxis movement) with much more accuracyand consistency. This provides an opportunity for improved quality, productivity, andreduced labor. Robotic arms come in many different sizes with different control options. Atypicalsoftware driven controller can manage color change, provide analog ﬂuid and aircontrol, part queuing, arm homing, conveyor synchronization, path and functionediting and simple lead through, and Cartesian teaching methods. With a slim wrist design, the robotic arm can provide 360◦ of roll and 90◦ of pitchand yaw with ﬂexible spatial coverage. Large, complex parts can be painted veryeffectively with exceptional precision using a robotic arm.126.96.36.199 SummaryThere is a wide variety of automatic spray equipment for liquid paint application. It isvery important to conduct testing of the equipment to determine the best system fora given application. When the application devices are tested, it is also important to evaluate the ﬂuidﬂow control devises. A ﬂuid ﬂow control system or device may work very well withone type of material and work poorly with a different material. The equipment must becompatible with the ﬂow rate and viscosity of the material being sprayed. For example,a very low ﬂow rate with a lower solids material, such as two-component urethaneon plastics, will need a small, sensitive regulator to provide the necessary control. Ifthe material type and ﬂow rate are changed, it may be necessary to change regulators.Remember that all of the ﬂuid handling devices (regulators, static mixers, and ﬂowmeters) are not inﬁnitely adjustable or interchangeable. They will work well within acertain range of ﬂow, so you need the correct size for the ﬂow rate that will be neededfor a certain production line.
138 Paint Technology Handbook Always make sure that employees are well trained in the operation and mainten-ance of the spray equipment. Follow safety guidelines and keep up to date on newinnovations in equipment and control options.6.7 ALTERNATIVE APPLICATION METHODSIn addition to spray application, there are several alternative ways to apply liquidpaint to industrial products.6.7.1 DIP COATINGIn a dip coating application, the part is simply immersed in a tank of paint. Excesspaint drains back into the tank once the part is removed. Parts may be handled inbatches or with a conveyor. Dip tanks can be built in any size needed for small or large parts. Provisions mustbe made for circulation, ﬁltering, and control of temperatures and viscosity. Becauseof the ﬁre hazard involved, dip operations using ﬂammable paints must be equippedwith CO2 ﬁre extinguishing systems and dump tanks.188.8.131.52 Advantages of Dip Coating • Simple equipment • Low-skilled labor requirement • Easily automated • Close racking of parts • Various part shapes can be mixed • Little paint is wasted if the part is allowed to drip over the tank184.108.40.206 Limitations of Dip Coating • Viscosity control is critical. If the paint is too viscous, too much paint is used (wasteful) and ﬁlm thickness is too high. Low viscosity results in paint ﬁlms that are too thin. Consequently, corrosion resistance may be too low for primers and hiding power may be inadequate for topcoats. • Possible settling of the paint in the circulation system. • Gradual tank contamination is possible. Parts entering the tank must be clean and dry to avoid carrying in contaminants. • Some parts are hard to immerse, because trapped air keeps them aﬂoat. • Tanks must be large enough to immerse the entire part. • There is a ﬁre and toxicity hazard associated with large volumes of paint solvents. • Film thickness control is a problem. Paint may become trapped in recesses and drain slowly or not at all. On vertical surfaces, the paint tends to be thicker at the bottom of a panel than at the top. This is caused by an increase in viscosity as the paint loses solvent while draining. It often results in fatty edges that can later break off under thermal or mechanical shock.
Liquid Paint Application Systems 139 Conveyor Nozzle Part Spray riser Enclosure Pump Paint reservoirFIGURE 6.26 Flow coating. • The drain-off area must be cleaned regularly. Since this is usually done manually, some dried paint may fall into the circulation system and clog the ﬁlters, pumps, and nozzles.6.7.2 FLOW COATINGIn a ﬂow coating operation, the part is held over a tank and a stream of paint is pumpedover the part through a nozzle (see Figure 6.26). The excess paint drains into the tankand is recirculated over the parts. The variables that are important for ﬂow coatinginclude pumping, ﬁltering, viscosity, temperature, ventilation, and ﬁre control.220.127.116.11 Advantages of Flow Coating • Simple equipment • Little labor required • Easily automated • Dead air spaces can be coated if a stream of paint can be directed upward into the recess • Smaller volumes of paint are required, because the parts need not be immersed • Little paint is wasted if the parts are allowed to drain over the tank18.104.22.168 Limitations of Flow Coating • High solvent loss by evaporation. Solvent must be replenished on a regular basis. • Possible settling of the paint in the circulation systems. • Fire and toxicity hazards associated with the high solvent loss. • Inability to coat certain recesses and inside surfaces. • Gradual paint contamination if the paint rinses dirt, salts, oils, and so forth from the parts.
140 Paint Technology Handbook • Film thickness control is a problem. Paint may become trapped in recesses and drain slowly or not at all. On vertical surfaces, wedging may occur resulting in fatty edges. • The drain-off area must be cleaned regularly. Since this is usually done manually, some dried paint may fall into the circulation system and clog the ﬁlters, pumps, and nozzles. Dip and ﬂow coating methods should be considered when high production paintingof relatively simple shapes is required and quality appearance and corrosion resistanceis not important. Viscosity and ﬁlm thickness control are the major problems to beexpected. Efﬁcient use of paint and low labor rates are the primary advantages. These processes are limited to waterborne coatings because of environmental con-siderations. High-solids coatings do not lend themselves to these types of applicationbecause of the higher viscosities that cause poorer ﬂow characteristics and high ﬁlmbuilds. Paints with high solvent content produce too much VOC for most installationsand they create an unsafe working environment.6.7.3 ROLLER COATINGA roller coating operation is capable of coating large areas in the form of sheet orstrip at high speed and with a continuous and even thickness of paint or varnish. Therollers can also be used to laminate plastic ﬁlm to metal substrates. There are two methods of liquid transfer for roll-coating systems on ﬂat sheets.One system uses three rollers and the second uses four rollers. In the ﬁrst process, theliquid is fed between the feed and applicator rollers rotating in opposite directions.The stream of paint is then fed through the rollers onto the sheet. The third roller actsas a pressure roller to ensure that the sheet comes into correct and even contact withthe wet applicator rolls (see Figure 6.27). In the four-roller process, a fountain roller picks up liquid from a trough, transfersit to the feed roller, which in turn presses it to the applicator roller. The fourth rolleracts as the pressure roller, as in the three-roll system. In coil coating applications,where both sides of the sheet are coated, the four-roller system is used. The applicatorrollers act as pressure rollers. Fountain and feed rollers are normally made of stainless steel, while theapplicator roller has a steel core covered with a rubber, gelatine composition, or 2 1 1. Feed roller 3 2. Application roller 3. Pressure rollerFIGURE 6.27 Roll coating.
Liquid Paint Application Systems 141polyurethane face. These surfaces become deformed during use and need to beremachined to offer a continuous smooth surface. Gelatine rollers are resistant tomany organic coatings but are not resistant to water-based coatings. Polyurethanerollers produce a solvent and abrasion resistant surface. They are normally found asapplicator rollers on fast running coil coat lines.22.214.171.124 Advantages of Roller Coating • Smooth, even, dust and “fat edge” free ﬁlms can be produced • Films dry relatively quickly • No excessive solvent or paint losses due to evaporation occur • There is no ﬁre hazard126.96.36.199 Disadvantages of Roller Coating • Limited to thin sheet stock • Not able to apply the variety of ﬁnishes used in spray coating6.7.4 CURTAIN COATINGCurtain coating is a sophisticated method of pouring a continuous ﬁlm of lacqueror paint over ﬂat sheets. The sheets are conveyed under a trough with an adjustableslot. The trough acts as a pouring head and control of the gap regulates the volumeof material, controlling the ﬁlm thickness deposited on the sheets. Curtain coatingworks well for coating ﬂat sheets of metal or wood. A second conveyor moves the coated panel away from the gap. Initial applica-tion efﬁciency is excellent and any material that does not adhere to the product isrecirculated to the trough by means of a pump. In some instances, moisture-containing substrates are prewarmed in a tunnel priorto coating. The warm panel aids the set-up characteristics of the paint or lacquer. Analternative is to heat the lacquer with a heat exchanger located between the reservoirand trough. The most important part of curtain coater is the adjustment slot (or gap) in thetrough. The gap can be accurately controlled to develop predetermined ﬁlm weights.The trough and slot must be kept scrupulously clean, because any dirt or solid materialwill break the curtain and cause a surface defect.
7 Transfer Efﬁciency and Spray TechniqueTransfer efﬁciency is the measurement of the percentage of the paint material sprayedthat provides coating on the parts versus the percentage that is lost in the spray process.The type of spray gun is very important, but it is only part of the picture. The extent ofautomation and electronic control equipment, the cleanliness and maintenance of thesystem, the skill and training of the operator, the coating material, the product beingsprayed, the ﬂow rates, and spray booth air velocities will affect the transfer efﬁciencyof any spray equipment. Table 7.1 provides a comparison of different technologies inﬁeld and lab tests, and shows the relative transfer efﬁciencies of each.7.1 SPRAY GUN CONTROLSThere are several related adjustment points on a gun that allow the operator to controlthe size and shape of the pattern, the amount of atomization, and the amount of ﬂuidcoming out of the gun. For manual guns, there are typically two adjustments located at the rear of thegun handle. One knob will adjust the amount of air going to the air nozzle, providingcontrol of the size and shape of the pattern. The other knob adjusts the ﬂuid needletravel, allowing more or less ﬂuid ﬂow. The ﬂuid volume should not be adjusted withthe knob on the gun unless the gun is being used with a siphon system. Adjustment TABLE 7.1 Transfer Efﬁciency of Liquid Paint Spray Equipment Spray Process Transfer Efﬁciency(%) Conventional air spray 15–40 Conventional airless 20–50 Conventional air-assisted airless 30–60 Conventional HVLP 30–60 Electrostatic airless 40–70 Electrostatic air spray 40–80 Electrostatic air-assisted airless 50–85 Electrostatic HVLP 60–90 Electrostatic bell atomization 70–95 Electrostatic disk atomization 80–95 Electrical atomization 95–98 143
144 Paint Technology Handbookby ﬂuid needle travel is unstable and causes premature wear to the needle and seat. Ifa spray gun is used with a pressure system, then the ﬂuid ﬂow should be controlledwith the ﬂuid regulator, and the knob should be left in the full open position. Adjustment starts by following the manufacturer’s recommendations for needleand nozzle selection from their charts. The charts will indicate the proper range ofﬂuid and air pressures. The ﬂuid pressure is set from the chart and the atomization pressure is addeduntil the pattern is uniform and consistent. A good starting point for the atomizationpressure could be as low as 5 psi. The pattern can then be tested to see if the paintis properly atomized and additional pressure can be added if it is needed. Excessatomization air will generate more velocity and reduce transfer efﬁciency. If the atomization is not ﬁne enough, the air pressure should be increased abouttwo or three pounds at a time and tested each time it is increased. Once the correctamount of atomization is reached the pattern size and shape can be adjusted with thepattern adjustment knob on the spray gun. The normal position for the ears on the air cap is parallel to the ﬂoor to producea vertical fan pattern. This assumes spray gun movement from left to right. To createa horizontal fan spray pattern, the operator can turn the ears or turn their wrist 90◦ . Usually, when the ﬂuid pressure is increased it is necessary to increase the atom-izing air pressure. The two air pressure controls are adjusted to provide the correctvolume of material with uniform atomization and a minimum of velocity. The bestoverall delivery pressure is always the lowest pressure that will adequately providethe correct volume of paint and the correct atomization. If the atomizing air is too high relative to the amount of ﬂuid being delivered,it may produce excess velocity and dry spray. If it is too low, the ﬂuid droplet sizemay be too large (inadequate atomization) and the surface may have orange peel. If too much ﬂuid is applied, the ﬁlm may be too heavy with more risk of sags. Ifthe amount of ﬂuid applied is too low, it may cause lightly coated areas on the partand dry spray.7.2 APPLICATION TECHNIQUEIt is possible to do several things wrong and still produce a good ﬁnished product.However, proper technique will improve the quality of the ﬁnish, reduce overspray,reduce labor, and increase the life of the spray equipment. Proper technique begins with an examination of the spray gun. A brief inspectionof the system may ﬁnd some detail that needs to be adjusted before the gun is triggered.Some of the things to look at include 1. Is the trigger easy to pull back, and does it return smoothly and quickly when released? 2. Are the air and ﬂuid nozzles properly installed? 3. Are the ﬂuid and air hoses the correct size? 4. Is the ﬂuid hose free of pinch points? 5. Are the hose connections tight?
Transfer Efﬁciency and Spray Technique 1457.2.1 ATOMIZATIONAfter the system inspection has conﬁrmed that the gun is ready for spraying, a testpattern should be sprayed on cardboard. A full oval shape with an even distributionof paint is needed to produce a quality ﬁnish. Spray enough paint on the cardboardto allow it to run. The runs should be equal all across the pattern. If the runs areheavier on one side of the pattern, the air cap may be defective. Rotate the air cap180◦ and respray the cardboard to see if the heavy runs shift sides. If they do, replacethe air cap. The amount of paint delivered to the gun tip is determined by the amount ofproduct to be painted and the time available to spray it. The amount of atomizingpressure is determined by how much energy it takes to break up the paint stream intoa uniform pattern. The best spray pressure is the lowest possible level at which thejob can be done.7.2.2 GUN POSITIONA spray gun needs to be held at a constant angle to the part to help apply uniformﬁlm buildup. If the spray gun is tilted, the distance between the nozzle and the partsurface is not consistent, and ﬁlm deposition will not be uniform. More paint at agreater velocity will contact the part in the one area of the pattern. This causes poorhiding and dry spray at one end of the pattern and heavy ﬁlm at the other. This tiltedposition is sometimes referred to as heeling or toeing the gun (see Figure 7.1).FIGURE 7.1 Improper stroke, tilting.
146 Paint Technology HandbookFIGURE 7.2 Improper stroke, fanning.FIGURE 7.3 Proper spray stroke. Heeling/toeing is an easy way to recognize technical error and one that is easilycorrected. Figure 7.1 shows the incorrect position. Proper application requires a levelstroke. Another common error is arcing or fanning the spray gun from side to side(see Figure 7.2). This will occur when the operator hinges the spray gun from the elbowinstead of the shoulder and wrist. The pattern is not kept at the same distance fromthe product during the entire spray stroke, and the ﬁlm deposits heavy in the centerand light at the edges. Proper spray application requires the use of the wrist, elbow, and shoulder workingtogether during the stroke. The average spray stroke is 36′′ . The arm moves side toside in a horizontal motion. The wrist must be ﬂexed as the arm strokes from side toside, attempting to maintain a consistent gun-to-target distance (see Figure 7.3). Theproper spray stroke will produce the most uniform ﬁlm with the least risk of runs,sags, or dry spray.7.2.3 GUN DISTANCEGun distance and gun speed are also very important factors in spray accuracy anduniform paint application. The distance from the nozzle tip to the product affects thewetting of the paint and the appearance of the coating.
Transfer Efﬁciency and Spray Technique 147FIGURE 7.4 Improper gun-to-target distance. Solvents evaporate as the coating leaves the gun. The correct gun-to-targetdistance works in harmony with the speciﬁc solvent blend in the coating and providesthe proper “wetness” when the coating hits the target. If the gun is too far from theproduct, there is more risk of dry spray. If the gun is too close to the target, the ﬁlmmay sag (see Figure 7.4). If the distance between the spray gun and the target increases or decreases, thewetness of the paint ﬁlm will be affected by the evaporation rate of the solvents inthe paint blend. The typical distance from the target for hand spray is 6′′ –12′′ . Eachcoating may have a slightly different distance that seems to work best, and the spraygun and gun adjustment will also affect the wetness of the ﬁlm. It is important to beas consistent as possible while stroking the gun.7.2.4 GUN SPEEDAnother important factor in accurate ﬁlm deposition is speed of the stroke. The strokespeed of the spray gun should be kept consistent for the best material utilization andto conserve the energy of the operator. The “gyroscopic painter” technique should be avoided. Excessive pivoting of thespray gun uses more paint material than necessary, makes a mess of the booth wallsand ceiling, and wastes energy. The correct speed allows for an even wet ﬁlm of material to be applied in onestroke. If the stroke is too slow, it may cause sags and runs, solvent pop may occur,
148 Paint Technology Handbookand it is more difﬁcult to keep up with production. If the stroke is too fast, it maycause dry spray, uneven ﬁlm buildup, and exhaustion of the operator. Gun speed should be maintained at a comfortable and even pace. The ﬂuid pressureand the air nozzle pressure are set to work in harmony with the speed of the stroke.7.2.5 LAPPINGThe gun stroke should be overlapped in a precise pattern to ensure complete anduniform coverage. The amount of the spray pattern that is overlapped should be 50%of the total pattern width. If the gun delivers a 12′′ pattern for each spray stroke andeach stroke overlaps by 6′′ , it is called a 50% overlap. The center of the spray patternis aimed at the wet edge of the previous stroke (see Figure 7.5). Sometimes a spray pattern is “crosshatched” to build additional ﬁlm thickness andto provide uniform thickness and coverage. Crosshatching refers to a pattern that isstroked vertically and then horizontally. The spray gun should be triggered before the pattern reaches the part and releasedafter the pattern leaves the part to avoid a heavy area. Triggering on the part will leavea large deposit of material in one area, because the coating will not be fully atomizedfor a split second after the trigger is pulled. The size of the spray pattern should be related to the part being coated. Largepanels can be efﬁciently coated with a full pattern. For slender work, the patternshould be small enough to avoid excessive overspray. In order to apply an even ﬁlm, the spray pattern must be uniform. It is useful tospray a sample pattern on a piece of cardboard to make sure that there is no problemwith the ﬂuid nozzle or air cap. Some examples of faulty spray patterns are shown inTable 7.2. When coating a large panel, the conventional method is to cover the surface withhorizontal strokes. The stroke starts about 6′′ off the part, and the trigger is pulled The first stroke is aimed at the edge of the panel The center of a stroke is aimed at the wet edge of the last strokeFIGURE 7.5 Proper overlap stroke.
Transfer Efﬁciency and Spray Technique 149TABLE 7.2Spray Pattern ProblemsPattern Cause Correction 1. One of the side ports of 1. Use paint thinner to the air nozzle is clogged remove dried paint; do not probe into the holes with anything harder than brass 1. Fluid build up on one side 1. Remove air nozzle and of the ﬂuid nozzle wipe off ﬂuid nozzle 2. Damaged ﬂuid nozzle 2. Replace damaged ﬂuid nozzle 1. Air pressure is too high 1. Reduce air pressure 2. Spray pattern is too wide 2. Reduce fan width 3. Fluid pressure is too low 3. Increase ﬂuid supply 1. Air pressure too low 1. Increase air pressure 2. Excessive ﬂuid velocity or 2. Use smaller ﬂuid nozzle too much ﬂuid oriﬁce, reduce ﬂuid pressureSpitting 1. Loose ﬂuid nozzle 1. Tighten ﬂuid nozzle 2. Fluid needle not seating 2. Clean ﬂuid nozzle seat (dirt) area 3. Loose or missing packing 3. Tighten packing nut or nut or dried ﬂuid packing replace missing or dried ﬂuid packing 4. Fluid connection is loose 4. Tighten all ﬂuid supply connections leading to the spray gunjust before the gun tip reaches the edge of the part. The trigger is released just afterthe gun tip moves off of the other end, and a new stroke begins in the other directionwith the gun moved down to produce a 50% overlap. The strokes can be vertical if the operator is comfortable with the motion and ableto produce consistent and uniform ﬁlm build. Coating the edge of the panel with parallel strokes can reduce the amount ofoverspray. The gun does not have to be moved off the edge of the part. An illustrationin Figure 7.6 shows this technique. A box shaped part should be coated on the corners ﬁrst, and then the ﬂat surfacesare covered with the same technique as a panel (see Figure 7.6).
150 Paint Technology HandbookFIGURE 7.6 Paint application on a corner. Cold paint inlet Heat transfer fluid Paint Hea t traPump nsfe Heat r flu Heating exchanger id element Heated er paint outlet id f flu ans Heat transfer tr at n fluid He tur Re Thermostat control Heated paint Heat transfer fluid to spray gunFIGURE 7.7 Paint heating system.7.2.6 HEATED SPRAYThe addition of an in line paint heater can provide several advantages, particularlyconsidering the high-solids content of a compliant liquid coating. The heater will notonly help to achieve a correct spray viscosity, but will also provide consistency so that
Transfer Efﬁciency and Spray Technique 151the paint is less sensitive to temperature, and the operator can apply a more uniformﬁlm without adding additional solvents. The spraying of heated paint enables the low boiling solvents to evaporate betweenthe spray gun and the surface, leaving the high boilers to level the material. Theincreased viscosity of the paint will allow more material to be deposited withoutsagging. Paint heaters can be ﬁtted for different types of application systems; they can beattached to a booth, or they can be portable for ﬁeld applications. There are several types of paint heaters that can provide consistent paint temper-atures at a speciﬁc ﬂow rate. A typical heater circulates heated water or oil througha heat exchanger. The paint is heated as it passes through the heat exchanger on itsway to the spray device (see Figure 7.7). Electric paint heaters are often used in medium to small paint supply andcirculation systems. Paint heaters are typically capable of raising the paint temperatureto 70◦ F from the temperature on the inbound side of the heater.
8 Spray BoothsA liquid spray booth is an enclosure around the spray operation that providescontainment of the oversprayed paint and controls the spray environment. The spraybooth includes an exhaust fan to create negative air pressure inside the booth. Theexhaust air contains the overspray, directs paint solids to the ﬁlters, and directs thesolvent vapors to atmosphere or an abatement system. The booth provides a cleanand safe environment for the operator and smooth airﬂow to enhance paint transferefﬁciency. For liquid spray systems, the airﬂow can be either vertical in a down draft designor horizontal in a cross draft design (see Figure 8.1). Airﬂow is necessary to containthe paint overspray by creating a slight negative pressure inside the spray booth.8.1 NFPA REQUIREMENTSThe agency that produces the standards that govern spray booth design and operationis the National Fire Protection Association (NFPA). NFPA 33 provides the safetyguidelines for spray booth construction and sets the standards for airﬂow and electricalrequirements. NFPA 33 requires that spray booths be substantially constructed of non-combustible materials and prohibits the presence of an open ﬂame or spark-producingequipment in a spray area. The dimensions of the “spray area” are deﬁned differently,if the ventilation system is interlocked to the spray equipment in a way that pre-vents operation of the spray equipment without ventilation. If the booth exhaust is Booth inlet airflow Exhaust Exhaust Booth inlet airflow Cross draft Down draftFIGURE 8.1 Dry ﬁlter spray booths. 153
154 Paint Technology Handbookinterlocked with the spray equipment, then electrical wiring or equipment within 5 ft(1.5 m) of the booth openings must be explosion proof or intrinsically safe. If theexhaust is not interlocked, the hazardous area extends to 10 ft (3 m). Spray booths are designed with sufﬁcient air turnover to maintain a solvent con-centration that is below 25% of the lower ﬂammable level (LFL) of the material beingsprayed. The LFL is the lowest ﬂammable concentration of a gas in air in which aﬂame can be propagated when given a source of ignition. This is also called 100% LFLand can be used interchangeably with %LEL (lower explosive limit) (see Table 8.1).Different solvents have different LFL values. TABLE 8.1 Lower Explosive Limit of Some Commonly Used Solvents ft3 /gal of Vapor of LEL in % by Volume of Solvent Liquid at 70◦ F Air at 70◦ F Acetone 44.0 2.6 Amyl acetate (iso) 21.6 (1) 1.0 Amyl alcohol (n) 29.6 1.2 Amyl alcohol (iso) 29.6 1.2 Benzene 36.8 (1) 1.4 Butyl acetate (n) 24.8 1.7 Butyl alcohol (n) 35.2 1.4 Butyl cellosolve 24.8 1.1 Cellosolve 33.6 1.8 Cellosolve acetate 23.2 1.7 Cyclohexanone 31.2 (1) 1.1 1,1 Dichloroethylene 42.4 5.9 1,2 Dichloroethylene 42.4 9.7 Ethyl acetate 32.8 2.5 Ethyl alcohol 55.2 4.3 Ethyl lactate 28.0 (1) 1.5 Methyl acetate 40.0 3.1 Methyl alcohol 80.8 7.3 Methyl cellosolve 40.8 2.5 Methyl ethyl ketone 36.0 1.8 Methyl n-propyl ketone 30.4 1.5 Naphtha (VM&P) (76◦ naphtha) 22.4 0.9 Naphtha (100◦ ﬂash) safety 23.2 1.0 solvent—Stoddard solvent Propyl acetate (n) 27.2 2.8 Propyl acetate (iso) 28.0 1.1 Propyl alcohol (n) 44.8 2.1 Propyl alcohol (iso) 44.0 2.0 Toluene 30.4 1.4 Turpentine 20.8 0.8 Xylene (o) 26.4 1.0
Spray Booths 155 NFPA also states that spray booth exhaust must have an adequate supply ofmake-up air to maintain proper operation of the exhaust system. Without air supply,there is a risk that the booth will lose its negative pressure and solvent vapors or paintsolids can escape the booth.8.2 AIR MAKE-UPAir make-up (AMU) systems are designed to supply air into the building or directlyto the spray booth. A fan draws outside air into the AMU housing and directs itthrough a discharge outlet into the building or directly into an air inlet plenum that isconnected to the booth. The volume of air should be adjustable for booth balancingpurposes. Dampers or variable frequency drives can be used for adjustment. Theair can be cooled or heated as needed. Humidity controls are also sometimes addedto the supply air. The AMU heater is often located on the roof of the building, butit may be mounted on the ground or suspended above the spray booth. The AMUshould be located far enough from the spray booth exhaust stack and in a positionwhere the vapors from the booth exhaust cannot be entrained in the AMU intake airstream.8.3 BOOTH EXHAUST STACKSThe exhaust stack height is affected by local environmental regulations, buildingheight, and the surrounding area. The exhaust stack should extend above the rooﬂinefor 30–50% of the building height to make sure that the exhaust is carried up intothe prevailing winds. A 20-ft building should have a stack height of 6′ –10′ abovethe roof. Stacks should be longer in areas with high buildings, tall trees, or other nearbyvertical obstructions. High neighboring obstructions can create low-pressure areasand interfere with the exhaust stream so that vapors and ﬁne paint solids may not becarried up into the prevailing winds.8.4 SPRAY BOOTH SIZINGThe interior work area of the booth can inﬂuence the transfer efﬁciency of the sprayedcoating and the ability of the spray booth to contain overspray. Spray booth sizingdepends on the size of the products to be sprayed, the equipment used to apply thepaint, and time required to achieve full coverage. Booths come in a variety of stocksizes from 4′ 0′′ W × 7′ 0′′ H × 6′ 0′′ D (work chamber) to 20′ 0′′ W × 10′ 0′′ H × 9′ 0′′ D.Many spray booths are custom fabricated to ﬁt the products that will be coated andpaint system. It is very important to make sure that a spray booth has enough area to efﬁcientlyapply the coating and maintain containment of the overspray. There are some verypractical guidelines to booth sizing that can help with selection. In some spray operations, the part is moved into the booth without an overheadconveying system. A small batch operation may use carts to bring parts into the booth.
156 Paint Technology HandbookA large truck frame or a piece of heavy equipment may be moved into a booth ontrack in the ﬂoor. These batch systems require a booth that is large enough to allowfreedom of movement around the part and clear access to all surfaces with enoughroom for the equipment, the part, and the operator. Conveyorized systems will have an overhead or ﬂoor mounted conveyor thataffects the booth sizing. Adequate vertical height, width, and depth are required tomake sure the booth functions properly.8.4.1 SPRAY BOOTH HEIGHTThe product being painted should be no lower than 30′′ off the ﬂoor so that the operatordoes not have to bend too much and the bottom of the part is accessible. From the topof the part to the hook site should be at least 30′′ in an electrostatic operation to avoidpainting the hook, and 36′′ is preferred. In a nonelectrostatic operation, the conveyorshould be at least 30′′ above the spray zone to avoid painting it.8.4.2 SPRAY BOOTH WIDTHThe width of the booth is related to the number of spray stations in the booth andthe size of the part to be coated. Each automatic spray station should be at least 4′ 0′′away from the booth walls or another station. Therefore, the minimum booth width(working chamber) for one automatic spray station is 8′ 0′′ . The minimum for twospray stations is 12′ 0′′ wide. This applies to conveyorized systems running at someproduction line speed. Very small batch operations, or conveyors at very slow speeds,can use a 6′ 0′′ wide booth for manual application.8.4.3 SPRAY BOOTH DEPTHThe depth of the work chamber is related to the thickness of the product. The productneeds to be kept at least 3′ away from the exhaust ﬁlter bank in a cross draft booth,and there must be adequate space for spray stations or manual operators to movefreely.8.4.4 INTERIOR WORKING DIMENSIONSThe sizes indicated above are minimums. In most cases, it is helpful to provide morework space so that no paint is lost from the booth interior and the ﬁlters are not tooclose to the spray guns. Containment of paint overspray can be assisted by the addition of entrance andexit vestibules that proﬁle the opening into the booth. In manual operations, the part size and line speed make a larger width necessaryto give the operator time to spray. In the case of two manual sprayers in the samebooth, 5–6 ft should be left between the sprayers and 5–6 ft from the booth wall. Also,manual spray operators tend to start spraying as soon as the part enters the booth, soan entrance and exit vestibule of at least 3′ 0′′ is recommended to help keep oversprayinside the booth.
Spray Booths 1578.5 SPRAY BOOTH EXHAUST SIZINGThe spray booth exhaust, measured in cubic feet per minute (CFM), is determ-ined by multiplying the width of the working chamber times the height, timesthe recommended air face velocity. Typical face velocity in a spray booth is100–120 feet per minute (FPM) for manual spray operations and 50–80 FPM forautomatic spray operations. Fans are often sized bigger to allow for paint load in the ﬁlters during production.As ﬁlters load with paint, the face velocity drops and the booth may not be able toproperly dilute the air and prevent solvent accumulation or contain overspray. A booth that is 10′ 0′′ wide × 10′ 0′′ high used for manual painting would require12,000 CFM with clean ﬁlters (10′ ×10′ ×120 FPM = 12,000 CFM). If the booth hasproduct openings, the square footage of opening should be multiplied by 100 FPMand added to the total CFM. For example, with a 2′ × 5′ product opening in each sideof the booth, the additional air needed for the booth is 2000 CFM. 2′ × 5′ product opening × 2 (one on each side) × 100 FPM = 2000 CFM The air volume for the booth openings is added to the volume needed to supplythe required face velocity to get the total exhaust volume. 12,000 + 2,000 = 14,000 CFM total8.6 FILTRATIONExhaust ﬁltration is designed to capture paint solids and allow solvent vapors topass through into the exhaust air stream. The exact ﬁlter arrangement is related tothe process requirements, the material being sprayed, application equipment transferefﬁciency, and amount of overspray. Bulk media is less expensive and easier to deal with than ﬁlter pads or bag ﬁlters.Many systems use two layers of ﬁlters to provide the needed particulate arrestingefﬁciency while keeping the overall cost down and simplifying ﬁlter change. Theﬁrst layer of ﬁlters is less expensive. It is designed to collect the bulk of oversprayand is less efﬁcient on the small particle sizes. The second ﬁlter layer is much moreefﬁcient on the small particle sizes and initially more expensive. This arrangementallows the operator to replace the lower cost media more frequently while extendingthe life of the high efﬁciency second-stage ﬁlter. A typical arrangement would bea 90% + efﬁcient bulk media over 99% + efﬁcient bag type ﬁlter. The ﬁltrationefﬁciency must effectively remove nearly all of the particulate from the air stream toprotect downstream equipment and the environment. In a dry ﬁlter booth, NFPA requires that a manometer or magnahelic ﬁlter gaugebe installed on the exhaust ﬁlters to measure pressure drop. A typical setting for thisﬁlter gauge might be 0.25′′ of water, as measured in inches of water column (WC),although this will vary dependent on how the fan was sized, booth velocity, and ﬁlterresistance.
Spray Booths 159 As the ﬁlters become loaded, the pressure will drop and the gauge will move up.When the ﬁlters reach a load level that restricts airﬂow, they are overloaded and needto be replaced. The point at which this happens should be noted on the ﬁlter gauge andthe ﬁlters should always be changed before they reach that level. If the ﬁlters seem toneed changing too frequently, the coating material may have changed, the spray guntransfer efﬁciency could be going down, there could be a problem with the exhaustfan, or other ﬁlter materials should be evaluated. The exhaust portion of the spray booth may use dry ﬁlters, or it may use a watercurtain to capture paint solids. As the ﬁlter media gets loaded with oversprayed paintsolids, the air volume will decline, and the ﬁlters will need to be changed to maintainoptimum airﬂow and transfer efﬁciency and to prevent loss of containment of theoversprayed paint solids and vapors. Dry ﬁlter booths are much less expensive thanwater wash booths, they require less maintenance, and they are also recognized asbest available technology. Used ﬁlters are typically less difﬁcult to dispose of thanliquid paint sludge (Figure 8.2). A water wash booth has a curtain of water that ﬂows at the back of the booth orin the ﬂoor of the booth, a pump, and some type of sludge separator with chemicalsto neutralize the coating material. Maintenance is typically higher than a dry ﬁlterbooth, and the wet sludge is a hazardous waste. The primary advantage of a waterwash booth is that the airﬂow remains constant, because the overspray is collectedin the sludge where it cannot restrict the exhaust. This also means that production isnot interrupted for a ﬁlter change in the middle of the day that requires large gaps ordown time in the line to minimize the risk of part contamination (Figure 8.3).
9 CuringCuring is the process of converting the applied wet paint to a dry ﬁlm. The paintmay cure by solvent loss (lacquers and emulsions), chemical reaction (enamels),oxidation (oil base house paints), melting and resolidifying, or melting and cross-linking (powder coatings). Energy is usually required for dependable and consistentdrying of industrial coatings. Air-dry paints rely on solvent evaporation into the surrounding atmosphere. Thetemperature and humidity will have a profound impact on the drying time. Lowtemperature and/or high humidity will not provide sufﬁcient atmospheric heat torapidly dry the paint. Ovens or dehumidiﬁcation equipment can be used to speed upthe drying time and make it more predictable. Paint cure ovens are enclosures in which the coating on the painted parts is forcedto cure more rapidly than by air-drying alone. Usually, they are insulated and providedwith a means of exchanging solvent-rich air for fresh air. They range from small batchtype boxes to large conveyor equipped structures that can be hundreds of feet long. Finishing systems often use convection ovens, infra red (IR) ovens, and ovensthat combine convection and IR equipment for drying and curing. Various ovensuppliers have their own design methods that can be effective. However, a fewstandard concepts should always be considered, regardless of the manufacturer.9.1 CONVECTION CURINGA convection oven cures by circulating heated air around the part to heat the substrate.The part conducts heat into the paint and the paint dries from the heat. The convectionoven uses a heating system that recirculates hot air through supply duct and distrib-utes it throughout the oven. The basic components include the insulated walls androof, the supply duct, and the burner box, which houses the fan(s) and heat source(Figure 9.1). The curing of organic coatings is a function of time and temperature as deﬁnedby the paint supplier. Typical oven cure cycles range from 10 to 30 min. The timeand temperature required depend on the type of coating and the substrate. The cyclemust be long enough to bring the substrate to the desired temperature, and maintainit for the prescribed time.9.1.1 DUCT DESIGNCure oven ductwork should be designed to circulate air in a way that will maintain evenheat throughout the oven without excess turbulence. The best location for the ductis the oven ceiling. Ductwork is located in the corners and between conveyor passesto provide uniform distribution of air. Adjustment cones can be used for air balance. 161
162 Paint Technology Handbook Burner box Recirculation fan Exhaust Burner Supply duct Return airFIGURE 9.1 Convection cure oven.The ﬂoor is also an acceptable location, arranged under the conveyor with air passingup through the parts (Figure 9.1). Floor duct will interfere with movement and cleaninginside the oven. Recirculation fans and ducts are designed to ensure adequate air movement withinthe oven. This prevents solvent vapor build-up in dead spots and provides for theconstant movement of hot air over the part surface. Without this air movement,paint heat-up would be slow and vent loss rates would vary, slowing the process,and possibly causing ﬁlm defects. Typical duct exit velocities are on the order of1000–2000 ft/min (305–610 m/min).9.1.2 OVEN FUELSGas is most commonly used in process ovens, because it is readily available, it iseasy to control, and it is less expensive than other fuels. High-quality gas burnersfeature up to a 40:1 turn down ratio, providing efﬁcient operation at various loadlevels. The gas burner is typically mounted in the side of the burner box upstreamfrom a centrifugal recirculating fan, which discharges through a transition duct andinto the distribution duct. The burner box can be mounted on top of the oven, on theside of the oven, on the end of the oven, or underneath the oven. An oven can function quite well with an electric heater, and the design is verysimilar to the gas burner box. Sheathed electric heating elements take the place ofthe gas burner in a package-type heater with a built-in centrifugal recirculating fan.Electric ovens require more time to reach the operating temperature and to cool toambient conditions. In addition, electricity is still more than twice as expensive asnatural gas. Using a gas price of $1.00 per 100 ft3 of gas the cost per 1M Btu is$10.00. Using an electric cost of $0.08 per kilowatt-hour, the cost per 1 M Btuis $23.43. Steam can also be used to provide heat to a convection oven. Like gas and electricheating systems, a steam heating system uses a recirculating convection-type burnerbox. The return air should be ﬁltered with high-efﬁciency air ﬁlters to prevent thesteam heat exchanger from clogging. For a steam heat exchanger, a self-operatingregulator with indicator should be used with a strainer to protect the valve. In addition,a bypass line with throttling valve and self-acting steam control valve should beinstalled for proper heat control. Steam is typically not practical for curing highertemperature products unless a facility already has a boiler with excess capacity.
Curing 1639.1.3 MATERIALS OF CONSTRUCTIONThe oven interior skin is typically 20-gauge aluminized steel, because it has superiorheat resistance compared to galvanized or cold-rolled steel. The outside oven skinis typically 20-gauge galvanized, aluminized, or painted cold-rolled steel. The oventrim material should match the oven skin. Mild steel interiors are not recommended,because the surface can rust and cause contamination inside the oven. The insulation is typically 4-lb density mineral wool or equivalent ﬁberglass,and the thickness should be 4′′ for processes up to 300◦ F and 6′′ for processes from300◦ F to 500◦ F. For temperatures greater than 500◦ F, 6-lb density mineral wool isrecommended. The roof and walls should have the same panel thickness, but theﬂoor may be plain concrete, aluminized skin, or insulated oven panels. Elevatedovens should have an insulated ﬂoor. Floor-mounted ovens are acceptable with analuminized skin; however, there will be signiﬁcant heat loss through the ﬂoor. Forexterior ovens exposed to the weather, 6-lb density insulation is typically providedin increased thickness.9.2 INFRA RED CURINGIR curing can be a great asset for faster oven process times, and it can also contributeto the quality of the ﬁnish. To use IR properly, it is important to understand of whatit is and how it works. IR energy is a form of electromagnetic radiation. There are three wavelengths of IRenergy, measured on the electromagnetic spectrum in microns, between visible lightand microwaves. These wavelength bands are shortwave (0.76–2.3 µm), mediumwave (2.3–3.3 µm), and long wave (3.3–1,000 µm) (Figure 9.2). IR energy is transmitted from an emitter and directed at a target. Depending onthe wavelength of IR and the nature of the coating, the energy can behave in one of 0.38 0.76 2.3 3.3 µm 1 mm Visible Short Med Long wave light wave wave IR IR IR Gamma X-Rays UV Infrared Microwaves and rays rays rays radiowaves 1 nm 1 µm 1 mm 1m 1 km 10−9 10−6 10−3 100 103mFIGURE 9.2 Electromagnetic spectrum.
164 Paint Technology Handbook Reflection Absorption Transmission Coating layer SubstrateFIGURE 9.3 Infra red behavior.three ways: reﬂection from the surface, absorption into the coating, or transmissioninto the substrate (Figure 9.3). Energy reﬂected from the surface has little or no beneﬁt, although it is possiblethat it will be reﬂected back to the part surface by the reﬂectors located around theemitters. Transmission into the substrate will contribute to the cure of the coating, butit may not be a very efﬁcient use of the IR energy with substrates that have relativelyfast thermal conductivity. The advantage of IR is fully realized when the energy isabsorbed by the coating, creating molecular oscillation, and generating heat. Most organic coatings will absorb the highest percentage of energy in the mediumwavelength. Short-wavelength absorption characteristics are quite low; most of theenergy is transmitted into the substrate, leading to a smaller processing window andmore color sensitivity. Long-wavelength IR provides less surface heating becauseof low electromagnetic energy levels. It is best suited for wood drying or similarlow-temperature applications. In order to ﬁne-tune the appropriate IR system for a speciﬁc coating, testing isrequired. Shortwave IR may be suitable for some preheat situations, but care mustbe taken to avoid overexposure. Shortwave systems are very useful for products thathave relatively simple geometry where the surface can be uniformly exposed to theemitters. Medium-wave IR provides good absorption characteristics with less intensitythan shortwave, and it is more ﬂexible for a variety of coatings and different parts.Long-wave IR is useful where low wattage per square inch is required. The nature of energy transfer by light makes it difﬁcult to maintain uniformityover irregular surfaces. In order to react to various parts of different mass and shape,the intensity or position of the emitters must be adjusted by the operator or a program-mable logic controller (PLC). This lack of ﬂexibility limits the number of applicationswhere it is practical to use IR alone for curing, particularly if the throughput will varyin size, shape, and mass. In situations where the mass-to-surface ratio and the partgeometry are changing rapidly, it may be difﬁcult to control the amount of energyand avoid excess or insufﬁcient cure. A combination of IR and convection can make an excellent oven, providing ﬂex-ibility, saving space, and offering dependability and reasonable energy efﬁciency. Forexample, an oven may be equipped with an IR section at the entrance to begin the cureprocess prior to entry into a larger convection zone. It can shorten the overall curecycle and reduce the risk of contamination that may occur in the convection zone.
Curing 165It can also be zoned to effectively react to different masses on the part and acceleratecure on heavy substrates. In some cases, IR can be the best, if not the only, way to cure a coating. Verymassive parts that would require impractical cure times with convection heating can becured fairly quickly in an IR oven that is properly designed. Testing is required todetermine the precise intensity of the emitters and the optimum arrangement.9.3 OVEN MAINTENANCE AND CLEANINGOven maintenance is a critical issue in the design. It will be necessary to clean theinside of the oven, so the duct interior and exterior must be accessible, and the surfacesshould be smooth so that they can be washed or vacuumed. Man doors and swing-indock lights should be included where possible. For high-quality ﬁnishing systems,such as clear-coat or plastic lines, interior lighting may be used to facilitate cleaningthe oven.9.4 OVEN EXHAUSTCure ovens must be exhausted to remove solvents, gases, and the by-products of thecombustion. Oven exhaust also creates a negative environment in the oven enclosure,which helps to contain the oven atmosphere at the product openings. The amount of air exhausted from the oven is based on the amount of solventthat is carried into the oven and the by-products of combustion. The exhaust volumemust be high enough to prevent a loss of gases from the openings. Excess exhaustwill unnecessarily increase the cost of oven operation. Exhaust is required to prevent the buildup of solvent vapors to explosive levels.Safety codes require that solvent vapor levels should not exceed 25% of the lowerexplosive limit (LEL). 10,000 ft3 (280 m3 ) of fresh air must be supplied for eachgallon (3.79 L) of solvent evaporated.9.5 OVEN FILTRATIONThe negative air pressure in the oven may attract particulate from the facility that cancause dirt defects on parts. Vacuuming the oven interior regularly will help to preventcontamination from building up in the oven and becoming a problem. Another way to help avoid an oven dirt problem is by providing return air ﬁltration.A ﬁlter framework is built into the return air opening of the burner box and high-temperature ﬁlters are installed in the frames. While the efﬁciency of the ﬁlters variesfor each application, a typical combination would feature a row of 30%-efﬁcientﬁlters serving as the preﬁlter layer for a secondary layer of 90%-efﬁcient ﬁlters. Thisprevents the blower from circulating dirt onto the parts and constantly sweeps theoven (Figure 9.4). High-efﬁciency ﬁlters may not require a preﬁltered air stream. If return air duct is used, the ﬁltration should not be located in duct that is inclose proximity to the parts. Return air ﬁltration should only be located in the returnopening.
166 Paint Technology Handbook Burner 90% Efficient Fan secondary filter Discharge Return air inletFIGURE 9.4 Return air ﬁltration.9.6 OVEN LOCATIONOvens can be located directly on the ﬂoor, elevated on support steel, or locatedon the building roof. A ﬂoor-mounted oven with product openings in the sidewallshould feature some method of heat containment as described previously, and theﬂoor should be insulated to reduce heat loss. Elevated ovens remove process heatfrom the ﬂoor and save ﬂoor space. An elevated oven can cost considerably more thana ﬂoor-mounted oven because of increased installation costs and additional materials.Bottom entry and exit openings in an elevated oven will provide the best possible heatcontainment.9.7 THE IMPACT OF CATALYSTS ON CURINGCatalysts are chemicals that are added to the paint to accelerate cure by chemicalreaction. Strictly speaking, they are not energy sources. Catalysts are effective,because they permit the paint chemicals to react more rapidly at any given temperat-ure than they normally would. Thus, curing can be achieved more quickly at the sametemperature or in the same time at a lower temperature. This can be important whencoating heat sensitive materials such as thermoplastics or when fuel conservation isimportant.9.8 HEAT RECOVERYA well-designed cure oven will not exhaust enough Btu’s to make it cost effectiveto install a heat exchanger for heat recovery. The volume of exhaust is based onthe amount of gases that must be removed from the oven interior to maintain a safeenvironment. Since the exhaust is gas laden, it is not possible to use the heated air
Curing 167without a heat exchanger. A good heat exchanger is expensive and the efﬁciency willbe around 75%. The stack gas temperature must be maintained above the dew point to avoidcondensation in the stack. This limits the amount of energy that can be recoveredfrom the stack gas. With the cost of the heat exchanger, duct and fan for recovery,limits on how much energy can be recovered, and limited efﬁciency, it does not makesense to recover heat from an oven. If volatile organic compound (VOC) abatement equipment is necessary, heatrecovery through the use of a secondary heat exchanger may be worthwhile becauseof the high temperature used in a thermal oxidizer. The recovered heat can be usedfor a boiler, hot oil heater, or heated stages of a pretreatment washer.9.9 SUMMARYA properly designed oven will have easy access and maintenance features such asplatforms, ladders, access doors, lights, and so forth. Providing good access andmaintenance features will help ensure proper maintenance, which will keep rejectsto a minimum, prevent unexpected shut-down, and provide maximum operatingefﬁciency. Convection heating is slow, but it is still the most dependable and ﬂexible methodof curing an organic coating. The use of IR or other means of accelerating the cureprocess should be carefully tested before a commitment is made. The burner used fora convection oven should be a modulating-type burner with a wide turndown ratio toprovide the best possible efﬁciency. The oven size should never be too short; a longer process time can be managed byreducing the oven temperature, but, if the oven is too small, no reasonable solutionsare available, particularly if production increases necessitate an increase in line speed.
10 Testing Paint Materials10.1 INTRODUCTIONTesting is an important part of the operation of a paint system. Testing is done tomonitor the system and to conﬁrm that the ﬁnish meets established quality stand-ards and the expectations of the customer. The end use of a painted product shoulddetermine what tests are important. The incoming paint material is sometimes tested to conﬁrm that the color andgloss are correct and the paint is free of defects. In some cases, the paint supplier willcertify that the paint they are providing meets all required physical properties. The paint should also be tested to conﬁrm that it is ready to spray. Some sprayedsample panels can be used to conﬁrm this before the paint is put into production.Viscosity, a measurement of the ﬂow characteristics of the paint, should always betested before using a fresh batch of coating.10.2 PAINT VISCOSITYViscosity is a very important paint property, usually determined by measuring thetime required for a given quantity of paint to ﬂow through a hole in the bottom of ametal cup. A number of cup sizes and drain hole diameters are available for use withdifferent viscosity paints. Three widely used viscosity cups are the Fisher, Ford, andZahn viscometer. Table 10.1 gives conversion values for use with these cups. It is important to correct the viscosity cup ﬂow-out times for the temperature of thepaint. The recommended spray viscosity is typically based on a temperature of 70◦ F.If the viscosity is measured at a colder or warmer temperature, the actual viscositycould be too low or too high. A paint supplier can provide the appropriate correctionsfor their product. Be sure that the type of Zahn cup or other viscosity cup used isconsistent. In addition, be sure that the method of measurement is consistent. Someoperators consider the ﬁrst break in the paint to be the stop point, while others maywait until the cup is virtually empty.10.3 FINISHED FILM TESTINGFinished ﬁlm testing is used to conﬁrm physical properties of the coating after it isapplied and cured. Daily tests might include such things as gloss, color, hardness,and adhesion. The particular tests used depend on the properties that the coating issupposed to provide and the established quality standards. 169
170 Paint Technology Handbook TABLE 10.1 Conversion Chart for Commonly Used Viscosity Cups Fisher #2 Ford #3 Ford #4 Zahn #1 Zahn #2 Zahn #3 5s 30 s 16 s 8 34 17 15 s 12 s 10 37 18 17 15 12 41 19 18 19 14 44 20 21 25 18 52 22 29 33 25 68 24 33 36 28 30 39 41 31 34 44 45 32 37 10 s 50 50 34 41 12 62 58 41 49 14 66 45 58 16 50 66 18 54 74 20 58 82 23 Finishing tests are an important task in conﬁrming that the ﬁnish meets thestandards and can provide the necessary performance characteristics.10.3.1 PAINT TEST STANDARDSMost of the ﬁnished ﬁlm tests used by industrial painters are based on the AmericanSociety for Testing Materials (ASTM) international standards (originally known asthe American Standards for Testing and Materials). ASTM has several publicationsthat provide the test methods and how to interpret the results. Some performancetests are based on other sources such as the American Architectural ManufacturersAssociation (AAMA) or European standards. It is important to have a precise test method and consistent standard to providemeaningful data and consistent results. A good test method describes how the testpanel will be prepared, how the test will be conducted, and how the results will bereported. If the test frequency is too random or the test methods are inconsistent, theresults will not be as useful.10.3.2 TYPES OF TESTSThere are standard tests that cover most properties of the ﬁnished ﬁlm that are rel-atively simple to do as part of a daily operation. Some of the more complicatedtests, or tests that involve expensive, specialized equipment, can be conducted bytesting labs.
Testing Paint Materials 171 Tests can also be created that will help to determine if the part will meet a particularreal-world condition. For example, if the part will be subjected to brake ﬂuid, then achemical test that subjects it to brake ﬂuid is useful.10.3.2.1 Film ThicknessThe thickness of a dry paint ﬁlm is important to the performance of the coating. Thinﬁlms may appear to be the wrong color, or they may not provide the necessary levelof performance. Water can more easily penetrate to the substrate if the ﬁlm is toothin. Thick ﬁlms can be a problem too. Thicker ﬁlms are more likely to crack in useor they may create problems when two mating parts must be ﬁtted together. Wet-ﬁlm thickness is measured for process control. It can be measured witha handheld immersion gauge that has a series of teeth along the edge of differentlengths. The gauge is placed on the freshly painted surface, and the edge of the gaugeis supported by two teeth of the same length for measurement control. All the otherteeth are different in length and shorter than the control teeth. The wet thicknessis measured as the last tooth that leaves a mark in the paint ﬁlm. Therefore, if thewet gauge reads 3 mil and the coating is 50% solids, then the dry-ﬁlm will be about1.5 mil. This is a rough method of predicting the ﬁnal dry-ﬁlm thickness, but it doesgive the painter an indication of whether or not he/she is applying the correct amountof paint without waiting until parts come out of the oven. This method of measuringleaves marks in the paint, requiring the part to be reworked. The dry ﬁlm thickness of paint on iron or steel surfaces is easily determined witha pull-off gauge. Pull-off gauges reﬂect the force required to pull a magnet suspendedon a spring inside a metal case away from the painted surface. The force will decreaseas the paint thickness increases, because the paint keeps the magnet further away fromthe metal. Pull-off gauges may be graduated in microns, mil (thousandths of an inch),or arbitrary units. They are direct measurement devices. Dry-ﬁlm thickness can be measured much more accurately with an electronicinstrument. If the base material is metallic, a device is used that measures the strengthof eddy currents induced in the metal by a probe containing a conducting coil.The strength of the eddy currents decreases as the paint thickness increases. Theread-out meter for eddy current strength can be graduated in any desired thicknessunits. If the dry paint is on a nonmetallic surface, ﬁlm thickness can be measured witha beta ray back scattering gauge. This instrument emits low-energy radiation in theform of beta rays (electrons) that pass through the paint and are reﬂected by the moredense material beneath it. The quantity of beta rays that are reﬂected back to the gaugedecreases as the ﬁlm thickness increases. These gauges also work when the paintedsurface is metallic. Dry-ﬁlm thickness on nonmetallic surfaces is sometimes determined by cuttinga “V” shaped trough through the paint and measuring the width of the cut at thetop of the trough. A thicker ﬁlm will produce a wider “V” at the top. A low-powermagnifying glass with internal calibrations is often used to make this measurement.It may be calibrated directly in thickness units.
172 Paint Technology Handbook10.3.2.2 Film HardnessThe hardness of the paint ﬁlm is important, because it is related to brittleness and waterpermeability. Films that have been over-cured or under-cured can often be detectedby hardness testing. Pencil hardness and indentation hardness are two widely usedtesting techniques. Pencil hardness tests measure resistance to indentation by a series of increasinglyhard pencils that have been sharpened to a chisel point. The higher the hardness ofthe pencil lead required to make a gouge into the paint, the harder the ﬁlm. Indentation hardness testers measure ﬁlm penetration, in a speciﬁed time, by ametal tip under certain mechanical loading conditions. The time factor is important,since many paints deform gradually under load.10.3.2.3 Impact ResistanceResistance to impact damage (chipping and cracking) is an important property fornearly every paint ﬁlm. It is difﬁcult to have both high impact resistance and highhardness. This is because impact energy is best absorbed when the ﬁlm is softer andable to deform upon impact. However, hardness is desirable, because it normallymeans better gloss retention and weatherability. Most paints are formulated with acompromise between hardness and impact resistance. Impact resistance testing usually involves striking a painted panel with a hardobject, such as a steel ball or hammer and measuring the indentation that results.Another test (Society of Automotive Engineers Test Procedure V400) is called agravel damage test. The gravel damage test uses stones hurled against the panel toinﬂict damage. The most common way to measure impact resistance is ASTM D 2794-93.A standard weight is dropped from a height onto a coated panel. The indentationis inspected to detect if the coating has cracked. The weight can be dropped fromdifferent heights, and the results are then measured in inch-pounds. The goal is to seehow many inch-pounds the coating can take without cracking.10.3.2.4 Tape AdhesionAdhesion of a paint ﬁlm to its substrate is often measured by jerking the paint awayfrom a scribed “X” or grid with a strip of tape. Three M Company’s #600 Crystalbrand transparent tape or another tape with strong adhesive properties will work forthis test. The tape is jerked back upon itself as nearly in the plane of the paintedsurface as possible. A numerical rating system from a 0 for total failure to a 5 for100% adhesion with no loss may be used to evaluate tape adhesion test results. If ascribed grid has been used, the failure of adhesion may be expressed as the percentageof squares that have some loss of paint (D 3359-97). A more severe test of adhesion is sometimes used on aluminum substrates. Thestandard ASTM D 3359 test is used, but the crosshatch pattern is subjected to boilingdemineralized water for 20 min before being tested with the tape pull. This test,AAMA 2604, 188.8.131.52, is useful on aluminum substrates that will be used in an outdoor
Testing Paint Materials 173environment where the paint ﬁlm will be subjected to water permeability and possibleoxidation under the ﬁlm.10.3.2.5 Humidity TestingWater vapor is one of the most severe agents to which a paint ﬁlm is exposed. Becausewater molecules are small and binder molecules are constantly vibrating, moisture caneasily penetrate lightly pigmented paints. Water also penetrates heavily pigmentedprimer ﬁlms, although at a much slower rate. Moisture in a paint ﬁlm can be warmed by sunlight or other sources of energy.When warmed, it will tend to vaporize and exert a pressure that causes the ﬁlm toswell. If the ﬁlm is ﬂexible or if the water occurs near a spot of grease or salt crystalunder the paint, the swelling will be more severe, possibly causing adhesion failureor discoloration of the ﬁlm. The condensing humidity test is widely used to measure humidity resistance. Inthis test, water vapor is allowed to condense on sample panels. The condensed waterdrips off the panel and is revaporized by means of an evaporative heater in the bottomof the test chamber. A typical test involves water at 60◦ C (140◦ F) for 24 h. Aftertesting, panels are checked for blistering, color changes, and loss of gloss. Another humidity test involves exposing the panels to 100% relative humidity at38◦ C (100◦ F) for 24 h. Neither of these tests can provide service life predictions. However, they areuseful for determining the best paint from a series of formulations.10.3.2.6 Salt Spray TestingThe use of salt solution spray testing is an attempt to accelerate the corrosion processand cause early paint failure. Panels are usually exposed for up to 14 days to a mistof 5% (w/v) sodium chloride solution at 33–36◦ C (92–97◦ F). The mist is producedby blowing hot saturated air through a 5% salt solution. The panels are evaluated for two types of corrosion: 1. Rust-through—the percentage of the surface, which has rust visible through the paint 2. “Creep”—the distance in 1/32 of an inch (0.8 mm) from the center of the scribe line that the paint ﬁlm breaks down and separates from the substrateThe results are measured on scale with a predetermined point described as failurein number of hours of exposure. Sometimes, acetic acid is added to the salt spraysolution to accelerate the corrosion. Salt spray testing has been used as a standard for performance by many coatersfrom all different types of industry. It is poorly understood and not necessarily reliableas a predictor of ﬁeld service. The most important value of salt spray testing iscomparison of different pretreatment methods and coatings to see what appears to bethe best combination for corrosion resistance. In all cases, the salt spray comparisonshould be done with the same steel panels and the same test cabinet.
174 Paint Technology Handbook One weakness with the results of a salt spray test is the substrate itself. Steelquality varies substantially and the failure in the salt spray test may be due to poorsteel, not pretreatment or the paint ﬁlm. For this reason, it is very important to alwaysrun standard q-panels as a control. Another factor to consider when evaluating the pretreatment or paint ﬁlm is thecure cycle. If the paint ﬁlm is not fully cured, it can cause failure in the salt spraytest that may be blamed on the pretreatment process or the paint. The cure of the ﬁlmshould be conﬁrmed before the panels are tested in salt spray.10.3.2.7 QUV TestingA Q-LAB Ultraviolet (QUV) test chamber reproduces the damage caused by sunlight,rain, and dew. Coated parts or test panels are placed inside the chamber and subjectedto alternating cycles of light and moisture at controlled, elevated temperatures. Parts can be measured for resistance to chalking, fading, color fastness, cracking,blistering, embrittlement, strength loss, and oxidation. The QUV test chamber provides a more accurate comparison of different processesand materials than salt spray testing alone. It is more helpful in evaluating the affectof outdoor exposure on different coating materials and a somewhat better predictorof actual ﬁeld life.10.3.2.8 Outdoor ExposureOutdoor exposure tests are slow, but they are the best way to predict weatherability.Three months of exposure takes a while, but it does provide good information abouthow well the paint ﬁlm will last in an outdoor environment. Long-term exposure isnot very useful for solving transient production problems, but it is a good way toqualify a paint material for use in the sun. The most common defects turned up by exposure testing are fading, cracking,checking, chalking, blistering, and peeling. Often a portion of the panel is buffedafter testing to see to what extent the original appearance can be restored. Exposure tests are usually conducted in a sunny climate such as Florida or Arizonato get the maximum ultraviolet radiation effect. Panels are usually exposed 5◦ fromthe horizontal, facing south. Florida is a preferred location in this country because ofthe sudden and frequent humidity changes that occur there. The test panel is held in aclamp that shields the top portion of the panel from exposure. Mirrors and mechanicaldevices are sometimes used to accelerate the exposure and produce earlier results.10.3.2.9 Temperature–Humidity TestingTemperature changes, especially if they are rapid, present a severe challenge topaint ﬁlms. Cracking is the most common failure related to temperature change.The ﬁlm fails because of stress that develops when pigments, binders, additives,water vapor, and micro-air bubbles in the ﬁlm expand and contract at different ratesas the temperature changes. Since expansion coefﬁcients for trapped air, water vapor,pigments, and other paint components may be quite different, large internal stresses
Testing Paint Materials 175can develop at various locations within the ﬁlm. The stress created in the ﬁlm cancause it to crack. A typical temperature–humidity test cycle is • 24 h at 38◦ C (100◦ F) and 100% relative humidity • 20 h at –23◦ C (–10◦ F) • 4 h at ambient temperatureThis cycle is often repeated 12–15 times. The panel is rated by evaluating the percentof the surface area that has cracked.10.3.2.10 Rinse BlisteringA rinse blister test helps to expose any unreacted salts left on the surface after evap-oration of a water rinse. The process water is applied as droplets to a panel andallowed to dry. After the droplets have dried, the panel is top-coated and subjected tohumidity testing. Blisters often occur where water-soluble salts have been left fromthe droplets. This is because moisture from the humidity chamber moves throughthe topcoat, collects around the salt crystals, dissolves them, and exerts a swellingpressure against the overlying ﬁlm. Panels are usually evaluated against a controlafter 24, 48, and 96 h. Sometimes a tape adhesion test is also run without a scribepattern being cut in the ﬁlm.10.3.2.11 Corrosion CyclingPaint ﬁlms in use are always exposed to a number of cyclic environmental factors.A corrosion cycle test measures the behavior of a ﬁlm under a combination of testconditions. Usually, a combination of salt, humidity, and changing temperature is used forcorrosion cycle testing. A typical sequence is listed below: • 4 h at 5% neutral salt spray • 18 h at 38◦ C (100◦ F) 100% relative humidity • 2 h at –23◦ C (–10◦ F)The resulting panels are rated against a control on the basis of the percent of rustedarea. Cycle testing can be a more accurate way of predicting comparative qualities ofcoatings than salt spray alone.10.3.2.12 Color MatchingColor matching is a very important step in the process of manufacturing. Colorsmust be consistent so that the product is identical and recognizable from part to part.In addition, many products have multiple components, sometimes with differentsubstrates, and each component must be the same color.
176 Paint Technology Handbook Color match can be difﬁcult at times because of human variability in colorperception. Two panels that appear to be the same color to one person may seemdissimilar to someone else. A color may also change when viewed under differentlighting, ﬂuorescent versus outdoor light, for instance. Usually, colors are compared under constant conditions of illumination and back-ground. Two light sources are often used to examine the panel, one predominantlyblue and one predominantly yellow. The important thing is that the paint buyer andseller mutually agree upon color standards and comparison methods. If standardizedcolor chips are used, they should be stored in the dark to minimize fading. Elaborate and expensive color measuring equipment is available for analyzing thecolor composition of a painted surface. These devices are used in paint formulationlaboratories. They are generally not of value in a production situation.10.3.2.13 GlossThe amount of light reﬂected to the viewer’s eye determines the gloss of a paint ﬁlm.More reﬂection of light will appear as higher gloss. It is the smoothness of the surfacethat affects the reﬂection of light. The smoother the surface, the better the incidentlight can be reﬂected toward a viewer without scattering. Gloss is often measured with a photoelectric device. The light reﬂected is conver-ted to an electric signal by a phototube. The strength of the signal is proportional tothe amount of light reﬂected. This reﬂected light, when compared to the original lightfalling on the surface, is a measure of gloss. There are a number of test variations.The angle of reﬂection may be 20◦ , 45◦ , 60◦ , 90◦ , or some other value. Usually, thegloss value is compared with a previously established standard.
11 Quality Control11.1 INTRODUCTIONSome coatings are applied to products for temporary protection or to providea temporary coating of some acceptable level. For example, oil ﬁlter canisters arecoated with paint or powder coating at the factory, but once the ﬁlter is installedin the car, the owner has little concern about the appearance or performance of thecoating. Most coatings are put on to provide a long-lasting and attractive ﬁnish. Thequality of the ﬁnish is affected by every step of the paint process. With the correctcoating material, appropriate pretreatment system, good application equipment, andthe proper curing system, it is possible to turn out a consistent ﬁnish with the desiredquality. Still, even the best systems sometimes do not always produce a perfect ﬁnish. Oneproblem is that the paint process has both mechanical elements and chemical elementsthat must be controlled. Manufacturers are often skilled and committed to the controlof mechanical variables such as line speed, but they are not always committed orprepared to control the paint material for spraying or able to ﬁgure out why the paintis not performing correctly. There are more complex variables that must be controlledwith a chemical process and they can be just slightly out of range and create severedefects.11.2 PROCESS CONTROLA consistent, high-quality ﬁnish is directly related to degree of control over the processand a commitment to keeping all parameters in balance at all times. Careful monit-oring and process control measures are needed to monitor and adjust the operatingparameters of the system. In order to do this successfully, the variables of the processmust be understood.11.2.1 SCHEDULINGThe ﬁrst step to be controlled is the scheduling of parts and colors to be painted. Thelonger the run of a particular part and a particular color, the more efﬁciently the paintline will run. Of course, the pressure of market demands and the need for just-in-time(JIT) production makes it difﬁcult to group parts and colors together. Still, everyeffort should be made to schedule groups of colors and parts as much as possible toreduce waste and maximize output. 177
178 Paint Technology Handbook11.2.2 RACKINGThe next area of concern is loading and racking. Proper rack design is necessaryfor getting a quality ﬁnish. If the parts are not presented properly to the applicationequipment, it can cause ﬁlm defects such as blistering and runs. Alternatively, theopposite can occur, light paint areas where the substrate shows through. In eithercase, the result is rejected parts that must be repaired and repainted. Rack design isan art and science in itself. Good racking is essential for ﬁlm build control, high ﬁrstpass yield, and good transfer efﬁciency. The paint rack is a tool and should be treated as an important part of the process.Parts should be hung as precisely as possible and in consistent position with goodexposure to the spray equipment. The available product window should be ﬁlled asmuch as possible in the vertical and horizontal dimensions. Parts need to be hung correctly on the rack. This should be simple, but it is notuncommon to see parts hanging at odd angles or hooks that have no part on themat all. It is important that a written or visual procedure be available at the loadingarea so that the workers who are hanging parts can refer to it to see the correct partpositions. Since the people loading parts on the line will handle every part, they canalso inspect the parts to make sure there are no obvious substrate defects that wouldcause painted parts to be rejected. By catching faults such as misshapen parts, metalgouges, deep scratches, and so forth, the cost of painting bad parts can be avoided. Good racking is especially important when robots are used. The robot will notadjust for a part that is not in the proper position so the precise application that a robotcan deliver is lost, if the part is not in the right position. Tooling for robotic paintingmust be more precise than racks used with other application equipment.11.2.3 PRETREATMENTPretreatment is one of the most important steps in getting a quality ﬁnish. The stepsin the pretreatment process are recommended by a qualiﬁed pretreatment chem-istry expert. They will evaluate the soils on the part and the substrates to be runand determine what chemistries will work best to meet a particular quality stand-ard. At a certain line speed with a certain density of product going through thepretreatment stage, the chemical supplier will recommend the proper chemicals, con-centrations, and temperatures of the various solutions used to obtain a clean andproperly treated part. The chemical supplier will also develop a schedule of tests to ensure that theproper concentration of chemicals is maintained. They can also provide tests thatwill determine the amount of carry over of chemicals into the rinse tanks and theamount of fresh water make-up required to ensure proper rinsing. All testing shouldbe recorded on work sheets so that if there is a problem, the actual test values may bechecked to see if the problem is related to pretreatment. Mechanical maintenance of the washer is also critical to successful cleaning andtreatment. Each section of a power washer should be checked on a regular basis to besure that all the nozzles are spraying properly and in the right direction. If nozzles arenot working or if they are misdirected, there is potential for improper pretreatment.
Quality Control 179Parts that are not cleaned, phosphated, or rinsed properly can produce immediatepaint rejects or failures that occur in the ﬁeld. Besides monitoring the chemicals and rinses on a daily basis, parts should beexamined as they come out of the spray washer before they go into the dry-off oven.At that point, the water should be sheeting off with no beads of water remaining onthe part. Beaded water or water spots indicate something present on the surface ofthe part that is not letting the water run off. If water is beading up on the surface, itindicates a soil that has not been removed. Soils left on the part surface can lead toadhesion failure of the paint to the substrate or premature corrosion. The line speed that the system was designed to operate at sets up the criticalcontact times inside the stages of the washer. If the pretreatment system is designedto give optimum cleaning, phosphating, and rinsing at a line speed of 10 ft/min and thespeed is increased to 15 ft/min, the pretreatment time has been reduced by one-third.More carryover and faster dilution of the chemistry will occur, and the rinses will becontaminated more quickly. With higher throughput and less time of exposure, thetreatment process may not be effective. Slower line speeds can cause problems too. Excess phosphate coating can leavea powder residue on the part or cause ﬂash rusting. Both these problems will cause alack of adhesion and reduce moisture resistance. If the line speed needs to be changedthen the system will need to be adjusted to the new line speed. A lot of these problems can be spotted before they are painted. Parts coming outof the dry-off oven should show an even color of phosphate, plus no mineral depositsand no powder buildup. A clean dry part should not yield dirt, oil, or powder when itis wiped with a clean cloth after it comes out of the dry-off oven. Some older paint lines may have pretreatment systems that provide marginalcleaning and treatment results. They may have been built for coatings with lowsolids, high solvent content or for a lower quality standard. The high solvent contentin these materials could help to wet out soils on the surface, and the long-chain resinscould bridge minor problem areas and give good adhesion. High-solids, low-solventpaints will not tolerate poor cleaning. The solvent level is very low, and in manycases, the solvents used are not aggressive enough to tolerate even small amountsof oil or other soils. The short-chain resins need more uniform sites to ensure goodpaint adhesion. Older systems may need upgrading to accommodate newer painttechnologies.11.2.4 DRY-OFF OVENSAfter leaving the pretreatment section, parts are usually run through a dry-off ovento remove the water from the parts. If parts have areas where water is cupped, thepuddles should be removed by the use of air. Boiling out the puddles with heat isexpensive and can cause mineral deposits on the part surface. Air can be blown ontothe part from the dry-off oven discharge duct or from a high velocity blow-off, orboth. Some puddles of moisture may require a manual blow-off operation, because thewater is not accessible to any other method. Proper racking to ensure good drainageis also important.
180 Paint Technology Handbook11.2.5 COOL DOWNWhen the parts exit the dry-off oven, they will be very hot. The parts can be cooledby time (length of conveyor) or forced-air cool downing. If a textured or orange peellook is desired, then a hot part will allow the solvents to evaporate more quicklyand cause less ﬂow. If a smooth ﬁnish is required, the part must be close to ambienttemperature.11.2.6 PAINT APPLICATION184.108.40.206 Spray Gun AdjustmentThere are some basic spray principles that should be reviewed to understand how thepaint will behave when it is sprayed. Control of droplet size affects the depositionand ﬂow of the paint. Droplet size affects solvent evaporation and inﬂuences paintﬂow-out on the surface. Since many wet paint defects are related to paint ﬂow-out,the ability to control droplet size is important. Delivery and atomization of the paint play a key role in droplet size. The ratioof ﬂuid pressure to atomizing pressure affects the break up of the paint. The ﬂuidviscosity of the paint and the balance of ﬂuid pressure to atomizing pressure willinﬂuence the droplet size. The droplet size can be decreased with added air pressureor reduced paint pressure. An increase in atomizing pressure will move the paint ata higher velocity and may cause more overspray. A decrease in ﬂuid pressure willreduce the amount of paint delivery and may cause coverage problems. Which controlto adjust depends on what adjustment will work best in a given situation, more airvelocity or less paint. The relationship between droplet size and ﬂuid ﬂow is best understood by con-sidering the relationship between the size of the droplets and their total surface area.In Table 11.1, a droplet has been divided into two and then into four smaller droplets.The total surface area increases as the droplets get smaller. If a known volume of paint is divided into more droplets, it will cover moresurface area. The larger total surface area allows more solvent loss while the paint isairborne and the droplet strikes the work in a drier, less runny state. Droplet size has little effect on ﬁlm thickness. Thickness is primarily determinedby the paint pressure, gun speed, gun-to-part distance, and number of passes. Changesin any of these variables can lead to wet ﬁlms that are too ﬂuid due to retained solvent.The effect of these parameters on paint ﬂow-out is indicated in Table 11.2. TABLE 11.1 Ratio of Droplet Size to Total Surface Area Number of Droplets 1 2 4 Droplet size (volume) 1 unit 1 unit 1 unit Total surface area 1 unit 1.2 units 1.4 units
Quality Control 181 TABLE 11.2 How Adjustment of Application Variable Affects the Fluidity Effect on Increasing Fluidity Air pressure Decrease Gun speed Decrease Gun distance Decrease Paint temperature Decrease Part temperature Decrease Solvent evaporation Decrease Paint pressure Increase Oriﬁce diameter Increase Line speed Increase Note: All other variables held constant. For hand spray operations, it is important to make sure that there is enough time toperform trials and develop the correct painting pattern. Manual spray gun adjustmentand spray patterns should be as consistent as possible. Automatic application should be closely monitored to make sure that the guns areclean, well maintained, and working properly at all times. When automatic equipment is used with hand reinforcement, a decision mustbe made on where to locate the manual stations, before or after application by theautomatic equipment. The manual operator can clearly see the areas where rein-forcement is needed, so it may be best to locate the automatics ﬁrst. If the manualspray is located before the automatics, the painter will tend to cover more area,because the entire part is bare. However, if the painters are well trained and knowexactly what areas to reinforce, the best ﬁnish results may be obtained by applyingthe manual coverage ﬁrst. The high-speed turbo bells or disks shear the paint more,causing a smoother ﬁnish and blending the lines from manual to automatic moreuniformly. In some cases, there will be a very slight visual difference in color and textureof manually sprayed areas versus automatically sprayed areas. In cases where handreinforcement is after the application by the automatic bells or disks, the touch-uppainters may literally repaint the whole part so that the paint appearance is consistent.Testing and training are the key elements to avoid mistakes in this area. The lead time (guns are triggered before the part is in front of the spray pattern)and the lag time (guns remain on after the part passes out of the spray pattern) on theautomatic equipment should be checked daily to make sure they are correct. If the leadstarts too soon, it may cause buildup and possibly cause runs or blisters on the leadcorner. If the lead starts too late, it may cause light paint and improper electrostaticwrap on the part. If the guns shut off too soon, there will be light coat areas on theparts, and if they run too long, it is a waste of paint and may cause fatty edges.
182 Paint Technology Handbook The automatic equipment should do as much of the painting as possible, sinceit is the most consistent painter. However, automatic guns do not have multiaxismotion unless they are mounted on a robotic arm, so penetration in angles or deeprecesses is somewhat limited. Increasing the ﬂow rate to get more depth of coveragemay increase the ﬁlm build on ﬂatter, more accessible surfaces. Automatic applicationshould be limited to the surfaces where uniform ﬁlm build is possible and not forcedto cover areas that are hard to reach. Once the automatic spray guns and hand spray pressures have been properly setto give the desired ﬁnish at the desired ﬁlm build, the settings should be recordedfor each part and used by all painters for set up and control. If the settings need tobe changed, it may indicate that some other process variable is out of control range.Worn equipment, a change of paint material, plugged hoses, or some other problemmay be affecting the gun settings. The correct air pressure is very important. If the air pressure is too low, it cancause poor paint break-up and give a rough orange peel look. It will increase thetendency for the paint to blister because of heavier ﬁlm build. Higher air pressurewill provide improved atomization and a smoother ﬁnish, but excess pressure mayblow more paint past the parts. The ﬂuid pressure determines the amount of paint delivered to the parts, and anadjustment to the ﬂuid pressure has a direct correlation to the amount of ﬁlm buildup.With bells, the settings for the shaping air should also be recorded and checked tomake sure that the pattern is set up correctly for the part surface. A record of spraygun settings should be logged for troubleshooting if something goes wrong.11.2.7 PAINT MATERIALThe paint material is another critical variable that must be controlled. If the paint is atthe same temperature and same viscosity every day, then it should apply the same wayevery day. This is very important since the viscosity of high-solids coatings changesvery dramatically with temperature. A paint that is 18 s viscosity on a #3 Zahn cup at 72◦ F may be 32 s viscosity onthe same cup at 64◦ F. If a paint line technician is unaware of the paint temperature,they may further reduce the paint with solvent to achieve the desired viscosity. Thiswill over-reduce the paint, which can then cause runs, sags, and blisters. The operatorthinks that the paint is the same as it was yesterday, but the viscosity is different. The paint supplier normally supplies the paint at a certain viscosity based on atemperature of 77◦ F. For many production environments, it is not feasible to meas-ure viscosity at that temperature. It is important to use a consistent temperature formeasuring the viscosity of paint. Each material has particular spray viscosity at aparticular temperature that works well. The viscosity of the paint should be checkedevery time it is used. This will show if there has been a lot of solvent evaporation orif the solvents have swelled the resin and caused the paint to thicken. A radical change in paint viscosity can indicate that paint break down is occurringor something may have been added by mistake. If paint line heaters are being used,the temperature of the paint at the end of the gun should be checked to make sure thatthe heaters are working correctly and the paint is at the desired temperature. If the
Quality Control 183paint is at too high a temperature, it may cause runs and sags. If the paint is too cool,it will be more resistant to atomization and that could lead to heavy paint buildup thatcould cause blistering. It would also tend to give more orange peel to the ﬁnish.11.2.8 FLASH-OFFAfter the paint has been applied, the solvents begin to evaporate from wet ﬁlm.A ﬂash-off area follows application to provide time for the solvents to evaporate, andthe paint ﬁlm begins to ﬂow and smooth out. If the ﬂash-off time is too hot, the surfaceof the ﬁlm may begin to form before the solvent can leave and cause blistering. Ifthe ﬂash-off area is too short or cold, the solvents may not be fully ﬂashed whenthe part reaches the next coat or the cure oven. Best results are obtained where theambient temperature is kept fairly constant. In some cases, it may be slightly elevatedto help with the evolution of the solvents. Flash time and temperature are basedon the paint material being applied and the ﬁlm thickness as recommended by thesupplier.11.2.9 CURINGThe ﬁnal step in the paint application process is the cure of the paint ﬁlm. In mostpainting operations, an oven of some sort is used either to cure or to accelerate drying.There are systems that cure with the use of ultra violet rays, electron beam, moisture,and induction. These coatings are very important but not as commonly used as thermalreactive or air-dry products. Ovens for thermal cure include convection, infrared, andcombination infrared/convection. The exact oven to use is based on the type of paint,the available space, parts to be painted, ﬁnish desired, available capital, and volumes.In general, gas-ﬁred convection ovens are the most dependable and ﬂexible. They useheated air to raise the substrate temperature so that the coating will cure from contactwith the hot surface. Oven balance is important for accurate and complete cure. A temperature-recording device, such as a Datapaq system, is used to measure the air and parttemperature in the oven and create a time/temperature proﬁle. The chart showswhether or not the part temperature was high enough for enough time to reach fullcure (Figure 11.1). If the proﬁle shows that the part does not reach sufﬁcient temperature for theminimum cure time, then the paint ﬁlm will be under-cured. An under-cured ﬁlm willnot adhere properly or perform properly. If the proﬁle shows that the part exceededthe cure time and/or temperature, it may be ﬁne. Most paint materials will toleratea certain amount of extra cure. However, it is possible to overcure the coating andcause the paint to turn brittle, discolor, loss of gloss, or other ﬁlm properties. Some companies run a temperature chart through their ovens every day. That maynot be necessary, but once a week or a month is good practice for process control.If the line speed is changed, a temperature proﬁle should be run at the new line speedto make sure that the cure cycle is within the speciﬁed guidelines. If the gauge of themetal being painted varies quite a bit, then it will probably be necessary to changethe oven temperature settings or line speed to get a proper cure on the various parts.
184 Paint Technology Handbook11.2.10 RECORD KEEPINGA record of the oven temperature setting and line speed for each part should be made,and that information should be readily available for the paint line operators. A runningrecord of the paint line conditions should be made as each different part is painted.A single form can be used to record the conditions of the system, or separate formscan be used for each component of the operation. By keeping careful records and using the recorded information for process control,the results will be more consistent. If careful records are maintained, variations in theﬁnish coat should be traceable and corrections can be made. There is a natural tendencyto gradually relax rules for accurate record keeping, because everything is going well.To keep things running at peak performance, diligent record keeping is a must.11.3 PAINT FILM DEFECTSThe causes of defects in a paint operation are too numerous to list and although allcoaters attempt to eliminate them, it is very difﬁcult and costly to cut defects to zero.Knowing some common causes of defects and implementing a good process controlprogram will keep the number of defects to a minimum. Some causes of paint defects are harder to identify and correct than others. Someof the common problems with paint ﬁlms are associated with material and processproblems. Defects can be controlled through better understanding of the processvariables associated with surface preparation, paint material control, application,and cure.11.3.1 PRODUCTION DEFECTSAvoiding defects is a function of understanding the variables that affect the process,measuring them, and controlling them. When defects do occur, it is important toidentify the cause and make adjustments to prevent additional rejects. 300 250 Temperature (°F) 200 150 100 0:00:00 0:05:00 0:10:00 0:15:00 0:20:00 0:25:00 TimeFIGURE 11.1 Temperature graph from cure oven.
Quality Control 185220.127.116.11 Orange PeelOrange peel is a textured effect that resembles the skin of an orange. The paint willusually feel smooth but will appear to have small depressions when viewed at anangle to the light. Orange peel often results when the paint droplets are properlyatomized. If they are not ﬂuid enough to ﬂow together smoothly on the surface,the ﬁlm will be somewhat textured. Orange peel is also affected by excess ﬁlmthickness or paint that is not sufﬁciently atomized. A thicker wet coat may not ﬂowout as smoothly. Orange peel may also be caused by uneven shrinkage as the paint loses solventand begins to cross-link. A certain amount of orange peel is nearly always found withenamels. Sometimes a textured surface beneath the paint will result in orange peel. Orange peel can often be reduced or eliminated by adjustment of the atomizing airpressure to achieve the proper droplet size. Adjustment of the gun-to-target distancecan accomplish the same thing.18.104.22.168 SaggingSagging occurs when there is too much wet ﬁlm applied. Paint will sag whenevergravity overcomes the internal ﬂow resistance of the ﬁlm. This occurs when the paintcontains too much solvent or is applied too thickly. Possible cures for sagging include • Increase the air pressure • Decrease the paint pressure • Move the gun more rapidly • Increase the gun-to-part distance • Use faster solvents • Use multiple coats of paintThese changes are designed to give better atomization (drier paint) or result in athinner wet ﬁlm.22.214.171.124 Flooding, Floating, and MottleThese terms, while describing technically different defects, are often used inter-changeably. They refer to a separation of pigments within the paint ﬁlm. If theheavyweight pigments come to rest in a different position than the lightweight pig-ments, the ﬁlm will have a dappled appearance (mottle). The pigments may separateby sinking or ﬂoating, or because there are whirlpool-like currents set up in thewet ﬁlm by evaporation. The heavier pigments are thrown to the outside of thesewhirlpools while the lighter pigment particles remain nearer the center. As solventevaporation continues, the paint becomes more and more viscous, ﬁnally trappingthe pigments in a ﬁxed position. Mottle is more noticeable with some colors than with others. Paints containingorganic pigments and high levels of aluminum ﬂake are especially likely to mottle,
186 Paint Technology Handbookbecause the ﬂakes tend to ﬂoat near the center while the dense color particles arelikely to be spun to the outside of the whirlpools. The mottle-spots may be as large as6 mm (0.25 in.) in diameter, although they are usually much smaller. The pigments do not separate to give the mottled effect unless the paint remainsﬂuid for too long a time. Extra-thick ﬁlms (more total solvent) or ﬁlms with insufﬁcientsolids are more likely to have this problem. Corrective adjustments for mottling are • Reduce ﬁlm thickness • Use a faster solvent • Move the gun back • Increase the ﬂash-off time between wet coats126.96.36.199 SilkingThe term “silking” describes the appearance of light or dark ﬂow lines in a paint ﬁlm.It occurs when pigment particles are unevenly distributed in the ﬁlm. Silking oftenappears where the wet paint has drained away from holes or edges, especially afterdipping. It can occur if there are adjacent areas of the paint that differ considerably inwet-ﬁlm thickness. The effect is easily observed when stirring a paint that containsaluminum ﬂake where the plate-like pigment particles tend to orient themselves innonrandom patterns due to the stirring motion. Silking can be reduced by making sure the solvent evaporates as quickly aspossible and by avoiding excessive paint ﬂow over the surface.188.8.131.52 Solvent Pop, Bubbles, Pinholes, and CratersThese terms, often used interchangeably, describe defects that arise when solvent islost too rapidly from a wet paint ﬁlm. More than one of these defects can be presenton a part and they may be located anywhere or everywhere on the surface. Thesedefects are usually caused by solvent vapors forming within the paint and rising tothe surface. The rising vapor lifts the paint ﬁlm and the paint may not recede to asmooth and continuous ﬁlm. A bubble occurs when the solvent vapor seeps throughthe paint ﬁlm skin without causing it to rupture. A crater results when the brokenbubble retains its jagged edge. Anything that makes the paint ﬁlm too solvent-rich, too thin, or causes it to losesolvent too rapidly may result in pops, bubbles, pinholes, or craters (Figure 11.2).The factors that may cause these defects include • Low air pressure • High paint pressure • Not enough ﬂash-off time • Slow line speed through the booth • Too much wet-ﬁlm build • Short gun-to-work distance
Quality Control 187 Bubble Pop Pinhole Crater PartFIGURE 11.2 Paint surface defects. Paint Contaminant Part Part Part Applied wet film During flash-off After cureFIGURE 11.3 Surface contamination. • Slow gun speed • Excess oven temperature early in the cure cycle184.108.40.206 Fisheyes and Silicone CratersFisheyes are round depressions in the ﬁlm. They vary in size from barely visible tomore than 6 mm (0.25 in.) in diameter. Sometimes they are deep enough to revealthe bare substrate. Pigment sometimes gets collected in the ﬁsheye giving it a darkcenter. They are caused by surface contamination that the paint cannot adhere to. As aresult, the ﬁlm forms around the contamination but not over it. A raised edge usuallyforms around the perimeter of the contaminant. Figure 11.3 shows how these defectscan occur. Fisheyes can be extremely frustrating, because it is so difﬁcult to identify thecause. Paint ﬂows away from the defect, because silicone or a similar oily substanceacts like a lubricant. As it ﬂows away from the contaminant, it creates a surfacedepression. If the repulsion is strong enough and the paint is very ﬂuid, the depressionmay actually reach the surface. The idea of a liquid ﬂowing away from a slipperysubstance can be understood by considering the behavior of water spread on a waxedsurface. Fisheyes are commonly caused by oil, grease, and silicone lubricants. Of these,silicones are the most likely source and the most troublesome, because they are sodifﬁcult to remove. Oil and grease can usually be removed by solvent wiping or hotalkaline cleaning. Silicones resist these and other cleaning techniques. Often, theymust be sanded off, a risky operation since the chance of further contamination bythe sanding dust is high. Sometimes spraying as dry as possible (high air pressure) is helpful, because thepaint will not ﬂow as much. Fisheye-reducing products are commercially available.They are chemicals which, when placed in the paint, are absorbed by the siliconecontaminant, changing its surface to one which is more paint-compatible, so the paintis less likely to ﬂow and form a depression.
188 Paint Technology Handbook The best solution to a ﬁsheye problem is to eliminate the source of the contaminant.Sources that can add silicone to a paint system include lubricants, mold releaseproducts, and aerosol spray products. If ﬁsheyes are a persistent problem, aninvestigation will usually reveal the use of a silicone product in the plant.220.127.116.11 Overspray and Dry SprayA rough, grainy surface is usually the result of dry-spray. This occurs when paintdroplets have lost so much solvent in the air that they do not blend into the wet ﬁlmon the painted part. Overspray is paint that originally missed the part and later settledon it (or another part). To prevent overspray and dry spray, the air pressure can be reduced, the ﬂuidpressure can be increased, the gun can be moved closer to the target, or the spraybooth face-velocity can be reduced.18.104.22.168 BlushingBlushing is a description of areas in the paint ﬁlm that are “whitish” in color. It resultsfrom the condensation of moisture droplets in the wet ﬁlm. The droplets condensefrom the air, because solvent evaporation lowers the air temperature below the dewpoint. Fast evaporating solvents should be avoided on humid days. The usual cureis to reduce the air pressure and/or add a slower evaporating solvent to the paint.A slightly elevated temperature in the ﬂash area can help, and adequate exhaust in theﬂash area is important.22.214.171.124 Dirt and ContaminationDirt on the surface of a painted part is a major concern for all painters, because itdiminishes the appearance of the paint ﬁlm. Dirt may come from the air around thespray environment, from the application equipment, or it may be in the paint. One ofthe ﬁrst things to do in searching for the cause of a defect is to look at where it is onthe part and where it is in the ﬁlm. If a defect is from dirty paint or manufacturing by-products that have not beenremoved by the cleaning process, it will usually be evenly distributed. If it is anexternal source, the defect will more likely be randomly distributed. If the dirt is on the part surface, it was most likely there before the part waspainted. If the paint application process involves multicoats, it is useful to determinewhat layer the dirt is in. It may be in a primer coat, a base coat, or a top coat, providinginsight into the source of the dirt. Analysis by microscope can reveal the depth of the“dirt” in the coating. If the dirt is in the paint material, it can be strained out. Dirt from ineffectivepretreatment can usually be corrected by changes in the process or control of thepretreatment system. Soils that are on the part from the manufacturing process thatcannot be removed by a spray washer can usually be tracked to the source and achange made to eliminate them. Air borne contaminants are the hardest to track andeliminate, because they can come from so many different sources.
Quality Control 189 High-solids paint formulas are less tolerant of dirt than more solvent-rich formulasare. The coating surface remains tacky, attracting, and holding dirt. Sources for thiskind of air-borne dirt are so numerous that it is impossible to name them all. The listbelow will name some of the common sources. • People—Air sampling of enclosed paint systems has shown that as much as 80% of the air-borne contamination came from the clothing, hair, and shoes of personnel. • Nature—Pollen, road dust, and other outdoor dirt are sometimes brought into the plant through doors, windows, and unﬁltered air supply systems. • The building—Concrete ﬂoors may wear and give off dust. • Manufacturing—Mechanical operations in the manufacturing process may generate dust, metal shavings, or wood dust. • Process equipment—Conveyor, oven, washer, or other operations within the paint line can generate or concentrate dirt that will create a paint defect.With all of these potential sources, the job of coating a part with no defects is achallenge to say the least. Here are some ways to help control dirt on painted parts.The level of dirt prevention that an operation adopts is directly related to their qualitystandards. Restrict access to the paint area or clean room to essential personnel as much aspossible. Have all entrants to the paint room put on nonlint paper suits, hairnets, andshoe covers. Isolate the paint application area from the rest of the plant and supply ﬁltered airto the enclosure that will create a slight positive pressure in the room to prevent airfrom inﬁltrating through the product openings. Have the concrete ﬂoors sealed in the area where workers put on their paper suitsand in the paint room. Build a vestibule at the entrance to the paint room and adddeionizing air in the vestibule to neutralize the workers before they enter. Clean all surfaces in the room as frequently as is necessary to avoid anaccumulation of dust. Use an inverted box track conveyor or sanitary pan under the conveyor. Use anautomatic lubrication system with a dry-ﬁlm, thin-ﬁlm lubricant, and do not over-lubricate. Clean the conveyor and chain components regularly. If it will work withthe product, a ﬂoor-mounted conveyor can help reduce dirt. One of the keys in controlling dirt is to use good recording and tracking of dirtrejects. Fiber, metal shavings, paper, and dust are examples of types of contaminants.Rejected parts should be recorded and categorized by the type of defect. The sourceof the dirt should be tracked and eliminated. A microscope can be used to identify thenature of the dirt speck.
12 Cost Analysis for Finishing Systems12.1 FACTORS THAT AFFECT COSTThe operation of a paint system has many variables that affect cost. Effective controlof these variables will provide the best quality at the lowest cost. Some cost variables are part of the design, some are part of the operation, andothers are related to decisions on how to run to the system. Each cost variable hasto be considered to know how much the system costs to operate and how much tocharge for painting a part.12.1.1 SYSTEM DESIGNThe subject of how to design a paint system is long and could ﬁll a book of its own.There are a few guidelines that can help with the sizing and equipment selection thatare mostly common sense. • Make sure that the largest parts can be moved through the system without interference • Design the system large enough for future volumes • Pay close attention to features that can lead to cost savings, safety, or efﬁciency and be willing to spend extra money for them • Consider operating cost as closely as capital cost • Use durable building materials (stainless steel, heavy gauges, high efﬁciency fans, etc.) • Consider maintenance issues and make sure all mechanical devices are easy to service12.1.2 QUALITYThe level of quality that is required for the ﬁnished product has a direct inﬂuenceon the cost of production. The desired level of quality will affect the pretreatmentprocess, the application process, and the amount of rework or touch-up required. Paint systems can be built to different standards of quality. The kind of systemthat will be required to produce top-quality appearance and performance will be quitedifferent from one designed to apply paint to products that do not require very highstandards for paint ﬁnish. The deﬁnition of quality for an automobile exterior body ﬁnish is quite differentfrom the quality standards for brake shoe. The car ﬁnish will require a very highstandard for both appearance and performance, while the brake shoe needs some 191
192 Paint Technology Handbookblack paint that will last for a relatively short time and visual imperfections are nota big issue. The paint system for car bodies will be designed to provide a ﬁnish that isnearly perfect. No paint line will produce a 100% ﬂawless ﬁnish, but there are manydifferent standards for what is acceptable. An absolutely ﬂawless ﬁnish may be possible, but the cost will be very high. Somedefects are likely on any paint line. Small defects in areas that are not right in theeye of the consumer may be acceptable. Larger defects in highly visible areas may bemore objectionable. The question is, what level of defect is acceptable and what levelof defect will cause a part to be rejected. A high-quality standard will require a bettersystem, better controls, more inspection, and possibly more rework. It costs more toproduce a better ﬁnish.12.1.3 SUBSTRATE CONDITIONThe condition of the part is also a major factor in the cost of the paint ﬁnish. Simpleparts in high volume with very light soils will not cost nearly as much per square footas complex shapes in low volume with heavy grease or other soils that need to beremoved prior to paint application. The substrate material, type of soil, volume of soil, and any other special consid-erations will impact the cost of part preparation. The part must be completely free ofcontamination before it can be painted. Castings have die release products, weldedsteel has burned-on oil, hot-rolled steel has mill scale, and aluminum has a tight oxidelayer that can interfere with adhesion. The chemical in an alkaline cleaner may not beable to remove such contaminates. They may require additional process steps suchas blasting or polishing. These additional steps will add to the cost.12.1.4 RACKINGAnother cost consideration is racking. Custom paint racks designed for a newlymanufactured part can be very expensive. If the racks will improve the output volumeand reduce costs, they may be worth the investment. To determine the value of pur-chasing custom-made tooling, the savings per piece and total run volume need to becompared to the cost of the tooling. In many cases, there are existing hooks that can be used to hang the parts, butthey are not always the most efﬁcient way to maintain good line density and goodthroughput. For example, consider a situation where improved tooling would holdtwice as many parts, and the cost for the tooling is $4000 (200 racks at $20 each).Existing utility racks are available that hold only two parts, while the new toolingwill hold four parts in the same space on the conveyor.126.96.36.199 Line Data Line speed—8 FPM Rack spacing—2 ft centers Hourly ﬁxed cost—$400.00 (ﬁxed cost includes administration, building cost, staff, etc.)
Cost Analysis for Finishing Systems 193 Fixed cost per piece with no racks purchased: 8 FPM × 60 min = 480 ft/h (FPH) 480 FPH 240 racks = 2′ hanging centers h 240 × 2 parts/rack = 480 parts/h $400.00 (ﬁxed cost/h) $0.83 = 480 parts/h part Fixed cost per piece with special tooling: 240 racks/h × 4 parts/rack = 960 parts/h 400 $0.42 = 960 part The savings per part is easy to calculate at $0.41. The other piece of informationthat must be entered into the equation is the volume of parts to be run over time.For example, assume a volume of 2000 parts a month. $0.41 savings/part × 2000 parts/month = $820.00 savings/month $4000.00 (new tooling cost) = 4.9 months return on investment (ROI) $820.00 (savings/month) The payback period for the special tooling in this example would be just under5 months. In this example, the tooling would appear to be an excellent investment,but if the volume were a total of only 50 parts/month, it would probably not pay.Table 12.1 shows the payback with different volumes of production. Of course, it is also possible to buy fewer racks, but they will cost more perrack. At any rate, it is important to evaluate the cost savings available from usingcustom-made tooling versus simple hooks that are used for utility purposes. TABLE 12.1 ROI for Different Volumes Volume of Parts/Month ROI 500 19 months 1000 9.5 months 2000 4.75 months 3000 3.17 months
194 Paint Technology Handbook12.1.5 REWORKRework and scrap must be accounted for in determining the cost of a paint operation.Applying a second coat to the part is expensive. A second coat will add thickness thatmay not be acceptable. Some parts may need to be stripped, and in some cases, thepart cannot be salvaged at all. The percentage of defects and the method for correctingthem is an important cost issue. Every effort should be made to limit rework. Partsthat are reworked need to be factored into any cost per part determination.12.1.6 COLOR CHANGEColor change time for liquid spray systems is very short, but has some impact on cost.Color change requires time and wastes material. Gaps in the line, cleaning solvents,and wasted paint are part of the total cost to paint the parts. This is particularly true if the material being sprayed is a plural componentmaterial. Catalyzed materials are mixed in batches or mixed automatically by a com-puterized mixing device. Either way, some material must be purged from the linesfor color change. The volume of catalyzed material that is purged to waste should beadded to the piece price along with lost time for color change. Of course, it must be recognized that we have a market economy, and the trendis to offer more color options, and current manufacturing trends are designed for justin time production and minimum inventories, limiting the control of the number ofcolor changes in a typical line. The equipment should be designed to color-changeas fast as possible with a minimum amount of wasted paint and solvent use.12.2 APPLIED COST OF PAINTThe applied cost per square foot of a paint material can be calculated to determine theactual cost of painting the part. Special considerations like masking, ﬁlm thicknessrequirements, and special part preparation should be factored into the total cost. The cost of coating application is related to the material and efﬁciency of thepaint application process. The following formulas provide a method of developingestimated coating cost per square foot. Actual costs of any process depend on thevariables of the material price per unit, percentage solids, transfer efﬁciency, materialutilization labor, and so forth.12.2.1 COST PER SQUARE FOOT OF LIQUID SPRAY COATINGThe number 1604 is used as a starting point (the coverage in square feet of 1 galof paint that is 100% solids, at a ﬁlm thickness of 1 mil and 100% efﬁciency).To determine the coverage of a gallon of paint, the ﬁrst piece of information that isfactored in is the percentage of solids. The solids content of the paint will provide theﬁlm, while the solvent and water content will evaporate. % Solids × 1604 = Theoretical coverage at 100% efﬁciency (ft2 /gal, 1 mil thick)
Cost Analysis for Finishing Systems 195 TABLE 12.2 Potential Transfer Efﬁciency of Spray Equipment Transfer Spray Process Efﬁciency (%) Conventional air spray 15–40 Conventional airless 20–50 Conventional air-assisted airless 30–60 Conventional HVLP 30–60 Electrostatic airless 40–70 Electrostatic air spray 40–80 Electrostatic air-assisted airless 50–85 Electrostatic HVLP 60–90 Electrostatic bell atomization 70–95 Electrostatic disk atomization 80–95 Electrical atomization 95–98The actual ﬁlm thickness and transfer efﬁciency is then added to the calculation. (Theoretical coverage/ﬁlm thickness) × Transfer efﬁciency = Actual coverage, ft2 /galAfter the actual coverage is determined, it is a simple step to calculate theapplied cost. Cost/gal/actual coverage = Applied cost/ft2 Table 12.2 shows the theoretical transfer efﬁciency for different spray devices.Actual transfer efﬁciency can be calculated by determining how much paint it takesto cover a known square footage of part surface.12.2.2 EXAMPLE OF COST CALCULATIONAssumed variables: Cost/gal: $21.00 % Solids: 60% Film thickness: 1.2 mil Application: electrostatic spray 0.60 × 1604 = 962 962/1.2 × 0.70 = 561 21/561 = $0.0374/ft 2
196 Paint Technology Handbook In most cases, the cost of operation for the components of the system is part ofa ﬁxed operational cost per hour. The washer and ovens may use slightly more energyfor a heavier part, but there is a cost to run them per hour no matter how much productis painted and shipped. It is useful to know how much it costs to operate the equipment so that the totalcost is known and so that equipment changes can be accurately evaluated. The cost tooperate a paint system includes utilities (compressed air, gas, and electricity), water,chemicals, and maintenance. Some of these costs can be determined with standardformulas based on the size of the motors, burners, and fans.12.2.3 COST OF SPRAY BOOTH EXHAUSTA spray booth exhausts air to dilute the concentration of solvents and contain over-sprayed paint solids. The exhaust volume from the plant must be made up with outsideair that must be heated when the outdoor temperature is cold. The amount of energyneed depends on the location of the plant and the average outdoor temperatures. The amount of spray booth exhaust, measured in cubic feet per minute (CFM),depends on the size of the booth opening and the required velocity of air to main-tain a satisfactory atmosphere inside the booth. The design face-velocity dependson both the design and the application conditions. Occupational Safety and HealthAdministration (OSHA) requirements traditionally called for a minimum face velocityof 100 ft/min (FPM) in an occupied booth. Lower velocities are permissible in anautomated booth, and the application system may also impact the design velocity.The opening area is multiplied times the design velocity to determine the exhaustvolume.Spray booth opening (ft2 ) × Design face velocity (FPM) = Exhaust volume (CFM) The temperature difference is used to determine the amount of energy con-sumed in British thermal units per hour (Btu/h) and the cost of the fuel used togenerate heat. Plant air temperature − Outside air temperature = Temperature rise The CFM is multiplied by the temperature rise and the value 1.1 to determine theBtu/h. The constant 1.1 is found by multiplying 0.018 (Btu/h required to raise 1 ft3of air 1◦ F at 100% efﬁciency) by 60 (converting CFM to cubic feet per hour, CFH).The value 1.08 is rounded to 1.1. CFM × Temperature rise × 1.1 = Btu/h at 100% efﬁciency The Btu/h can be multiplied by the cost per 100 ft3 of gas to determine the costof the exhaust air; 100 ft3 of gas is equal to 100,000 Btu/h. Btu/h/100,000 × cost per 100 ft3 of gas = Spray booth exhaust $/h.
Cost Analysis for Finishing Systems 197188.8.131.52 Example Booth opening ft2 : 200 Design face velocity: 120 FPM Outside air temperature: 50◦ F (from Table 12.3 of average degree days) Plant air temperature: 70◦ F Cost per 100 ft3 : $0.45 200 × 120 = 24,000 CFM 70 − 50 = 20 temperature rise TABLE 12.3 Average Temperature (Canadian Cities are in ◦ C) Location Averagea Location Average Albany, NY 48 Memphis, TX 62 Albuquerque, NM 55 Miami, FL 75 Atlanta, GA 62 Milwaukee, WI 48 Baltimore, MD 56 Minneapolis, MN 45 Bismarck, ND 41 Mobile, AL 68 Boston, MA 50 Montreal, Que. 7 Buffalo, NY 47 Nashville, TN 60 Burlington, VT 45 New Orleans, LA 70 Calgary, Alta. 4 New York, NY 52 Cheyenne, WY 45 Oklahoma City, OK 60 Chicago, IL 50 Omaha, NE 51 Cleveland, OH 49 Philadelphia, PA 54 Columbia, SC 64 Phoenix, AZ 70 Concord, NH 44 Portland, ME 46 Dallas, TX 66 Providence, RI 50 Denver, CO 50 Quebec, Que. 5 Des Moines, IA 50 Rapid City, SD 47 Detroit, MI 49 Reno, NE 50 Great Falls, MT 46 Richmond, VA 58 Hartford, CT 50 St. Louis, MO 50 Honolulu, HI 75 Salt Lake City, MO 51 Houston, TX 69 San Francisco, CA 56 Indianapolis, IN 53 Seattle, WA 52 Jacksonville, FL 69 Toronto, Ont. 8 Juneau, AK 42 Vancouver, D.C. 11 Kansas City, MO 55 Washington, D.C. 56 Little Rock, AR 62 Wichita, KS 57 Los Angeles, CA 63 Winnipeg, Man. 3 Louisville, KY 57 a Source: Weather Bureau/Department of Commerce.
198 Paint Technology Handbook 24,000 × 20 × 1.1 = 528,000 Btu/h 528,000/100,000 × 0.45 = $2.37/hThis formula for cost per Btu/h can be applied to washer burners or any otherequipment.12.2.4 SOLVENT-BASED LIQUID COATING OVEN EXHAUST REQUIREMENTSAn oven used for solvent-based paint must exhaust air to remove the volatile contentfrom the solvents in the paint and the gases given off by the oven burner. The volumeof exhaust, measured in CFM, and the temperature difference are the key variables. Gallons of paint/h × % Solvent = Gallons of solvent/h The National Fire Protection Association (NFPA) recommends a minimum of167 CFM of exhaust per gallon of solvent sprayed per hour. Gallons of solvent/h × 167 CFM/gallon = Exhaust CFM The CFM must be corrected for the temperature, as the air will expand whenheated. The temperature correction uses the constant of 460, a number related toabsolute zero, a hypothetical temperature characterized by the complete absence ofheat and equivalent to approximately minus 460◦ F. The standard CFM (SCFM) areconverted to actual CFM (ACFM) in the following equation: SCFM × (460 + Maximum design temperature) = ACFM 460 + Ambient Temperature The by-products of combustion must be added to the exhaust volume. The max-imum burner Btu/h is divided by a recommended dilution rate to calculate the exhaustrequirements. The recommended dilution rate to ensure that enough oxygen is presentin the oven is 95 ft3 /s. Maximum burner Btu/h (95 CFM × 60 s) = SCFM As in the ventilation requirement for the solvent concentration, the SCFM must beconverted to ACFM with a temperature correction. The ventilation for solvents andburner gases are added together to determine the total CFM of exhaust. The exhaustcan be converted to Btu/h, and the Btu/h can be used to determine cost as shownabove with the spray booth calculation.
Cost Analysis for Finishing Systems 199184.108.40.206 Example Oven set temperature: 375◦ F Ambient air temperature: 70◦ F Total exhaust: 1403 CFM Cost per 100 ft3 : $0.45 375 − 70 = 305 1403 × 305 × 1.1 = 470,707 Btu/h 470,707/100,000 × 0.45 = $2.12/h12.2.5 HEAT LOSS FROM LOADINGAnother factor that adds to the cost of operating the oven is the amount of productand conveyor that travels through. Energy is expended to heat the product, racks,and chain. Oven set temperature − Ambient temperature = Oven temperature rise Conveyor weight/ft × FPM × 60 min = Pounds of chain and trolley/h (see Table 12.4)(Use same formula for racks and parts) Conveyor chain and trolleys pounds/h + Racks pounds/h + Parts pounds/h = Total loading Oven temperature rise × Total loading × Speciﬁc heat load = Btu/h220.127.116.11 Example Oven set temperature: 375◦ F Ambient air temperature: 70◦ F Chain: 3′′ I-Beam TABLE 12.4 Approximate Weight per Foot of Chain Conveyor Type Chain Weight/Foot Trolley Weight Enclosed track 3.5 pounds 0.5 pounds (H-attachment) X348 2.14 pounds 2.34 pounds X458 3.14 pounds 5.18 pounds X678 6.39 pounds 16.5 pounds
200 Paint Technology Handbook TABLE 12.5 Speciﬁc Heat Load of Some Common Materials Metals Steel—0.125 Iron—0.130 Aluminum—0.248 Zinc—0.095 Brass—0.092 Plastics ABS—0.3 Nylon—0.4 Phenolic—0.4 Polystyrene—0.32 Vinyl—0.2 TABLE 12.6 Panel Loss Factor Panel Panel Loss Thickness Factor 3′′ 0.40 4′′ 0.35 5′′ 0.30 6′′ 0.25 8′′ 0.20 Line speed: 10 FPM Product loading: 6000 pounds (racks and parts, average) Material: Steel 375 − 70 = 305 10 FPM × 4.5 lb/ft × 60 min = 2700 lb chain/h 2700 lb chain + 6000 lb product = 8700 lb/h 305 × 8700 × 0.125 (from Table 12.5) = 331,688 Btu/h12.2.6 RADIANT LOSSESThe last item that contributes to energy consumption in an oven is the radiant lossesthrough the oven panels (see Table 12.6). The amount of loss depends on the oventemperature, the amount of insulation, and the oven size. The formula is shownbelow. Total oven surface area ft2 × Oven panel loss factor × Oven temperature rise = Btu/h18.104.22.168 Example Oven size: 10′ H × 25′ W × 50 L Panel thickness: 5′′ Oven temperature rise: 305◦ F
Cost Analysis for Finishing Systems 201 Oven surface: Ends: 10 × 25 = 250 250 × 2 (ends) = 500 Sides: 10 × 50 = 500 500 × 2 (sides) = 1000 Top and bottom: 25 × 50 = 1250 1250 × 2 = 2500 Total oven surface area, ft2 4000 oven area 4000 × 0.30 × 305 = 366,000 Btu/h12.2.7 LABOR AND MAINTENANCE COSTSObviously, the labor cost to run a system will vary with the size of the system, thelevel of quality expected, hours of production, frequency of color change, and manyother variables. The following calculations are an outline of how to determine the costto run a paint system. In order to accurately determine the cost of labor for coatinga product the variables must be actual data from a particular line.22.214.171.124 Application Labor for Liquid Spray Coating Labor costs w/fringes $/h: Supervision—$15.00 Paint mix—$12.00 Applicators (2)—$27.00 Total operator labor $/h—$54.00Clean-up cost $/h (man-hours/shift × $/h)/operating h/shift 1 h × $15 = 15 15/8 h = $1.88Maintenance labor cost (man-hours/wk × $/h)/operating h/wk 8 h/wk × $15 = 120 120/40 = $3.00Spare parts cost (yearly parts cost/operating h/yr) 15,000/2,000 = $7.50Sludge disposal (lbs/h of coating × % transfer efﬁciency) × (% solids × disposalcost per gallon) 10.7 lb of coating × 0.30 TE × 0.60 solids = 1.93 1.93 × 3.50 = $6.76Labor and maintenance cost $/h 54 + 1.88 + 3.00 + 7.5 + 6.76 = $73.14
202 Paint Technology Handbook126.96.36.199 System Support LaborThe cost per year for support labor, such as rackers, hi-lo drivers, system main-tenance, technicians, and so forth, will vary depending on the size of the system.A typical system might need one technician to oversee the mechanical and chemicalmaintenance of the system, one quality control manager, one hi-lo driver, and fourrackers. At an average cost per hour of $15.00/person, the support labor would cost$105.00/h. 7 workers × 15.00/h = $105.00/h. Therefore, the total labor cost for the system might typically be $178.05/h(73.05 + 105.00) To determine the cost per piece, the hourly cost is divided into the total ft2 paintedper hour, then, the cost per ft2 is multiplied times the ft2 per piece.188.8.131.52 Example Total ft2 /h: 6000 ft2 /piece: 0.5 Total application labor/h: 50.78 Total support labor/h: 105.00 50.78 + 105.00 = 155.78 155.78 0.025 = 6000 ft 2 /h ft 2 0.025 × 0.5 = $0.0125/piece12.2.8 ELECTRICAL CONSUMPTIONFor single-phase motors, the full load amps (FLA) can be found on the motor chart(Table 12.7). To convert FLA to kilowatt-hours (kWh), the FLA is multiplied timesthe motor voltage to get watts and divided by 1000 to get kilowatts. The formula for single-phase motors is: FLA × volts = watts Watts = kilowatts 1000 The formula for three-phase is Volts × amps × 1.73 × power factor = watts Watts = kilowatts 1000 Kilowatts × cost/kWh = hourly operating cost
Cost Analysis for Finishing Systems 203 TABLE 12.7 Motor FLA at 1800 rpm HP 230 V 460 V HP 230 V 460 V HP 230 V 460 V FLA of three-phase induction motors 60 cycles, 1800 rpm 1/4 0.96 0.48 10 24.5 12.3 100 233 116 1/3 1.16 0.58 15 36.7 18.4 125 289 144 1/2 1.68 0.84 20 49.0 24.5 150 346 173 3/4 2.33 1.17 25 62.7 31.3 200 460 230 1 2.75 1.38 30 72.8 36.4 250 572 286 1.5 4.17 2.09 40 98.0 49.0 300 685 342 2 5.56 2.78 50 121 60.5 3 7.87 3.94 60 143 71.5 5 12.7 6.34 75 178 89.0 7.5 19.2 9.60 FLA of single-phase induction motor 60 cycles, 1800 rpm 1/8 2.80 1.40 3/4 10.20 5.10 3 34.00 17.00 1/6 3.20 1.60 1 13.00 6.50 5 56.00 28.00 1/4 4.60 2.30 1 1/2 18.40 9.20 7 1/2 80.00 40.00 1/3 5.20 2.60 2 24.00 12.00 10 100.00 50.00 1/2 7.40 3.70 The power factor will vary with different motors between 0.7 and 0.9. Using 0.75as a typical number will give relatively close accuracy.184.108.40.206 Example10-hp motor, 460/3/60 460 × 12.6 × 1.73 × 0.75 = 7520 7520 = 7.5 kWh 1000 These costs are based on the motor running at full load, which they rarely doin production. Actual numbers can be determined by taking an amp draw fromthe motor and following the formula, substituting the actual amps for the FLAlisted on the chart. The current draw at start-up will be higher than the currentdraw during operation. Some larger motors will need a power correction factor of1.1 or 220.127.116.11.9 COMPRESSED AIRCompressed air is used to operate the spray equipment, pumps, and valves and it mayalso have several other uses within the operation of a paint system. Compressed airis measured by volume in SCFM and by pressure in pounds per square inch (psi).
204 Paint Technology HandbookOne SCFM of compressed air requires approximately 0.21 kWh to generate. At a costof approximately $0.08/kWh, the cost of one SCFM of compressed air is around$0.017/h. 0.21 kWh × 0.08/kWh = 0.017/h. Spray equipment manufacturers can supply the maximum compressed air con-sumption for their equipment. Some typical maximum consumption volumes areshown next for various components in a sample paint system. Spray gun: 8 CFM Agitator: 3 CFM Pump: 7 CFM Other: 5 CFM A typical automated system for liquid application might have several stations forapplication, some automatic and some manual. A typical system might have as manyas 10–14 guns or more. Compressed air consumption will average around 100 CFM.The air compressor sizing should consider the maximum consumption at any onetime, not the average consumption (see Table 12.8). Air leaks in the system should be avoided. Table 12.9 shows the losses associatedwith air leaks. Air leaks can occur from worn valves, bad seals, poor connections (hose to ﬁtting),and leaky disconnects. It is wise to inspect the lines periodically to see if all of theconnections are leak free. TABLE 12.8 Air Compressor Sizing Based on Horse Power Compressor HP 3 5 7.5 10 15 20 25 30 50 Maximum CFM at 100 psi 12 20 30 40 60 80 100 120 200 TABLE 12.9 Cost of Air Leaks Hole Size ft3 Waste at 100 psig Cost/Month at of Loss and 720 h/Month $0.20/1000 ft3 1/2′′ 17,928,000 $3,585.60 3/8′′ 10,108,800 $2,021.76 1/4′′ 4,492,800 $898.56 1/8′′ 1,123,200 $224.64 1/16′′ 280,370 $56.07
Cost Analysis for Finishing Systems 20512.2.10 TOTAL COST OF PAINT APPLICATIONThe total cost of application can be calculated using a standard accounting formula.The costs can be included in whatever heading a company chooses as long as eachcost item is captured. Historical data are always best, but the costs can also be estimated based onstandard formulas. The following outline shows a step-by-step quote for the cost ofpaint application.12.2.11 QUOTING A PARTWhen quoting the cost of application of a particular paint to a particular part the ﬁrststep is to create a list of production information that deﬁnes how the part will be run.The annual volume to be painted will be important when making decisions aboutinvestment in tooling or other items that can improve efﬁciency. The set-up volume(number of parts per run) is also important as it will affect the amount of tooling andinﬂuence set-up costs, color change, and other adjustments that will be necessary forthat part. The square footage of the part must be measured to determine the surface area thatwill be painted. Parts with complex geometry can be broken down into measurablegeometric shapes as shown in Appendix B. Process data are used to determine the parts per hour so that the hourly costscan be broken down into a cost per part. • Design racking conﬁguration (total parts per rack or hook) • Rack or hook spacing on the conveyor (rack center distance in feet) • Conveyor line speed (FPM) • Downtime factor (15–20% typical) This information is used to calculate the cost of each item that inﬂuences theultimate cost to paint the part, including the material cost, labor, burden, ﬁxed cost,and scrap cost. The ﬁrst step is to determine a production rate. Conveyor speed (FPM) × 60 min = FPH Parts/rack = Parts/foot Rack spacing FPH × Parts/foot = Parts/h at 100% uptime Add downtime factor: Parts/h at 100% uptime × 0.80 = Parts/h at 80% uptime
206 Paint Technology Handbook18.104.22.168 Material CostThe material cost follows the formulas supplied for liquid coatings. % Solids × 1604 = Theoretical coverage at 100% Efﬁciency (ft2 /gal, 1 mil thick)(Theoretical coverage/ﬁlm thickness) × Transfer efﬁciency = Actual coverage,ft2 /gal • Adjust the ft2 for paint losses on the rack; assume a percentage of the part ft2 • For large parts the percentage will be lower, because there will be more part and less rack • For smaller parts, the percentage will be higher • For ﬁlm thickness use a default of 1 mil Cost of paint = cost/ft 2 ft 2 /gallon Cost/ft2 × ft2 /part = material cost/part Add start up waste (purging and charging the system) to the cost of material. Cost/gal × waste = total start up material cost Start up material cost = cost per part of waste addition parts per typical run Material cost per part + Waste material per part = Total material cost/part22.214.171.124 LaborTo determine the cost of labor the number of people and the costs for their labor istotaled and compared to the output per hour. Line personnel include sprayers, quality control people, supervisors, rackers(online and off-line) and others (masking, blow-off, etc.). The average straight wage is used to determine the total cost of labor per hour,and then the total labor cost is divided by the production volume to determine thecost per part. Average wage/h × Number of people = Total straight wage Total straight wage = $/part Parts/h126.96.36.199 BurdenBurden is a cost that is added to labor and line operation for additions to hourlywage (insurance, uniforms, training, taxes, etc.) and special materials used to runa particular part (utilities, packaging, supplies, testing, etc.).
Cost Analysis for Finishing Systems 207 Variable labor can often be expressed as a percentage of straight wages,say 25%. Total direct labor × Addition % = Variable labor addition Variable line burden can be calculated by collection of data for items that ﬁt intothis category. The cost of the items that support the line is broken down into an hourlycost, added to the hourly cost of variable labor, and then divided by the productionrate to determine the cost per part. Hourly cost of burden = Cost/part Parts/h188.8.131.52 Fixed CostFixed cost is the cost of operating a business that is steady and ongoing, regardless ofthe number of parts that are painted. This includes building cost, debt, administration,and maintenance. Data for these costs is collected and divided into an hourly ﬁxedcost. The hourly ﬁxed cost is divided into the production rate to determine the costper part. Total ﬁxed cost/h = Cost/part Parts/h184.108.40.206 Scrap CostScrap and rework should be added to the cost per part. The cost of parts that haveto be repainted and the number that have to be thrown away should be totaled anddivided into the production volume and added to the total cost per part.220.127.116.11 Add CostThe total cost of painting the part is the sum of the all the items listed above. • Material cost • Labor cost • Burden • Fixed cost • Scrap cost The ﬁnal price may be adjusted for special considerations. Things like maskingand special packaging should be factored into the cost. Low volumes may make theprice higher just as high volumes may reduce the cost. Any cost that requires payment by the company should be reﬂected in the per piececost. It may not be immediately clear what category the item should be placed in andsome items may ﬁt into more than one category. It does not matter what categorya cost item is put into as long as it is included and the method is consistent.
Cost Analysis for Finishing Systems 209APPENDIX BCOMMON GEOMETRIES AND FORMULAS FOR CALCULATION OF AREACIRCLE Area = 0.785 × Square of the diameter = 0.785 × (A)2 = 0.785 × A × AExample—The circle is 4′′ in diameter Area = 0.785 × (4)2 = 0.785 × 4 × 4 = 12.56 in.2 AELLIPSE Area = 0.785 × Long diameter × Short diameter = 0.785 × B × CExample—Ellipse 4′′ × 3′′ Area = 0.785 × 4 × 3 = 9.42 in.2 B CPARABOLA Area = 2/3 Base × Height = 2/3 × D × EExample—Base is 3′′ and the height is 5′′ Area = 2/3 × 3 × 5 = 10 in.2 E D
210 Paint Technology HandbookSPHERE Area = 3.14 × Square of diameter—3.14 × (F)2 = 3.14 × F × FExample—Sphere is 5′′ in diameter Area = 3.14 × (5)2 = 3.14 × 5 × 5 = 78.5 in.2 FCYLINDER 1. Hollow Area = Circumference × Length = 3.14 × H × G Example— Tube 4′′ in diameter and 12′′ long Area = 3.14 × 4 × 12 = 150.7 in.2 2. Solid Area = Circumference × Length plus twice cross − sectional area 3.14 × H × G + 1.57 × H × H = Area to be covered Example— Round bar is 4′′ in diameter and 12′′ long Area = 3.14 × 4 × 12 = 150.7 +1.57 × 4 × 4 = 25.1 = 175.8 in.2 G H
Cost Analysis for Finishing Systems 211CONE 1. Hollow Area = 1/2 of circumference of base × slant height1.57 × K × J Example— Cone is 4′′ in diameter at base and 6′′ slant height Area = 1.57 × 4 × 6 = 37.68 in.2 2. Solid Area = 1.57 × K × J + 0.785 × K × K Example— Same as above Area = 1.57 × 4 × 6 + 0.785 × 4 × 4 = 37.68 + 12.56 = 50.24 in.2 J KFRUSTRUM OF CONE 1. Hollow Area = 1/2 sum of circumference of bases × slant height = 1.57 × (M + N) × L Example— A tapered tube 4′′ diameter at small end, 6′′ diameter at large end, and 6′′ slant height Area = 1.57 × (6 + 4) × 6 = 94.2 in.2 2. Solid Area = 1/2 sum of circumference of bases + slant height + sum of areas of bases 1.57 × (M + N) × L + 0.785 × (M2 + N2 ) = in.2
212 Paint Technology Handbook Example— A tapered bar 4′′ diameter at small end, 6′′ diameter at large end and 6′′ slant height Area = 1.57 × (6 + 4) × 6 + 0.785 × (6 × 6 + 4 × 4) = 94.2 + 40.8 = 135 sq. in. On all cylinders, cones, and frustums of cones that are hollow and where it is desired to know the area that must be covered, if outside and inside areas are to be determined, the average of the outside and inside diameters should be used in the formulas and the result doubled. N L MSQUARE Area = O × PExample—Square 5′′ on a side Area = 5 × 5 = 25 in.2 O PRECTANGLE Area = S × TExample—Rectangle 5′′ × 3′′ Area = 5 × 3 = 15 in.2 S T
Cost Analysis for Finishing Systems 213CUBE(All sides equal) Area = 6 × square of one sideExample—Cube 6′′ on one side Area = 6 × (6)2 = 216 in.2 W V UTRIANGLE 1/2 × base × altitude Area = 1/2 × Y × ZExample—Base of triangle is 8′′ and height is 6′′ Area = 1/2 × 8 × 6 = 24 in.2 Z YHEXAGON(Six equal sides—all angles equal) Area = 3/2 × length of one side × distance between any two parallel sides Area = 3/2 × B × A
214 Paint Technology HandbookExample—Hexagon 2′′ on a side and 4′′ between ﬂats Area = 3/2 × 2 × 4 = 12 in.2 A BPARALLELOGRAM(Opposite sides parallel) Area = Length of side × Vertical distance to parallel side = C × DExample—A parallelogram with one side of 6′′ and a distance of 4′′ between this side and theparallel side. Area = 6 × 4 = 24 in.2 D CRECTANGULAR PARALLELOPIPED(Opposite sides parallel) Area = 2 × (E × F + F × G + G × E) = Surface
Cost Analysis for Finishing Systems 215Example—A block having sides 4′′ , 6′′ , and 8′′ long, respectively Area = 2 × (4 × 6 + 6 × 8 + 8 × 4) = 208 in.2 F G ETRAPEZOID(One pair of opposite sides parallel) Area = 1/2 sum of the parallel sides × vertical distance between them = 1/2 × (H + J) × KExample—A trapezoid having parallel sides 6′′ and 4′′ long respectively, distance between thembeing 4′′ Area = 1/2 × (6 + 4) × 4 = 20 in.2 J K H